1,013 122 20MB
English Pages [789] Year 2011
Table of contents :
Title
Contents
1 MATERIALS PROPERTIES AND REQUIREMENTS
2 CRYSTAL STRUCTURE
3 CHARACTERISATION OF MATERIALS
4 COHESION BETWEEN ATOMS
5 CRYSTAL IMPERFECTIONS
6 CLASSIFICATION OF SOLIDS
7 ELECTRON THEORY OF SOLIDS
8 STATISTICS AND BAND THEORY OF SOLIDS
9 PHASE DIAGRAM
10 TRANSPORT PROPERTIES OF SEMICONDUCTORS
11 MECHANICAL PROPERTIES
12 THERMAL PROPERTIES
13 OPTICAL PROPERTIES OF MATERIALS
14 LUMINESCENCE
15 DISPLAY DEVICES
16 PHOTOCONDUCTIVITY
17 THERMOGRAPHY
18 DIELECTRIC MATERIALS
19 MAGNETIC MATERIALS
20 SUPERCONDUCTING MATERIALS
21 COMPOSITE MATERIALS
22 ADVANCED CERAMICS
23 POLYMER MATERIALS
24 METALLIC GLASSES
25 NONLINEAR MATERIALS
26 BIOMATERIALS
27 SHAPE MEMORY ALLOYS
28 NANOMATERIAL SYNTHESIS
29 NANODEVICES
Appendix 1 1PERIODIC TABLE OF THE ELEMENTS
Appendix 2 THE INTERNATIONAL SYSTEM OF UNITS
Appendix 3 LIST OF FUNDAMENTAL PHYSICAL CONSTANTS
Appendix 4 THE GREEK ALPHABET
Index
Materials Science
ABOUT THE AUTHOR
RAJENDRAN V, FUSI, FASI, FInstP, is the Director, Research & Development, K S R Group of Institutions and Centre for Nano Science and Technology (CNST), K S Rangasamy College of Technology, Tamil Nadu. He has been pivotal in developing the stateoftheart facilities at Centre for Nano Science and Technology Research, KSRCT at par with international standards, in coordination with science and technology faculty. He obtained his Ph.D. degree in Ultrasonics from Annamalai University. He completed his MTech in Nanotechnology from Anna University. He is currently engaged in various collaborative research works with many leading research laboratories both in India and abroad. He is currently working in the areas of nano metal oxides for different industrial applications, nanosilica from rice husk for applications such as textiles and biomedical, nano bioactive glasses and nano herbal particles for biomedical applications and nanoparticles for energy applications. Dr Rajendran has made many innovative contributions to materials characterisation using online ultrasonic techniques and other conventional techniques. He has also received many prestigious awards such as, National NDT Man of the Year 2004, TANSA Award, Outstanding Organiser Award, DAAD from Germany, INSA, TNSCST Young Scientist, DAE /BRNS Visiting Scientist, among others. Apart from this, he has organised three National Level conferences on Ultrasonics, Acoustics and Instrumentation, two International Conferences on Nanomaterials and several workshops towards fulfilling his vision of imparting knowledge to the young and budding research scholars. His passion towards research led him to be the Principal Investigator of 15 completed sponsored research projects with a fund involvement to the tune of INR 20 million. Six ongoing sponsored research projects to the tune of INR 15 million are under progress with the sponsorship from Nanomission DST, DRDO, IGCAR, etc. Under his able guidance, eight scholars have completed their doctoral degree and 15 others are pursuing their PhD degree. He has to his credit more than 110 research papers in reputed International journals, 99 papers in conference proceedings, 25 referred books, eight edited proceedings, two research and development book and 12 patents. He has also visited as guest scientist to various research laboratories, universities and conferences in more than 27 countries which includes USA, UK, Germany, Italy, France, Sweden, Finland, Brazil, West Indies, Singapore, Hong Kong, Taiwan, South Africa, Australia and South Korea. He is a member in the Board of Studies and Doctoral Committee in several universities (including Anna University). He is a fellow and life member in many scientific societies, both in India and abroad. He is the present President of Acoustical Society of India. Dr Rajendran is the coordinator for the Innovation in Science Pursuit for Inspired Research (INSPIRE) programme sponsored by Department of Science and Technology (DST), New Delhi with a major funding to attract and to motivate young talented students to make them as future Scientists of India. He is the chair of the forthcoming International Symposium on Macro and Supramolecular Architectures and Materials (MAM 2012) which will be held during November 21–25, 2012.
Materials Science
V Rajendran Director and Research and Development Centre for Nano Science and Technology K S R College of Technology and K S R Group of Institutions Tiruchengode Tamil Nadu
Tata McGrawHill Publishing Company Limited NEW DELHI McGrawHill Offices New Delhi New York St Louis San Francisco Auckland Bogotá Caracas Kuala Lumpur Lisbon London Madrid Mexico City Milan Montreal San Juan Santiago Singapore Sydney Tokyo Toronto
Tata McGrawHill Published by Tata McGrawHill Publishing Company Limited, 7 West Patel Nagar, New Delhi 110 008. Copyright © 2011, by Tata McGrawHill Publishing Company Limited. No part of this publication may be reproduced or distributed in any form or by any means, electronic, mechanical, photocopying, recording, or otherwise or stored in a database or retrieval system without the prior written permission of the publishers. The program listings (if any) may be entered, stored and executed in a computer system, but they may not be reproduced for publication. This edition can be exported from India only by the publishers, Tata McGrawHill Publishing Company Limited. ISBN (13 digits): 9780071328975 ISBN (10 digits): 0071328971 Vice President and Managing Director—McGrawHill Education, Asia Pacific Region: Ajay Shukla Head—Higher Education Publishing and Marketing: Vibha Mahajan Publishing Manager—SEM & Tech Ed.: Shalini Jha Asst Sponsoring Editor: Tina Jajoriya Copy Editor: Preyoshi Kundu Sr Production Manager: Satinder S Baveja Proof Reader: Yukti Sharma Marketing Manager—Higher Ed.: Vijay Sarathi Sr Product Specialist—SEM & Tech Ed.: John Mathews General Manager—Production: Rajender P Ghansela Asst General Manager—Production: B L Dogra Information contained in this work has been obtained by Tata McGrawHill, from sources believed to be reliable. However, neither Tata McGrawHill nor its authors guarantee the accuracy or completeness of any information published herein, and neither Tata McGraw Hill nor its authors shall be responsible for any errors, omissions, or damages arising out of use of this information. This work is published with the understanding that Tata McGrawHill and its authors are supplying information but are not attempting to render professional services. If such services are required, the assistance of an appropriate professional should be sought.
Typeset at Tulyasys Technologies, No. 1 Arulananthammal Nagar, Thanjavur 613 007, and printed at Avon printers, Plot No. 16, Main Loni Road, Jawahar Nagar, Industrial Area, Shahdara, Delhi  110 094. Cover Printer: A.P. Offset RAXLCRBWDLXRD
FOREWORD
Materials Science has emerged as a fast growing multidisciplinary field involving experts from several related and seemingly unrelated specializations. It embraces ceramics, polymers, semiconductors, magnetic materials, optical materials, medical implant materials and biological materials. These may be in bulk form or as thin layers with thicknesses going down to nano meters. Besides ever increasing applications requiring materials conforming to stringent specifications there is always an underlying motive to understand the relationship between properties and materials characteristics, namely composition, impurities, crystallographic structure and lattice imperfections. A newly emerging branch, Combinatorial Materials Science is great potential. The book, Materials Science by Dr V Rajendran is designed to provide a good understanding of the basics of materials, in terms of their structural, optical, electrical, magnetic and mechanical properties. It constitutes an important and critical area of study for the students of various engineering disciplines. One of the major highlights of the book is the inclusion of nanophase materials, shape memory alloys, ceramics, polymers, and biocompatible materials. To write a book on a subject like Materials Science requires writing skill and thorough knowledge of the subject. Being an expert on the subject and having authored many books, Dr Rajendran has succeeded in writing this book, which explains the basics of materials, in terms of their structure, optical, electrical, magnetic and mechanical properties. The author has adopted studentfriendly approach throughout the book. I am sure this book will act as a strong foundation for all students in various engineering and technology disciplines and also help teachers in nurturing an interest into this challenging yet exciting field of Materials Science in the minds of students.
Prof. Dr. Krishan Lal President, Indian National Science Academy DST Ramanna Fellow Past President, CODATA Former Director, National Physical Laboratory, New Delhi
CONTENTS
1.
MATERIALS PROPERTIES AND REQUIREMENTS 1.1 1.2 1.3 1.4 1.5
2.
3.
Introduction ..................................................................................................................................... 1 Levels of Structure .......................................................................................................................... 1 Structure – Property Relationship ................................................................................................... 2 Material Selection for Engineering Application.............................................................................. 4 Classification of Engineering Materials .......................................................................................... 5 Key Points to Remember������������������������������������������������������������������������������������������������������������������ 7 Solved Problems ������������������������������������������������������������������������������������������������������������������������������ 8 ObjectiveType Questions���������������������������������������������������������������������������������������������������������������� 9 Short Questions ������������������������������������������������������������������������������������������������������������������������������� 9 Descriptive Questions ������������������������������������������������������������������������������������������������������������������� 10 Exercises���������������������������������������������������������������������������������������������������������������������������������������� 10
CRYSTAL STRUCTURE 2.1 2.2 2.3 2.4 2.5 2.6 2.7 2.8 2.9
11–56
Introduction ................................................................................................................................... 11 Fundamental Terms of Crystallography ........................................................................................ 12 Types of Crystals ........................................................................................................................... 15 Relation Between the Interplanar Distance and the Interatomic Distance .................................... 19 Crystal Structures of Materials ...................................................................................................... 21 Simple Cubic Crystal Structure ..................................................................................................... 21 Body Centred Cubic Structure ...................................................................................................... 22 Face Centred Cubic Structure or Cubic Close Packed Structure .................................................. 24 Hexagonal Closed Packed Structure ............................................................................................. 26 Key Points to Remember���������������������������������������������������������������������������������������������������������������� 29 Solved Problems ���������������������������������������������������������������������������������������������������������������������������� 29 ObjectiveType Questions�������������������������������������������������������������������������������������������������������������� 54 Short Questions ����������������������������������������������������������������������������������������������������������������������������� 55 Descriptive Questions ������������������������������������������������������������������������������������������������������������������� 56 Exercises���������������������������������������������������������������������������������������������������������������������������������������� 56
CHARACTERISATION OF MATERIALS 3.1 3.2 3.3 3.4 3.5 3.6 3.7
1–10
57–98
Introduction ................................................................................................................................... 57 Discovery of Xrays ...................................................................................................................... 58 Diffraction of Xrays ..................................................................................................................... 59 Determination of Crystal Structure ............................................................................................... 63 Bragg’s Law and Crystal Structures .............................................................................................. 67 Optical and Other Instruments ...................................................................................................... 69 Optical Microscope ....................................................................................................................... 71
viii Contents
3.8 3.9 3.10 3.11 3.12 3.13 3.14 3.15 3.16 3.17 3.18 3.19
4.
COHESION BETWEEN ATOMS 4.1 4.2 4.3 4.4
5.
Focusing of Electron Beams........................................................................................................ 72 Electron Microscope.................................................................................................................... 74 Scanning Electron Microscope (SEM) ........................................................................................ 75 Transmission Electron Microscope (TEM) ................................................................................. 76 Scanning Transmission Electron Microscope (STEM) ............................................................... 77 Microhardness (NanoHardness)................................................................................................. 79 Classifications of Hardness Test .................................................................................................. 79 Microhardness Test...................................................................................................................... 80 Nano Indenter .............................................................................................................................. 82 Comparison Between Micro and NanoIndentations .................................................................. 83 Atomic Force Microscope ........................................................................................................... 84 Electron Diffraction ..................................................................................................................... 87 Key Points to Remember �������������������������������������������������������������������������������������������������������������� 88 Solved Problems �������������������������������������������������������������������������������������������������������������������������� 89 ObjectiveType Questions ������������������������������������������������������������������������������������������������������������ 94 Short Questions ��������������������������������������������������������������������������������������������������������������������������� 97 Descriptive Questions ������������������������������������������������������������������������������������������������������������������ 98
Introduction ................................................................................................................................... 99 Classification of Solids .................................................................................................................. 99 Bonding in Solids ........................................................................................................................ 101 Classification of Bonds ............................................................................................................... 101 Key Points to Remember�������������������������������������������������������������������������������������������������������������� 110 Solved Problems �������������������������������������������������������������������������������������������������������������������������� 110 ObjectiveType Questions������������������������������������������������������������������������������������������������������������ 111 Short Questions ��������������������������������������������������������������������������������������������������������������������������� 111 Descriptive Questions ����������������������������������������������������������������������������������������������������������������� 112
CRYSTAL IMPERFECTIONS 5.1 5.2 5.3 5.4 5.5 5.6 5.7 5.8 5.9
99–112
113–133
Introduction ................................................................................................................................. 113 Classification of Imperfections ................................................................................................... 113 Point Defect or Imperfection ....................................................................................................... 114 Line Imperfection ........................................................................................................................ 118 Dislocation Climb ....................................................................................................................... 121 Multiplication of DislocationFrank Read Generator ................................................................. 121 Surface Defect or Planar Defect .................................................................................................. 122 Volume Defect or Bulk Defect .................................................................................................... 126 Deformation in Metals................................................................................................................. 127 Key Points to Remember�������������������������������������������������������������������������������������������������������������� 129 Solved Problems �������������������������������������������������������������������������������������������������������������������������� 130 ObjectiveType Questions������������������������������������������������������������������������������������������������������������ 131 Short Questions ��������������������������������������������������������������������������������������������������������������������������� 132 Descriptive Questions ����������������������������������������������������������������������������������������������������������������� 133 Exercise ��������������������������������������������������������������������������������������������������������������������������������������� 133
Contents
6.
CLASSIFICATION OF SOLIDS 6.1 6.2 6.3 6.4 6.5 6.6
7.
8.
146–171
Introduction ............................................................................................................................... 146 Electrical Conduction ................................................................................................................ 147 Classification of Conducting Materials ..................................................................................... 147 Classical Free Electron or Drude – Lorentz Theory of Metals ................................................. 148 Expression for Electrical Conductivity and Drift Velocity ........................................................ 149 Thermal Conductivity ................................................................................................................ 153 Expression for Thermal Conductivity ....................................................................................... 153 Wiedemann–Franz Law ............................................................................................................. 155 Verification of Ohm’s Law ........................................................................................................ 157 Classical Free Electron Theory: Advantages and Drawbacks ................................................... 158 Key Points to Remember ������������������������������������������������������������������������������������������������������������ 159 Solved Problems ������������������������������������������������������������������������������������������������������������������������ 160 ObjectiveType Questions ���������������������������������������������������������������������������������������������������������� 169 Short Questions ������������������������������������������������������������������������������������������������������������������������� 170 Descriptive Questions ���������������������������������������������������������������������������������������������������������������� 171
STATISTICS AND BAND THEORY OF SOLIDS 8.1 8.2 8.3 8.4 8.5 8.6 8.7 8.8 8.9 8.10 8.11 8.12 8.13 8.14
134–145
Introduction ................................................................................................................................. 134 Classification of Solids on the Basis of Band Theory ................................................................. 134 Classification of Semiconductors ................................................................................................ 136 Elememental and Compound Semiconductors............................................................................ 140 Crystal Structure and Bonding in Si And Ge .............................................................................. 141 Applications ................................................................................................................................ 142 Key Points to Remember�������������������������������������������������������������������������������������������������������������� 143 Solved Problems �������������������������������������������������������������������������������������������������������������������������� 143 ObjectiveType Questions������������������������������������������������������������������������������������������������������������ 144 Short Questions ��������������������������������������������������������������������������������������������������������������������������� 145 Descriptive Questions ����������������������������������������������������������������������������������������������������������������� 145
ELECTRON THEORY OF SOLIDS 7.1 7.2 7.3 7.4 7.5 7.6 7.7 7.8 7.9 7.10
ix
172–226
Introduction ............................................................................................................................... 172 FermiDirac Statistics ................................................................................................................ 172 Carrier Concentration (Free Electron Density) in Metals ......................................................... 177 Effect of Temperature on Fermi Energy Function..................................................................... 178 Significance of Fermi Energy.................................................................................................... 180 Effective Mass of an Electron ................................................................................................... 182 Concept of Hole......................................................................................................................... 185 Band Theory of Solids – Origin of Energy Gap ........................................................................ 186 KronigPenney Model ............................................................................................................... 191 Brillouin Zone ........................................................................................................................... 195 Explanation of Band Gap .......................................................................................................... 198 Conductivity of Copper and Aluminum .................................................................................... 201 Effect of Temperature and Impurity on Electrical Resistivity of Metals (Matthiessen’s Rule) 202 High Resistivity Materials ......................................................................................................... 204
x
Contents
Key Points to Remember ������������������������������������������������������������������������������������������������������������ 207 Solved Problems ������������������������������������������������������������������������������������������������������������������������ 208 ObjectiveType Questions ���������������������������������������������������������������������������������������������������������� 224 Short Questions ������������������������������������������������������������������������������������������������������������������������� 225 Descriptive Questions ���������������������������������������������������������������������������������������������������������������� 226 Exercises ������������������������������������������������������������������������������������������������������������������������������������ 226 9.
PHASE DIAGRAM 9.1 9.2 9.3 9.4 9.5 9.6
10.
11.
Introduction ............................................................................................................................... 227 Classification of Metal Alloys ................................................................................................... 227 Ferrous Alloys ........................................................................................................................... 228 Phase Diagram........................................................................................................................... 233 Nonferrous Alloys ..................................................................................................................... 235 Titanium and its Alloys.............................................................................................................. 237 Key Points to Remember������������������������������������������������������������������������������������������������������������ 238 Short Questions ������������������������������������������������������������������������������������������������������������������������� 239 Descriptive Questions ��������������������������������������������������������������������������������������������������������������� 239
TRANSPORT PROPERTIES OF SEMICONDUCTORS 10.1 10.2 10.3 10.4 10.5 10.6 10.7 10.8 10.9
241–294
Introduction ............................................................................................................................. 241 Carrier Concentration in an Intrinsic Semiconductor.............................................................. 241 Conductivity of Semiconductors ............................................................................................. 247 Extrinsic Semiconductor ......................................................................................................... 249 ntype Semiconductor.............................................................................................................. 250 ptype Semiconductor.............................................................................................................. 252 Hall Effect ............................................................................................................................... 254 Variation of Electrical Conductivity with Temperature ........................................................... 258 Variation of Fermi Level with Temperature in Extrinsic Semiconductor ................................ 264 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 266 Solved Problems ���������������������������������������������������������������������������������������������������������������������� 267 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 291 Short Questions ����������������������������������������������������������������������������������������������������������������������� 293 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 294 Exercises ���������������������������������������������������������������������������������������������������������������������������������� 294
MECHANICAL PROPERTIES 11.1 11.2 11.3 11.4
227–240
295–336
Introduction ............................................................................................................................. 295 Mechanical Properties and their Measurements...................................................................... 296 Strengthening Mechanism to Improve the Mechanical Properties.......................................... 315 Fracture.................................................................................................................................... 323 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 331 Solved Problems ���������������������������������������������������������������������������������������������������������������������� 332 Fill in the blanks ���������������������������������������������������������������������������������������������������������������������� 333 Short Questions ����������������������������������������������������������������������������������������������������������������������� 334 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 336 Exercises ���������������������������������������������������������������������������������������������������������������������������������� 336
Contents
12. THERMAL PROPERTIES 12.1 12.2 12.3 12.4 12.5 12.6 12.7
337–359
Introduction ............................................................................................................................. 337 Heat Capacity .......................................................................................................................... 337 Thermal Expansion.................................................................................................................. 340 Thermal Conductivity .............................................................................................................. 343 Melting Point ........................................................................................................................... 346 Thermal Stress ......................................................................................................................... 347 Thermal Fatigue and Thermal shock ....................................................................................... 349 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 349 Solved Problems ���������������������������������������������������������������������������������������������������������������������� 350 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 357 Short Questions ����������������������������������������������������������������������������������������������������������������������� 357 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 358 Exercises ���������������������������������������������������������������������������������������������������������������������������������� 358
13. OPTICAL PROPERTIES OF MATERIALS 13.1 13.2 13.3 13.4 13.5 13.6
xi
360–376
Introduction ............................................................................................................................. 360 Fundamentals .......................................................................................................................... 361 Classification of Optical Materials .......................................................................................... 364 Optical Properties of Materials................................................................................................ 364 Excitons ................................................................................................................................... 367 Colour Centres......................................................................................................................... 370 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 374 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 375 Short Questions ����������������������������������������������������������������������������������������������������������������������� 376 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 376
14. LUMINESCENCE
377–387
14.1 Introduction ............................................................................................................................. 377 14.2 Principle .................................................................................................................................. 377 14.3 Photoluminescence .................................................................................................................. 378 14.4 Phosphors ................................................................................................................................ 381 14.5 Cathodoluminescence.............................................................................................................. 381 14.6 Electroluminescence................................................................................................................ 382 14.7 Applications ............................................................................................................................. 384 14.8 Nonlinear Materials ................................................................................................................. 385 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 385 Solved Problems ���������������������������������������������������������������������������������������������������������������������� 386 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 387 Short Questions ����������������������������������������������������������������������������������������������������������������������� 387 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 387 Exercises ���������������������������������������������������������������������������������������������������������������������������������� 387 15. DISPLAY DEVICES 15.1 15.2
388–408
Introduction ............................................................................................................................. 388 Display Devices ....................................................................................................................... 388
xii Contents
15.3 15.4 15.5 15.6 15.7 15.8
16.
PHOTOCONDUCTIVITY 16.1 16.2 16.3 16.4 16.5 16.6 16.7
17.
420–428
Introduction ............................................................................................................................. 420 Principle .................................................................................................................................. 420 Classification of Thermography .............................................................................................. 421 Experimental Techniques ........................................................................................................ 421 Noncamera Detectors .............................................................................................................. 424 Advantages and Limitations of Thermography ....................................................................... 424 Applications ............................................................................................................................. 425 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 426 Fill in the blanks ���������������������������������������������������������������������������������������������������������������������� 426 Short Questions ����������������������������������������������������������������������������������������������������������������������� 427 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 428
DIELECTRIC MATERIALS 18.1 18.2 18.3 18.4 18.5
409–419
Introduction ............................................................................................................................. 409 Photoconductivity .................................................................................................................... 409 Characteristics of Photoconductive Materials ......................................................................... 412 Photodetectors ......................................................................................................................... 413 Photodetector Bias Circuit ...................................................................................................... 414 Performance of Photodetector ................................................................................................. 415 Applications ............................................................................................................................. 416 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 416 Solved Problems ���������������������������������������������������������������������������������������������������������������������� 416 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 417 Short Questions ����������������������������������������������������������������������������������������������������������������������� 419 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 419 Exercises ���������������������������������������������������������������������������������������������������������������������������������� 419
THERMOGRAPHY 17.1 17.2 17.3 17.4 17.5 17.6 17.7
18.
Active Display Devices ........................................................................................................... 389 Passive Display Devices .......................................................................................................... 395 Different Modes of LCD ......................................................................................................... 398 Liquid Crystal Display System ............................................................................................... 399 Comparison Between LEDs and LCDs ................................................................................... 403 Applications ............................................................................................................................. 403 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 404 Solved Problems ���������������������������������������������������������������������������������������������������������������������� 406 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 406 Short Questions ����������������������������������������������������������������������������������������������������������������������� 407 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 408
429–481
Introduction ............................................................................................................................. 429 Definitions ............................................................................................................................... 430 Different Types of Polarisations .............................................................................................. 432 Local or Internal Field ............................................................................................................. 438 Types of Dielectric Materials .................................................................................................. 440
Contents
xiii
18.6 Classification of Electrical Insulating Materials ................................................................... 442 18.7 ClaussiusMosotti Equation .................................................................................................. 443 18.8 Experimental Determination of Dielectric Constant ............................................................. 445 18.9 Dielectric Loss....................................................................................................................... 447 18.10 Dielectric Breakdown ............................................................................................................ 448 18.11 Ferroelectric Material ............................................................................................................ 450 18.12 Dielectric Properties .............................................................................................................. 452 18.13 Active and Passive Dielectrics ............................................................................................... 453 18.14 Frequency and Temperature Dependence of Dielectric Properties ....................................... 453 18.15 Uses of Dielectric Materials .................................................................................................. 456 18.16 Application ............................................................................................................................ 458 Key Points to Remember ��������������������������������������������������������������������������������������������������������� 459 Solved Problems ��������������������������������������������������������������������������������������������������������������������� 460 ObjectiveType Questions ������������������������������������������������������������������������������������������������������� 477 Short Questions ���������������������������������������������������������������������������������������������������������������������� 479 Descriptive Questions������������������������������������������������������������������������������������������������������������� 480 Exercises ��������������������������������������������������������������������������������������������������������������������������������� 481 19. MAGNETIC MATERIALS
482–556
19.1 Introduction ........................................................................................................................... 482 19.2 Magnetic Parameters ............................................................................................................. 483 19.3 Bohr Magneton ...................................................................................................................... 484 19.4 Classification of Magnetic Materials .................................................................................... 485 19.5 Origin of Permanent Magnetic Moment ............................................................................... 489 19.6 Diamagnetism........................................................................................................................ 491 19.7 Paramagnetism ...................................................................................................................... 494 19.8 Ferromagnetic Materials........................................................................................................ 505 19.9 AntiFerromagnetic Materials ............................................................................................... 517 19.10 Ferrimagnetic Materials ........................................................................................................ 520 19.11 Hard and Soft Magnetic Materials ........................................................................................ 523 19.12 Energy Product of Magnetic Materials ................................................................................. 526 19.13 Ferrite Core Memory ............................................................................................................. 528 19.14 Magnetic Recording Materials .............................................................................................. 529 19.15 Magnetic Principle of Analog Recording and Recording ..................................................... 530 19.16 Magnetic Bubble Memory..................................................................................................... 531 19.17 Magnetic Principle in Computer Data Storage...................................................................... 534 19.18 Magnetic Tape ....................................................................................................................... 534 19.19 Floppy Disk ........................................................................................................................... 536 19.20 Magnetic Hard Disk .............................................................................................................. 537 19.21 Computer Aided Tomography ............................................................................................... 538 Key Points to Remember�������������������������������������������������������������������������������������������������������� 540 Solved Problems �������������������������������������������������������������������������������������������������������������������� 541 ObjectiveType Questions ����������������������������������������������������������������������������������������������������� 549 Short Questions ��������������������������������������������������������������������������������������������������������������������� 553 Descriptive Questions ����������������������������������������������������������������������������������������������������������� 555 Exercises ������������������������������������������������������������������������������������������������������������������������������� 556
xiv
20.
Contents
SUPERCONDUCTING MATERIALS 20.1 20.2 20.3 20.4 20.5 20.6 20.7
21.
22.
583–606
Introduction ............................................................................................................................. 583 Classification of Ceramics....................................................................................................... 583 Structure of Ceramics .............................................................................................................. 584 Ceramic Fabrication ................................................................................................................ 587 Ceramic Materials ................................................................................................................... 593 Properties of Ceramics ............................................................................................................ 600 Applications of Ceramics ........................................................................................................ 602 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 603 Short Questions ����������������������������������������������������������������������������������������������������������������������� 604 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 606
POLYMER MATERIALS 23.1 23.2 23.3 23.4 23.5 23.6 23.7 23.8
573–582
Introduction ............................................................................................................................. 573 Classification of the Composite Materials .............................................................................. 573 Particle Reinforced Composites .............................................................................................. 575 Fiber Reinforced Composites .................................................................................................. 577 Processing Techniques for Composite Materials .................................................................... 579 Applications ............................................................................................................................. 581 Short Questions ����������������������������������������������������������������������������������������������������������������������� 582 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 582
ADVANCED CERAMICS 22.1 22.2 22.3 22.4 22.5 22.6 22.7
23.
Introduction ............................................................................................................................. 557 General Properties of Superconducting Materials................................................................... 558 Types of Superconductors ....................................................................................................... 560 Bardeen, Cooper and Schrieffer (BCS) Theory ...................................................................... 562 Electron–Phonon Interaction ................................................................................................... 562 High Temperature Superconductors ........................................................................................ 563 Applications ............................................................................................................................. 565 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 568 Solved Problems ���������������������������������������������������������������������������������������������������������������������� 568 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 570 Short Questions ����������������������������������������������������������������������������������������������������������������������� 571 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 572
COMPOSITE MATERIALS 21.1 21.2 21.3 21.4 21.5 21.6
557–572
607–629
Introduction ............................................................................................................................. 607 Polymerisation Mechanism ..................................................................................................... 608 Degree of Polymerisation ........................................................................................................ 611 Classification of Polymers....................................................................................................... 611 Structure of Polymer ............................................................................................................... 615 Polymer Processing ................................................................................................................. 617 Properties of The Polymers ..................................................................................................... 619 Applications ............................................................................................................................. 624
Contents
xv
Key Points to Remember ���������������������������������������������������������������������������������������������������������� 625 Solved Problems ���������������������������������������������������������������������������������������������������������������������� 625 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 626 Short Questions ����������������������������������������������������������������������������������������������������������������������� 627 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 628 Exercises ���������������������������������������������������������������������������������������������������������������������������������� 629 24. METALLIC GLASSES
630–642
24.1 Introduction ............................................................................................................................. 630 24.2 Origin of Metallic Glasses....................................................................................................... 631 24.3 Principle .................................................................................................................................. 631 24.4 Preparation............................................................................................................................... 632 24.5 Properties ................................................................................................................................. 634 24.6 Applications ............................................................................................................................. 639 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 640 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 641 Short Questions ����������������������������������������������������������������������������������������������������������������������� 642 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 642 25. NONLINEAR MATERIALS
643–656
25.1 Introduction ............................................................................................................................. 643 25.2 Basic Principle......................................................................................................................... 644 25.3 Classification of Nonlinear Materials...................................................................................... 645 25.4 Nonlinear Properties ................................................................................................................ 646 25.5 Nonlinear Materials ................................................................................................................. 651 25.6 Applications ............................................................................................................................. 653 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 654 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 654 Short Questions ����������������������������������������������������������������������������������������������������������������������� 655 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 656 26. BIOMATERIALS
657–670
26.1 Introduction ............................................................................................................................. 657 26.2 Biomechanism ......................................................................................................................... 657 26.3 Development of Biomaterials .................................................................................................. 659 26.4 Classification of Biomaterials ................................................................................................. 664 26.5 Processing and Properties........................................................................................................ 667 26.6 Applications ............................................................................................................................. 667 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 669 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 669 Short Questions ����������������������������������������������������������������������������������������������������������������������� 670 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 670 27. SHAPE MEMORY ALLOYS 27.1 27.2
671–686
Introduction ............................................................................................................................. 671 Origin of Shape Memory Alloys ............................................................................................. 672
xvi
Contents
27.3 27.4 27.5 27.6 27.7 27.8 27.9
28.
NANOMATERIAL SYNTHESIS 28.1 28.2 28.3 28.4 28.5 28.6 28.7 28.8 28.9 28.10 28.11
29.
Principle of Phase Transformation in Shape Memory Alloys ................................................. 672 Shape Memory Alloys—Properties ......................................................................................... 675 Processing Techniques............................................................................................................. 677 Characterisation Techniques.................................................................................................... 677 Commercial Shape Memory Alloys ........................................................................................ 679 Shape Memory AlloysApplications ....................................................................................... 683 Shape Memory AlloysDisadvantages...................................................................................... 684 Key Points to Remember ���������������������������������������������������������������������������������������������������������� 685 ObjectiveType Questions �������������������������������������������������������������������������������������������������������� 685 Short Questions ����������������������������������������������������������������������������������������������������������������������� 686 Descriptive Questions �������������������������������������������������������������������������������������������������������������� 686
Introduction ............................................................................................................................. 687 Synthesis of Nanostructured Materials.................................................................................... 688 TopDown ApproachNanomaterials Synthesis ...................................................................... 690 Bottom Up Process—Synthesis of Nanoparticles ................................................................... 698 Vapour Phase Deposition ......................................................................................................... 698 Epitaxial Techniques—Synthesis of Nanomaterials ............................................................... 702 Chemical Methods—Nanomaterial Synthesis....................................................................... 707 Hybrid Methods—Synthesis of Nanomaterials..................................................................... 710 Nanotechnology and Environment ........................................................................................ 715 Properties and Possible Applications .................................................................................... 716 Storage ................................................................................................................................... 720 Key Points to Remember �������������������������������������������������������������������������������������������������������� 720 ObjectiveType Questions ������������������������������������������������������������������������������������������������������ 721 Short Questions ��������������������������������������������������������������������������������������������������������������������� 723 Descriptive Questions ������������������������������������������������������������������������������������������������������������ 724
NANODEVICES 29.1 29.2 29.3 29.4 29.5 29.6 29.7 29.8 29.9 29.10 29.11 29.12 29.13 29.14
687–724
725–756
Introduction ........................................................................................................................... 725 Nanomagnets ......................................................................................................................... 726 Classifications of Nanomagnetic Materials ........................................................................... 727 Magneto Resistances ............................................................................................................. 730 Probing Nanomagnetic Materials .......................................................................................... 732 Nanomagnetism in Technology ............................................................................................. 733 Applications of Semiconductor Nanostructures and Devices ............................................... 734 Applications of Semiconductor Nanostructure...................................................................... 735 Organic Semiconductor Materials Devices ........................................................................... 740 Carbon Nanotubes ................................................................................................................. 744 Types of Carbon Nanotubes .................................................................................................. 745 Synthesis of Carbon Nanotubes ............................................................................................ 746 Properties of CNT ................................................................................................................. 748 Applications ........................................................................................................................... 751 Key Points to Remember �������������������������������������������������������������������������������������������������������� 753 ObjectiveType Questions ������������������������������������������������������������������������������������������������������ 753 Short Questions ��������������������������������������������������������������������������������������������������������������������� 754 Descriptive Questions ������������������������������������������������������������������������������������������������������������ 755
Contents
xvii
APPENDIX 1
757–757
APPENDIX 2
758–758
APPENDIX 3
759–759
APPENDIX 4
760–760
INDEX
761–769
PREFACE
This book, Materials Science has been revised as a tailor made textbook, to cover the syllabi for different branches of Engineering and Technology. The previous edition of the book has greatly helped both students and teachers to understand the materials science in depth knowledge. The revised edition covers the fundamentals, different properties of wide range of material materials along with applications. All the chapters are supplemented with key points to remember, objective questions in additions to numerous diagrams and illustration to make the students to understand the concepts in a simple and easy way. The students can use the chapterend exercises and review questions to test their understanding for self improvement.
Salient Key Features Detailed coverage of Modern Engineering Materials: Biomaterials, Advance Ceramics, Polymers, Composites, Nonlinear Materials, Nano materials synthesis and applications Indepth coverage of Semiconducting and Optical materials Richly illustrated with reproducible diagrams – Over 400 figures, for better understanding of the concepts The book also contains a rich pedagogy: ¤ Review questions and answers: 550 ¤ Short answertype review questions: 778 ¤ Descriptivetype review questions: 171 ¤ Solved examples: 182 ¤ Exercises: 48
Chapter Organisation The book contains 29 chapters and 4 Appendices. The total content of the book has been revised by including objectives, key points and objectives questions in each chapters. Chapters 1 to 9 of the book covers on various fundamental knowledge on materials like crystal geometry, bonding, imperfections, and classifications of solids along with the necessary theories to understand the solid materials. In the second part of the book, the different materials properties like transport, mechanical, thermal, optical, luminescence, photoconductivity, dielectric, magnetic, superconducting, thermography, etc., are discussed with suitable examples and applications. In additional to materials properties, newer materials like nonlinear materials, shape memory alloys, biomaterials, polymer materials, advanced ceramics and composite materials are included with process methods, properties and applications of each materials. The book also includes the nano materials and nano devices for the benefit of readers.
Acknowlegments The author is thankful to Dr Krishnan Lal, INSA President, Indian National Science Academy and former Director, National Physical Laboratory, New Delhi for his foreword message. I am thankful to
xx
Preface
Dr K S Rangasamy (Chairman) and Shri R Srinivasan (Secretary) and all my colleagues, particularly Dr K Thyagarajah, Principal, K S R College of Technology for facilitating a wonderful environment and for the encouragement showered on me in bringing out this book. I would also like to thanks Mr K Sakthipandi and Mr R Yuvakkumar for their contributions in typesetting and proof corrections. I am grateful to Vibha Mahajan, Ebi John, Shalini Jha, Tina Jajoriya, Heragu Nagaraja, Yukti Sharma, Preyoshi Kundu and John Mathews of Tata McGrawHill for their keen interest in bringing out this book. I am indebted to many of my friends both in India and abroad for their continuous support and feedback during the development of the manuscript. The patience and care shown by my family members also deserves a special mention. The author is grateful to Tata McGrawHill for their interest in bringing out this revised edition of this book in a short period of time. The constructive, criticism and suggestions from the users of this book for its further improvement are most welcome. V Rajendran
Feedback To improve and make the book more useful in future reprints and editions, constructive feedbacks/opinions from the readers will be of great help and the authors would be grateful for the same. Readers can send their feedback to [email protected]
Publisher’s Note We look forward to receiving from teachers and students their valuable views, comments and suggestions for improvements, all of which may be sent to [email protected], mentioning the title and author’s name on the subject line. Report of any piracy related problems will be highly appreciated.
Chapter
1
MATERIALS PROPERTIES AND REQUIREMENTS
OBJECTIVES To give an introduction to engineering materials. To explain the different levels of structures and structure – property relationship. To understand the requirements for selection of materials for engineering applications. To study the classification and properties of materials.
1.1 INTRODUCTION The world in the recent years has reached new heights in all spheres of science and technology. Today, sophisticated techniques require newer materials for enterprises such as aerospace, computer, electronics, communications, etc., for the development of newer materials especially at nanoscale. Thus, the selection of right materials for application is more essential as it is a very complex process. Therefore, the operating process, manufacturing process, functional requirements and cost of production are essentially required on the newer materials. In this chapter, the different levels of structure, structureproperty relationship, material selection for engineering applications and the classification of engineering materials are given in brief with a view to understand the engineering materials.
1.2 LEVELS OF STRUCTURE The structure of the materials is nothing but the internal structure. The internal structure of the materials can be studied by means of various levels of observations. The structural information obtained at one level is different from the other levels. The different levels of observation can be made with physical instruments having very high magnification and resolution. The process of enlarging the internal studies
2
Materials Science
is the magnification whereas obtaining the finer details of the structure is the level. The structures of the materials are classified in the following ways depending on their levels: (1) Macrostructure (2) Microstructure (3) Substructure (4) Crystal structure (5) Electronic structure, and (6) Nuclear structure Let us discuss the above classes of structure in brief. (1) Macrostructure The macrostructure can be examined by naked eye or using a physical aid having a low magnification power. The external form of the crystalline materials, depends on the arrangement of the atoms in the materials. (2) Microstructure The structure of materials which cannot be observed through naked eye or low magnification power i.e., using the optical microscope, is known as microstructure. The resolution of the human eye is 0.1 mm, i.e., the eye can distinguish between two lines when their distance of separation is 0.1 mm. The optical microscope is used to magnify (lines) the structure up to 1500 times and to resolve the structure up to 0.1 µm. (3) Substructure The information such as crystal imperfections or the details of very fine particles in a minute scale is known as substructure. Generally, the structure of the materials obtained using a microscope with higher magnification and resolution reveals the submatter of the materials. The electron microscope with a linear magnification power of 1,00,000 times are used to obtain the substructure. The substructure of the materials can also be revealed using the modern microscope such as field ion microscope, atomic force microscope, atomic force acoustics microscope and so on. (4) Crystal structure The representation of lattice with a group of atoms each at a lattice point is known as crystal structure. The unit cell is the smallest one which consists of one or more number of atoms. The crystals consist of very large number of unit cells. The techniques which are used to study the crystal structure are Xrays, neutrons, and electrons, among others. (5) Electronic structure The electrons in the various shells and subshells around the nucleus in an atom is distributed based on the application of four quantum numbers and Pauli exclusion principle and is known as electronic structure or electronic configuration. The electronic structure is determined using the spectroscopic studies. (6) Nuclear structure The structure of the nucleus is studied by spectroscopic studies such as nuclear magnetic resonance (NMR), Mossbauer studies, etc.
1.3
STRUCTURE – PROPERTY RELATIONSHIP
In view of the everincreasing application of the engineering materials, the knowledge of the internal structure of materials and how it is correlated with properties is essentially required. Therefore, the different levels of structures such as microstructure, substructure and crystal structures, and their dependence with the composition of materials is more interesting. Similarly, the properties of materials such as mechanical,
Materials Properties and Requirements
3
thermal, electrical, magnetic, optical, chemical and physical form a basis for the evaluation of the behaviour of various materials under different conditions. The above properties are used to characterise the materials. Let us discuss these properties in brief.
1.3.1
Mechanical Properties
Mechanical properties are the behaviour of the materials under applied forces and loads. The behaviour of the materials, depends on the structure of the arrangements of atoms and molecules. One can change the above structure by means of changing the processes and subjecting the material to different treatments. The important mechanical properties are elastic modulus, stress, strain, ductility, hardness, toughness, creep, malleability, fatique, fracture, etc. The force per area (F/A) is known as stress. Generally, the stress encountered in engineering materials is in the range of megapascal (MPa). Strength of the materials is the critical stress to initiate the failure. Strain is the ratio of the change in length to the original length (DL/L0). When a tensile stress is applied, the strain is positive and the same is negative during the application of compressive stress. Further, the strain may be either permanent (i.e., plastic) or reversible (i.e., elastic). The elastic modulus is the ratio of the stress to elastic strain.
E=
F/A DL / L0
(1.1)
Ductility is the capacity of the material to undergo deformation under tension without rupture. Hardness is the resistance of the material to penetration. Similarly, the progressive deformation of the material with time under constant stress gives the creep.
1.3.2
Thermal Properties
The behaviour of the materials when subjected to different thermal conditions is known as thermal properties. Thermal conductivity, thermal expansion, specific heat, and shock resistance are some of the important properties required for better understanding of the engineering materials.
1.3.3 Electrical Properties The electrical property is the behaviour of the material to permit or resist the flow of electricity. Resistivity, temperature coefficient, polarisability, and dielectric constant are some of the important electrical properties of materials. The resistivity of the material is r = R (A/L)
(1.2)
where L is the length, A is the crosssection area, and R is the resistance of the material. The electrical conductivity is the reciprocal of the resistivity, i.e., s = 1/r.
1.3.4 Magnetic Properties The behaviour of the materials under the influence of applied magnetic field is known as magnetic properties. Permeability, susceptibility and hysteresis are some of the important magnetic properties of materials.
4
Materials Science
1.3.5
Physical and Chemical Properties
The physical properties namely, density, porosity, microstructure, and the chemical properties such as corrosion resistance are important for the characterisation of the materials.
1.3.6
Optical Properties
The optical properties are the behaviour of the materials under the action of light. The knowledge on the optical properties helps in understanding the different transition which takes place at the optical frequencies.
1.4
MATERIAL SELECTION FOR ENGINEERING APPLICATION
One can select the right material for a particular engineering application based on the structureproperty performance. For example, the application of the material for an internal circuit indicates the requirement of various properties. The material with the above required properties can be identified by revealing the internal structure and the service performance. Similarly, for a mechanical tool application, one has to consider a material with specific hardness, durability, economy in cost of the raw materials, carry fabrication process, etc. Therefore, a systematic approach on structureproperty relationship provides a good solution for selecting the right materials, for the right purpose. The different factors to be considered during the selection of materials are listed in Table 1.1 for easy understanding.
Table 1.1
Engineering Requirements of Materials
Nature of property
Requirements
Mechanical properties
Tensile strength Hardness Ductility Impact strength Wear resistance Corrosion resistance Density
Thermal properties
Specific heat Thermal conductivity Thermal expansion Thermal resistance Thermal diffusivity
Electrical properties
Resistivity Dielectric constant
Contd.
Materials Properties and Requirements
Table 1.1 Nature of property
5
(Continued) Requirements
Magnetic properties
Magnetic energy product Permeability coercivity
Chemical properties
Atomic weight Molecular weight Chemical composition
Optical properties
Refractive index Band gap Absorption coefficient
Materials structure
Atomic arrangements Bonding nature
1.5 CLASSIFICATION OF ENGINEERING MATERIALS The engineering materials are classified into different categories based on the nature of the materials and their properties. They are as follows. (1) (2) (3) (4) (5) (6) (7)
Metals Polymers Ceramics Composites Nanocrystalline Nonlinear, and Biomaterials
Each of the above class of materials will have certain distinct properties. Metals are good conductors of electricity and heat. On the other hand, ceramics are in general good insulators, brittle and retain their strength at very high temperatures. Similarly, the polymers are nonconductors and cannot be used above a certain temperature. The combinations of two or more groups of above materials are known as composite materials. These materials are high in strength but light in weight.
Table 1.2 Classification of Engineering Materials Materials class
Metals
Examples
Ferrous (Magnetic)
Cast ion, mild steel, high carbon steel, low alloy steel, high speed steel, and Austenitic SS.
Nonferrous (Nonmagnetic
Copper, Zinc, Aluminium, Tin, Brass, and Bronze.
Thermoplastic
Polyethylene, Polypropylene, Polystyrene, ABS, PTFE, and Nylon.
Thermosetting
Polyethylene, Phenolics, Polyurethanes.
Polymers Ceramics
Cementitious materials, stones, clay.
Contd.
6
Materials Science
Table 1.1 (Continued) Materials class
Examples
Composites
Plywood, GRP, wood, cermets.
Nanophase
Metal, alloys intermetallic and ceramics.
Nonlinear
Ammonium dihydrogen phosphate, Potassium dihydrogen phosphate, Lithium niobate, Barrium sodium niobate, and Proustite.
Biomaterials
Metals and alloys
316L Ss, CoCR, CoCrMo
Bioactive glass
Na2OCaOSiO2P2O5
Bioactive glass ceramics
Al2O3SiO2
Polymers
PET, PMMA
Composites
Carbon fibre reinforced, Oxirane.
The materials such as nanophase or nanocrystalline, shape memory and biomaterials are newer materials that have emerged out to suit the technological requirements of the developing entrepreneurs. Table 1.2 gives the classification of engineering materials along with examples. In addition, some of the other important properties of engineering materials are given in Table 1.3. (1) Metals Based on the arrangement of atoms or molecules, the metals are classified into two broad categories namely, metallic and nonmetallic. The metallic materials will have high thermal and electrical conductivity, at the same time they may be either magnetic or nonmagnetic in nature.
Table 1.3 Features Tensile strength (M Nm2) Hardness Density (kg m3) Tensile modulus (G Nm2) Melting point (°C) Thermal expansion Thermal conductivity Electrical conductivity
Properties for Different Types of Materials Metals 300–2500 Medium 2–8 ¥ 103 40–400 200–3500 Medium High Conductor
Polymers 30–100 Low 1–2 ¥ 103 0.7–3.5 70–200 High Low Insulator
Ceramics 10–400 High 2–17 ¥ 103 150–450 2000–4000 Low Medium Insulator
Composites (Wood) 20–110 Low 0.5–1 ¥ 103 4–20 Low Low Insulator
The metallic materials are further classified into ferrous and nonferrous materials. The materials which contain ferrite or iron atoms are known as ferrous metals. On the other hand, metals which do not contain any ferrous or iron atoms are known as nonferrous metals. The ferrous materials are magnetic in nature, while the nonferrous materials are nonmagnetic materials. The atoms are arranged in periodic or regular manner and hence, nonferrous materials are crystalline in nature. The most common structure of the materials are face centered, body centered and closely packed hexagonal structure.
Materials Properties and Requirements
7
(2) Polymers It is a kind of material which are deformable at higher temperatures but become hard on cooling. The basic principles, classifications, structures, formations, properties and applications of the polymers have discussed in detail in a separate chapter. (3) Ceramics The ceramics are inorganic and nonmetallic solids. The atoms are arranged in a periodic manner and are hence known as crystalline materials. The applications of this class of materials are wide in range, i.e., from industries to household articles. The principle, preparation, structure and the properties of ceramic materials are discussed in detail in a separate chapter. (4) Composites The composite materials are a combination of two or more materials which have different properties from the constituent materials of composites. In view of their significant properties such as high strength, heat resistance, stiffness, stability, etc., composites are better than any individual component. For example, Glass Reinforced Plastic (GRP) is an artificial composite material which has the combined properties of glass fibre and plastics. One can study the presence of two or more materials from the structures of composites. The structure of composites is represented by matrix and reinforcements. Matrix is the base material, while reinforcements are other materials which are arranged above the matrix. Composite materials can be classified into the following different categories based on the shape and size of the reinforcing materials such as, a. b. c. d.
Dispersions Particle Laminated, and Fibre
Most of the industrial and plant components are replaced by composite materials due to their high strength, lightweight, stability and other properties. Moreover, one can obtain the required properties by the reinforcements of any suitable materials on the matrix.
Key Points to Remember The structure of materials are classified as macrostructure, microstructure, substructure, crystal structure, quantum structure and nuclear structure. Microstructures are not seen using naked eye and require optical microscope to view. The details of fine particles in minute scale is known as substructure. The representation of lattice with a group of atoms each in a lattice point is known as crystal structure. The distribution of electrons in various shells and structures around the nucleus in an atom is based on four quantum numbers and Pauli’s exclusion principle is known as electronic structure or electronic configuration. Elastic modulus is the ratio of stress to strain i.e., (F/A)/(DL/Lo) DL. The resistivity of materials is R (A/L). Based on the structureproperty relationship, the right material can be selected for a particular application. Different classes of engineering materials are metals, polymers, ceramics, composites, nanocrystalline, nonlinear and biomaterials.
8
Materials Science
Solved Problems Example 1.1 A copper wire has a diameter of 0.9 mm. Determine the resistance of a 30 cm wire. Given that the resistivity is 17 ¥ 109 ohm m. Given Data:
Solution:
The radius of the wire
r = 0.45 ¥ 103 m
The length of the wire
L = 0.30 m
The resistivity
r = 17 ¥ 109 ohm m
We know that,
R = r (L/A) L =r p r2 Substituting the value of r, L and r in the above equation, we get The resistance
R = 17 ¥ 109
0.30 p (0.45 ¥ 10 3 )2
= 0.008 ohm. The resistance of the wire is 0.008 ohm. Example 1.2 Determine the extension of a wire with diameter 2.5 mm and 3 m long is subjected to a force of 4900 N. Given that the modulus of elasticity of steel is 205,000 MPa. Given Data:
Solution:
The diameter of the wire
r = 1.25 ¥ 103 m
The length of the wire
L=3m
The applied force
= 4900 N
The elastic modulus
= 2.05 ¥ 1011 Pa
We know that,
E=
Stress Strain
=
F /A Strain
F /A F = E AE Substituting the value of A = pr2 in the above equation, we get Therefore, the strain
=
or,
=
F p r2 E
Materials Properties and Requirements
9
Substituting the values of F, r and E in the above equation, we get Strain
=
4900 p ¥ (1.25 ¥ 103 )2 ¥ 2.05 ¥ 1011
= 0.005 Therefore, the extension
= 0.005 ¥ 3
The extension of the wire is 0.015 m.
ObjectiveType Questions 1.1. 1.2. 1.3. 1.4. 1.5. 1.6.
The The The The The The
structure of fine particles in a minute scale is known as _________ resolution of human eye is _______ mm. resolution of an optical microscope is ___________ mm. techniques which are used to study the crystal structure are _______, ________ and ______. electronic structure of materials are obtained based on the ____________ and ________. elastic modulus of the material is equal to
(a)
F/A DL / L0
(b)
FA DL / L0
F/A FA (d) DL L0 DL L0 1.7. The resistivity of materials is equal to ____________. 1.8. The two different types of metals are _______ and _________. 1.9. The material which has the combined properties of glass fibre and plastics is ________. (c)
Answers 1.1. substructure
1.2. 0.1
1.3. 0.1
1.4. xrays, neutrons, electrons
1.5. four quantum numbers, Pauli’s exclusion principle
1.6.
1.7. R (A/L)
1.8. metalic, nonmetallic
1.9. glass reinforced plastic
Short Questions 1.1. 1.2. 1.3. 1.4.
What is meant by levels of structure? Explain the different levels of structure. What is meant by structureproperty relationship? What are the different properties of materials?
F/A DL / L0
10
Materials Science
1.5. 1.6. 1.7. 1.8. 1.9. 1.10. 1.11. 1.12. 1.13. 1.14. 1.15. 1.16. 1.17. 1.18. 1.19.
Define elastic modulus. Explain the electrical properties of materials. What is the classification of engineering materials? Mention the various properties of materials. Differentiate metallic and nonmetallic materials. What is meant by ferrous material? Give an example. What is by nonferrous material? Give an example. What is meant by polymers? Explain ceramic materials. What is meant by composite materials? Mention the classification of composite materials? What is meant by nanocrystalline materials? Mention the properties of nanocrystalline materials. What is meant by nonlinear materials? What is meant by biomaterials?
Descriptive Questions 1.1. Describe in detail the structure – property relationship in engineering materials. 1.2. What is the classification of engineering materials? Explain the various materials in brief.
Exercises 1.1. What will be the stress on a 1 mm diameter wire that is supporting 3 kg of load? 1.2. Determine the end to end resistance of a brass strip having 5 cm long by 5 mm wide by 0.5 mm thick. The resistivity of brass is 62 ¥ 109 ohm m. Also determine the conductivity of the brass. 1.3. Determine the elastic strain in a brass rod that is stressed 49 MPa. Given that the density is 8.5 g cm3 and its elastic moduli is 110 GPa.
Chapter
2
CRYSTAL STRUCTURE
OBJECTIVES To To To To To
develop knowledge in crystal structure and its properties. explain the fundamental terms in crystallography. discuss the various crystal systems according to Bravais lattices. discuss Miller indices in crystal planes and their applications. discuss the importance of packing factor in crystal structure.
2.1 INTRODUCTION Crystallography deals with the study of all possible types of crystals and determination of the actual structure of the crystalline solids by Xrays, neutron beams or electron beams. Solids are classified into two categories based on the arrangement of atoms or molecules. They are given below. (1) Crystalline solids, and (2) Amorphous solids
2.1.1
Crystalline Solids
In crystalline solids, atoms are arranged in a regular manner, i.e., the atomic array is periodic. Each atom is at regular intervals along the arrays in all directions of the crystal. The crystalline solids have directional properties and are also known as anisotropic substances. The structure may be made up of metallic crystals or nonmetallic crystals. The metallic crystals find wide application in engineering because of their strength, conductivity, reflection, etc. Example of metallic crystals are copper, silver, aluminium, tungsten, etc.
12
Materials Science
2.1.2
Amorphous Solids (Nonmetallic crystals)
In amorphous solids, the atoms or molecules are arranged randomly. The amorphous solids have no regular structure (no directional property) and hence they are known as isotropic substances. Such materials have no specific electrical property, but have only plasticity. Examples are glass, plastics and rubber.
2.2 FUNDAMENTAL TERMS OF CRYSTALLOGRAPHY The structure of all crystals is described in terms of lattice with a group of atoms, each in a lattice point. The group is termed as basis. The basis is repeated in space to form the crystal structure. Let us now consider the various crystallographic terms in detail.
2.2.1
Lattice
A lattice is a regular and periodic arrangement of points in three dimensions. Figure 2.1 represents a twodimensional lattice. R E¢ a E a F a b
A
D 5a C 2a a B
D¢ 5a C¢ 2a
F¢ a A¢
a
B¢
a P
Q
Fig. 2.1 A twodimensional lattice Consider the points P, Q and R. Let us join the points P and Q by a straight line, and the points P and R by another straight line. The line PQ is taken as an axis, say Xaxis. Similarly, the line PR is taken as another axis, say Yaxis. The distance between any two successive lattice points in the X direction is taken as a. Similarly, the distance between any two successive lattice points along the Y direction is taken as b. Here, a and b are said to be lattice translational vectors. Consider a square lattice in which a = b. Consider two sets of points A, B, C, D, E, F and A´, B ´, C ´, D ´, E ´, F ´. In these two sets, the surrounding environment looks symmetrical, i.e., the distances AB and A´B´, AC and A´C ´, AD and A´D ´, AE and A´E ´ and AF and A´F ´ are equal.
Crystal Structure
13
The term lattice can be defined in another way. In an arrangement of points, if the surrounding environment looks the same when the arrangement is viewed from different lattice points, then that arrangement is said to be a lattice.
2.2.2
Basis
To construct a crystal structure, some basic arrangement is to be fixed at each and every lattice point. This basic arrangement is said to be a basis. Consider Fig. 2.2(a) and 2.2(b). To obtain the structure shown in Fig. 2.2(c), the arrangement shown in Fig. 2.2(b) is to be fixed in each and every lattice point. So, the arrangement shown in Fig. 2.2(b) is said to be a basis.
(a) Lattice
(b) Basis
(c) Crystal structure
Fig. 2.2 Arrangement of basis and lattice point
2.2.3
Crystal Structure
A crystal structure is obtained by arranging the basis in each and every lattice point. It can be written as, Crystal structure = lattice + basis The above equation is not a mathematical expression, but it is used to explain the formation of crystal structure. According to this equation, a crystal structure is formed by arranging the basis in each and every lattice point.
2.2.4
Unit Cell
In the construction of a wall, bricks are arranged one above the other. So, in the case of the wall, a brick is said to be a unit cell. Similarly, in the case of a crystal, a smallest unit is arranged one above the other. This smallest unit is known as a unit cell. Thus, a unit cell is defined as a fundamental building block of a crystal structure. Figure 2.3 shows a cubic unit cell.
14
Materials Science
Fig. 2.3 Unit cell
2.2.5
Crystallographic Axes
Consider a unit cell consisting of three mutually perpendicular edges OA, OB and OC as shown in Fig. 2.4. Draw parallel lines along the three edges. These lines are taken as crystallographic axes and they are denoted as X, Y and Z axes. Y
B
g A
a O
X
b C Z
Fig. 2.4 Crystallographic axes
2.2.6
Primitives
Consider the unit cell shown in Fig. 2.5. Let OA be an intercept along the Xaxis. Similarly, the intercepts made by the unit cell along the Y and Z axes are OB and OC, that is, OA, OB, and OC are the intercepts made by the unit cell along the crystallographic axes. These intercepts are known as primitives. In crystallography, the intercepts OA, OB and OC are represented as a, b and c. Y B
A O C Z
Fig. 2.5 Primitives
X
Crystal Structure
2.2.7
15
Interaxial Angles (or Interfacial Angles)
In a crystal, the angles between X, Y and Z axes are known as interaxial angles. The angle between X and Y axes is represented as g. Similarly, the angle between Y and Z, and Z and X axes are denoted by a and b, respectively, as shown in Fig. 2.4. The angles a, b and g are said to be interfacial angles.
2.2.8
Lattice Parameters
In order to represent lattice, the above three interfacial angles and the corresponding intercepts are essential. These six parameters are said to be lattice parameters.
2.2.9
Primitive Cell
It is the smallest unit cell in volume constructed by primitives. It consists of only one full atom as shown in Fig. 2.6. If a unit cell consists of more than one atom then it is not a primitive cell. A simple cubic unit cell is said to be a primitive cell, whereas a bodycentred cubic unit cell is not a primitive cell.
c b a
Fig. 2.6 Primitive cell of a space lattice
2.3 TYPES OF CRYSTALS Crystals are classified into seven systems on the basis of the shape of the unit cell. These are classified in terms of lengths of unit cells and the angle of inclination between them. The seven systems are cubic, tetragonal, orthorhombic, monoclinic, triclinic, trigonal and hexagonal.
2.3.1
Bravais Lattices
Bravais in 1948, showed that there are 14 different types of unit cells under the seven crystal systems as shown in Fig. 2.7. They are commonly called Bravais lattices. Table 2.1 shows the seven crystal systems, the relation between primitives and angles, lattice symbols and the number of possible lattices. The lattice symbol P, I, F and C represents, respectively, primitive, body centred, face centred and base centred crystal structures.
16
Materials Science
Cubic P
Cubic I
Tetragonal P
Orthorhombic P
Tetragonal I
Orthorhombic C
Monoclinic P
Trigonal
Cubic F
Orthorhombic I
Monoclinic C
Orthorhombic F
Triclinic
Trigonal and hexagonal P
Fig. 2.7 Bravais lattices
Crystal Structure
Table 2.1 Sr. No.
Name of the system
The Seven Crystal Systems
Relation between primitives and angles
Lattice symbols
No. of possible lattices
Examples
1.
Cubic
a = b = c, a = b = g = 90°
P I F
3
Po Na,W,a  Fe Ag, Au, Pb
2.
Tetragonal
a = b π c, a = b = g = 90°
P I
2
TiO2, SnO2 KH2PO4
3.
Orthorhombic
a π b π c, a = b = g = 90°
P I F C
4
— PbCO3, BaSO4 KNO3, K2SO4 aS
4.
Monoclinic
a π b π c, a = b = 90° π g
P C
2
CaSO4.2H2O K2MgSO4.6H2O
5.
Triclinic
a π b π c, a π b π 90° π g
P
1
K2Cr2O7
6.
Trigonal
a = b = c, a = b = g π 90° (but less than 120°)
P
1
Calcite, As, Sb, Bi
7.
Hexagonal
a = b π c, a = b = 90° g = 120°
P
1
SiO2, AgI
2.3.2
17
Miller Indices
Miller devised a method to represent a crystal plane or direction. In this method, to represent a crystal plane, a set of three numbers are written within the parentheses. Similarly, crystal direction is represented as a set of three numbers written within the square brackets. Miller index is one in which the crystal plane is represented within the parenthesis.
Rules to Find the Miller Indices of a Plane To find the Miller indices for a given plane, the following steps are to be followed: a. b. c. d. e.
The intercepts made by the plane along X, Y and Z axes are noted. The coefficients of the intercepts are noted separately. Inverse is to be taken. The fractions are multiplied by a suitable number so that all the fractions become integers. Write the integers within the parentheses.
18
Materials Science
Notes (i) While writing Miller indices, a comma or dot between any two numbers may be avoided. (ii) The positive X axis is represented as (100), Y axis as (010) and Z axis as (001). Similarly, the negative X axis as 100 , negative Y axis as 010 and negative Z axis as 001. (iii) The Miller indices for a plane (101) is read as ‘one zero one’ and not as one hundred and one. For example, Miller indices of the plane shown in Fig. 2.8 can be found by the following method: (i) The given plane ABC makes intercepts 2a, 3b and 2c along the X, Y and Z axes, respectively. Hence, the intercepts are 2a, 3b and 2c. (ii) The coefficients of the intercepts are 2, 3 and 2. The inverse are 1/2, 1/3, 1/2. (iv) The LCM is 6. Multiply the fractions by 6, so that they become integers as 3, 2, 3. (v) The integers are written within the parenthesis as (323). (323) represents the Miller indices of the given plane ABC. Y 4b B
3b 2b b a
c
2a
3a
4a
A
X
2c C
3c Z
Fig. 2.8 Miller indices of a plane
Salient Features of the Miller Indices (1) A plane parallel to one coordinate axis is taken, as that plane will meet the axis at infinity. Therefore, the intercept is taken as infinity. The index number (Miller indices) for that plane in that coordinate axis is zero. (2) A plane passing through the origin is defined in terms of a parallel plane having nonzero intercepts. (3) Equally spaced parallel planes have same Miller indices. (4) Planes which have negative intercepts are represented by a bar, like (100) . The Miller indices (100) indicates that the plane has an intercept in the negative X axis.
Important Features of Miller Indices The Miller index notation is especially useful for cubic systems. Its desirable features are listed below. (1) The angle q between any two crystallographic directions [u1 v1 w1 ] and [u2 v2 w2] can be calculated easily. The angle q is given by Eq. (2.1), cos q =
u1u2 + v1v2 + w1w2 (u + v + w12 )1/ 2 (u22 + v22 + w22 )1/ 2 2 1
2 1
(2.1)
(2) The direction [hkl] is perpendicular to the plane (hkl) (3) The relation between the interplanar distance and the interatomic distance is given by Eq. (2.2),
Crystal Structure
19
a d=
2
h + k2 + l2
(for cubic)
(2.2)
(4) If (hkl) is the Miller indices of a crystal plane, then the intercepts made by the plane with the crystallographic axes are given as a/h, b/k, c/l, where a, b, and c are the primitives.
Procedure to Find the Miller Indices of a Direction To find the Miller indices of a direction, choose a perpendicular plane to that direction. Find the Miller indices of that perpendicular plane. The perpendicular plane and the directions have the same Miller indices value. Therefore, the Miller indices of the perpendicular plane is written within a square bracket to represent the Miller indices of the direction. To find the Miller indices of a line (direction), find the direction ratios of that line and then write them within the square brackets. It represents the Miller indices of that line. The Miller indices of some of the important cubic crystal planes like (100) plane, (010) plane, (111) plane, (110) plane, (011) plane and (002) plane are shown in Fig. 2.9.
2.4 RELATION BETWEEN THE INTERPLANAR DISTANCE AND THE INTERATOMIC DISTANCE Consider a cubic crystal with cube edge ‘a’. Let (hkl) be the Miller indices for the plane ABC as shown in Fig. 2.10. The intercepts made by the above plane are a/h, a/k, a/l. Consider another parallel plane to the above plane ABC passing through the origin O. A perpendicular line drawn from the origin O to the plane ABC represents the distance between two parallel planes. Let ON be the distance d between the two parallel planes. Let a ´, b ´ and g ´ be the angles made by the line ON with X, Y and Z axes. The direction cosines, cos a ´, cos b ´ and cos g ´ are written as, ON d dh cos a ´ = OA = a / h = a
(2.3)
ON d dk cos b ´ = OB = a / k = a
(2.4)
cos g ´ =
ON d dl = = OC a / l a
(2.5)
From the properties of the direction cosines of any line, we can write, cos2 a ´ + cos2 b ´ + cos2 g ´ = 1 i.e.,
or,
(dh/a)2 + (dk/a)2 + (dl/a)2 = 1 d 2 (h2 + k2 + l2) = 1 a2 a d= 2 h + k2 + l2
(2.6)
Equation (2.6) gives the relation between the interatomic distance a and the interplanar distance d.
20
Materials Science
Y
Y
X
X Z
Z
(a) (100) plane
(b) (010) plane Y
Y
X
X Z
Z
(c) (111) plane Y
(d) (110) plane Y
X
X Z
Z (f) (002) plane
(e) (011) plane
Fig. 2.9 Miller indices of some cubic crystal planes Y
Z N g¢ B b¢
C
O
A
X
a¢
Fig. 2.10 Spacing of planes in crystal latties
Crystal Structure
21
2.5 CRYSTAL STRUCTURES OF MATERIALS In this section, first consider some of the important parameters which are used to describe the crystal structure of the materials. (1) Atomic Radius (r) It is half the distance between any two successive atoms. For a simple cubic unit cell, the atomic radius a r= (2.7) 2 where a is the interatomic distance. (2) Coordination Number It is the number of nearest neighbouring atoms to a particular atom. For a simple cubic unit cell, the coordination number is 6. (3) Packing Density It is the ratio between the total volume occupied by the atoms or molecules in a unit cell and the volume of unit cell. i.e., Density of packing =
Total volume occupied by atoms in a unit cell Volume of the unit cell
Number of atoms present in a unit cell ¥ Volume of one atom = Volume of the unit cell
(2.8)
2.6 SIMPLE CUBIC CRYSTAL STRUCTURE A simple cubic crystal structure (scc) unit cell consists of eight corner atoms as shown in Fig. 2.11. In actual crystals, each and every corner atom is shared by eight adjacent unit cells. Therefore, each and every corner atom contributes 1/8 of its part to one unit cell. Hence, the total number of atoms present 1 in a unit cell is ¥ 8 = 1. 8 a (1) Atomic Radius For a simple cubic unit cell, the atomic radius is given by, r = 2 (2) Coordination Number The coordination number of a simple cubic unit cell can be calculated as follows. Let us consider any corner atom. For this atom, there are four nearest neighbours in its own plane. There is another nearest neighbour in a plane which lies just above this atom and yet another nearest neighbour in another plane which lies just below this atom. Therefore, the total number of nearest neighbours is six and hence, the coordination number is 6.
Fig. 2.11 Arrangement of atoms in a SC unit cell
22
Materials Science
(3) Packing Density The packing density of a simple cubic unit cell can be calculated as follows. For simple cubic, the total number of atoms present is one. Therefore, from Eq. (2.8), the packing density of the simple cubic can be written as follows. Packing density
=
1 ¥ (4 / 3) ¥ p r 3 a3
(2.9)
Substituting the value r = a/2 in Eq. (2.9), we get \ Packing density
=
1 ¥ (4 / 3) ¥ p (a / 2)3 a3
Therefore, packing density
=
p = 0.52. 6
(2.10)
Thus, 52 percent of the volume of simple cubic unit cell is occupied by atoms and the remaining 48 percent volume of the unit cell is vacant.
2.7
BODY CENTRED CUBIC STRUCTURE
A body centred cubic (bcc) structure has eight corner atoms and one body centred atom. The diagrammatic representation of a body centred cubic structure is shown in Fig. 2.12(a). In a body centred crystal structure, the atoms touch along the diagonal of the body. In a bcc unit cell, each and every corner atom is shared by eight adjacent unit cells. Therefore, the total number of atoms contributed by the corner atoms is (1/8) 8 = 1.
Fig. 2.12(a) Arrangement of atoms in a bcc unit cell A bcc unit cell has one full atom at the centre of the unit cell. Therefore, the total number of atoms present in a bcc unit cell is 2. (1) Atomic Radius 2.12(b) as follows.
For a body centred cubic unit cell, the atomic radius can be calculated from Fig.
Crystal Structure
G
23
H F 4r
E a
D C A
B
Fig. 2.12(b) Calculation of atomic radius From Fig. 2.12(b), AH = 4r and DH = a From the triangle ADH, AD2 + DH 2 = AH 2
(2.11)
To find AD, consider the triangle ABD, From the triangle ABD, AB2 + BD2 = AD2 i.e., Therefore,
or
a2 + a2 = AD2
AD2 = 2a2 AD =
2a
(2.12)
Substituting AD, AH and DH values in Eq. (2.11), we get AD2 + DH 2 = AH 2 2a2 + a2 = (4r)2
or, i.e.,
The atomic radius
16r2 = 3a2 r2 =
3 2 a 16
r=
3 a 4
(2.13)
(2) Coordination Number The coordination number of a body centred cubic unit cell can be calculated as follows. Let us consider a body centred atom. The nearest neighbour for a body centred atom is a corner atom. A body centred atom is surrounded by eight corner atoms. Therefore, the coordination number of a bcc unit cell is 8. (3) Packing Density The packing density of a body centred cubic unit cell can be calculated as follows. The number of atoms present in a unit cell is 2.
24
Materials Science
Therefore, from Eq. (2.8), the packing density of the bcc unit cell can be written as follows. Packing density
=
2(4 / 3)p r 3 a3
(2.14)
Substituting the value of r = ( 3 / 4) a in Eq. (2.14), we get
\ Packing density
ÈÊ 3 ˆ ˘ 2(4 / 3)p ÍÁ ˜ a ˙ ÍÎË 4 ¯ ˙˚ = a3 =
3
3p = 0.68 8
(2.15)
Therefore, the packing density, of a bcc unit cell = 0.68. This shows that 68 percent of the volume of the body centred cubic unit cell is occupied by atoms and the remaining 32 percent volume of the unit cell is vacant.
2.8
FACE CENTRED CUBIC STRUCTURE OR CUBIC CLOSE PACKED STRUCTURE
A face centred cubic (fcc) unit cell consists of eight corner atoms and six face centred atoms. A face centred cubic or cubic close packed (ccp) unit cell is shown in Fig. 2.13(a). The atoms in a face centred cubic unit cell touch along the face diagonal. The fcc unit cell consists of eight corner atoms and six face centred atoms. Each and every corner atom is shared by eight adjacent unit cells. Therefore, each and every corner atom contributes 1/8 of its part to one unit cell. The total number of atoms contributed by the corner atoms is (1/8) 8 = 1.
Fig. 2.13(a)
Arrangement of atoms in a fcc unit cell
Each and every face centred atom is shared by two unit cells. Therefore, a face centred atom contributes half of its part to one unit cell. The total number of atoms contributed by the face centred atom is (1/2) 6 = 3. Therefore, the total number of atoms present in an fcc unit cell is 4.
Crystal Structure
25
(1) Atomic Radius The atomic radius can be calculated from Fig. 2.13(b) as follows. From Fig. 2.13(b), consider the triangle ABC, AC2 = AB2 + BC2 (4r)2 = a2 + a2 16r2 = 2a2 The atomic radius
a 2 2
r=
(2.16)
G
H
D
4r
C
F E A
B
Fig. 2.13(b) Calculation of atomic radius (2) Coordination Number The coordination number can be calculated as follows. Let us consider a corner atom. In its own plane, that corner atom has four face centred atoms. These face centred atoms are its nearest neighbours. In a plane which lies just above this corner atom, it has four more face centred atoms as nearest neighbours. In a plane which lies just below this corner atom, it has yet four more face centred atoms as its nearest neighbours. Therefore, for an atom in an fcc unit cell, the number of nearest neighbours is 12. (3) Packing Density The packing density of the fcc unit cell can be calculated as follows. The number of atoms present in an fcc unit cell is 4. Therefore, from Eq. (2.8), the packing density of the fcc unit cell can be written as follows. Packing density Substituting the value of r = a \ Packing density
=
4(4 / 3)p r 3 a3
(2 2 ) =
(2.17)
in Eq. (2.17), we get
(
4(4 / 3)p ¥ a / 2 2 a
3
Therefore, the packing density of the fcc unit cell
3
)
=
p 3 2
= 0.74
(2.18)
That is 74 percent of the volume of an fcc unit cell is occupied by atoms and the remaining 26 percent volume of the unit cell is vacant.
26
Materials Science
2.9
HEXAGONAL CLOSED PACKED STRUCTURE
The hexagonal closed packed (hcp) structure is shown in Fig. 2.14(a). The hcp structure consists of three layers of atoms as shown in Fig. 2.14(b). The bottom layer has six corner atoms and one face centred atom. The middle layer has three full atoms. The upper layer has six corner atoms and one face centred atom.
A c/2
C
A
B
A
B
c
A C
A C B b
A
A
a (b) Arrangement of atoms
(a) hcp unit cell
Fig. 2.14 hcp structure The arrangement of atoms in a hexagonally closed packed structure as shown in Fig. 2.14 is explained as follows. In the bottom layer, the central atom is surrounded by six other atoms having equal radius. The bottom layer of atoms is denoted by the letter A. Three places are marked as B and the remaining three places are marked as C over the bottom layer. The second layer of atom is placed either over the point marked as B or the point marked as C. Consider that the second layer is placed in the places marked as B. The third layer can be arranged in two ways, (i) the third layer of atoms placed directly over the first layer, and (ii) the third layer placed over the points marked as C. The stacking sequence goes on as ABABAB ... for case (i) representing the hcp structure, and as ABCABCABC for case (ii) representing the Fcc structure. The total number of atoms present in the case of an hcp crystal structure is 6. To calculate this, first consider the bottom layer of atoms. The bottom layer consists of six corner atoms and one face centred atom. Each and every corner atom contributes 1/6 of its part to one unit cell. The total number of atoms contributed by the corner atoms is (1/6) 6 = 1. The face centred atom contributes 1/2 of its part to one unit cell. Therefore, the total number of atoms present in the case of the bottom layer is 1 + (1/2) = 3/2. Similarly, the upper layer also has 3/2 number of atoms. The middle layer has three full atoms. Therefore, the total number of atoms present in a unit cell is 3/2 + 3/2 + 3 = 6.
a
a
Fig. 2.15 Calculation of atomic radius
Crystal Structure
27
(1) Atomic radius The atomic radius of an hcp crystal structure can be calculated as follows. Let us consider any two corner atoms. Each and every corner atom touches each other as shown in Fig. 2.15. Therefore, from Fig. 2.15 a = 2r a r= 2
i.e., The atomic radius
(2.19)
r = a/2
(2) Coordination Number The coordination number of an hcp structure can be calculated as follows. Let us consider a face centred atom in the bottom layer. This face centred atom is surrounded by six corner atoms. These corner atoms are the nearest neighbours. The middle layer has three atoms which are nearest neighbours to the face centred atom. A unit cell, which lies below our reference unit cell also has three middle layer atoms. These three atoms are also the nearest neighbours for the face centred atom. Therefore, the total number of nearest neighbours is 6 + 3 + 3 = 12. (3) Packing Density The density of packing of an hcp crystal structure can be calculated as follows. From Eq. (2.8), the packing density of the hcp unit cell can be written as follows. Packing density
=
6(4 / 3)p r 3 6
(
(2.20)
)
3 4 a 2c
Substituting the value of r = a/ 2 in Eq. (2.20), we get \ Packing density Substituting the value of c/a = \ Packing density
=
6(4 / 3)p (a / 2)3 6
(
)
2
3 4 ac
=
2p a 3 3c
(2.21)
(8 / 3) in Eq. (2.21), we get =
2p 3 p = = 0.74 3 3 8 3 2
Therefore, the packing density of hcp unit cell
(2.22)
= 0.74.
That is, 74 percent of the volume of hcp crystal structure is occupied by atoms and the remaining 26 percent volume is vacant. (4) Relation Between C and A Consider the bottom surface of a hexagonally closed packed structure. It has six corner atoms and one face centred atom. The face centred atom touches all the corner atoms. The arrangement of atoms is shown in Fig. 2.16(a). The second layer of atoms are placed directly over the first layer. In Fig. 2.16(a), A, B, C, D, E, F and O represent the bottom layer of atoms. G, H, I represents the middle layer of atoms. Consider the arrangement of the atoms A, F, O and G as shown in Fig. 2.16(b). In Fig. 2.16(b), A, F and O represent the bottom layer of atoms and G represents one of the atoms in the second layer. Now, let us bisect the line AF, by drawing a normal from O. OE´ bisects the line AF into two. Consider the triangle AE´O. Since, the triangle AFO is an equilateral triangle, –AOE´ = 30°. Draw another perpendicular line from F to the line AO. The line FJ bisects the line AO and hence, AJ = JO = a/2. From Fig. 2.16(b), –AOE´ = 30° and –JXO = 60°
28
Materials Science
F
E G
H
F
O
A
G
D E' I
X A
B C (a) Bottom surface of hcpunit cell
J (b) Triangle AFO
O
Fig. 2.16 Arrangement of atomshcp structure Consider the triangle XJ ´O, the angles of the triangle are 30°, 60° and 90° and hence, it faces are in the ratio of 1: 3 :2. Therefore, in triangle JXO XJ : JO : OX = 1 : OX =
3: 2
2 JO 3
(2.23) (2.24)
Substituting the values of JO (=a/2) in Eq. (2.24), we get OX =
2 a 3 2
OX =
a 3
(2.25)
OG2 = OX 2 + GX 2
(2.26)
In triangle XOG
Substituting OG, OX and GX values in Eq. (2.26), we get 2
Ê a ˆ Ê cˆ a2 = Á ˜ + Á ˜ Ë 2¯ Ë 3¯ a2 
a2 c2 = 3 4
2
or,
2a 2 c 2 = 3 4
a2 = 3 8 c2 c = 8 / 3 = 1.633 a Hence, the axial ratio c/a for a hcp structure is
8/3 .
(2.27)
Crystal Structure
29
Key Points to Remember Based on the arrangement of atoms or molecules, solids are classified into two categories, namely, crystalline solids and amorphous solids. In crystalline solids, atoms or molecules are arranged randomly and have isotropic properties. The smallest unit cell in a crystal structure is known as a unit cell. A simple cubic unit cell is said to be a primitive cell. Types of seven crystal systems are cubic, tetragonal, orthorhombic, monoclinic, triclinic, trigonal and hexagonal. The different types of unit cells under the seven crystal structures are called Bravis lattice. Miller indices are a set of three numbers written within the parenthesis and is used to represent a crystal plane. The coordination number is the nearest number of neighbouring atom to a particular atom. Density of packing, or packing density is defined as the ratio of total volume occupied by atoms in a unit cell to the volume of the unit cell. The coordination number for simple cubic, bcc, fcc and hcp structures are 6, 8, 12 and 12, respectively. The packing density for simple cubic, bcc, fcc and hcp structures are 0.52, 0.68, 0.74 and 0.74, respectively. In the hcp structure, the atoms are arranged in stacking sequences.
Solved Problems Example 2.1 Show that the crystal plane (hkl) is perpendicular to the direction [hkl]. Solution:
The Miller indices of the given plane = (hkl) The intercept made by the plane = a/h, b/k, c/l The equation of the plane x y z =1 + + a/h b/k c/l xh yk zl + + =1 a b c
i.e., For cubic unit cell a = b = c
Therefore, the equation of the plane can be written as, xh + yk + zl = a
(i)
The direction ratio of normal to the plane is h, k, l. The equation of a line passing through the points (x1, y1, z1) and having direction ratios h, k, l is x  x1 y  y1 z  z1 = = h k l
(ii)
30
Materials Science
Equation (ii) is an equation for a line perpendicular to the plane given by Eq. (i). The direction ratios of Eq. (ii) is h, k, l. The Miller indices of the line given in this problem is [hkl]. Hence, the Miller indices are nothing but the direction ratios. The angle between two lines having the direction ratios u1, v1, w1 and u2, v2, w2 is given by, cos q =
u1u2 + v1v2 + w1w2 [u12 + v12 + w12 ]1/ 2 [u22 + v22 + w22 ]1/ 2
(iii)
where u1 = u2 = h ; v1 = v2 = k and w1 = w2 = l Equation (iii) can be written as, cos q = Therefore,
h2 + k 2 + l 2 =1 [h 2 + k 2 + l 2 ]1/ 2 [h 2 + k 2 + l 2 ]1/ 2
q = 0.
That is, the normal to the plane and the direction [hkl] are parallel. It means, the direction [hkl] is perpendicular to the plane. Example 2.2 Find the Miller indices of a set of parallel planes which make intercepts in the ratio 3a: 4b on the X and Y axes and parallel to the Z axis. a, b, c are primitive vectors of the lattice of the lattice. Also calculate the interplaner distance of the planes taking the lattice to be a cubic with a = b = c = 2 A°. Given Data:
Solution:
The intercept along X axis
= 3a
The intercept along Y axis
= 4b
The intercept along Z axis
=
The intercepts made by the plane along the three axes are 3a, 4b, The coefficient of the intercepts are 3, 4, The inverse of the coefficients are 1/3, 1/4, 1/ , The LCM of these above fractions is 12 Multiplying these fractions by 12, we get 4, 3, 0 Therefore, the Miller indices of the plane is (430). The distance between any two successive parallel planes is given by
d=
a h2 + k 2 + l2
Crystal Structure
31
Substituting the values for 430 planes, we get d 430 =
2 ¥ 1010 42 + 32 + 02
= 0.4 ¥ 1010 m. The lattice spacing for the plane 430 is 0.4 ¥ 1010 m. Example 2.3 Sodium is a bcc crystal. Its density is 9.6 ¥ 102 kg m3 and atomic weight is 23. Calculate the lattice constant a for sodium crystal. Given Data:
Solution:
Density of sodium
= 9.6 ¥ 102 kg m3
Atomic weight of sodium
= 23
The mass of the unit cell of the sodium crystal = density ¥ volume of the unit cell = 9.6 ¥ 102 a3
(i)
where a is the interatomic distance. The mass of the unit cell of the sodium crystal is given by another relation, Mass =
Number of atoms in a unit cell ¥ Atomic weight Avogadro constant
Since sodium is a bcc crystal, the number of atoms present in one unit cell is 2. Therefore, mass of one unit cell =
2 ¥ 23 6.022 ¥ 1026
= 7.638 ¥ 1026 kg
(ii)
From Eqs. (i) and (ii),9.6 ¥ 102 ¥ a3 = 7.638 ¥ 1026 a = 4.30 ¥ 1010 m The lattice constant of sodium is 4.3 Å. Example 2.4 CsCl crystallises in simple cubic crystal structure. The atomic weight of Cs is 132.9 and that of Cl is 35.5. The density of CsCl is 4 ¥ 103 kg m3. Determine the value of the Avogadro constant. Given that the lattice constant of Cesium chloride is 4.12 Å. Given Data: The density of CsCl
= 4 ¥ 103 kg m 3
The atomic weight of Cs
= 132.9
The atomic weight of Cl
= 35.5
The lattice constant a
= 4.12 Å = 4.12 ¥ 1010 m
32
Materials Science
Solution:
The mass of the CsCl unit cell = Density ¥ volume of the unit cell = 4 ¥ 103 (4.12 ¥ 1010)3 = 2.797 ¥ 1025 kg
(i)
Let N be the Avogadro constant, then the mass of the CsCl unit cell is given by, Mass =
Number of atoms in one unit cell ¥ Molecular weight Avogardro’s constant
Since, CsCl belongs to simple cubic, the number of atoms present in a unit cell is one. Therefore, the mass of one unit cell of CsCl =
1(132.9 + 35.5) N =
168.4 N
(ii)
From Eqs. (i) and (ii), , we get 168.4 = 2.797 ¥ 1025 N N=
168.4 = 6.0199 ¥ 1026 per kg mole 2.797 ¥ 10 25
The value of the Avogadro constant = 6.0199 ¥ 1026 per kg mole. Example 2.5 Xrays of 1.5418 A° wavelength are diffracted by (111) planes in a crystal at an angle of 30° in the first order. Calculate the interatomic spacing. Given Data: The wavelength of Xrays
l = 1.5418 A°
The angle of diffracted angle
q = 30°
Miller indices for diffracted plane hkl = (111) Solution:
We know that the interplanar distance d for the firstorder diffraction is d=
l 2sin q
We also know, that the interplaner distance between the planes is d=
a 2
h + k2 + l2
Crystal Structure
33
Equating the above equation, we get the lattice constant is a=
l ¥ h2 + k 2 + l 2 2sin q
Substituting the values of l h, k, l, s, q in the above equation, we get =
1.5418 ¥ 1010 ¥ 3 2 ¥ (1 / 2)
= 2.6705 ¥ 1010 m. The lattice constant a is 2.6705 ¥ 1010 m. Example 2.6 Calculate the value of dspacing for (110) planes in a rock salt crystal of a = 2.814 A°. Given Data: The lattice constant Solution:
a = 2.814 ¥ 1010 m
The distance between any two successive parallel planes is given by a d= 2 h + k2 + l2 Substituting the values for (100) planes, we get d100 =
2.814 ¥ 1010 12 + 02 + 02
= 2.814 ¥ 1010 m The lattice spacing for the plane (100) is 2.814 ¥ 1010 m. Example 2.7 Calculate the interplaner distance for the (321) planes in SCC lattice with interatomic spacing equal to 4.12 A°. Given Data: The lattice constant Solution:
a = 4.12 ¥ 1010 m
The distance between any two successive parallel planes is given by a d= 2 h + k2 + l2 Substituting the values for (321) plane, we get d321 =
4.2 ¥ 1010 32 + 22 + 12
= 1.1011 ¥ 1010 m The lattice spacing for the plane (321) is 1.1011 ¥ 1010 m.
34
Materials Science
Example 2.8 Calculate the interplaner spacing for (101) and (221) planes in a simple cubic whose lattice constant is 0.42 nm. Given Data: The lattice constant Solution:
a = 4.2 ¥ 1010 m
The distance between any two successive parallel planes is given by a d= 2 h + k2 + l2 Substituting the values for the (110) plane, we get d101 =
4.2 ¥ 1010
= 2.9698 ¥ 1010 m
12 + 02 + 12
Substituting the values for the (221) plane, we get d101 =
4.12 ¥ 1010 22 + 22 + 12
= 1.4 ¥ 1010 m
The lattice spacings for the planes (110) and (220) are 2.968 ¥ 1010 m and 1.4 ¥ 1010 m, respectively. Example 2.9 (a) Calculate the next neighbour’s distance in a body centred cubic crystal, (b) In a body centred cubic lattice, find the ratio of the nearest neighbour’s distance to the next neighbour’s distance. Solution:
(a) In a body centred cubic crystal, body centred atom is the nearest neighbour to a corner atom. The distance between these two is 3 / 2a , where a is the lattice constant. For a corner atom, the next nearest neighbour is another corner atom. The distance between the two corner atoms is a. Therefore, the next neighbour distance in a bcc lattice is a. (b) In a bcc lattice, the next neighbour distance is a. The nearest distance is. The ratio between these two is
3 / 2a neighbour
d1 : d2 = 3 / 2a : a Here d1 is the nearest neighbour distance and d2 is the next neighbour distance. Therefore, d1 : d2 =
3 / 2 : 1,
i.e.,
d1 : d2 = 0.866 : 1
The ratio between the nearest neighbouring distance and the next neighbour distance is 3 / 2 : 1. Example 2.10 In a crystal, lattice planes cut intercepts of lengths 2a, 3b and 4c along the three axes. Deduce the Miller indices of the plane.
Crystal Structure
35
Given Data:
Solution:
The intercept along Xaxis
= 2a
The intercept along Yaxis
= 3b
The intercept along Zaxis
= 4c
The intercepts made by the plane along the three axes are 2a, 3b and 4c. The coefficients of the intercepts are 2, 3, 4 The inverse of the coefficients are 1/2, 1/3, 1/4 The LCM of the above three fractions is 12 Multiplying these fractions by 12, we get 6 4 3 Therefore, the Miller indices of the plane is (643).
Example 2.11 In a crystal whose primitives are 1.2 Å, 1.8 Å and 2 Å. A plane (231) cuts an intercept of 1.2 Å along the Xaxis. Find the lengths of intercepts along the Y and Z axes. Given Data: The primitives are
Solution:
1.2 Å, 1.8 Å and 2 Å
The Miller indices of the plane
= (231)
The intercept made by the plane along the Xaxis
= 1.2 Å
Method I Let l1, l2 and l3 are the intercepts made by the plane along the X, Y and Z axes. Hence, the ratio of the intercepts is l1 : l2 : l3
(i)
The Miller indices of the plane
= (231)
The inverses of the Miller indices
= 1/2, 1/3, 1/1
Multiplying these fractions by 6, we get 3, 2, 6. Therefore, the intercepts are in the ratio of 3a : 2b : 6c
(ii)
Equating Eqs. (i) and (ii), we get l1 : l2 : l3 = 3a : 2b : 6c The a, b, c values are given as 1.2 Å, 1.8 Å, 2 Å Therefore, l1 : l2 : l3 = 3.6 Å : 3.6 Å : 12 Å, The value of l1 is given as 1.2 Å.
i.e., l1 : l2 : l3 = 3.6 : 3.6 : 12
36
Materials Science
1.2 1.2 3.6 = 1.2 Å and l3 = 12 = 4 Å 3.6 3.6 The lengths of the intercepts made by the plane along Y and Z axes are 1.2 Å and 4 Å.
Therefore, l2 = Method II
Let (hkl) be the Miller indices of a crystal plane. If Miller indices are known, then the intercepts made by the plane is given by a, b, c h k l The values of a, b and c are given as a = 1.2 Å, b = 1.8 Å, c = 2 Å Substituting the values of a, b and c, we get the ratios of intercepts as 1.2Å 1.8Å 2Å = 0.6 Å : 0.6 Å : 2 Å : : l 3 1 Let these ratios be x : y : z Therefore,
0.6 Å : 0.6 Å : 2 Å = x : y : z
Substituting, the x axis intercept, we get 0.6 Å : 0.6 Å : 2 Å = 1.2 Å : y : z The y intercept is determined by considering x and y intercepts. i.e.,
0.6 Å : 0.6 Å = 1.2 Å : y y = 1.2 Å
The z intercept is, 0.6 Å : 2 Å = x : z z=4Å The y and z intercepts are 1.2 Å, 4 Å. Example 2.12 The Miller indices of a crystal plane in a simple cubic crystal is (110). Find the ratio of the intercepts on the three axes. Given Data:
Solution:
The Miller indices of the plane
= (110)
The Miller indices of the given plane The inverses of the Miller indices
= (110) = 1/1, 1/1, 1/0,
i.e.,
1, 1,
The intercepts made by the plane in terms of lattice parameters is 1a, 1b,
c.
Let l1, l2 and l3 be the lengths of the intercepts made by the plane along the X. Y and Z axes. The ratios of these three lengths is l1 : l2 : l3. If l1 : l2 : l3 are the ratios of the intercepts, then they are related to the lattice parameters as,
Crystal Structure
l1 : l2 : l3 = 1a : 1b :
37
c
Since, the given crystal is a simple cubic a = b = c Therefore, the ratio l1 : l2 : l3 = 1a : 1a :
c
=1:1: The intercepts made by the given plane along the Z axis is is parallel to the Z axis.
. It means that the plane
Example 2.13 The lattice constant of a cubic lattice is 4.12 Å. Find the lattice spacings between (111), (112) and (123) lattice planes. Given Data: The lattice constant Solution:
a = 4.12 Å
The distance between any two successive parallel planes is given by d=
a 2
h + k2 +l2
(i) For (111) plane, d111 =
4.12 ¥1010
= 2.3787 ¥ 1010 m
12 +12 +12
(ii) For (112) plane, d112 =
4.12 ¥1010 12 +12 + 22
= 1.68198 ¥ 1010 m
(iii) For (123) plane, d123 =
4.12 ¥1010 12 + 22 + 32
= 1.1011 ¥ 1010 m
The lattice spacing for the planes (111)
= 2.3787 ¥ 1010 m.
The lattice spacing for the planes (112)
= 1.6820 ¥ 1010 m.
The lattice spacing for the planes (123)
= 1.1011 ¥ 1010 m.
Example 2.14 Show that in a simple cubic lattice, the separation between the successive lattice plane (100), (110) and (111) are in the ratio of 1 : 0.71 : 0.58. Solution:
The interplanar distance is given by d=
a 2
h + k2 +l2
38
Materials Science
For (100) plane, d100 = For (110) plane, d110
a
=a 1 + 02 + 02 a a = 2 2 2 = 2 1 +1 + 0
For (111) plane, d111 =
2
a 2
2
2
1 +1 +1 a a = a: : 2 3
=
a 3
The ratio of
d100 : d110 : d111
i.e.,
d100 : d110 : d111 = a : 0.707a : 0.577a
The ratio of
d100 : d110 : d111 = 1 : 0.71 : 0.58
or,
d100 : d110 : d111 =
6: 3: 2
Example 2.15 The lattice constant for a Fcc structure is 4.938 A°. Calculate the interplaner spacing of the (220) plane. Given Data: The lattice constant Solution:
a = 4.938 ¥ 1010 m
The distance between any two successive parallel planes is given by a d= 2 h + k2 + l2 Substituting the values for the (220) plane, we get d 220 =
4.938 ¥ 1010 22 + 22 + 02
= 1.7458 ¥ 1010 The lattice spacing for the plane (110) is 2.968 ¥ 1010 m. Example 2.16 The unit cell of aluminum is Fcc with lattice constant a = 0.405 nm. How many unit cells are there in a 0.054 cm thick and 25 cm2 square aluminum foil? Given Data: The lattice constant
a = 0.405 ¥ 109 m.
The thickness of Al foil
t = 0.005 ¥ 102 m
The side length of the Al foil Solution:
A = 25 ¥ 104 m
We know that the number of unit cells in the Al foil is =
Volume of Al foil Volume of unit cell
Crystal Structure
i.e.,
=
t¥A a3
=
0.005 ¥ (25 ¥ 10 2 ) (0.405 ¥ 10 10 )3
39
Substituting the values, we get
=
1.25 ¥ 105 28 6.643 ¥ 1029 = 1.88 ¥ 10
Therefore, the number of atoms in the Al foil is 1.88 ¥ 1028. Example 2.17 The lattice constant of a metal with cubic lattice is 2.88 A°. The density of the metal is 7200 kg m3. Calculate the number of unit cell present in the 1 kg of the metal. Given Data:
Solution:
The lattice constant
a = 2.88 ¥ 1010 m.
Density of metal
r = 7200 kg m3
We know that the number of unit cells in 1 kg of the metal is 1 Mass of the unit cell 1 = Volume of the unit cell ¥ Density
= i.e.,
Substituting the values, we get =
1 = 5.8142 ¥ 1024 (0.288 ¥ 1010 )3 ¥ 7200
Therefore, the number of unit cells present in 1 kg metal is 5.8142 ¥ 1024. Example 2.18 Metallic iron changes from bcc to fcc form at 910°C. At this temperature, the atomic radii of the iron atoms in the structures are 0.1258 nm and 0.1292 nm, respectively. Calculate the volume changes in percentage during this structural change. Given Data:
Solution:
The atomic radius at bcc state
= 0.1258 ¥ 109 m
The atomic radius at fcc state
= 0.1292 ¥ 109 m
We know that, the lattice constant for bcc
a=
4r 3
Substituting the values, we get 4 ¥ 0.1258 ¥ 1010 = 3
= 2.9052 ¥ 1010 m
40
Materials Science
Therefore, the volume occupied by one atom in bcc is =
a3 2
Substituting the values, we get =
(2.9052 ¥ 1010 )3 2
= 1.226 ¥ 1029 m3
The volume occupied by one atom in Bcc state is = 1.226 ¥ 1029 m3. 4r We know that, the lattice constant for fcc a = 2 Substituting the values, we get 4 ¥ 0.1292 ¥ 1010 = 2
= 3.6543 ¥ 1010 m
Therefore, the volume occupied by one atom in fcc is =
a3 4
Substituting the values, we get =
(3.6543 ¥ 1010 )3 = 1.22 ¥ 1029 m3. 4
The volume occupied by one atom in Fcc state is = 1.22 ¥ 1029 m3. Therefore, change in volume in percentage is =
(1.226 ¥ 1029  1.22 ¥ 1029 ) ¥ 100 = 0.4894 1.226 ¥ 1029
The volume change in percentage during the structural changes is 0.4894. Example 2.19 Copper has fcc structure and its atomic radius is 1.273 Å. Find the lattice parameter and the density of copper. Atomic weight of copper
= 63.5 g
Avogadros number
= 6.023 ¥ 1026 atoms k mol1
Given Data: The atomic radius for fcc system
r = 1.273 Å
Atomic weight of copper
A = 63.5 g = 63.5 ¥ 103 kg
Solution:
Number of atoms per unit cell for Fcc
n=4
We know that lattice parameter for Fcc
a=
4r 2
Crystal Structure
41
Substituting the values, we get =
4 ¥ 1.273 ¥ 1010 1.414
a = 3.6 ¥ 1010 m Density of the material is
nA Na 3
r =
Substituting the given values, we get Density
r =
4 ¥ 63.5 ¥103 6.023 ¥1026 ¥ (3.6 ¥1010 )3
= 9.0388 Therefore, the density of copper is 9.0388 gm m3 Example 2.20 airon of 55.85 atomic weight solidifies into bcc structure and has a density of 7860 kg m3. Calculate the radius of an atom. Given Data:
Solution:
The density of airon
r = 7860 kg m3
The atomic weight of airon
M = 55.85
Number of atoms per unit cell for Bcc
n=2
Avogadro’s number
N = 6.023 ¥ 1026 atoms k mol1.
We know that the volume of the cube is
i.e.,
a3 =
Number of atoms per unit cell ¥ Molecular weight Avogadro’s number ¥ Density
a3 =
nM N ¥r
Substituting the values, we get =
2 ¥ 55.85 ¥ 103 = 2.3595 ¥ 1032 m3. 6.626 ¥ 1026 ¥ 7860
i.e.,
a = 3 2.3596 ¥ 1032
or,
a = 0.2868 ¥ 1010 m.
The lattice constant of airon is 0.2868 A˚. We know that the atomic radius for bcc is r=
a 3 4
42
Materials Science
Substituting the values, we get r=
1.732 ¥ 0.2868 ¥ 1010 = 0.12418 ¥ 1010 m 4
The atomic radius of the airon is 0.12418 ¥ 10
10
m.
Example 2.21 Copper crystalline in the fcc structure. The density and atomic weight of copper are 8960 kg m3 and 63.54, respectively. Calculate its lattice constant. Given Data: The density of copper
r = 8960 kg m3.
The atomic weight of copper
Solution:
M = 63.54
Number atoms per unit cell for fcc
n=4
Avogadro’s number
N = 6.023 ¥ 1026 atoms k mol1.
We know that, the volume of the cube is
i.e.,
a3 =
Number of atoms per unit cell ¥ Molecular weight Avogadro’s number ¥ Density
a3 =
nM N ¥r
Substituting the values, we get =
4 ¥ 63.54 ¥ 103 = 4.7096 ¥ 1032 m3. 6.023 ¥ 1026 ¥ 8960
i.e.,
a = 3 4.7096 ¥ 1032
or,
a = 0.3611 ¥ 1010 m.
The lattice constant of copper is 0.3611 A°. Example 2.22 Calculate the glancing angle for incidence of Xrays of wavelength 0.58 Å on the plane (132) of NaCl which results in second order diffraction maxima taking the lattice spacing as 3.81 Å. Given Data: Lattice spacing
a = 3.81 ¥ 10l0 m
Miller indices for the plane (h k l ) = (1 3 2) Wavelength f the Xrays
l = 0.58 ¥ 1010 m
Order of diffraction
n=2
Crystal Structure
Solution:
43
We know that the distance between any two successive parallel planes a d= 2 h + k 2 + l2 Substituting the values for h, k, l, and a values in the above equation, we get d123 =
3.81 ¥ 1010 12 + 32 + 22
= 1.018 ¥ 1010 m According to Bragg’s condition, nl = 2d sinq Therefore, the angle of diffraction is Ê nl ˆ q = sin1 Á ˜ Ë 2d ¯ Substituting the values of n, l and d in the above equation, we get
Ê 2 ¥ 0.58 ¥ 1010 ˆ = sin1 Á Ë 2 ¥ 1.018 ¥ 1010 ˜¯ = sin1 (0.5697) = 34.73∞ Therefore, the angle of glancing at which second order diffraction pattern of NaCl occurs is 34.73∞. Example 2.23 A monochromatic Xray beam of wavelength 0.7 Å undergoes firstorder Bragg reflection from the plane (302) of a cubic crystal at a glancing angle of 35∞. Calculate the lattice constant. Given Data: Miller indices for the plane (h k l) = (3 0 2)
Solution:
The glancing of angle
q = 35∞
Wavelength f the Xrays
l = 0.7 ¥ 1010 m
Order of diffraction
n=1
According to Bragg’s condition, nl = 2d sinq Therefore, the interplanar spacing for the plane (302) d302 =
nl 2 sin q
44
Materials Science
Substituting the values of n, q and d in the above equation, we get =
1 ¥ 0.7 ¥ 1010 2 ¥ sin 35∞
= 6.102 ¥ l011 The interplanar distance for (302) is 6.102 ¥ 1011 m. We know that the lattice constant a = d ¥ h2 + k 2 + l2 Substituting the values of d, h, k, and l, we get a = 6.102 ¥ 1011 ¥ 32 + 02 + 22 = 2.2 ¥ l010 Therefore, the lattice constant is 2.2 ¥ 1010 m. Example 2.24 Draw the following planes in a cubic unit cell (0 0 1), (1 0 1) and (1 1 1). Solution:
For (0 0 1) plane The intercepts are
1 1 1 , and 0 0 1
i.e., the intercepts made by the plane along the x, y and z axis are respectively , and 1. Therefore, the plane makes an intercept along y and z axis at a unit distance while at the xaxis, is parallel and hence does not make any intercept. The representation of (001) plane is shown in Fig. 2.17. z
y x (001)
Fig. 2.17 101 plane For (101) plane The intercepts are,
1 1 1 , and 1 0 1
i.e., the intercepts made by the plane along the x, y and z axis are respectively l, and 1.
Crystal Structure
45
Therefore, the plane makes an intercept along y and z axis at unit distance while at the xaxis, it is parallel and hence does not make any intercept. The representation of (101) plane is shown in Fig. 2.18. For (0 1 1) plane The intercepts are,
1 1 1 , and 0 1 1
i.e., the intercepts made by the plane along the x, y and z axis are respectively , 1 and 1. Therefore, the plane makes an intercept along y and z axis at a unit distance while at the xaxis it is parallel and hence does not makes any intercept. The representation of (101) plane is shown in Fig. 2.19. z
z
y
–y
y
x (011)
x (101)
Fig. 2.19 (0 1 1) plane
Fig. 2.18 (1 0 1) plane Example 2.25
A beam of monochromatic Xrays is diffracted by NaCl crystal with a glancing angle of 12∞ for first order. Calculate the wavelength of the Xray if the d spacing of the crystal is 2.82A∞. [VTU OS July 2003] Given Data: The glancing angle
q =12∞
The interplanar spacing l = 2.82 ¥ 1010 The order of diffraction n = 1 Solution:
We know that the interplanar spacing d=
nl 2sin q
Substituting the values of n, l and d in the above equation, we get =
1 ¥ 2.82 ¥ 1010 2 ¥ sin 12∞
= 6.782 ¥ 1010 Therefore, the interplanar spacing is 6.782 ¥ 1010 m.
46
Materials Science
Example 2.26 A sodium chloride crystal is used as a diffraction grating with Xrays. For the d111 spacing of the chloride ions, the angle of diffraction 2q is 27.5∞. If the lattice constant of the crystal is 0.563 nm, what is the wavelength of Xrays? Given Data: The glancing angle
q = 27.5∞/2 = 13.75∞
Lattice constant
a = 0.563 ¥ 109
The order of diffraction n = 1 Solution:
We know that the interplanar distance is d=
a h2
+ k 2 + l2
Substituting the values for (111) planes in the above equation, we get d111 =
0.563 ¥ 10 9 12 + 12 + 12
= 3.25 ¥ 1010 m The lattice spacing for the plane (111) is 3.25 ¥ 1010 m. We know that the de Broglie wavelength l=
2d sin q n
Substituting the values d, q and n in the above equation, we get =
2 ¥ 3.25 ¥ 1010 ¥ sin 13.75∞ 1
= 1.544 ¥ l010 The deBroglie wavelength of the neutrons is 1.544 ¥ 1010 m Therefore, the lattice spacing for the plane (111) is 3.25 ¥ 1010 m The deBroglie wavelength of the neutrons is 1.544 ¥ 1010 m. Example 2.27 The interplanar spacing of (110) planes is 2 A for a cubic crystal. Find out the atomic radius. Given Data: Miller indices for the plane (h k l ) = (1 1 0) The interplaner spacing
d = 2 ¥ 1010 m
Crystal Structure
Solution:
47
We know that the lattice constant a = d ¥ h2 + k 2 + l2 Substituting the values of d and (h k l ) in the above equation, we get a = 2 ¥ 1010 ¥ 12 + 12 + 02 = 3.112 ¥ 1010 The lattice constant is 3.112 ¥ 1010 m. We know that atomic radius of the cubic crystal is 2 2R = a R=
a 2 2
= 1010 The atomic radius of the crystal is 1010 m Therefore, the lattice constant is 3.112 ¥ 1010 m The atomic radius of the crystal is 1010 m. Example 2.28 Calculate the energy of electrons that produces Bragg’s diffraction of first order at an angle of 22∞ when incident on the crystal with interplanar spacing of 1.8 Å. Given Data: The glancing angle
q = 22∞
The interplanar spacing
l = 1.8 ¥ 1010
The order of diffraction n = 1 Solution:
We know that the de Broglie wavelength of the neutron 2d sin q n Substituting the values of d, q and n, in the above equation, we get l=
2 ¥ 1.8 ¥ 1010 ¥ sin 22∞ 1 10 = 1.349 ¥ l0 =
The de Broglie wavelength of the neutron is 1.349 ¥ 1010 m. Therefore, the energy of the neutron E=
1 Ê hˆ Á ˜ 2m Ë l ¯
2
48
Materials Science
Substituting the values of m, h and l, we get =
1 Ê 6.626 ¥ 1034 ˆ 31 2 ¥ 9.11 ¥ 10 ÁË 1.349 ¥ 1010 ˜¯
2
= 1.324 ¥ l017 J 1.324 ¥ 10 17 =
1.609 ¥ 10 19
= 82.29 eV Therefore, the energy of the neutron is 82.29 eV. Example 2.29 If the lattice constant of a cubic crystal is 3 Å, find the interplanar spacing between (111) planes. Given Data: Lattice spacing
a = 3 ¥ 1010
Miller indices for the plane (h k l ) = (1 1 1) Solution:
We know that the distance between any two successive parallel planes d=
a h2 + k 2 + l2
Substituting the values for (111) planes, we get d111 =
3 ¥ 1010 12 + 12 + 12
= 1.732 ¥ 1010 Therefore, the interplanar spacing is 1.732 ¥ 1010 m. Example 2.30 Copper has fcc structure of atomic radius 0.1278 nm. Calculate the interplanar spacing for (3 2 1) plane. Given Data: The atomic radius at fcc state Solution:
= 0.1278 ¥ 109 m.
We know that the lattice constant for fcc a =
4r 2
Substituting the values, we get 4 ¥ 0.1278 ¥ 1010 = 2 The lattice constant = 3.615 ¥
1010
m.
Crystal Structure
49
We know that the interplanar distance d=
a h2
+ k 2 + l2
Substituting the values for (321) planes in the above equation, we get d321 =
3.615 ¥ 1010 32 + 22 + 12
= 9.66 ¥ 1011 m Therefore, the lattice spacing for the plane (321) is 9.66 ¥ 1011 m. Example 2.31 The unit cell of aluminum is fcc with lattice constant a = 0.4049 nm. How many unit cells are in an aluminum foil which is 0.005 cm thick and side 25 cm square? Given Data: Lattice constant
a = 0.4049 ¥ 109 m
Thickness of the foil, t = 0.005 ¥ 102 m Area of the foil, Solution:
A = 25 ¥ 104 m2
We know that the number of unit cells in the Al foil
i.e.,
=
Volume of Al foil Volume of unit cell
=
t¥A a3
Substituting the values of t, A and a in the above equation, we get =
0.005 ¥ (25 ¥ 102 ) (0.4049 ¥ 1010 )3
=
1.25 ¥ 105 6.643 ¥ 1029
= 1.88 ¥ l028 Therefore, the number of atoms in the Al foil is 1.88 ¥ 1028. Example 2.32 Calculate the energy of the neutrons that produces first order Bragg diffraction at 20∞ when incident on planes separated by a distance of 2 A. (Mass of neutron = 1.67 ¥ 1027 kg) Given Data: The order of diffraction n = 1 The glancing angle
q = 20∞
The interplanar spacing l = 2 ¥ 1010
50
Materials Science
Solution:
We know that the de Broglie wavelength of the neutron 2d sin q n Substituting the values d, q and n in the above equation, we get l=
2 ¥ 2 ¥ 10 10 ¥ sin 20∞ 1 = 1.368 ¥ l010 =
The de Broglie wavelength of the neutron is 1.368 ¥ 1010 m. Similarly, we know that the energy of the neutron E=
1 Ê hˆ Á ˜ 2m Ë l ¯
2
Substituting the values of m, h and l in the above equation, we get =
1 Ê 6.626 ¥ 1034 ˆ 27 2 ¥ 1.67 ¥ 10 ÁË 1.349 ¥ 1010 ˜¯
2
= 7.03 ¥ 1021 J =
7.03 ¥ 1021 1.609 ¥ 1019
= 0.0437 eV Therefore, the energy of the neutron is 0.0437 eV. Example 2.33 Find the Miller indices of a set of parallel planes which make intercepts in the ratio 3a: 4b on the X and Y axis and are parallel to Zaxis, a, b, c being primitive vectors of the lattice. Given Data: The intercept along Xaxis = 3a The intercept along Yaxis = 4b The intercept along Zaxis = Solution:
The intercepts made by the plane along the three axes are 3a, 4b, The coefficients of the intercepts are 3, 4, The inverses of the coefficients are 1/3, 1/4, l/ The LCM of the above fractions is 12 Multiplying these fractions by 12, we get 4, 3, 0 Miller indices of the plane are (430) Therefore, the Miller indices of the plane are (4 3 0).
Crystal Structure
51
Example 2.34 Obtain the Miller indices of a plane with intercepts a, b/2, 3c in a sample cubic unit cell. Given Data: The intercept along Xaxis = a The intercept along Yaxis = b/2 The intercept along Zaxis = 3c Solution:
The intercepts made by the plane along the three axes are a, b/2, 3c The coefficient of the intercepts are 1, 1/2, 3 The inverses of the coefficient are 1, 2, l/3 The LCM of the above fractions is 3. Multiplying these fractions by 3, we get 3, 6,1 Miller indices of the plane are (361) Therefore, the Miller indices of the plane are (3 6 1).
Example 2.35 A monochromatic beam of electrons with a kinetic energy of 235.2 eV undergoes firstorder Bragg reflection in a crystal at the glancing angle of 9∞ 12´ 35˝. Calculate the interplanar spacing. Given Data: The kinetic energy of the electron Ek = 235.2 eV = 235.2 ¥ 1.602 ¥ 1019 = 3.77 ¥ 1017 The order of diffraction n = 1 The glancing angle q = 9∞ 12´ 35˝ = 9.21∞ Solution:
We know that the de Broglie wavelength of the electron l=
h 2mE
Substituting the values of h, m and E in the above equation, we get 6.626 ¥ 1034 = 2 ¥ 9.11 ¥ 1031 ¥ 3.77 ¥ 1017 = 7.995 ¥ l011 m The de Broglie wavelength of the electron is 7.995 ¥ 1011 m.
52
Materials Science
We know that from Bragg’s equation, nl = 2d sinq Therefore, the interplanar spacing d=
nl 2sin q
Substituting the values of n, l and d in the above equation, we get =
1 ¥ 7.995 ¥ 1011 2 ¥ sin 9.21∞
= 2.498 ¥ 1010 Therefore, the interplanar spacing is 2.498 ¥ 1010 m. Example 2.36 Find the Miller indices of a set of parallel planes which make intercepts in the ratio 3a:4b and parallel to Zaxis and also calculate the interplanar distance of the planes taking the lattice to be cubic with a = b = c = 2 A∞. Given Data: The intercept along Xaxis = 3a The intercept along Yaxis = 4b The intercept along Zaxis = Solution:
Step I Determination of Miller indices of the plane The intercepts made by the plane along the three axes are 3a, 4b, The coefficients of the intercepts are 3, 4, The inverses of the coefficients are 1/3, 1/4, 1/ , The LCM of these above fractions is 12 Multiplying these fractions by 12, we get 4, 3, 0 Therefore, the Miller indices of the plane is (430) Step II Determination of lattice spacing We know that the distance between any two successive parallel planes d=
a h2
+ k 2 + l2
Crystal Structure
53
Substituting the values for (430) planes, we get d430 =
2 ¥ 1010 42 + 32 + 02
= 0.4 ¥ 1010 m. Therefore, the lattice spacing for the plane 430 is 0.4 ¥ 1010 m. Example 2.37 Find the Miller indices of a plane making the intercepts 2a, 3b and 6c, respectively on (100), (010) and (001) directions, a, b and c represent the basic vectors. Given Data: The intercept along (100) axis = 2a The intercept along (010) axis = 3b The intercept along (001) axis = 6c Solution:
The intercepts made by the plane along the three axes are 2a, 3b, 6c The coefficients of the intercepts are 2, 3, 6 The inverses of the coefficients are 1/2, 1/3, 1/6 The LCM of the above fractions is 6 Multiplying these fractions by 6, we get 3, 2, 1, Miller indices of the plane are (321) Therefore, the Miller indices of a plane are (321).
Example 2.38 Draw the following planes in a cubic unit cell (0 1 1) and (1 1 2) Solution:
For (0 1 1) plane Therefore, the intercepts along x, y and z axes are,
1 1 1 , and respectively 0 1 1
i.e., the intercepts made by the plane along the x, y and z axes are , l and 1, respectively. Therefore, the plane makes an intercept along y and z axes at a unit distance while at the xaxis it is parallel and hence does not make any intercept. The representation of the (0l1) plane is shown in Fig. 2.20(a). For (112) plane The intercepts are,
1 1 1 , and 1 1 2
54
Materials Science
i.e., the intercepts made by the plane along the x, y and z axes are 1, 1 and 1/2, respectively. Therefore, the plane makes an intercept along y and z axis at a unit distance while at the xaxis it is parallel and hence does not make any intercept. The representation of (1 1 2) plane is shown in Fig. 2.20(b). z z
–y
y
y x (112) PLANE
x
Fig. 2.20(a) (0 1 1) plane
Fig. 2.20(b) (1 1 2) plane
ObjectiveType Questions 2.1. Anisotropic structures have _________ properties. 2.2. Examples for metallic crystals are _________, _________ and _________. 2.3. The structures which are not having directional properties are known as _________ substances. 2.4. Complete the equation, Crystal structure = Lattice + _________. 2.5. _________ is the fundamental building block of a crystal structure. 2.6. Body centered cubic unit cell is not a primitive cell. (True/False) 2.7. In a cubic crystal structure, the values of angles a = b = g = _________. 2.8. The crystal plane is represented by a set of three numbers within _________. 2.9. Crystal directions are represented by a set of three numbers within _________. 2.10. The interatomic distance is equal to _________ (a) d = (c) d = 2.11. 2.12. 2.13. 2.14.
a h2 + k 2 + l2 a2 h2 + k 2 + l2
(b) d = (d) d =
a2 h2 + k 2 + l2 a2 h2 + k 2 + l2
The coordination number for a simple cube is _________. The packing density for a simple cube is equal to _________. _________ is the coordination number for body centered cubic structure. _________ and _________ are the coordination number and packing density for fcc structure, respectively. 2.15. The coordination number and packing density for hcp structure are _________ and _________, respectively.
Crystal Structure
55
2.16. In the hcp structure, the relation between c and a is _________. (a)
c 8 = a 3
(b) c = 8 a 3
(c)
c 8 = a 3
(d)
c 8 = a 3
2.17. Three examples for cubic crystal planes are _________, _________ and _________. 2.18. In bcc structure, the packing density of crystal is equal to (a)
3p 8
(c)
p 3 8
(b)
3p 8
(d) 3 3p 8
Answers 2.1. Directional 2.5. Unit cell
2.2 Copper, silver, aluminium 2.6 True
2.9. Parenthesis 2.10. (c) 2.13. 8 2.14. 12, 0.74 2.17. (110), (010), (101) 2.18. (b)
2.3. Isotropic 2.7. 90º 2.11. 6 2.15. 12, 0.74
2.4. Basis 2.8. Parenthesis 2.12. 0.52 2.16. (c)
Short Questions 2.1. 2.2. 2.3. 2.4. 2.5. 2.6. 2.7. 2.8. 2.9. 2.10. 2.11. 2.12. 2.13. 2.14. 2.15. 2.16.
Define space lattice. What is meant by basis? Define the term crystal structure. What are interfacial angles? Define the term unit cell. What is meant by lattice Parenthesis? What is primitive cell? Distinguish between the primitive cell and unit cell. Name the seven types of crystal systems. What is Bravais lattice? Name the crystal structure of the following (a) Gold, (b) Geranium, (c) Bartu, and (d) Zinc. Bismith has a = b = c = 4.74 AU and angles a = b = g = 60° what is its crystal structure? What are Miller indices? Explain how the miller indices are determined. Describe the structure of hcp. Define the following terms: (a) Atomic radius (b) Coordination number, and (c) Packing density
56
Materials Science
2.17. 2.18. 2.19. 2.20. 2.21. 2.22. 2.23. 2.24. 2.25. 2.26.
State the values of coordination number for hcp structure. Calculate the packing factor for a simple cubic structure. Calculate the packing factor for a body contracte cubic. Calculate the packing factor for a face centred cubic. Define the coordination number and the calculate the same for fcc lattice Show that for a bcc crystal structure, the lattice constant is given by a = 4r/ 3 , where r is the atomic radius. Establish the relation between the radius and the interatomic distance for a face centred cubic crystal. Draw the diagram of the unit cell of the close packed hexagonal lattice. For a cubic lattice, draw the followig plane showing the value of intercept with the coordination axis (a) [110], (b) [111] and (c) [021]. Draw the schematic diagrams of a simple cubic, body centred cubic and face centred cubic unit cells.
Descriptive Questions 2.1. What are Miller indices? How will you determine the Miller indices of a given plane? What are the distinct features of Miller indices? 2.2. Define the terms coordination number, atomic radius, and packing density. Calculate the above factors for a simple cubic, body centred cubic and face centred cubic crystals. 2.3. Determine the coordination number and packing density for a hexagonally closed packed structure. Show that a hcp structure demands an axial ratio of 1.633. 2.4. What is packing factor? Prove that the packing factor of hcp is 0.74.
Exercises 2.1. Calculate the density of the NaCl crystal from the following data: Molecular weight of NaCl = 58.45; Lattice constant a = 5.64 Å; Avogadro constant = 6.023 ¥ 106 per kg mole. 2.2. Calculate the lattice constant of potassium bromide. Density of potassium bromide is 2.7 ¥ 103 kg m3 and belongs to fcc lattice. The molecular weight of KBr is 119 and the Avogadro constant is 6.022 ¥ 106 per kg mole. 2.3. Calculate the next neighbour’s distance in a simple cubic lattice and also determine the ratio between the nearest neighbour’s distance and the next neighbour’s distance for a simple cubic lattice. 2.4. Find the Miller indices of a plane, which makes intercepts at 3a, 2b and 2c. 2.5. A crystal plane makes intercepts at 2a, 3b and 6c along the three crystallographic axes. Here a, b and c are the primitive vectors of the unit cell. Determine the Miller indices of the given crystal plane. 2.6. The lattice parameters of a unit cell is 1.6 Å, 2.22 Å and 1.84 Å. A plane having Miller indices value of (231) makes an intercept at 1.84 Å along the Z axis. Find the lengths of the intercepts made by the plane along X and Y axes. 2.7. Calculate the interplanar spacing for a (321) plane in a simple cubic lattice whose lattice constant is 4.12 ¥ 1010 m.
Chapter
3
CHARACTERISATION OF MATERIALS
OBJECTIVES To study the principle, experiments and determination of crystal structures. To study generation and diffraction of Xrays and their applications. To study the different experimental methods such as Laue’s powder crystal, rotating crystal, neutron diffraction, and Bragg’s law for determination of crystal structure. To study the principle, mechanism and applications of optical based instruments. To explore the method to find the attitude of sun and height of a tower or building. To understand the operating principle and applications of optical microscope, TEM, SEM and STEM. To understand the role of optical instruments in material characterisation. To know the principle, measurements and application of micro and nanoindentations. To compare the micro and nanoindentations of metals. To explore the possible applications of micro and nanoindentations.
3.1 INTRODUCTION The modern science and technology requires new materials for different applications in our daytoday life. The knowledge on the new materials is more essential for complete usage of these materials. The structural, physiochemical, electrical and mechanical properties are used to characterise the materials. The material charactersisation plays a significant role in design, development, process optimisation and performance evaluation, to meet the stringent requirements for engineering applications. One has to select the right material for a particular application which requires all the above said properties. Thus, the knowledge on the new material is more essential.
58
Materials Science
The analytical instruments used for the characterisation of materials are classified into different categories namely spectroscopy, mechanical, electrochemistry and chromatography techniques. In addition, due to technological advancements, some of the new techniques are also emerging. Techniques like Xray Diffraction (XRD), Neuron Diffraction (ND), Electron Diffraction (ED), Transmission Electron Microscopy (TEM), Scanning Electron Microscopy (SEM) and Atomic Force Microscopy (AFM) are examples for spectroscopic techniques. Generally, spectroscopic techniques are used to determine the structure, size or shape of the particles and subsurface microscopic nature of materials. The mechanical methods such as Vickers hardness testing, Knoop hardness testing and nano indenter are used to explore the mechanical properties like hardness and elastic properties of materials. In this chapter, (i) the spectroscopic techniques like Xray, electron or neutron diffraction, transmission electron microscopy, scanning electron microscopy, scanning transmission electron microscopy and atomic force microscopy techniques, and (ii) the mechanical methods like Vickers hardness testing, Knoop hardness testing and nano indenter are discussed briefly.
3.2
DISCOVERY OF XRAYS
A German physicist, Roentgen, in 1895, while doing some experiments on the effect of cathode rays on the luminous property of certain chemicals, noticed a flash of light from a sheet of paper coated with barium platinocyanide. After performing a series of experiments, Roentgen concluded that when a beam of cathode rays strike a solid target, it produces invisible and penetrating radiations. Because of its unknown nature, he called these radiations as Xradiation or Xrays. These rays are also known as Roentgen rays. Xrays are electromagnetic waves of short wavelengths, ranging from 0.5 to 10 Å. The longer wavelength of the Xray spectrum is known as soft Xrays and Xrays of shorter wavelength are known as hard Xrays.
3.2.1
Generation of Xrays
Xrays are produced when a beam of fast moving cathode rays (electrons) strike a heavy target material such as tungsten or molybdenum. The experimental set up for the production of Xrays uses the Coolidge tube.
Coolidge Tube It is a specially designed and partially evacuated hard glass tube enclosed in a lead box, as shown in Fig. 3.1. The electrons are emitted thermionically by the filament F using a Low Tension (LT) supply. These emitted electrons are focussed on the target material using a hollow metallic cylinder C by giving a small negative potential. This electron beam is then accelerated by a high positive potential applied between the anode and the filament. The anode is made up of a thick copper rod and the front face of the anode is inclined at an angle of 45°. The target material, tungsten or molybdenum, is embedded in the cut face of the copper rod. The accelerated electrons are focussed by the cylinder C on the target T. When the accelerated electrons strike the target, about 99.8% of the electrons are wasted in heating the target material. Due to heavy bombardment of electrons on the target material, while the remaining 0.2% of electrons penetrate through the target material, a large quantity of material gets melted. Hence, the target
Characterisation of Materials
59
material should have high atomic number, high melting point and high thermal conductivity, such as molybdenum and tungsten. The heat produced by the electrons is easily conducted by the copper anode. To conduct the heat produced in the anode, a cooling arrangement is used in the copper anode. The penetrating electrons are converted into Xrays. – + 50100 kV
A T
C F
LT
Xrays
Cooling water
R
Fig. 3.1 Xrays Coolidge tube
Intensity and Quality The intensity of Xrays depends on the number of electrons striking the target material. The number of electrons striking the target material depends upon the concentrations of the electrons produced by the filament. Thus, the number of electrons emitted by the filament is determined by the current flowing through the filament. Hence, by controlling the filament current with the help of a rheostat, the intensity of the Xrays can be controlled. Based on the penetrating power of electrons, the quality of Xrays is termed as soft and hard Xrays. Xrays having low penetrating power are known as soft Xrays, while those having high penetrating power are known as hard Xrays. The penetrating power of Xrays depend upon the potential difference applied between the filament and the anode. Therefore, by varying this potential difference, one can control the quality of Xrays. Thus, the intensity and quality of Xrays are controlled in this apparatus, but they cannot be controlled in other methods of generation.
3.3 DIFFRACTION OF XRAYS Like ordinary light rays, Xrays also exhibit diffraction phenomenon. To observe the diffraction pattern, the number of lines ruled on the grating must be in the order of the wavelength of the rays used. In ordinary grating, 106 lines are drawn in 1 m, i.e., 1 line is drawn in 106 m. The wavelength of light is also in the order of 106 to 107 m. To observe the diffraction pattern, the spacing between any two lines drawn on the grating should be in the order of the wavelength of the light used. The wavelength of Xrays are 1000 times shorter than that of ordinary light rays. Hence, ordinary grating cannot be used to observe the diffraction pattern of Xrays. Von Laue suggested that a crystal can be used as diffraction grating for the diffraction of Xrays, (since, the spacing between the atoms in the crystals and the wavelength of Xrays are in the same order, i.e., 1 Å).
60
Materials Science
3.3.1
Bragg’s Law
The fundamental equation which gives a simple relation between the wavelength (l) of Xrays, the interplanar distance (d), and the glancing angle (q), is known as Bragg's law. It is given as, 2d sin q = nl
(3.1)
where n = 1, 2, 3, etc., represents the order of the spectrum.
3.3.2
Derivation of Bragg’s Law
Let us consider a set of parallel planes in a crystal spaced by interplanar distance d. Consider a narrow, monochromatic Xray beam of wavelength l, incident on the first plane, at a glancing angle q, as shown in Fig. 3.2. The incident beam undergoes multiple reflections between the parallel planes of the crystal. A C A' C'
B
q d
D
q
q
E
B'
Fig. 3.2 Reflection of monochromatic beam in a crystal plane Consider a ray AB, incident on the first plane and is reflected in the direction BC from that plane by the atom B. Let the incident beam AB make a glancing angle q to the first plane. Similarly, consider a parallel ray A' B' is reflected in the direction B' C' by another atom B' in the second plane. To determine the path difference between the two rays ABC and A' B'C', draw normals from the point B to the lines A'B' and B'C'. Let the normals be BD and BE. Therefore, the path difference between these two rays is equal to B'D' + B'E'. In the triangle BDB', sin q = DB'/BB' Therefore, DB' = BB' sin q = d sin q Similarly, B'E = d sin q Therefore, the path difference is given as, d sin q + d sin q = 2d sin q
(3.2)
Characterisation of Materials
61
Therefore, the two rays BC and B'C' will reinforce with each other and produce a maximum intensity when 2d sin q = nl
(3.3)
where n (= 1, 2, 3, etc.) is the order of the spectrum, and l the wavelength of the Xrays used. Equation (3.3) is known as Bragg’s law.
3.3.3
Bragg’s Xray Spectrometer
The construction of Bragg’s spectrometer is similar to an optical spectrometer. The essential parts of a Bragg’s spectrometer are shown in Fig. 3.3.
S1
S2
Turn table q S
S3
R
Xray tube
E
Fig. 3.3 Bragg’s spectrometer The spectrometer consists of the following two parts, namely (1) A circular table, and (2) An ionisation chamber
Description Bragg's Xray spectrometer consists of a circular table on which a crystal is mounted. It is capable of rotating through any desired position by a vertical axis. The position of this circular table can be found out by using a circular scale S, attached to the table. A radial arm R, is linked with this turn table. The radial arm carries an ionisation chamber. The radial arm R is geared such that, when the turn table rotates through an angle of q, the radial arm turns through an angle of 2q. The reflected beam is collimated by a slit S3 and is collected by an ionisation chamber. Using the electrometer E, the ionisation current in the chamber is measured.
Working The collimated beam is allowed to fall on the crystal. The glancing angle (q) for the incident beam is kept very small while starting the experiment. The ionisation chamber is adjusted so as to receive the maximum intensity of the reflected beam. The glancing angle q and the intensity of the Xrays are measured. The glancing angle q is varied in steps and the corresponding values of the intensity of the reflected Xrays are noted. A graph is drawn between the glancing angle and intensity, as shown in Fig. 3.4.
62
Materials Science
A1
Intensity
A2 A3
q1
q2
q3
Glancing angle
Fig. 3.4 Glancing angle versus intensity The above graph is known as the Xray spectrum. The angles corresponding to the prominent peaks A1, A2 and A3 are taken as q1, q2, and q3, respectively. It is found that sin q1: sin q2: sin q3 = 1: 2: 3
(3.4)
This shows that the peaks A1, A2 and A3 refer to first, second and third order reflection respectively, of the same wavelength. By substituting the values of q, n, d, and l, the Bragg’s law is verified using the relation. 2dsin q = nl
(3.5)
Measurement of Wavelength of Xrays The wavelength of Xrays is determined using Eq. (3.5). The glancing angle, q, is experimentally determined from the graph. Therefore, the wavelength can be calculated by knowing d.
Calculation of d Let a be the distance between any two neighbouring atoms of the same kind and r be the density of the crystal. Therefore,
Mass of the unit cell = Volume ¥ Density
For a cubic unit cell, the volume is a3. mass = a3r
Therefore, The mass of the unit cell =
Number of atoms in a unit cell ¥ Moleculaar weight Avagadro’s constant
=
nM NA
i.e.,
ra3 =
nM NA
1/ 3
È nM ˘ Therefore, the interatomic distance a = Í ˙ Î rN A ˚
(3.6)
Characterisation of Materials
63
By knowing the molecular weight, the density and the number of atoms in the unit cell, the lattice constant of the crystal, can be calculated. For a cubic unit cell, the interplanar distance d can be calculated using the following relation, d=
a
(3.7)
h2 + k 2 + l2
where h, k and l are the Miller indices of the plane and a the interatomic distance.
3.4 DETERMINATION OF CRYSTAL STRUCTURE The crystal structure of a given specimen is determined with Xrays using the following methods: (1) Laue’s (2) Powder crystal, and (3) Rotating crystal
3.4.1
Laue’s Method
This method is used to determine the crystal orientation and to find whether the given crystal is a single crystal or a polycrystalline material. In this method, a white beam of Xrays is used, in which the different colours overlap with each other and hence, it is not possible to determine the crystal structure and cell constants of the given crystal. S1
S2
P C
Xray tube
Fig. 3.5 Laue's method The experimental arrangement for Laue’s method is shown in Fig. 3.5. A white beam of Xrays produced by a Xrays tube is collimated by thin slits S1 and S2. The collimated beam is made to fall on the given single crystal C. The crystal is rotated so that the Xrays are made incident on different planes of the crystal. The diffracted pattern is recorded on a photographic film, P. The film is exposed for several hours (nearly 5 to 6 hours) and then, it is developed. The developed film consists of a number of spots known as Laue’s spots as shown in Fig. 3.6(a). From these spots, one can identify the orientation of the crystal. Instead of spots, if circular rings are seen (Fig. 3.6(b)), then the sample is polycrystalline in nature. In Laue’s method, the reflected Xray beam is collected and studied by suitably mounting the film to record it. Figure 3.6(a) shows the Laue’s spot for a single crystal, while Fig. 3.6(b) shows the pattern for polycrystalline material. The dark spot at the centre of Fig. 3.6(a) is obtained due to the direct beam of Xrays.
64
Materials Science
(a) Laue’s spot
(b) Circular ring
Fig. 3.6 Diffraction pattern
3.4.2
Powder Crystal Method
This technique is used to find the crystal structure of powder samples when single crystals of reasonably large sizes are not available. One form of this powder crystal technique is DebyeScherrer method, which is named after its inventors. In this technique, the given sample is taken in the form of powders, either in a small capillary tube of a nonconducting material or it is just stuck on a hair by means of gum and interposed in the path of a monochromatic beam of Xrays. This technique is based on the principle of Bragg’s reflection. When a monochromatic beam of Xrays is made to fall on millions of tiny crystals having different orientations, all possible planes will be available for Bragg’s reflection.
Powder Diffractometer—DebyeScherrer Camera The schematic representation of a powder diffractometer is shown in Fig. 3.7. The monochromatic beam of Xrays emerging from a Xray tube is passed through the lead slits S1 and S2. The slits produce a fine beam of Xrays. This beam is made to fall on a thinwalled capillary tube, in which the given sample is taken in the form of powder. The photographic film is mounted in a circular frame as shown in Fig. 3.7.
Filter S1 S2
C R
Reflected ray D 2q Incident ray
Xray tube
Cylindrical camera
q q Direct ray Crystal
Photo film
Fig. 3.7 Powder diffractometer The incident Xray beams are reflected by the different crystal planes, as the powdered materials will have random orientations. The reflected rays will form a cone of Xrays with Bragg’s angle of 4q, whose axis lies along the direction of the incident beam. The exposed film is found to have concentric rings as shown in Fig. 3.8.
Characterisation of Materials
S1 S2
65
R
C
2q 2q
(a) Cone
(b) Diffraction pattern
D
(c) Film
Fig. 3.8 Diffracted cones—Powder camera method In the concentric ring, the distance D between two diffraction lines corresponding to a particular plane on the film is related to the Bragg’s angle by the equation: 4q = D/R radians
(3.8)
where R is the distance between the specimen and film, and D is the diameter of the corresponding circular diffraction lines. The values of D and R are measured. Using Eq. (3.8), the value of the Bragg’s angle q is determined. The interplanar distance d is then determined using Bragg’s equation, 2d sin q = nl. After finding the interplanar distance, the interatomic distance and the Miller indices are determined. The calculation of interatomic distance and the Miller indices for a cubic crystal is given below. For a cubic unit cell, the interplanar distance is given by a
d=
h2
+ k 2 + l2
Substituting the value of d in Bragg’s equation, we get 2a h2
+ k 2 + l2
sinq = nl
Squaring and rearranging the above equation, we get sin2 q =
n2 l 2 2 ( h + k 2 + l2 ) 4 a2
(3.9)
= K 2 ( h2 + k 2 + l2 ) 2 2 where K2 is a constant and is equal to n l . 4 a2 The constant K2 is determined by finding the values of sin2 q for all the concentric rings.
(3.10)
To find the Bragg’s angle for various rings, the values of Dl, D2,D3, etc., are determined from the film strip, as shown in Fig. 3.9. The measured values of D are recorded as shown in Table 3.1. By measuring the radius of the camera and the Bragg’s angle, the value of q is determined. After finding the Bragg’s angle for all the concentric rings, sin2 q value is determined. All the sin2 q values are individually written as a product of a constant K2 and a respective integer. The constant K2 is used to find the lattice constant a, whereas the respective integers are used to find the Miller indices of the corresponding planes.
66
Materials Science
Table 3.1 Determination of Miller Indices—Powder Crystal Method Sr. No.
Microscope reading Left
Difference D
= D/4R
sin2
sin2 = K2 (h2 + k2 + l2)
hkl
Right
D2
D1
Fig. 3.9. Diffraction film strip The cell constant a, is given by the relation a=
nl 2K
(3.11)
Advantages Following are the some of advantages of the powder crystal method: a. There is no need of single crystals because powder samples are used in this method. b. It is used to determine the Miller indices. c. The lattice parameters are accurately determined by measuring the spectrum at high angles.
Limitations The powder crystal method is not suitable for the determination of structure of crystals because of the multiplicity factor and the difficulty in indexing.
3.4.3
Neutron Diffraction
Large number of neutrons are produced during nuclear fission reactions. These neutrons are slowed down by moderators, and hence, thermal neutrons are produced. The velocity of these neutrons are not same. However, the root mean square velocity of the neutrons is used to find the energy of the neutrons. The thermal energy of the neutrons = (3/2) kBT, where kB is the Boltzmann’s constant and T the temperature of the reactor. For neutrons, we have 1 2 3 mv = kBT 2 2
Characterisation of Materials
Therefore,
v=
3kBT m
67
(3.12)
According to de Broglie equation, the wavelength of the neutron is given by l=
h h = p mv h
= m Therefore, the wavelength of neutron
l=
3kBT m
h 3kB mT
(3.13)
Substituting the values of h, kB and the mass of the neutrons (mn = 1.675 ¥ 1027 kg), in the above equation, we get 6.626 ¥ 1034
l= ie.,
l ( nm) =
3 ¥ 1.38 ¥ 1023 ¥ 1.675 ¥ 1027 ¥ T 2.516 T
in nm thickness, the electron beams with energy in the order of 50–100 keV are needed. The diffraction pattern produced by electrons is used to analyse the thin surface layers such as oxides on metals. Using Xrays, it is not possible to get such detail. But Xray diffraction gives the characteristics of either bulk or nonphase materials. The electron diffraction pattern of an amorphous thin film consists of difused rings, whereas for polycrystalline thin films, arranged spots are seen.
3.5 BRAGG’S LAW AND CRYSTAL STRUCTURES 1 The Bragg’s law is given by 2d sin q = nl. For a particular value of l and n = 1, sin q µ . For (1 0 0), d (1 1 0) and (1 1 1) planes, the above equation can be written as 1
1
:
:
d100 d110
1 = sin q1 : sin q2 : sin q3 d111
(3.14)
This ratio for a simple cubic unit cell is given as 1
:
1
d100 d110
:
1 = 1: 2 : 3 d111
For a body centred cubic unit cell 1 1 1 1 : : = 1: : 3 d100 d110 d111 2
(3.15)
68
Materials Science
and for a face centred cubic unit cell 1
:
1
:
d100 d110
1 3 = 1: 2 : d111 2
(3.16)
1 1 1 : : , one can identify whether the crystal is simple cubic, d100 d110 d111 body centred cubic or face centred cubic. Therefore, by finding the ratio
The Xrays made to incident on KC1 crystal produce diffraction patterns at 5.22°, 7.30° and 9.05°. These three Bragg’s angles correspond to the first order, second order and third order diffraction patterns. KC1 crystallises in cubic crystal structure. Therefore, for KC1 crystal sin q1: sin q2: sin q3 = sin 5.22°: sin 7.30°: sin 9.05° sin q1: sin q2: sin q3 = 0.09098: 0.127: 0.1573 = 1: 0.716: 0.5784 ª 1: i.e.,
1
:
1
:
d100 d110
1 2
:
1 3
1 = 1: 2 : 3 d111
(3.17)
This shows that KC1 crystal crystallises in simple cubic unit cell. The relation between the interplanar distance and the Miller indices is given by the following relations for cubic, tetragonal, orthorhombic and hexagonal crystal systems: Cubic
1 h2 + k 2 + l2 = d2 a2
(3.18)
Tetragonal
1 h2 + k 2 l2 = + d2 a2 c2
(3.19)
Orthorhombic
1 h2 k 2 l2 = + + d 2 a2 b2 c2
(3.20)
1 4 ( h2 + hk + k 2 ) l2 = + d2 3 a2 c2
(3.21)
Hexagonal For a cubic unit cell, one can write
2
n2 l 2 È h2 + k 2 + l2 ˘ È nl ˘ sin2 q = Í ˙ = ˙ 4 ÍÎ a2 Î 2d ˚ ˚
(3.22)
By knowing the values of q, n and l, one can determine the values of h, k, l and a. Thus, the crystal system in which a crystal crystallises can be determined.
Characterisation of Materials
69
3.6 OPTICAL AND OTHER INSTRUMENTS 3.6.1
Introduction
Some instruments like photographic camera, telescope, microscope, eyepiece, lenses, sextant, etc., are based on the principle of the properties of light like reflection, refraction, etc. They are known as optical instruments. Some other instruments, like an electron microscope, use an electron beam, which obeys the optical principles, like refraction, etc. The branch of science, which deals about the optical properties of the electrons, is known as electron optics. In this chapter, the instruments based on the principle of optics and electron optics are discussed.
3.6.2
Sextant
The diagrammatic representation of a sextant is shown in Fig. 3.10. It consists of a circular arc SS' of about 60°. The circular arc (circular scale) SS' is attached with two fixed radial arms A and B. At the centre, there is a movable arc C, known as index arm. A mirror M1 is placed at one end of the index arm. This mirror is known as index mirror. In another end, a vernier scale V is attached with the index arm. A semitransparent silvered glass M2, known as horizon glass, is fixed in the arm A. A telescope is attached with the arm B. X
M1index mirror
Y
Y
M2
T A
B C
SS
100
80 60
0 0 40 2 S¢
Fig. 3.10 Sextant The sextant is based on the principle that if the index mirror M1 is rotated through an angle of q, then the reflected ray rotates through an angle of 2 q. Since the reflected ray rotates through an angle of 2 q, the scale SS' is graduated into 120° by taking 0.5° = 1°. To measure the angle between the points Y and X, the sextant is initially fixed so the telescope receives the image of the point Y directly through the mirror M2. Then the index mirror is rotated in such a way so as to get the image of the point Y in the field of view of the telescope (T). The light ray coming from Y reaches the telescope after getting reflected by the index glass M1 followed by another reflection by the mirror M2. The two images obtained are made to lie side by side and then the vernier scale is
70
Materials Science
coincided to zero of the main scale (SS'). If it is not possible to coincide the vernier scale to zero of the main scale, note the vernier scale reading and it should be added or subtracted depending on the errors. Then the index mirror M1 is adjusted so as to get the reflected image of the point X in the field of view of the telescope. The image of X reflected by the index glass M1 and the image of Y through the horizon glass should be made to lie side by side and the position of scale is noted. From the difference between the two readings, the angle between the points X and Y is determined. A sextant is also used to measure the height of an inaccessible tower and the altitude of the sun.
Measurement of the Height of an Inaccessible Tower Let A and B be the bottom and top portions of a tower. Consider our aim is to find the distance between the points A and B using a sextant. To measure the distance between the points A and B of the tower, a base line is drawn from the tower. The direct image of A is seen through the telescope. The mirror M1 is adjusted so as to get the image of A in the telescope side by side [Fig. 3.11(a)] and the reading in the scale SS' is noted. Then the mirror M1 is rotated so as to receive the image of the top of the building or tower. The image of the top of the tower or building B and the image of the bottom level A are seen side by side [Fig. 3.11(b)] in the telescope. The reading in the scale is noted and the angle q1 through which the index arm rotated is found out. M1
A
T A M2 (a) B M1 A T A M2 (b)
Fig. 3.11 Sextant—height of a tower Now move the sextant through a distance of d meter (say 10 m) and repeat the entire experiment again. The angle q2 through which the index arm rotated is determined. Let the sextant be first positioned at C and then at D. AD AC From Fig. 3.12, cotq1 = and cotq2 = h h By measuring the distance between C and D, we get
\
cot q2  cot q1 =
AD  AC d = h h
h=
d cot q2  cot q1
The height of the building or the tower is calculated using the above equation.
Characterisation of Materials
71
B
h
q2
q1
A
C
D d
Fig. 3.12 Measurement of the height of an inaccessible tower
Measurement of the Altitude of the Sun To measure the altitude of the sun, an artificial horizon is used. A dish containing mercury is used as an artificial horizon. The telescope of the sextant is turned towards the mercury surface. One image A' of the sun from the mercury is seen through a transparent mirror M2 and another image due to the reflection from the index glass M1 and the horizon glass M2 are obtained in the field of view of the telescope (Fig. 3.13). These two images should be made to lie side by side and the reading in the scale is noted. From these readings q1 is determined. The index glass is now rotated to receive the image of the sun directly and mirror M2 reflects it. This image should lie side by side with the image of the sun in mercury as seen through the transparent mirror M2. The position of the scale is also noted. The value of q2 is determined from these readings. The angular elevation of the sun, a is determined using the relation, a = (q2  q1)/2.
Sun A q1 q2
Mercury
Sun A¢
Fig. 3.13 Measurement of the altitude of the sun
3.7 OPTICAL MICROSCOPE In a biological microscope, the transmitted light is used to view the specimen. Since the metals are opaque to light, the metallurgical microscope uses reflected light to view the specimen. The diagramatic representation of a metallurgical microscope is shown in Fig. 3.14. In a metallurgical microscope, a beam of light produced by an incandescent lamp (halogen or xenon lamp) is made to fall
72
Materials Science
on a glass plate inclined at an angle of 45°. The light reflected by the inclined glass plate is used to illuminate the object. An objective lens receives the light reflected from the object and it focuses the image at its focal point. An eyepiece receives the image and enlarges it. The enlarged image is seen through the eyepiece lens. Usually, the objective lens with different magnifications like 5 ¥, 10 ¥, 20 ¥, 50 ¥ and 100 ¥ are provided in a turret mount. The eyepiece lenses with different magnifications like 5 ¥, 10 ¥, 20 ¥, etc., are also provided. The total magnification of the microscope depends upon the product of the magnifications of the eyepiece lens and that of the objective lens. Thus, a magnification from 20 ¥ to 2000 ¥ is easily achieved using a metallurgical microscope.
Eye piece lens system
Plane glass reflector Objective lens Specimen
Fig. 3.14 Metallurgical microscope The overall magnification is approximately given by DN/F, where D is the length measured from back of objective to lower end of eyepiece, N the power of eyepiece and F the focal length of the objective lens. The resolution of image is given by c = 0.5 l (m sin a) where l is the wavelength of light used, m the refractive index between lens and specimen and a half the angle subtended by maximum cone of rays entering the objective. For l = 5000 Å, the theoretical value of the resolution cannot exceed 2000 Å. Resolution may be increased either by decreasing refractive index of the medium in between the sample and the objective lens or by increasing l. A drop of oil of high refractive index (e.g., cedar oil of m = 1.5) is placed between the objective and specimen to increase the resolution and then viewed.
3.8
FOCUSING OF ELECTRON BEAMS
An ordinary beam of light is focused with the help of lenses. Since electrons are charged particles, they cannot be focused using ordinary lenses. Focusing of parallel or diverged electron beams are achieved with the help of an electrostatic lens or an electromagnetic lens.
Characterisation of Materials
3.8.1
73
Electrostatic Lens
The first electrostatic lens was built by Bruch and Johnson in 1932. Electrostatic lens consist of two coaxial cylinders A and B maintained at different potentials as shown in Fig. 3.15. The potential difference of B is greater than that of A. If a beam of electrons is passing through axis of these coaxial cylinders, it moves normal to the equipotential surface and finally comes to focus at F. By varying the potential difference of the coaxial cylinders A and B, the electron beams are focused either near to the lens or far away from the lens. This setup acts as lens for an electron beam similar to an optical lens for visible light. In some cases, more than two coaxial cylinders are used to get good focusing of the electron beams. B A
F
A B
Fig. 3.15 Electrostatic lens
3.8.2
Electromagnetic Lens
Electromagnetic lens is based on the principle that a magnetic field produces deflection when an electron beam is obliquely passing through it. The diagrammatic representation of an electromagnetic lens is shown in Fig. 3.16. There is a small hole (separation) between the pole pieces of the magnetic lens of an electromagnet for the electrons to pass through. The pole pieces of the electromagnet consists of iron shells wounded with the coil of wire and air gaps for air circulation. If the electromagnet is switched on, the magnetic field is established in the fine perforated section. When an electron beam is passing through the magnetic field, it takes a spiral path and brings to focus just like glass lenses focuses a beam of ordinary light. P P¢
F F (b)
(a)
Fig. 3.16 Electromagnetic lens
74
Materials Science
3.9
ELECTRON MICROSCOPE
The principle of an electron microscope is similar to that of an optical microscope. An optical microscope uses optical lenses at various stages of the microscope for magnification. In an electron microscope, either an electrostatic lens or an electromagnetic lens is used at different stages of the microscope. Using an optical microscope, a magnification of about 1500 times is achieved, whereas an electron microscope magnifies the image up to 100,000 times. Since the wavelength of the electron beam is 104 to 105 times smaller than that of an ordinary light ray, greater resolution can be achieved using electron microscope. The first electron microscope was designed in the year 1932. Today, with considerable improvement in technique, the electron microscopes with a number of facilities are available in the market. Most of the instrument uses the electromagnetic lens for magnification, even though both electrostatic and electromagnetic lenses can be used for magnification. A schematic diagram of an electron microscope is shown in Fig. 3.17 with an optical microscope. In an electron microscope, E is an electron gun and it produces electron beams, whereas in an optical microscope, an incandescent lamp S is used as a source. An electron microscope is operated at very high vacuum. Hence, the apparatus is evacuated to very high vacuum using a vacuum pump P. The electromagnetic lens in the electron microscope acts as a condensing lens, similar to the lens L1 in the optical microscope. The condensed electron beam in the electron microscope is made to fall on the sample kept at O. The sample is mounted on a thin film of cellulose supported on a wiregauze. Highspeed electrons pass through the sample and the remaining are stopped by it. The electron beam passing through the specimen is magnified 100 times by the electromagnetic objective lens L2. Then, the image is made to fall on an intermediate screen S1. The electromagnetic lens L3 again magnifies the image 100 times and then the image is made to fall on a fluorescent screen S2. The lens L3 is known as the projector lens, since it projects a small portion of the first image on the screen S2. The window W can view the image
S
E L1 L1 O L2
L2 S1
S1 L3
L3
W P S2
S2 (a)
(b)
Fig. 3.17 (a) Optical microscope (b) Electron microscope
Characterisation of Materials
75
on the screen S2. The image seen through the window has a magnification of about 10,000 times. This image is further magnified 10 times with the help of an optical lens, so as to get a total magnification of 105 times. When photomicrographs are required, the viewing screen is replaced by a photographic plate. An electron microscope is very useful for research on smoke and dust particles, on pigments for paints and on diseasebearing bacteria and viruses. The surface of the crystalline materials is studied by it. Though the principle of the electron microscope is same as that of an optical microscope, it differs from the optical microscope with regard to its size, weight, appearance and cost.
3.10 SCANNING ELECTRON MICROSCOPE (SEM) Knoll invented scanning electron microscope in 1935. The schematic representation of a scanning electron microscope is shown in Fig. 3.18. It is used to produce a threedimensional image of a specimen of any size and thickness. The electrons produced by the hot filament are accelerated by electric and magnetic fields. The emerging electrons with a spot size of nearly 10 nm is made to be incident on a conducting sample under study. If the sample is nonconducting, a thin layer of 5–50 nm thick gold or any other metal coating is made and then the sample is used for study. A scanning coil deflects the electron beam, so that the sample is scanned point by point. The electrons striking on the sample produce secondary electrons. The number of secondary electrons produced depends upon the geometry and other properties of the samples. The secondary electrons are collected by a positively charged electron detector, which accelerates the electrons to very high energy in the order of 10 keV. Then, the electrons are made to strike a scintillator. The scintillator produces a large number of photons. These photons are made to fall on a photomultiplier tube. The photomultiplier tube converts the electrons into a highly amplified electric signal. This amplified electric signal is passed into a cathode ray tube, through which the image of the scanned surface is seen. Electron source Aperture Magnetic lens IS
Secondary electrons
Electron detector
Sample (10 nm spot)
Scanning coils
Ic CRT
Video amplifier
Scan generator
Fig. 3.18 Scanning electron microscope The resolution of the image is about 10–20 nm. The magnification of the microscope can be continuously varied from 15 to 105 times. The magnification depends upon the ratio of the variable current Is in the scanning coil to the current Ic in the deflection coil of the cathode ray tube.
76
Materials Science
Nowadays, due to considerable development in electron optics, the electron probes with a diameter of nearly 2.5 nm are used in scanning electron microscope. This instrument is known as Electron Probe Microanalysis (EPMA). It is used to find the chemical compositions of alloys, metals, semiconductors, etc.
3.11
TRANSMISSION ELECTRON MICROSCOPE (TEM)
Transmission Electron Microscope (TEM) is one of the modern characterisation tools used to obtain structural images of the materials. One can explore the surface nature, structure and the properties of the materials using TEM. It finds wide applications in almost all areas like chemistry, materials science, geology and biology. The basic composition of the materials can be explored with the help of detectors through the energy loss spectrum of the transmitted electrons. On the other hand, the modern TEMs are used to produce the images in the scanning range of 0.1 nm with a magnification of 50 million times. The schematic representation of the TEM is shown in Fig. 3.19. A stream of monochromatic electron beam is produced by the electron gun namely, virtual source located at the top. Two condenser lenses
Electron beam source
First condenser lens
Second condenser aperture
Second condenser lens
Objective lens Thin sample Diffracted electrons
Transmitted electrons
Objective aperture
Viewing screen photographic media
Fig. 3.19 Transmission electron microscope
Characterisation of Materials
77
are used to obtain coherent electron beam as shown in Fig. 3.19. The first lens is used to determine the spot size while the second lens is used to change the size of the spot on the sample. The electron beam is made incident on the selected points on the sample. A part of the beam is transmitted into the sample while the remaining part is being scattered. The transmitted portion is focused by the objective lens. The objective aperture enhances the contrast of the image by preventing larger diffracted electrons. Thus, the image is formed after passing through the projector lenses. The transmitted beam of electron strikes the phosphor image screen and thereby, it generates light. The obtained image consists of dark and bright patterns. The dark pattern refers to the less transmission of electron from the sample which may be due to denser or thicker nature of the sample. Similarly, the bright pattern reveals the high transmission of electron beam through the sample. A high intensity electron beam is made to be incident on the sample. The interaction of electron beam in crystalline material is based on the diffraction principle. The intensity of the diffraction pattern depends on the orientation of atomic planes in the crystal. The intensity of the transmitted beam may be altered by the volume and density of the materials through which it passes. A high contrast image is obtained by TEM only by allowing the transmitted electrons through the sample along the optic axis. The scattered electrons are deflected from the optical axis and hence, prevented from reaching the phosphor screen using the objective apertures. The scattered electrons are not taken into account during the formation of an image. In High Resolution Transmission Electron Microscopy (HRTEM), the image can be formed due to the differences in the phases of the scattered electron waves through the sample during transmission. The images obtained using HRTEM will facilitate to explore the crystal structure of the material.
Applications The applications of the TEM are given below. a. One can obtain the imaging of individual molecules (or) macromolecular assemblies. b. It is used heavily in materials, metallurgy and biological sciences. c. Computer modelling of the images is an added advantage in TEM characterisation.
Limitations Following are the limitations of TEM. a. The sample must be thin enough to characterise using TEM and hence, it requires extensive sample preparation (electron transparent). b. The structure may be changed during the process of sample preparation. c. In biological materials, the electron beam may damage the samples.
3.12 SCANNING TRANSMISSION ELECTRON MICROSCOPE (STEM) Scanning Transmission Electron Microscope (STEM) is an advanced version of Transmission Electron Microscope (TEM) used for research and development in all fields. Like other electron microscopes, the high energy electron beam is made to be incident on the sample not only at a particular point, but line by line with the help of scanning coils. The incident high energy electron beam is transmitted into the sample. The transmitted electrons are collected by number of detectors and hence, the images are formed. The scanning of electron beam across the sample provides details of the material such as mass determination and mapping.
78
Materials Science
These data are used extensively for the direct correlation of image and the structures quantitatively. In STEM, the image and the structural informations of the sample can be obtained simultaneously. It is one of the most versatile tools used for the determination and mass mapping of bimolecular structures. The schematic diagram for the STEM is shown in Fig. 3.20. The field emission gun is placed at the top of the instrument, which emits the high energetic electron beam. A fine narrow beam of electrons of size 2.5 Å diameter is obtained using an objective lens. Electron source
Objective lens
CRT Display Scanning coils Sample
Elastically scattered electrons Annular detector Central detector
Unscattered + inelastically scattered electrons
Fig. 3.20 Schematic diagram of scanning transmission electron microscope The direction of the beam of electrons can be controlled employing the scanning coils. The transmitted electrons are of three categories, namely, elastically scattered, inelastically scattered and the unscattered electrons. The various detectors which are placed in different angles below the sample, collect the above three categories of electrons. A high energetic electron beam is made to be incident on the sample and scan in a 2dimensional raster across the sample with the help of the scanning coils. During the transmission, the electron scattering has occurred both in elastically and inelastically. The scattering angle of the elastically scattered electrons is relatively low with the same scattering region of unscattered electrons. The above electrons are collected by the same central detector. However, the elastically scattered electrons are scattered over a large solid angle and these can be collected by annular detector below the sample. All the scattered electrons are collected by a variety of detectors which are placed behind the sample. The image is generated by stepbystep movement of the focused beam over the sample. Variety of signals collected simultaneously can be discriminated depending on the different scattering angle and/or energy loss. The different structural and chemical informations of the sample are obtained from the images due to the various scattered angles.
Characterisation of Materials
79
The simultaneous and controlled acquisition of information can give good quantitative analysis which cannot be obtained by other microscopes. The inelastic and unscattered electrons can be differentiated using their difference in energies with the help of magnetic prism near the central detector. During the scanning process, the analog signal from the detector is fed into the Cathode Ray Tube (CRT) for display. The magnification factor is the ratio of the raster of CRT and electron probe as given below. Magnification =
CRT raster Electron probe raster
(3.23)
Advantages Following are some of the advantages of STEM: a. High elemental mapping resolution while comparing with any other analytical techniques. b. Provides crystallographic information of even small area of the sample c. It is used to characterise the nanoparticle, agglomeration due to annealing, etc.
Limitations
Following are some of the limitations of the STEM:
a. The sample preparation is tedious as that of STEM. b. Some materials not stable to high energetic electron beam.
3.13 MICROHARDNESS (NANOHARDNESS) 3.13.1 Introduction Hardness is one of the important characteristic property of a material which enables to resist plastic deformation, penetration, indentation and scratching. The measurement of hardness of material is more essential than to select right material for engineering applications. Generally, the hardness of various materials are determined by means of using indentation hardness test. The indentation hardness test on materials gives the hardness of a material to deformation. The hardness of the materials are tested using a variety of techniques and materials namely, macrohardness testing, microhardness testing and nanoindentation testing. In this section, the microindentation principle, experimental methods of testing and applications of both micro indentations and nanoindentations are discussed in brief.
3.14 CLASSIFICATIONS OF HARDNESS TEST The hardness test on materials are classified into three categories namely macroindentation, microindentation and nanoindentation test. The classification of hardness test is shown in Fig. 3.21. The different types of macroindentation tests available for testing the materials are Vickers hardness test (HV), Brinell hardness test (HB), Knoop hardness (HK), Janka hardness test, Meyer hardness test, Rockwell hardness test (HR), Shore durometer hardness test and Brinel hardness test. In contrast to macroindentation test, there are only two tests available for microindentation test namely, Vickers hardness test and Knoop hardness test. In macroindentation hardness test, the load applied to test the material is larger
80
Materials Science
and is in the order of 1 kg or more. On the other hand, in microindentation, the load applied to test the material is very low, i.e., below 1 kg. Similarly, a new method was developed to measure the hardness of small volume sample in the year 1930 known as nanoindentation technique. The nanoindentation technique is used to obtain the hardness of small volume of materials. Hardness Test
Macroindentation Test
Microindentation Test
Nanoindentation Test
Fig. 3.21 Classification of hardness test
3.15 MICROHARDNESS TEST In microindentation test, the hardness of the materials is tested by applying a low load in the order or 1 to 1000 kg. Generally, a diamond indenter with a specific geometry is used to obtain the penetration on the surface of the test specimen. The force applied to obtain the indentation is very small, i.e., 2 N. Thus, the depth of penetration achieved in microindentation is about 50 mm. The microindentation is used to explore the relative hardness of various phases or microconstitutes which are present on the materials.
3.15.1
Vickers Hardness Test
Vickers hardness test, also known as Diamond Pyramidal Hardness (DPH) test was developed in the year 1925. The Vickers hardness test is available in two different force range namely micro (10 g to 1000 g) and macro (1 kg to 100 kg). However, in both the methods, one can use the same indenter to measure the hardness in the range HV 100 to HV 1000.
Working The required load on the Vickers hardness test is selected (10 g to 1 Kg) and then the indenter is pressed on the surface of the sample. The applied force is maintained for a particular time period known as dwell time i.e., 10 to 15 s. The indenter is resolved from the sample after the dwell time. The indenter leaves a square indent as shown in Fig. 3.22. The two diagonal length of the square indenter on the sample surface is measured using optical microscope. One can determine the Vickers microindentation of the sample by measuring the surface area of the indent using the relation. HV = or,
Load Area of the pyramidal impression HV = 1.854
F A
(3.24) (3.25)
where F is the applied load and A the area of indentations. Equation (3.25) gives the Vickers hardness of the materials.
Characterisation of Materials
81
Operating position h 136° 136°
D
Fig. 3.22 Vickers TestSquare intender
Applications The following are the applications of Vickers microindentations: a. It is used to obtain the hardness of small volume samples. b. It is used to obtain the hardness of small very thin foil. c. It is used to measure the individual microstructures. d. It is used to measure the relative hardness of different phases or microconstituents.
Advantages Following are the advantages of HV over other test methods: a. b. c. d.
It is a nondestructive method. It covers the entire hardness range. Wide range of test forces meet all applications. It is a nonindenter method and hence sample can be further used.
Limitations Following are the limitations of HV over other test methods: a. The indent size is to be measured accurately and hence, it requires highly finished test points. b. It consumes more time to complete the measurements.
3.15.2 Knoop Hardness Test The Knoop hardness test (HK) was developed in the year 1939. The force applied in HK testing is in the range of 10 to 1000 g. The Knoop test is used only for the microindentation of materials and hence, it is known as microhardness test or microindentation test. The surface of the samples is to be polished to obtain more accurate indentation. In view of the above reason, it requires high power microscope to measure the indent size. The diamond indenter is pressed into the surface of the sample after selecting the required test force. The test force is maintained constantly for a dwell period of time say 10–15 s. The indenter is removed after the dwell time. The indenter produces an elongated diamond shaped image on the surface of the sample. The size of the indenter on the surface of the sample is measured using high resolution optical microscope. One can determine the Knoop microindentation of the sample by measuring the indenter area using the relation
82
Materials Science
Operating position h w
17230° 130°
w
Fig. 3.23 Knoop test method HV = or,
Load Area of the pyramidal impression
HV =14.229
F A
(3.26) (3.27)
where F is the applied load and A is the area of the indentation. Equation (3.27) is used to obtain the Knoop microindentation of materials.
Applications The following are the applications of HK microindentations: a. It can be applied for any metallic materials. b. It is specifically designed for microindentations. c. It is mainly used for small points, thin sections, etc. d. It is used to measure individual microstructures. e. It is used to measure the depth core hardening.
Advantages Following are the advantages of Knoop microindentation test: a. The low test force and elongated indenter facilitate to explore materials features than other methods. b. It covers the entire hardness range. c. A wide range of test force to cover entire range of applications.
Limitations Following are the limitations of Knoop microindentations: a. The accurate measurement of indenting size is very difficult and requires high polished surface. b. It consumes time for measurements.
3.16 NANOINDENTER The idea of nanoindentation is realised from the indentation test on materials. The principle behind nanoindentation is that a small hard tip is used to make an indentation on the sample. The sample is very small in volume. In this method, while doing indentation on materials, the load and displacement of the indentations are recorded. The constant area and mechanical properties of the sample are obtained from the recorded load and displacement data. Nanoindentation means depth sensing indentation testing in the range
Characterisation of Materials
83
of submicrometer. This is possible only if the machines make such a tiny indentation using the applications of load and displacement with very high accuracy and precision, and the analysis of the resultant data to obtain information such as hardness, modulus and other mechanical properties. The nanoindentation method is used to obtain features across less than 100 nm on powders or thin films less than 5 nm thick etc.
Working Generally, nanoindentation is performed using the tip in AFM. The necessary load is selected based on the requirements. The nanoindentation can be made by means of using a threesided pyramid shaped diamond probe tip. The indentation can be made either by indent or scratching the sample. The indentation is achieved by using a required force to tip, while the scratch is done by dragging the AFM probe across the sample surface. One can control the force, rate, angle and length of scratch using the softwares. After doing the indentation, the image is obtained using the tapping mode of AFM. The hardness of the sample is evaluated by measuring the depth of indentations. The mechanical and physical properties of the samples are obtained from the forcedisplacement curve which is observed while doing the indentation.
Applications Following are the applications of nanoindentation: a. It is used to obtain the hardness of sample to explore the submicron size features. b. It is used to evaluate the adhesion in thin film. c. It is used to evaluate the durability of coating. d. It is used to evaluate the elastic constants of samples.
3.17 COMPARISON BETWEEN MICRO AND NANOINDENTATIONS Even though both microindentation and nanoindentation measure the hardness of materials, there are some differences and special features. A comparison between microindentation and nanoindentation is given in Table 3.2.
Table 3.2 Comparison Between Micro and NanoIndentations Sr. No.
Microindentation
Nanoindentation
1.
The required constant load is applied when the indenter is in contact with the sample.
The required constant load is applied when the indenter is in contact with the sample.
2.
After the dwell time, the indenter is resolved and the area of the indenter is measured.
When the load is applied, the depth of penetration is measured.
3.
The area is obtained by using the width of indenter after the dwell time and recovering the load.
The area is obtained using the applications of full load by measuring the depth of impression and the angle of radius of the indenter.
4.
The hardness is obtained by The hardness is obtained by obtaining the ratio of obtaining the ratio of applied load to applied load to the area. the area.
84
Materials Science
3.18 ATOMIC FORCE MICROSCOPE The Atomic Force Microscope (AFM) was developed in 1986 in order to overcome the limitations of Scanning Tunneling Microscope (STM). The AFM is used to obtain the high resolution image of the individual atom on both conducting and insulating surfaces. The principle behind the AFM technique is the interaction between a double force sensing tip known as cantilever and the sample. The cantilever which contains the tip, scans the surface of the sample in a raster pattern to obtain the image of the sample. We know that when two atoms are close to each other, the force of attraction and repulsion between the two atoms is, F=
B A R12 R6
(3.28)
where R is the distance between the atom A and B. Equation (3.28) shows that the force of attraction or repulsion between the atoms depend on the separation distance R between the two atoms. When two atoms are brought closer, the repulsive force (first term) dominates than the attractive force (second term). Thus, the tip in the cantilever experiences a repulsive force and hence, produces a small bending in the cantilever. A schematic diagram of the AFM is shown in Fig. 3.24. It consists of PZT scanner, cantilever, Laser source, position sensitive detector and sample holder. When the mounted tip in the cantilever approaches the sample surfaces, it experiences a repulsive force. The repulsive force exists between tip and the sample produces a small bending on the cantilever. A laser beam is used to monitor the displacement of the cantilever. The laser beam incident on the cantilever gets reflected. The reflected laser beam is recorded using a position sensitive photodiode. A small bending in the cantilever leads in a corresponding change in the position of the reflected laser beam. The same is recorded by the photodiode. The signal received by the detector is then send as feedback into the Piezoelectric Transducer (PZT), which helps the sample to move up and down. The movement of the sample helps to maintain a constant force
Laser
Feedback Control PSPD
Mirror Cantilever
Sample
xyz piezo x tube scanner
y x
z
Fig. 3.24 Schematic representation of atomic force microscope
Characterisation of Materials
85
between the sample and tip. Thus, by scanning the surface of the sample by raster pattern and recording the reflected laser beam using photodetector, the topographical image of the sample is obtained. The image of the sample gives the information about the surface nature and subsurface nature of the sample.
Working One can operate the AFM in three different modes namely contacting mode, noncontacting mode and tapping mode. The performance of the cantilever and the tip is used to obtain the information on the surface and subsurface information.
Contact Mode In the contact mode of operation, the tip is in contact or forced to make contact with the surface of the sample. The representation of the contact mode operation of AFM is shown in Fig. 3.25. Due to the existence of repulsive force of attraction between the tip and the sample, the tip gets repelled. This in turn results in bending of the cantilever and hence, the laser beam gets deviated from its original position. The reflected laser from the cantilever is detected by the photodiode and maps the image of the sample. In contact mode, the repulsive force is dominant since the atoms are very close. The main disadvantage of the contact mode is the damage of the tip due to close contact of the tip and sample. The resolution of the image obtained by this method is high than any other mode of operation.
sample
water droplet
Fig. 3.25 Contacting mode–AFM
Noncontact Mode In noncontact mode of operation, the tip is not in contact with the sample. However, the tip is moved at a small distance from the surface of the sample. The schematic representation of the noncontact mode of operation of AFM is shown in Fig. 3.26.
sample
water droplet
Fig. 3.26 Noncontacting mode–AFM In this mode of operation, the attractive force (second term in Eq. (3.31)) is dominant than the repulsive force since the tip is not in contact with the sample. Under this condition, the Vander Waals force of interaction is present mainly due to either permanent dipole or induced dipole or electronic polarisation between the two atoms. The image resolution in the noncontact mode of operation is less compared to contact mode of operation.
86
Materials Science
Tapping Mode The tapping mode is the combination of both contact and noncontact mode of operations of AFM. The high resolution image obtained by the contact mode of operation is higher than noncontact mode due to close contact of the tip and surface of atoms. Therefore, the resolution of tapping mode lies in between the two methods. One can achieve various kinds of microscope by changing the interaction between the tip and surface of the sample. For example, the magnetisation of the tip helps to investigate the magnetic interactions of the sample. The corresponding AFM is known as Magnetic Force Microscope (MFM). Similarly, one can also vibrate the samples in its resonance frequency by means of using an ultrasonic transducer and the corresponding AFM is known as Atomic Force Acoustic Microscopy (AFAM).
Applications Following are the applications of AFM in the field of science and technology: a. It is used to obtain the topographical images of the sample. b. It is used to obtain the growth morphology and grain size of the thin films. c. It is used to measure the physical parameters like elasticity, hardness, adhesive and surface charge densities of the samples. d. It is used to obtain the information about the dust particles in solutions. e. It is used to obtain the image of both conducting and nonconducting surfaces. f. It is used to obtain images for biological systems like amino acid, organic monolayer.
Table 3.3 Difference Among these Diffraction Techniques Sr. No.
Xray diffraction
Electron diffraction
Neutron Diffraction
1.
Monochromatic Xray beam is used to obtain the Xray diffraction pattern. It is used to obtain the characteristics of bulk materials. It fails to provide information like surface analysis of thin film or layers of oxide metals.
Fast moving electrons are used to obtain the cluster diffraction patterns. It is used to analyse the thin surface such as oxides on metals. It is obtained using transmission electron microscope.
Monochromatic beam of neutron is used to obtain the neutron diffraction pattern. It is used to study the magnetic structure, i.e., orientations of spins in an atom. Neutron scattering will be taken by nuclei of an atom only when the elements have magnetic moments. It is possible to determine the position of oxygen in Pb and hence it produces the complete structure. It cannot be recorded on film like Xray and electron diffraction. The sample region requires special care like high vacuum.
2.
3.
4.
5. 6.
7.
8.
It is not possible to determine Electron incident on the the position of oxygen in Pb metal, gets scattered being a heavy atom. and hence, produce the diffraction pattern. It can be recorded on film or It can be recorded on photographic plate. film. The sample region can be A high vacuum in the kept under normal conditions. sample region is required It is not suitable for metals. to obtain the diffraction patterns. It is available commonly due Limitation due to to simple experimental setup. sophistication and high cost. It is used to obtain the lattice constant and hence, the structure of the materials.

Due to the limitation in the availability of neutron beam, it cannot be used commonly. It is used to locate the lighter elements like hydrogen, in the presence of heavy elements.
Characterisation of Materials
87
3.19 ELECTRON DIFFRACTION According to de Broglie, the electrons behave as wave. Therefore, the wavelength of the matter wave is, l=
h mv
(3.29)
where h is the Planck’s constant and mv is the momentum of the electron. The wave nature of electron is experimentally verified by Davisson and Germer. The wavelength of the electron is expressed in terms of kinetic energy as h
l=
2 Em
(3.30)
In terms of the accelerating potential, the wavelength can be written as l=
Therefore, the wavelength of the electrons l =
h 2emV 1.227 V
(3.31)
where l is obtained in nanometres, if V is expressed in volts. In Eq. (3.31), if V = 150 V, the wavelength of the electrons is 1 Å. The wavelength of the electrons is in the order of Angstroms as it behaves as waves. Therefore, it can be used for crystallographic analysis by producing diffraction patterns. The electron diffraction pattern is taken using a transmission electron microscope. An electron microscope is similar to an optical microscope. In optical microscopes, lenses made up of glass are used to converge or magnify images, whereas in electron microscopes, either electromagnetic lenses or electrostatic lenses are used to converge or magnify the images. EIectron microscopes can be operated both in the diffraction mode and the imaging mode. There is a considerable difference between electron diffraction and Xray diffraction. In fact, the atoms scatter the electrons more strongly by several powers of ten for the energies involved. Therefore, for normal incidence, the electrons can penetrate up to a distance of 500 Å, and for oblique incidence, the electrons can penetrate up to 50 Å. To penetrate through a specimen of 100 nm thickness, electron beams with an energy in the order of 50–100 keV are needed. The diffraction pattern produced by electrons is used to analyse the thin surface layers such as oxides on metals. Using Xrays, it is not possible to get such detail. But Xray diffraction gives the characteristics of a bulk material. The electron diffraction pattern of an amorphous thin film consists of diffused rings, whereas for polycrystalline thin films, arranged spots are seen.
88
Materials Science
Key Points to Remember There are two types of Xrays known as soft and hard Xrays. When a beam of cathode rays strike a solid target, it produces invisible and penetrable radiations known as Xrays or Xradiations. The penetration power of soft Xrays are low while it is high for hard Xrays. Bragg’s law for diffraction is 2d sin q = nl where l is the wavelength of light, d he interplaner distance, n the order of the spectrum, and q the glancing angle. The different methods used to determine the crystal structure using Xrays are Laue’s powder crystal and rotating crystal method. The cell constant for a given crystal is equal to a = nl/2k where k is a constant, l the wavelength of incident light and n the order of the spectrum. The rotation (oscillation) method is used for the glacial determination of lactice constant. The de Brogile wavelength of matter waves is l = h/mv, where h is Planck's constant, m the mass of electrons and v the velocity of electrons. The wavelength of electron is equal to 1.227 / V , where V is the applied potential. The wavelength of neutron is equal to 2.516 / T where T is the temperature. The metallurgical microscope is based on the priniciples of reflections of light, while the biological microscope is based on the principles of transmission of light. Electrostatic and electromagnetic lenses are used to focus the electron beams in microscope. Electron microscope is different from optical microscope in terms of size, weight, appearance and cost. Electron Probe Microscope Analysis (EPMA) is used to find the chemical composition of alloys, metals and semiconductors. Transmission Electron Microscope (TEM) is one of the modern characterisation tool used to obtain the information such as surface nature, structural and properties of materials. In TEM, the contrast image is obtained by allowing the transmitted electrons through the sample along the optic axis. In High Resolution Transmission Electrons Microscope (HRTEM), the image is obtained due to the difference in the phases of the scattered electron waves through the sample. STEM is used to determine and mass mapping of biomolecular structures. In STEM, there are three types of transmitted electron namely, electrically scattered, inelastically scattered and unscattered electrons. Hardness is one of the important characteristic property of materials which enables to resist plastic deformation, penetration, indentation and scratching. The hardness test is classified into three types, namely macroindentations, microindentation and nanoindenation test. The load applied in microhardness test is in the order of 1 to 100 kg. A square indent is obtained in Vickers Hardness Test. The time of force which is maintained on the indenter is known as dwell time. The Vickers hardness is equal to HV = 1.854(F/A). Vickers hardness is a nondestructive method. The force applied in Knoop hardness test is 10 to 100 g. The equation to measure the knoop indention is equal to 14.229 (F/A). Nano indention is used to test the small load and displacement with high accuracy and precision.
Characterisation of Materials
89
Solved Problems Example 3.1 Find the shortest wavelength of Xrays produced by an Xray tube operated at 10 kV, and hence, calculate the frequency of the Xray beam emitted? Given h = 6.626 ¥ 1034 J s, e = 1.6 ¥ 1019 C, c = 3 ¥ 108 m s1. Given Data: Planck’s constant h = 6.626 ¥ 1034 J s Charge of the electron e = 1.6 ¥ 1019 C Velocity of light c = 3 ¥ 108 m s1 Potential difference applied V = 10 kV = 10 ¥ 103 V Solution:
(i)
The wavelength of Xrays emitted lmin = =
hc eV 12, 400 ∞ 12, 400 ∞ A= A 10 ¥ 103 V
= 1.24 A∞ (ii) The frequency of the Xray beam emitted v= =
c l 3 ¥ 108 = 2.419 ¥ 1018 Hz. 1.24 ¥ 1010
Therefore, the frequency of the Xray emitted from tube is 2.4 ¥ 1018 Hz. Example 3.2 An Xray tube operates at a potential difference of 10 kV and the current passing through it is 2 mA. Calculate (i) the number of electrons striking the target per second and the speed at which they strike, and (ii) the shortest wavelength of Xrays coming from the tube. Given Data: The potential difference applied V = 10 kV = 10 ¥ 103 V
Solution:
Current
I = 2 mA = 2 ¥ 103 A
(i)
I=
We know that, Current
Charge Q ne = = Time t t
I t 2 ¥ 10 3 ¥ 1 = = 1.25 ¥ 1016 e 1.6 ¥ 10 19 The number of electrons striking the target per second = 1.25 ¥ 1016. Therefore,
(ii) The velocity of electron n =
n=
2eV m
90
Materials Science
=
2 ¥ 1.6 ¥ 1019 ¥ 10 ¥ 103 9.1 ¥ 1031
= 5.92999 ¥ 107 m s1 . (iii)
The wavelength of the Xrays lmin = =
hc 12, 400 = Å eV V 12, 400 = 1.24 Å. 10 ¥ 103
The number of electrons striking the target per second = 1.25 ¥ 1016 The velocity of the electron = 5.93 ¥ 107 m s1 The wavelength of the Xrays = 1.24 Å. Example 3.3 GaAs has its principal planes separated at 5.6534 Å. The first order Bragg’s reflection is located at 13°40¢. Calculate (i) the wavelength of the Xrays, and (ii) the angle for the order Bragg’s reflection. Given Data: Interplanar spacing d = 5.6534 Å = 5.6534 ¥ 1010 m Glancing angle
q1 = 13°40¢
Order of diffraction n = 1 Solution:
(i)
According to the Bragg’s law 2d sinq1 = nl l=
2d sin q1 2 ¥ 5.6534 ¥ 1010 ¥ sin 13∞40 = n 1
= 2.671 ¥ 1010 m. (ii)
For secondorder diffraction, n=2 Therefore, sin q2 =
nl 2d
È nl ˘ q2 = sin1 Í ˙ Î 2d ˚ È 2 ¥ 2.671 ¥ 1010 ˘ = sin1 Í ˙ = 28∞11⬘38.54⬙ ◊ Î 2 ¥ 5.6534 ¥ 1010 ˚ The wavelength of the Xrays l = 2.67 ¥ 1010 m The second order Bragg reflection occurs at q2 = 28°11¢38.54≤.
Characterisation of Materials
91
Example 3.4 An Xray tube operates at a potential difference of 24,800 V and has a copper target. The first order glancing angle for NaCl crystal for Ka line at l = 1.54 Å is 15.8°. Calculate (i) the grating spacing for NaCl crystal and (ii) the glancing angle for minimum wavelength of the continuous spectrum. Given Data: Potential difference applied V = 24,800 V Order of diffraction n = 1 The wavelength of Xray beam l = 1.54 Å = 1.54 ¥ 1010 m Glancing angle q = 15.8° Solution:
(i)
According the Bragg’s law 2d sin q = n l or,
d=
=
nl 2 sin q 1 ¥ 1.54 ¥ 1010 2 ¥ sin 15.8∞
= 2.827968 ¥ 1010 m. (ii)
Minimum wavelength of Xrays emitted l min = =
hc eV
12, 400 12, 400 = = 0.5 Å. V 24, 800
Let the glancing angle for minimum wavelength is q. Then, 2d sin q = nl È nl ˘ q = sin1 Í ˙ Î 2d ˚ È 1 ¥ 0.5 ¥ 1010 ˘ = sin1 Í ˙ = 5∞4⬘18⬙ Î 2 ¥ 2.828 ¥ 1010 ˚ The grating spacing for NaCl crystal = 2.828 ¥ 1010 m The glancing angle for minimum wavelength = 5°4¢18≤. Example 3.5 The Ka line from molybdenum has a wavelength of 0.7078 Å. Calculate the wavelength of the Ka line of cadmium. (Atomic number of molybdenum = 42, atomic number of cadmium = 48.
92
Materials Science
Given Data: The wavelength of Ka
l
line from molybdenum l = 0.7078 Å
The atomic number of molybdenum ZMo = 42 The atomic number of cadmium ZCd = 48 Solution:
The Moseley’s law is n = a ( Z  b ) For K series, b = 1 For cadmium, the Moseley’s law can be written as c = a2 ( 48  1)2 lCd
(i)
Similarly, for molybdenum, the Moseley’s law can be written as c lMo
= a2 ( 42  1)2
(ii)
Dividing Eq. (i) by Eq. (ii), we get lCd a2 ( 41)2 = lMo a2 ( 47)2 lCd = lMo ¥
412 472
= 0.7078 ¥ 1010 ¥
412 472
= 0.55386 Å The wavelength of cadmium Ka radiation = 0.5386 Å. Example 3.6 Show that the energy of a neutron of wavelength 1 Å is 0.08 eV. Given Data: The wavelength of neutron l = 1 Å Solution:
We know that the energy of thermal neutron E=
h2 2ml 2
Substituting the values of h, m and l in the above equation, we get 2 6.626 ¥ 1034 ) ( E= 2 2 ¥ 1.675 ¥ 1023 ¥ (1 ¥ 1010 )
Characterisation of Materials
93
= 1.3106 ¥ 1020 or,
=
1.3106 ¥ 1020 1.602 ¥ 1019
= 0.081eV Therefore, the energy of thermal neutron with wavelength 1 Å is 0.08 eV. Example 3.7 Find the decrement of wavelength of the thermal neutron when the temperature is doubled. Given Data: The temperature of thermal neutron T2 = 2T1 Solution:
The wavelength of thermal neutron l(nm) =
2.516 T
Let l1 and l2 be the wavelength of thermal neutron respectively at temperatures T1 and T2. Therefore, l1 =
2.516 T1
and 2.516
l2 =
T2
Substituting the value T2 in above equation, we get 2.516
l2 =
2T1
Simplifying the above equation, we get =
1 2
l1
= 0.707l1 Therefore, the temperature of the thermal neutron is doubled when the wave length of the neutron is decreased by 0.707.
94
Materials Science
Example 3.8 Find the temperature of the thermal neutron when the wavelength is 1 Å. Given Data: The wavelength of neutron l = 1 Å Solution:
The wavelength of thermal neutron l( nm) =
2.516 T
Rearranging the above equation, we get T=
(2.516)2 l2
.
Substituting the value of l in above equation, we get T=
(2.516)2 0.01
= 633 K The temperature of thermal neutron corresponded to 1 Å is 633 K.
ObjectiveType Questions 3.1. 3.2. 3.3. 3.4. 3.5. 3.6. 3.7. 3.8. 3.9.
3.10.
Xrays are discovered by _______. The wavelength of Xrays ranges from _______ to _______. The intensity of Xrays depends on the number of _______ striking the target material. The penetrating powers of soft Xrays are _______. _______ Xrays have high penetrating power. The penetrating power of Xrays depend upon the potential difference applied between the filament and anode. True/False The wavelength of Xrays is _______ times shorter than ordering light. The spacing between the atoms in the crystals and the wavelength of Xrays are in the same order. True/False Bragg's law for diffraction is (a) 2d sin q = l (b) 2d sin q = n (c) 4d sin q = l (d) 2d sin q = nl The interatomic distance is equal to Ê nM ˆ (a) a = Á Ë r N A ˜¯ Ê nM ˆ (c) a = Á Ë r N ˜¯
3
1/ 3
Ê nM ˆ (b) a = Á Ë r N A ˜¯ Ê rM ˆ (d) a = Á Ë nN ˜¯
2/3
1/ 3
Characterisation of Materials
3.11. The interplaner distance in crystal is given by a (a) d = (b) d = h+k +l (c) d = 3.12. 3.13. 3.14. 3.15. 3.16. 3.17. 3.18. 3.19. 3.20. 3.21. 3.22.
a h2
+ k2
+ l2
(d) d =
a /2 h2 + k 2 + l2 2a h2
+ k 2 + l2
Xrays are monochromatic beam. True/False The rotation method is not suitable for quick determination of lattice constant. True/False. The best method for structure determination and indexing is _______ method. Neutrons are produced during _______. The wavelength of neutrons at temperature T is equal to l = _______. The wavelength of neutron at 373 K is equal to _______ Å. The neutrons are scattered by the nuclear of an atom when the elements are having magnetic moments. True/False. The penetration power of electrons for normal incidence is _______ Å. _______ Å is penetrating power for an electron under oblique incidence. The structure of KC1 crystals is _______ crystal structure. The relationship between interplaner distance and the miller indices for cubic crystal structure is _______ (a)
1 h2 + k 2 + l2 = d a
(b)
1 h+k +l = d a
(c)
1 h2 + k 2 + l2 = d2 a2
(d)
1 h+k +l = d2 a2
3.23. For an orthochromatic structure, the interplaner distance and the miller indices are related as (a)
1 h2 k 2 l2 = + + d a2 b2 c2
(b)
1 h k l = + + d a b c
(c)
1 h2 k 2 l2 = + + d2 a b2 c2
(d)
1 h k l = + + d 2 a2 b2 c2
3.24. In hexagonal system, the interplaner distance and Millar indices are related as
3.25. 3.26. 3.27. 3.28.
95
(a)
1 4 ( h2 + hk + k 2 ) l2 = + d2 3 a2 c
(b)
1 4 ( h + hk + k 2 ) l2 = + d2 3 a c
(c)
1 4 ( h2 + h + k 2 ) l2 = + d 3 a2 c2
(d)
1 3 ( h2 + hk + k 2 ) l2 = + d2 7 a2 c2
The The The The
wavelength of electrons for an applied voltage of 150 V is equal to _______ Å. transmitted light used to view the specimen is _______ microscope. reflected light used to view the specimen is _______ microscope. magnification of metallurgical microscope is equal to
(a)
DN F
(c) DN
(b)
DN F2
(d) DNF
96
Materials Science
3.29. The resolution of the image in a metallurgical microscope is 0.5 l 0.5l 2 (a) (b) m sin a m sin a
3.30. 3.31. 3.32.
3.33. 3.34. 3.35. 3.36. 3.37. 3.38. 3.39. 3.40. 3.41.
0.5 m sin a
0.5l sin a Electron beams are focused using _______ or _______ lenses. Wavelength of electron beam is smaller than ordinary light. True/False. The electron microscope is not different from optical microscope in terms of (a) Size (b) Weight (c) Principle (d) Cost Acronym for SEM _______. In SEM, the energy fo the accelerated electrons is in the order of _______. The chemical composition of alloys and metals are analysed using _______. Acronym for EPMA is _______. Acronym for TEM is _______. HRTEM is used to explore _______ of material. Expand DRTEM is _______. Acronym for STEM is _______. Acronym for AFM is _______. (c)
(d)
Answers 3.1. 3.3. 3.5. 3.7. 3.9. 3.11. 3.13. 3.15. 3.17. 3.19. 3.21. 3.23. 3.25. 3.27. 3.29. 3.31. 3.33. 3.35. 3.37. 3.39.
Roentgen Electrons Hard 1000 (d) (c) False Nuclear fission 1.3 500 Cubic (b) 1 metallurgical (b) True Scanning Electron Microscope Electron Probe Microscope Transmission Electron Microscope High Resolution Transmission Electron Microscope 3.41. Atomic Force Microscope
3.2. 3.4. 3.6. 3.8. 3.10. 3.12. 3.14. 3.16. 3.18. 3.20. 3.22. 3.24. 3.26. 3.28. 3.30. 3.32. 3.34. 3.36. 3.38. 3.40.
0.5, 10A∞ Low True True (a) True Oscillation 2516/ T True 50 (c) (d) biological (a) electrostatic or electromagnetic (c) 10 ke V Electron Probe Microanalysis Crystal structure Scanning Transmission Electron Microscope
Characterisation of Materials
Short Questions 3.1. 3.2. 3.3. 3.4. 3.5. 3.6. 3.7. 3.8. 3.9. 3.10. 3.11. 3.12. 3.13. 3.14. 3.15. 3.16. 3.17. 3.18. 3.19. 3.20. 3.21. 3.22. 3.23. 3.24. 3.25. 3.26. 3.27. 3.28. 3.29. 3.30. 3.31. 3.32. 3.33. 3.34. 3.35. 3.36. 3.37. 3.38.
What are Xrays? How are Xrays produced? What are the advantages of Coolidge tube apparatus over the other apparatus? Write the expression for the wavelength of the continuous Xrays and explain the terms. State Bragg’s law. What is the basic principle of Xray spectrometer? Mention the advantages and drawbacks of powder diffraction method. What are the advantages and drawbacks of rotation crystal method? List out the advantages of neutron diffraction method. What is a sextant? What are the uses of a sextant? Explain how the altitude of the sun is measured using a sextant. Explain how the height of a tower is measured using a sextant. What is an optical microscope? What is a metallurgical microscope? What is the difference between an optical microscope and a metallurgical microscope? What is an electron microscope? What are the uses of an electron microscope? What is a scanning electron microscope? What is the principle behind transmission electron microscope? Explain the principle of scanning transmission electron microscope. Compare the merits and demerits of SEM and STEM. What is meant by hardness test? What are the different methods of hardness testing? Expand HV, HB, HK and HR. What is meant by macroindentation? Explain microindentation. What is meant by nanoindentation? Explain the principle behind the macromicro and nanoindentation. What is the difference between micro and nanoindentation? What is the level of force required in Vickers hardness indentation testing? Mention few applications of Vickers microindentation. What is meant by dwell time? What is the difference between Vickers and Knoop microindentation? What are the applications of Knoop indentation? Mention the drawbacks of Knoop indentation. Explain the principle behind the nanoindentation. Mention the applications of nanoindentation.
97
98
Materials Science
Descriptive Questions 3.1. What are Xrays? Describe an experimental method used to produce Xrays? 3.2. What is meant by diffraction of Xrays? Explain an experimental method used to study the diffraction of Xrays. 3.3. Describe the construction and working of Bragg’s Xray spectrometer with a neat sketch. 3.4. Describe the working of a powder diffraction camera and hence, explain how lattice parameters are determined using powder diffractogram? 3.5. Describe the construction and working of a rotation camera and hence, explain how lattice parameters are determined using oscillation photographs? 3.6. (a) Explain how the electron diffraction is used to determine the crystal structure. (b) Explain the merits and demerits of neutron diffraction. 3.7. Explain with neat sketch, the construction and working of a sextant. Explain how is a sextant used to find the height of a tower and the altitude of the sun. 3.8. Explain the construction and working of a metallurgical microscope. 3.9. Explain with neat sketch, the construction and working of an electron microscope. 3.10. Explain with neat sketch the construction and working of a scanning electron microscope. 3.11. Explain with a neat sketch, the working of TEM with STEM. Mention their applications and limitations. 3.12. Describe with neat sketch the measurements of macro hardness using Vickers hardness and Knoop methods. 3.13. Explain with neat sketch the working of nanoindentation. 3.14. Compare the merits and demerits of microindentation and nanoindentation. 3.15. Write short note on (a) Vickers macro hardness testing (b) Knoop macro hardness testing, and (c) Nanoindentation
Chapter
4
COHESION BETWEEN ATOMS
OBJECTIVES To understand the crystalline and amorphous solids. To study the nature of bonding in solids. To understand the principle, bond formation and properties of primary bonds namely, ionic, covalent and metallic bonds. To understand the principle, bond formation and properties of secondary bonds namely, Van der Waals and hydrogen bonds.
4.1 INTRODUCTION The evaluation of nature of bonding between atoms helps to understand the physicochemical and mechanical properties of materials. Atoms are the building blocks of all types of matter. Generally, atoms of all elements have the ability to interact with the other atoms to form more complex structures. The distance between two atoms and the type of nature of atoms determines the type of bonding and amount of interactions. Atoms link to other atoms through chemical bonds resulting from strong attractive forces which exist between the atoms. In solids, the atoms and molecules are electrostatic in nature due to the strong mutual force of attraction resulting in the change in arrangement of electrons. Thus, rearrangement of electrons takes place until a stable configuration is formed which results in the formation of different types of bonds. In this chapter, brief discussions about the different types of bonds along with suitable illustrations are given.
4.2 CLASSIFICATION OF SOLIDS Based on the structural arrangement of atoms and molecules, solids are classified into two categories namely, crystalline and amorphous solids.
100
Materials Science
4.2.1
Crystalline Solids
The substances whose elements are arranged in a definite orderly arrangement (regular and periodic manner) are known as crystalline solids. The solid substances which exist naturally are in the crystalline form. Examples of crystalline solids are sodium chloride, sulphur and diamond. The crystalline solids posses characteristic geometric shapes and the constituent particles in the crystals which are usually held by strong interatomic, interionic or intermolecular forces. Crystalline solids have sharp melting points, indicating the existence of a long range order arrangement of atoms or molecules or ions. The long range order is due to the regular arrangement of the constituents molecules or atoms or ions throughout the threedimensional network.
4.2.2
Amorphous Solids
The substances whose constituents are arranged in an irregular manner are known as amorphous solids. They are also known as pseudo solids and differ from the crystalline solids in many aspects. Examples of amorphous solids are glass, rubber, fused silica, plastics, etc. The amorphous solid does not occur in characteristic geometric shapes. The mechanical, electrical and optical properties of the crystal do not depend upon the direction along which they are measured. Therefore, it is known as isotropic crystals. Amorphous solids do not have sharp melting points like crystalline solids. On the other hand, they have some orderly arrangement but it is not extended to more than a few angstrom units. Thus, an amorphous solid does not have any orderly arrangement and hence, will have only short range arrangements of atoms or molecules. The amorphous solids begin to flow like liquids during heating. When cut or hammered they break in an irregular manner. In crystalline solids, bonds are stronger due to the existence of long range order, while in noncrystalline solids, the strength of the bonds varies due to the lack of long range order. One can classify the solid based on the nature of binding forces holding the constituent atoms or molecules. The nature and origin of chemical bonds are most important, since the basis of chemical reactions is the forming and breaking of bonds, and the changes in bonding forces. The chemical bond forms when electrons from different atoms interact with each other. The classification of solids based on the binding force and their characteristic properties are given in Table 4.1.
Table 4.1 Sr. No.
Nature of bonding
Crystalline Solids, Binding Force and their Characteristic Properties Nature of forces
Electrical property
Mechanical property
Example
1.
Molecular
Nondirectional, secondary valence, (Van der Waals) weak
Insulators
Soft, plastic
Solid Ar, Kr Xe, etc.
2.
Metallic
Nondirectional electrostatic (metallic) medium
Good conductors
Soft, malleable and ductile
Al, Cu, Ag, Zn, etc.
Cohesion Between Atoms
101
4.3 BONDING IN SOLIDS In solids, the bonding of atoms or ions is mainly due to the existence of bonding forces. There are two types of forces namely attractive force (Fa) and repulsive force (Fr). When the two atoms are separated by a larger distance, the force that exists between the atoms is known as attractive force, i.e., negative force. Therefore, the atoms come closer to form bonds. On the other hand, when the atoms are closer, a repulsive force (i.e., positive) dominates and hence, the atoms move apart. The attractive and repulsive forces balance each other and the net forces become zero at a particular distance. Under this equilibrium condition, the distance between the two bonding atoms is known as bond lengths.
ao o
x
Ftotal
Energy
Interatomic force
Fa
ao o
x
Em Fr
(a) Attractive, repulsive and total forces
(b) ao and Em at zero resultant force
Fig. 4.1 Solid – Interatomic forces The interatomic forces which are present in a solid are shown in Fig. 4.1. At equilibrium position, the atoms vibrate due to the existence of thermal energy. When the bondings are formed at ao, the energy of the atom is lowered by a value of Em known as binding energy. The minimum energy required to break a bond is known as binding energy. Generally, the binding energy of solids depends on the type of bonding and it ranges from 0.02 eV to 10 eV. An increase in equilibrium spacing ao, results a decrease in Em as shown in Fig. 4.1. As a result, a free movement of atoms takes place and hence, the change of phase from solid, liquid and gas occurs.
4.4 CLASSIFICATION OF BONDS The nature of chemical bonds is classified as primary and secondary bonds based on bond strength and directionality. The interatomic bonds are known as primary bonds, whereas the intermolecular bonds are known as secondary bonds. The attractive forces in primary bonds are directly associated with the valence electrons. The electrons in the outermost orbit are in a state of high energy and are relatively unstable. The primary bonds are formed by borrowing, lending or sharing the valence electrons. Secondary bonds are significantly weaker than primary bonds.
102
Materials Science
The bond strength is determined using the cohesive energy. It is defined as the energy which is required to separate the atoms or ions in the solid into neutral free atoms or ions. The cohesive energy depends on the type of bonding prevailing in the solids. The cohesive energy of selected elements along with their bonding type is given in Table 4.2.
Table 4.2 Cohesive Energy of Selected Elements at 0 K at 1 atm Sr. No.
Bonding Type
Material
Cohesive energy (kJ mol1)
Bond length (1010 m)
1.
Ionic
LiF
430
2.11
2.
Ionic
NaCl
315
2.79
3.
Ionic
KBr
300
3.29
4.
Covalent
Carbon
711.00
1.54
5.
Covalent
Silicon
446.00
2.34
6.
Covalent
Germanium
372.00
2.44
7.
Metallic
Lithium
158.00
3.04
8.
Metallic
Sodium
107.00
3.72
9.
Metallic
Potassium
90.1
4.54
10.
Metallic
Magnesium
145
3.20
11.
Van der Waals Argon
12. 13.
7.74
3.76
Van der Waals Krypton
11.20
4.04
Hydrogen
20.5
1.97
Water
Let us now discuss the various types of primary bonds which occur in molecules and solids.
4.4.1
Primary Bonds
The primary bonds are further classified into three types namely, ionic, covalent and metallic. The ionic bonds are formed between a metal and a nonmetal (e.g., NaCl). The bond which is formed between nonmetals, i.e., molecules (e.g., CO2) is known as covalent bond. Similarly, the metallic bonds are formed between the atoms of metallic elements (e.g., bronzes). In addition, there are also bonds which are not pure ionic, covalent, etc., but have some partial character of different bonds and are known as mixed bonds. The primary bonds are stronger in nature with higher energy in the range from 1 to 5 eV.
Ionic Bonding An ionic bond or electrovalent bond is a type of chemical bond which is formed between atoms of any two different types of ions i.e., very often between the metal and nonmetal ions through electrostatic interactions. In short, it is a bond formed by the attraction between the electropositive metal and electronegative metal. The transfer of electrons from one atom to the other atom results in stable outer shells. The attractive bonding forces are columbic, i.e., positive and negative ions by virtue of their net electrical charge. The number of positive and negative charges is equal in ionic bonded materials. This type of bond is mainly formed in inorganic compounds like NaCl, KOH, MgO, MgCl2, etc.
Cohesion Between Atoms
103
The Coulomb interaction energy responsible for the bonding is U=
e2 4peo R
(4.1)
where e is the charge of the electron, eo the permittivity of free space and R is the distance between the oppositely charged ions. The cohesive energy of NaCl per molecule is 7.9 eV.
Na (2, 8, 1)
Cl (2, 8, 1) (a) Ionic bonding
Cl–
Na+
Cl–
Columbic Na+ bonding force
Cl–
Na+
Cl–
Na+
Cl–
Na+
Cl–
Na+
Cl–
Na+
Cl–
Na+
Cl–
Na+
Cl–
}
Na+
(b) Electrostatic interaction
Fig. 4.2 Ionic bonding  Sodium Chloride (NaCl) In case of NaCl, there are more electrons around Cl forming Cl and fewer electrons around Na forming Na+. The transfer of one valence electron from its outermost shell of sodium atom to the chlorine atom which has seven electrons in the outermost shell results in the formation of stable electronic configuration (Fig. 4.2(a)). After the exchange of valence electrons, all sodium atoms exist as positive ions and chlorine atoms exist as negative ions. The ionic bond formation in NaCl is illustrated schematically in Fig. 4.2. The energy required to remove an electron from a metal atom like sodium is known as energy of ionisation. The energy required for sodium is 5.1 eV per atom. Similarly, the electron affinity of chlorine is 3.8 eV per atom. Following are the properties of the ionic bonds: (1) (2) (3) (4) (5) (6)
It is easy to describe and visualise. It exists in compounds which are composed of metallic and nonmetallic elements. It is termed as nondirectional, i.e., the magnitude of the bond is equal in all directions around an ion. Ionic bonds are the strongest bonds. Ionic solids possess crystalline structure. Ionic materials are characteristically hard and brittle and furthermore, electrically and thermally insulative. (7) Polar liquid like water is a good solvent for ionic crystals.
104
Materials Science
Covalent Bonding Covalent chemical bonding is formed between the two atoms by sharing a pair of valence electrons between like atoms rather then electron transfer. Therefore, it is known as homopolar or homonuclear bonding. Generally, covalent bonds are existing in all organic compounds and semiconductors. Let us consider some examples of molecules with the existence of covalent bonding. Hydrogen gas forms the simplest covalent bond in the diatomic hydrogen molecule. In H2 molecule, hydrogen atomic number is 1 and it has its one electron in 1s shell. The hydrogen atom is more stable if there are two electrons in 1s shell. When two hydrogen atoms come very close to each other, their 1s shells overlap, to form a molecule by sharing their valence electron as shown in Fig. 4.3. H
H
1s
1s
(a) Hydrogen atom
(b) Hydrogen molecule – Electron sharing
Fig. 4.3 Covalent bond  Hydrogen molecule Similarly, the existence of covalent bond between the atoms of carbon and hydrogen in case of methane (CH4) molecules is shown in Fig. 4.4. H
Hydrogen nucleus H
C
H
Carbon nucleus Shared electron from hydrogen Shared electron from carbon
H
Fig. 4.4 Covalent bonding  Methane
Cohesion Between Atoms
105
The methane molecule has one carbon atom and four hydrogen atom. The four valence electrons available in carbon atom is shared with one valence electron in 1s shell. The sharing of four additional electrons from each hydrogen atom gives four covalent bonds as shown in Fig. 4.4. This results in the formation of methane structure. In case of elemental semiconductor Si (Z = 14), it has four free electrons (3s23p2) in the outermost shell. In order to complete the structure, Si requires four electrons. The required four electrons are shared with the nearest neighbours. Thus, by sharing the four electrons from the nearest atom, it completes four covalent bonds and hence, the structure becomes stable. The sharing of electron pairs between the atoms and the formation of covalent bonds is shown in Fig. 4.5.
Si e–
Fig. 4.5 Covalent bond  Silicon Examples of molecules with covalent bonds are diamond, germanium, silicon, silver, nitrogen, oxygen, etc. The values of bond length and energies of the covalent materials are given in Table 4.3.
Table 4.3 Values of Bond Length and Bond Energy of Materials Sr. No.
Bond
Bond Bond Energy Length (nm) (kJ mol1)
1.
H–H
0.07414
435
2.
O–O
0.12074
220
3.
P–P
0.18931
212
4.
Cl – Cl
0.19879
243
5.
C–C
0.12425
370
6.
Si – Si
0.2246
173
7.
Ge – Ge
0.2403
154
8.
C∫C
0.120
890
9.
C=C
0.133
680
10.
C–H
0.110
435
11.
C – Cl
0.180
340
12.
O – Si
0.160
375
106
Materials Science
The properties of covalent bonds are as follows. (1) Covalent bond is directional. (2) Covalent bonding can be either very strong or very weak bonds, depending upon the atoms involved in the bond. (3) Covalent solids generally leads to low melting and boiling points compared to ionic solids, e.g., CCl4 melting point is 296 K. (4) Nonpolar liquids like CCl4, benzene are good solvents for covalent molecules. (5) Covalent solids are hard, brittle and possess crystalline nature. (6) Different physical properties of the solid material are due to their bonding type. Because of the nature of ionic and covalent bonds, the materials produced by those bonds tend to have quite different macroscopic properties. The atoms of covalent materials are bound tightly to each other in stable molecules, but those molecules are generally not very strongly attracted to other molecules in the material. On the other hand, the atoms (ions) in ionic material show strong attractions to other ions in their vicinity.
Metallic Bonding Metallic bonding is the last of primary bonding type. It is existing both in metals and their alloys. In metals, the metal atoms lose their outer electrons to form metal cations. The electrons from all the metal atoms form an electron sea or cloud which can flow throughout the space occupied by the atoms. These electrons are often described as delocalised electrons. Metallic bonding is different from both ionic and covalent bonding. The metal cations and electrons are oppositely charged, and hence, they are attracted by each other. The electrostatic forces are called metallic bonds. When the variable number of electrons is shared by variable number of atoms, the formation of metallic bond takes place. The nucleus of the crystals constitutes the ion core, while the electrons produce a space charge around the ion as shown in Fig. 4.6.
+
+
+
+ Ion cores
+
+
+
+
+
+
+
+ Clouds of valence elctron
+
+
+
+
Fig. 4.6 Metallic bonding  illustration Consider sodium as an example, which has the electronic structure of 1s22s22p63s1. When sodium atoms come together, the outer most valence electron in the 3s atomic orbital of sodium atom shares the space with the corresponding electron on a neighbouring atom to form a molecular orbital. Each sodium atom is being touched by eight other sodium atoms and the sharing occurs between the central atom and the 3s orbitals in all the eight atoms. All 3s orbital in all atoms overlap to give a vast number of molecular orbitals which extend over the whole piece of metal. The electrons can move freely within
Cohesion Between Atoms
107
these molecular orbitals. Therefore, each electron is separated from its parent atom. The electrons are said to be delocalised. The metal is held together by strong forces of attraction between the positive nuclei and the delocalised electrons. The properties of metallic bonds are as follows. (1) The metallic bond is nondirectional in character. (2) Metallic bonds are good conductors, forming electron cloud and having high melting point and low ionisation energies. (3) Metallic crystals are ductile and strong due to the ability of the bond electrons to make and break bonds readily. (4) They have characteristic properties such as bright luster, high electrical and thermal conductivity, malleability, ductility and high tensile strength. (5) Metals tend to have high melting points and boiling points suggesting strong bonds between the atoms.
4.4.2
Secondary Bonds
Secondary bonds are much weaker than primary bonds. Secondary bonds exist virtually between all atoms or molecules, but its presence may be reduced if any of the three primary bonding types are present. They often provide a weak link for deformation or fracture. The interatomic distance is larger i.e., 2 – 5 Å and hence, the strength of secondary bonds is in the range of 0.02 – 0.5 eV. Examples of secondary bonds are Hydrogen and Van der Waals bond.
Hydrogen Bonding Hydrogen bond is formed when a charged part of a molecule having polar covalent bonds forms an electrostatic interaction with a substance of opposite charge. Molecules which are having non  polar covalent bonds do not form hydrogen bonds. Hydrogen bonds are common in covalently bonded molecules which contain hydrogen, such as water (H2O). It is primarily a covalent bond, the electrons are shared between the hydrogen and oxygen atoms. However, the electrons tend to spend more time around the oxygen atom. This leads to a small positive charge around the hydrogen atoms, and a negative charge around the oxygen atom. Figure 4.7 shows the schematic illustration of hydrogen bonding. When molecules
+ –
+ –
–+ + –
+ –
Fig. 4.7 Hydrogen bonding  Water
108
Materials Science
of the same type of charge transfer are nearby, the negatively charged end of one molecule will be weakly attracted to the positively charged end of the other molecules. The attraction is weak because the charge transfer is small. Therefore, they have enough strength to exist in liquid and gaseous states. Hydrogen bond is also known as hydrogen bridge and is found in molecules of ammonia, nitric oxide and CH4. The energy of a hydrogen bond (typically 5 to 30 kJ mole1) is comparable to that of weak covalent bonds (155 kJ mole1). A typical covalent bond is only 20 times stronger than an intermolecular hydrogen bond. These bonds can occur between molecules or within different parts of a single molecule. The hydrogen bond lies in between a covalent bond and an electrostatic intermolecular attraction. The properties of the hydrogen bonds are as follows. (1) (2) (3) (4) (5)
Hydrogen Hydrogen Hydrogen Hydrogen Hydrogen
bonds are directional and have low melting point. bonded solids do not have any valence electrons and hence, they are solid insulators. bonds are stronger than dispersion bonds but are weaker than primary bonds. bonded solids may be crystalline or noncrystalline. bonded solids are soluble both in polar and nonpolar solvents.
Van der Waals Bond The dipole bond is known as secondary bond. The energy of the dipole bonds is very less than any other bonds. Consider two atoms of an inert gas having completed electronic shells. When the atoms are at neutral, the positive and negative charge centers are exactly at the same location as shown in Fig. 4.8(a). When the two atoms are brought closer together, a displacement of positive and negative charge centers takes place relatively. Then, the positive and negative charges are separated as shown in Fig. 4.8(b). As a result, it creates an electric dipole and hence, results in fluctuating dipole mode. The fluctuating dipole bonds are known as Van der Waals bonds.
±
+
±
–
(a) Single atom
+
–
(b) Induced dipoles
Fig. 4.8 Bonds – induced dipole The applied electric field causes an induced dipole moment between the neighbouring atoms. The fluctuating dipole moment and induced dipole moment interacts to form a weak bond. Therefore, the cohesive energy due to the dipole – dipole interaction is ÈÊ s ˆ U = 4 e ÍÁ ˜ ÍÎË R ¯
12
Ês ˆ  Á ˜ Ë R¯
6˘
˙ ˙˚
(4.2)
Cohesion Between Atoms
109
where R is the distance between the dipoles, e and s are characteristics constants. The first and second term in the above equation represents repulsive and attractive potentials, respectively. Eq. (4.2) gives the value of Lennard  Jones potential. In the case of CH4 molecules, no additional bond is formed with neighbouring CH4 molecules. However, the binding forces from fluctuation dipole interaction results in the formation of bonding known as Van der Waals force. The properties of the Van der Waals bonds are as follows. (1) It is a very weak bond compared to other bonds. (2) It is nondirectional. (3) The binding energy of the molecular crystal is very small and hence, it has low melting and boiling points. (4) Organic compounds like He, Ne, etc., are inert and poor in electrical conductivity. The comparison of various classifications of bonds and their properties are given in Table 4.4.
Table 4.4 Comparison of Various Types of Bonds Sr. No.
Properties
Ionic Bonds Electrostatic force between positive and negative ions
Covalent Bonds
Metallic Bonds
Van der Waals Bond
1.
Bonding force
Mutual sharing of valence electrons between atoms
Electrostatic force between negative electron cloud and positive ions
Electrostatic force due to oscillating dipoles
2.
Character of Nondirectional bond
Directional
Nondirectional
Directional for dipole and hydrogen bonds. Nondirectional for dispersion bonds
3.
Bond formation condition
For elements having small number of valence electrons
Molecules forming dipoles
4.
Bond energy 150 – 370 kcal/mol 125 – 300 kcal/mol 25 – 200 kcal/mol >n), Eq. (5.1) can be written as, Ê E ˆ n = N exp Á v ˜ Ë kT ¯
(5.2)
When Ev = 1eV and T = 300 K, then the value of n/N = 1.64 ¥ 1017. Consider that there is 1028 atoms m3 in a crystal. Therefore, the number of lattice vacancy is in the order of 1011 m3.
5.3.2
Substitutional Defect
A substitutional defect is produced when an atom is replaced by different types of atom. Consider a lattice arrangement of a pure metallic crystal as shown in Fig. 5.3. A pure crystalline metal may have defects
116
Materials Science
such as impurity atoms, absence of a matrix atom and/or the presence of impurity atom in a wrong place. An impurity that occupies a normal lattice site is known as a substitutional impurity atom. In Fig. 5.3(b), a regular lattice site is occupied by an impurity atom. The defect in which an impurity atom occupies a normal lattice site is known as a substitutional defect. The addition of impurity having larger or smaller size compared to that of the host atom produces or disturbes lattice and are shown in Fig. 5.3.
(a)
(b)
Fig. 5.3 Substitutional defect produced due to the doping of impurities. Doping of (a) a big size atom produces lattice disturbances, and (b) a small size atom produces lattice disturbances
5.3.3
Interstitial Defect
The small size impurity atoms doped to a crystal may occupy an intermediate position in the parent crystal without dislodging the parent atoms from their sites and is known as interstitial defect. An impurity atom can enter the interstitial position or void only when it is smaller in size when compared to the parent atoms. The addition of carbon in iron produces, interstitial impurity defect. The interstitial defect is shown in Fig. 5.4. The FCC form of iron has octahedral and tetrahedral voids of radii 0.414 r and 0.225 r, respectively, where r is the radius of the parent FCC atoms. The radius of the FCC iron is 1.29 Å and hence, the radius of void is 0.414 ¥ 1.29 Å = 0.53 Å, whereas the carbon atom present in the covalent bond of a graphite is 0.71 Å. The radius of carbon atom is small compared to the parent FCC iron atom and hence interstitial defect is produced. As the radius of carbon atom is greater than that of void, there are strains around the voids. The solubility of carbon in FCC iron is limited to 2 %.
Fig. 5.4 Interstitial defect
5.3.4
Schottky Defect
The missing of a pair of one anion and one cation from an ionic crystal is known as Schottky defect. The Schottky defect is shown in Fig. 5.5. In pure alkali halides, the most common defects are Schottky
Crystal Imperfections
117
defect. As the ionic crystals require charge neutrality, the existence of positive ion vacancy creates the negative ion vacancy also. The number of Schottky defects present in binary ionic crystals such as NaCl and MgO at ordinary temperature is Ê ES ˆ n = N exp Á Ë 2kBT ˜¯
(5.3)
where N is the total number of cationanion pairs, E S is the average energy required to produce a Schottky defect and n the number of Schottky defects.
Schottky defect
Absence of anion and cation
Fig. 5.5 Schottky defect
5.3.5
Frenkel Defect
In nonmetallic crystals such as ionic crystal, when an ion leaves its position and occupies an interstice position, then it is said to be Frenkel defect and is shown in Fig. 5.6. In ionic crystal, the cation size is smaller than the void space. Therefore, a cation may get displaced from its position to an intermediate position. The anions do not get displaced like cations, since the size of the anion is larger than that of the void space. In order to maintain charge neutrality in ionic crystals, a cation vacancy must have associated with it either a cation interstitial or an anion vacancy.
Frenkel defects
Cation occupies void
Fig. 5.6 Frenkel defect In pure silver halide, the most commonly existing defects are Frenkel defects. The number of Frenkel defect in an ionic crystal is Ê Ef ˆ n = NNi exp Á Ë 2kBT ˜¯
(5.4)
where Ef is the average energy required to displace a cation from its normal lattice position to an interstitial, Ni the number of interstitial sites and N the total number of cations.
118
Materials Science
5.4
LINE IMPERFECTION
Consider a crystal in which an extra line of atoms is introduced from the upper portion of the crystal and this line of atoms terminates at the middle of the crystal. This type of imperfection along a line of the crystal is known as line imperfection, i.e., in crystalline solids, the defects which produce distortions centered around a line is known as a line imperfection. A line defect occurs only in one dimension and it measures only up to a few atomic distances at right angles to their length. There is only one type of line defect, namely, dislocation. The term, dislocation means any general discontinuity in crystal, and by convention, it is used to denote only the line imperfection. The reasons for producing dislocations are thermal stresses, crystal growth, phase transformation and segregation of solute atoms causing mismatches. The dislocations are responsible for the useful property of ductility of metals, ceramics and polymers. There are two types of line imperfection namely, edge dislocation and screw dislocation.
5.4.1
Edge Dislocation
The defect produced in a perfect crystal by inserting a half plane of atoms between the regular planes is known as edge dislocation. Figure 5.7 shows that an extra layer of atom is inserted from the upper portion of the crystal. This defect is known as an edge dislocation. When an extra layer of atoms is inserted from the upper portion of the crystal, it is represented by the letter, ^ (inverted Tee). On the other hand, when an additional layer of atoms is inserted from the bottom of the crystal, the edge dislocation produced is represented by the letter, T (Tee). The vertical line of the symbol ^ points in the direction of dislocation line. The application of shear stress from the upper portion of the crystal in one direction and in the opposite direction from the bottom portion moves the lattice along a plane known as slip plane. The atoms lying in the upper portions are compressed, whereas the atoms which are lying in the lower portions exhibit tension. Therefore, in an edge dislocation compressive stress, tensile stress and shear stress are acting around the dislocation region.
Edge disloction line
Fig. 5.7 Line defectsedge dislocation
Crystal Imperfections
5.4.2
119
Burger Vector
A dislocation is characterised by considering an atomic circuit around the dislocation region. This atomic circuit is known as Burger circuit. The Burger circuit for a perfect crystal is shown in Fig. 5.8(a). The Burger circuit is drawn by making x number of steps in the upward direction (in Fig. 5.8(a), x = 6) from the starting point P. This is followed by y number of steps (in Fig. 5.8(a), y = 5) to the right in the horizontal direction. Then it is processed with x steps (6 steps) towards the downward direction and finally y steps (5 steps) to the left in the horizontal direction. Finally, the starting point P is reached. The closed circuit drawn is known as Burger circuit. If one draws a Burger circuit for a crystal having edge dislocation as discussed above, one can reach the point Q, to reach the point P. This closure failure in the circuit is known as Burger vector and it is represented as b . In the case of edge dislocation, Burger vector is perpendicular to dislocation. Let n be the unit vector along the edge dislocation, then b.n = 0. The magnitude the Burger vector gives the measure of dislocation.
b Q P
P (a) Perfect crystal
(b) Crystal with edge dislocation
Fig. 5.8 Edge dislocationBurger vector
5.4.3
Screw Dislocation
The defect produced by displacement of atoms in two separate perpendicular planes is known as screw dislocation. A screw dislocation can be explained by cutting a part of a perfect crystal and then skewing the crystal through one atom spacing. It is observed that the effect on the crystal appears as a screw or a helical surface or it resembles a spiral staircase. The screw dislocation marks the boundary between slipped and unslipped parts of a crystal. The axis of helical surface is known as the dislocation line. The circular arrow j is the symbol used to represent screw dislocation. In Fig. 5.9, the upper part of crystal is slightly displaced in the direction parallel to dislocation line AB. The Burger vector b = EF is parallel to dislocation line. In some crystals, the edge and screw dislocations may occur simultaneously. Such a crystal is said to possess mixed dislocations. In Fig. 5.11, both screw and edge dislocations are shown and the dotted line represents the dislocation line. For screw dislocation, Burger vector is parallel to the dislocation lines, i.e., if n is the unit vector along the dislocation line, then b.n = 1. The circular arrows j j and i j are used to represent the Burger vector and dislocation line, respectively when they are in the same direction or in the opposite direction.
120
Materials Science
A D B C
Dislocation line
Fig. 5.9 Screw dislocation
Dislocation line A
B
Atoms in the upper portion
Atoms in the lower portion D
C
Fig. 5.10 Screw dislocation  viewed from upper portion
Dislocation line
Fig. 5.11 Mixed dislocation
Crystal Imperfections
121
5.5 DISLOCATION CLIMB The movement of dislocation in a direction perpendicular to slip plane is known as dislocation climb. Consider a crystal consisting of edge dislocation as shown in Fig. 5.12(a). The numbers 1, 2, 3, and 4 represent the positions of atoms present in the extra layer of atom. Consider that the crystal also possesses a lattice vacancy. The atom 1 is generally loosely bound and has a tendency to move towards the vacancy. Consider that atom 1 moves towards the vacant site and hence, occupies that site. Thus, atom 1 position is occupied by the vacancy. This results in the movement of dislocation through one atomic distance. The length of dislocation plane is reduced from 1234 to 123. It means that the dislocation plane is pushed up by one atomic distance. The upward movement of dislocation plane through one atomic distance is known as positive direction of climb. Similarly, downward movement of dislocation plane through one atomic distance is known as negative direction of climb. When a dislocation moves from one slip plane to another, it creates a step called Jog in dislocation line. 4 3 2 1
(a) Before dislocation climb 3 2 1
(b) After dislocation climb
Fig. 5.12 Dislocation climbs
5.6 MULTIPLICATION OF DISLOCATIONFRANK READ GENERATOR Multiplication of dislocation represents the process by which many dislocations are produced one after the other automatically. Several mechanisms are proposed about the multiplication of dislocations. Let us discuss the most common mechanism known as FrankRead source (generator).
122
Materials Science
(a)
(b)
(d)
(c)
(e)
Fig. 5.13 Multiplication of dislocations  FrankRead Generator The sequence of events in which the dislocation multiplies is shown in Fig. 5.13. The dislocation line OO’ in a slip plane (Fig. 5.13(a)) is anchored at both ends. Figure 5.13(b) shows that the dislocation line OO’ is bowed outwards due to the application of shear stress. Due to continuous growth of dislocation line, it starts to sweep around fixed end as a semicircular arc (Fig. 5.13(c)). The dislocation line spirals about the points OO’. The further growth of dislocation line brings two sections of spirals together (Fig. 5.13(d)). The growth of dislocations again causes the dislocation line OO’ to join together (Fig. 5.13(e)) and a new dislocation line OO’ is produced. Thus, the process of dislocation continues and starts a new cycle. The differences between the edge and screw dislocations are given in Table 5.2 for comparision.
Table 5.2 Differences Between Edge and Screw Dislocations Sr. No.
Edge dislocation
Screw dislocation
1.
It is produced when there is a slight mismatch in It is produced during crystallisation, the orientation of adjacent part of growing crystal. when there is a twist in stacking sequence of atoms.
2.
The region of disturbances extends along an edge of the lattice.
3.
Burger vector is perpendicular to edge dislocation. Burger vector is parallel.
4.
It has shear, tensile and compressive stresses.
Only shear stress exists.
5.
It can glide or slip in a direction perpendicular to its length.
It can move by slip.
6.
It has an incomplete plane which lies above or below the slip plane.
It has lattice planes which spirals around the lattice planes like a lefthand or righthand screw.
5.7
The region of disturbances extends in two separate planes which are perpendicular to each other.
SURFACE DEFECT OR PLANAR DEFECT
The defect formed due to the change in the stacking of atomic planes on or across a boundary is known as surface defect. This defect is a twodimensional one. There are three different types of surface defects namely, grain boundaries, twin boundaries and stacking fault.
Crystal Imperfections
5.7.1
123
Grain Boundaries
A polycrystalline material consists of a number of small sized crystals. They are said to be grains. A grain is a portion of material within which the arrangement of atoms is identical. The line separating each and every grain is said to be grain boundary. Growing of a flawless crystal is very difficult. Growing a crystal using melt (liquid) growth technique requires special skill and scientific knowledge. When a melt is cooled to grow into a crystal, it will take a week or more than a week to solidify. The growth of a crystal takes place from a tiny portion of the crystal known as nuclei. The size of the nuclei is nearly in the order of 50 to 100 atoms. The various stages of crystal growth are shown in Fig. 5.14.
Liquid
(a) Nucleation
(b) Growth
(c) Solidified Polycrystalline Material
Fig. 5.14 Growth of crystal Whenever a crystal is grown, the atoms diffuse into the nuclei and hence, the size of the nuclei increases. This process is known as nucleation. A fully grown polycrystalline material consists of a number of grains as shown in Fig. 5.14(c). These materials have defects such as void, broken bond, selfinterstitial atom and foreign impurities due to the separation of each and every grain by a region. This type of defect is due to grain boundary imperfection. A grain boundary is the surface which separates individual grains and is a narrow zone in which the atoms are not properly spaced. The grain boundary imperfection is shown in Fig. 5.15. Foreign impurity Selfinterstitial type atom Void, Vacancy Strained bond
Grain boundary
Broken bond (Dangling bond)
Fig. 5.15 Grain boundary imperfection in polycrystalline material
Small Angle Grain Boundary The small angle grain boundary is produced by an array of dislocation, causing an angular mismatch q between the lattices on either side of boundary. The angle of dislocation for small angle grain boundary is less
124
Materials Science
than 10∞. There are two types of small angle grain boundaries namely, tilt boundary and twist boundary. The tilt boundary is produced by edge dislocation, whereas the twist boundary is produced by screw dislocation. q
q 2
Fig. 5.16 Tilt boundary The tilt boundary is defined as a boundary between two adjacent perfect regions in the same crystal which are slightly tilted with respect to each other. Usually, this defect is accompanied with edge dislocation and is shown in Fig. 5.16. It is observed from Fig. 5.16 that there is a tilting in the upper and lower portion of crystal due to the presence of edge dislocation and hence, it is said to be tilt boundary.
5.7.2
Twin Boundaries
Twinning is one of a plastic deformation which takes place along two planes due to the application of a set of forces on a given metal piece. The arrangement of atoms before twinning is as shown in Fig. 5.17. After twinning, the arrangement of atoms is shown in Fig. 5.18. The deformation is produced at the planes AB and CD. The other portions on either side of AB and CD are not disturbed. Therefore, the crystal is distorted along a plane. The mirror image of one undistorted portion looks like the other one. The mirror plane is called as the twin boundary. Twin boundary is formed during the crystal growth or it may be the result of dislocation caused by an applied stress. Twin boundary is also produced during recrystallisation (mechanical working) or as a result of annealing after plastic deformation. Therefore, the twin boundaries are classified into two types namely, mechanical twins (deformation twins) and annealing twins. The mechanical twin is produced by mechanical deformation, i.e., due to the movement of specific dislocations. These are produced in bcc and hcp metals. The twinning produced due to annealing of cold work metal is known as annealing twins. These are produced in certain fcc metals such as Cu, Ag, etc. Twinning occurs in certain specific planes and directions. They are called twin planes and twin directions. The common twin planes in bcc (such as alpha iron), fcc (Cu, Ag) and hcp (Zn, Mg) metals are (112), (111) and (1012), respectively.
Crystal Imperfections
125
Fig. 5.17 Before twinning – arrangement of atoms Distorted region
Perfect region
Perfect region
Fig. 5.18 Twin boundaries Twinning becomes more significant in the case of HCP metals at room temperature. It reorients the crystal region between the twin planes and helps in changing the shape of the surface. Twinning occurs suddenly and is accompanied by sound.
5.7.3
Stacking Faults
Most of the metals crystallise either in FCC or HCP structures. The cubic closed packed structure is formed whenever a crystal is built by a stacking sequence of ABCABCABC… and so on. A stacking fault occurs, if the sequence goes wrong. For example, in series ABCABCBCABC…, layer A is missing (Fig. 5.19(a))
126
Materials Science
or an extra layer A is inserted as in the series ABCABCABACABC…as shown in Fig. 5.19(b). In some crystals, the stacking faults extend through the entire crystals and in some crystals they occupy only a part of the plane. In a hcp unit cell, the stacking sequence is ABABAB… It will also have the stacking fault, if an extra layer C is introduced or can be substituted for a layer of type B. When an additional layer is inserted between the two opposite dislocation, the stacking fault is said to be extrinsic. On the other hand, if an atomic layer is withdrawn then the stacking fault is said to be intrinsic. A B C A B A C
A B C B C A B C (a) In the regular stacking sequence, the layer A is absent at the shaded region
A B C (b) An extra layer of atom A is inserted at the shaded portion
A
A B C A B
B C A B
A C A B C
C A B C
(c) The stacking fault is produced by inserting a layer A at the shaded portion and it terminates within the crystal
Fig. 5.19 Stacking faults
5.8
VOLUME DEFECT OR BULK DEFECT
The presence of large vacancies or voids such as inclusions of foreign particles, missing cluster of atoms and formation of noncrystalline regions for at least a few angstroms is known as volume defect. The volumes defect such as crack arises either during the growth of crystal or while using the crystal. During the growth of a crystal, the crack arises due to a small electrostatic dissimilarity between the stacking sequences in metal. The crack is generated in a crystal when it is used for device application
Crystal Imperfections
127
because of thermal vibrations produced. The volume defects are studied with the help of an optical microscope.
5.9 DEFORMATION IN METALS The above discussion reveals the imperfections in crystals. Similarly, the knowledge on the defects produced in metals is equally important. Let us discuss the defects produced in metals in the following sections. Generally, in metals, the various operations such as rolling, drawing, forging, spinning etc. produce defects. During these operations, there is a change in the shape of metals. The changes in shape produced in metals under the action of a single force or a set of forces is known as deformation or mechanical deformation. There are two types of deformations namely, elastic deformation and plastic deformation.
5.9.1
Elastic Deformation
In certain metals, the application of stress within its elastic limit produces some changes in the shape of metal. The metal regains its original shape immediately after the removal of stress. This deformation is known as elastic deformation. Consider the front face [(100) plane] of fcc lattice of a metal as
(a) Tensile strength
(b) Tensile strength deformations
(c) Compressive stresses
(d) Compressive stresses deformation
Fig. 5.20 Elastic deformation
128
Materials Science
shown in Fig. 5.20. The applications of compressive and tensile stress to the metals are shown in Fig. 5.20(a) and (c). The deformations produced by these two stresses are shown in Fig. 5.20(b) and (d).
5.9.2
Plastic Deformation
The plastic deformation is the permanent deformation produced in metals. When a metal is subjected to a stress beyond its elastic limit, there is a change in the shape of metal. Thus, the metal is not able to regain its original shape even after the removal of stress. This type of deformation is known as plastic deformation. The plastic deformation in crystalline materials occurs at temperature lower than 0.4Tm, where Tm is the melting point of metal. There are two types of plastic deformation namely, slip or glide and twinning. The slip occurs in metals at ambient and at elevated temperatures. The deformation process changes to twinning at low temperatures.
Slip The deformation produced in metals or crystals due to the application of a shear stress is known as slip. The atoms move through many atomic distances relative to their original positions. Consider the arrangement of atoms in a crystal as shown in Fig. 5.21. Consider that a shearing stress is applied in the upper part of the crystal. There will be a displacement in the upper two layers over a distance of one atomic distance due to the application of stress. The slip occurs when the shearing stress exceeds a critical value. The atoms displace along a plane. The plane in which gliding of atoms takes place is known as slip plane. Due to the slip process, a step in atomic arrangement is produced. A careful examination of the slip shows the presence of a group of parallel lines. These lines correspond to the step on the surfaces. These lines are called as slip line. The direction in which slip takes place is known as slip direction. Generally, atomic density of slip plane is high and hence slip direction is in closedpacked direction within the slip plane. The slip plane and slip directions are together known as slip system. The resistance for slip is very low since the slip plane has the greatest atomic density. Slip planes Step Slip line (a) Before slip
(b) After slip
Fig. 5.21 Slip The slip direction and slip plane in fcc metals such as aluminium, copper, silver, nickel etc., are and (111), respectively. The slip occurs in bcc metals such as alpha iron on the planes such as (110), (112) and (123), while the slip direction is always (111) direction. In hcp metals such as cadmium, magnesium and cobalt, the slip occurs at the basal plane and the slip direction is diagonal axes . However, zirconium and titanium have low c/a values and hence, the slip occurs at the prismatic (101 0) and pyramidal (1011) planes in the directions. The bcc, fcc and hcp metals have 48, 12, and 3 slip systems, respectively. However, the slip direction remains the same but there is a change in slip plane due to change in temperature.
Crystal Imperfections
129
Key Points to Remember Different classifications of imperfections are point, line, surface and volume imperfections. In crystal, the imperfect point like region is known as point imperfections. The point defects are further classified as vacancy, substitutional, interstitial, Frankel and Schottky defects. The missing of an atom from the atomic site of a crystal is known as vacancy. The substitutional defect arises due to the replacement of an atom by different types of atom. The doped impurity atom occupies an intermediate position in the parent crystal without dislodging the parent atoms known as intersititial defect. Schottky defect is defined as the missing of a pair of one anion and one cation from an ionic crystal. Line imperfection is the defect produced in crystalline solids due to the distortions centered about a line. Edge dislocation is the defect produced in a perfect crystal by inserting a half plane of atoms between the regular planes. The effect produced by the displacement of atoms in two separate perpendicular planes is known as screen dislocation. The movement of dislocation in a directions perpendicular to the slip plane is known as dislocation climbs. Multiplication dislocation is the process by which many dislocations are produced one after the other automatically. FrankRead source, i.e., generator is one of the mechanism used to produce multiple dislocations. The defect formed due to the change in the stacking of atomic planes on or across a boundary is known as surface defects. Surface defects are of three types namely, grain boundaries, twin boundaries and stacking fault. The process of diffusion of atoms into the nuclei and hence the increase in size of the nuclei is known as nucleation. Grain boundary surface defects are the surface that separates the individual grains and is a narrow zone in which the atoms are not properly placed. The stacking fault arises due to the coring sequence of the stacking sequence of structures. Volume defects arise due to the large vacancies or voids, missing of a cluster of atoms and the formation of noncrystalline region in the order of few angstroms are known as volume defect. Deformations in metals are two types namely, elastic and plastic deformations. The regaining of its original shape of the materials immediately after removal of strain is known as elastic deformations. In plastic deformations, beyond elastic limit, the material does not regain its shape after removal of stress. The deformations obtained in metals due to the applications of shear stress are known as slip.
130
Materials Science
Solved Problems Example 5.1 A small angle grain boundary is tilted 0.75∞ in fcc copper. Calculate the average distance between the dislocations. Given Data: Angle of tilting, q = 0.75∞. Solution:
Copper is an fcc metal. The Burger vector in fcc Cu is (110). The interatomic distance of copper is 3.615 Å. Therefore, the length of the Burger vector is, a
d110 =
=
3.615 ¥ 1010
h2 + k 2 + l2
1+1+ 0
= 2.557 ¥ 1010 m.
The angle of the grains is tilted by Burger vector. Therefore, the angle of tilt tan
2.557 ¥ 1010 q b = = 2 D D
Rearranging the above equation, we get b D= tan
q 2
=
2.557 ¥ 1010 = 3.9 ¥ 108 m. tan 0.375o
The average distance between the dislocations is 0.039 Å. Example 5.2 Suppose the lattice parameter of CsCl is 4.0185 Å and the density is 4.285 gm3. Calculate the number of Schottky defects per unit cell. Given Data: Lattice parameter = 4.0185 Å Density = 4285 kg m3. Solution:
Number of atoms per unit cell =
Density ¥ Volume ¥ Avogadro ’snumber Molecular weight 3
=
4285 ¥ ( 4.0185 ¥ 1010 ) ¥ 6.022 ¥ 1026
(132.9 + 35.5)
= 0.99435 Cesium chloride is a special type of cubic crystal. It consists of one atom per unit cell. The difference must be the presence of Schottky defects. Schottky defects =
1  0.99435 ¥ 100 = 0.565%. 1
The number of Schottky defects per unit cell = 0.00565 or 0.565%.
Crystal Imperfections
131
ObjectiveType Questions 5.1. In solids, the presence of dislocations produces a change in _______ properties. 5.2. The mechanical properties are _______ sensitive. 5.3. The point defects are not introduced by the following methods: (a) Movement of atoms due to gain in energy (b) During processing of materials (c) Removing the impurities (d) Introduction of impurities 5.4. In point defect, the energy for the formation of vacancy is less than _______ eV. 5.5. The vacancy concentration in a metal is (a)
n Ê E ˆ = exp Á  v ˜ Ë kT ¯ N n
(b)
n ÊE ˆ = exp Á v ˜ Ë kT ¯ N n
(c)
n Ê E2 ˆ = exp Á  v ˜ Ë kT ¯ N n
(d)
n Ê E ˆ = exp Á  v ˜ Ë 2kT 2 ¯ N n
5.6. The radius of fcc iron is ________ A° 5.7. The radius of wide in fcc iron is ________. 5.8. The Schottky defects present in binary ionic crystal is Ê E ˆ (a) N exp Á v ˜ Ë kT ¯
Ê Es ˆ (b) N exp Á Ë 2 K BT ˜¯
Ê Es ˆ (c) N exp  Á Ë 2 K BT ˜¯
Ê Es ˆ (d) N exp  Á Ë 2 K BT ˜¯
5.9. The number of Frenkel defect in an ionic crystal is (a)
Ê E f ˆ NNi exp Á Ë RBT ˜¯
(b)
Ê Ef ˆ N1 Ni exp Á Ë 2 RBT ˜¯
(c)
Ê  E6 ˆ NNi exp Á Ë 2 RBT ˜¯
(d)
Ê Ef ˆ NNi exp Á Ë 2 K BT ˜¯
5.10. The line defects occur only in _____ dimension. 5.11. In edge dislocation, one of the following is not in the dislocation region. (a) Compressive stress (b) Tensile stress (c) Longitudinal stress (d) Shear stress 5.12. A boundary between slipped and unslipped parts of the crystal is made ________ dislocation. 5.13. The change in the stanching of atomic planes on or across a boundry is known as ______. 5.14. The small sized crystals in polycrystalline materials are known as ________. 5.15. The small angle grain boundary, the angle of dislocation is less than _________. 5.16. The tilt boundary dislocation is accompanied along with _______ dislocating. 5.17. In volume defect, the crack is generated in a crystal due to the _______ vibrations produced. 5.18. When the metal regains its original shape after removal of stress, then the type of deformation is known as ______ deformation.
132
Materials Science
5.19. The deformation, during which the metal is not able to regains its original shape even after removal of the stress is known as _________ deformation. 5.20. The number of slip for a bcc crystal is ________. 5.21. The two different types of twins are _________ and _______ twins. Answers 5.1. 5.6. 5.11. 5.16. 5.21.
Mechanical 5.2. 1.29 5.7. (c) 5.12. Edge 5.17. Mechanical unending
Structure 0.53 A∞ Screw Thermal
5.3. 5.8. 5.13. 5.18.
(c) (c) Surface defects Elastic
5.4. 5.9. 5.14. 5.19.
1 (d) Grains Plastic
5.5. 5.10. 5.15. 5.20.
(a) One Po’ 48
Short Questions 5.1. 5.2. 5.3. 5.4. 5.5. 5.6. 5.7. 5.8. 5.9. 5.10. 5.11. 5.12. 5.13. 5.14. 5.15. 5.16. 5.17. 5.18. 5.19. 5.20. 5.21. 5.22. 5.23. 5.24. 5.25. 5.26.
What do you mean by crystal imperfections? Mention the different types of crystal imperfections. List out the changes in the physical properties due to crystal defect. Mention the structure sensitive mechanical properties. What is point defect? Mention the different types of point defects. What is vacancy defect? Write an expression to find out the number of vacancies present in a metal and explain the terms. What is substitutional defect? What is an interstitial defect? What are Schottky defect? Write the mathematical expression for Schottky defects and explain the terms. What are Frenkel defects? Write the mathematical expression for Frenkel defects and explain the terms. What are line imperfections? Distinguish between point imperfection and line imperfection. What is edge dislocation? What is screw dislocation? What is Burger vector? List out the similarities and differences between edge and screw dislocations. What is mixed dislocation? Explain the mixed dislocation with a neat sketch. What is dislocation climb? Explain with a neat sketch, the process of dislocation climb. What do you mean by multiplication of dislocation? What are surface defects? What do you mean by grain boundary defects?
Crystal Imperfections
5.27. 5.28. 5.29. 5.30. 5.31. 5.32. 5.33. 5.34. 5.35. 5.36. 5.37. 5.38. 5.39. 5.40.
133
Explain small angle grain boundary with a suitable sketch. Explain tilt boundary with a suitable sketch. Explain stacking fault defect. What is bulk defect or volume defect? What do you mean by deformation in metals? What is elastic deformation? What is plastic deformation? What do you mean by slip? What are slip systems? What are slip planes and slip directions? Mention the slip direction and slip plane in fcc and bcc metals. What are twin boundaries? What is the reason for the production of twin boundary? Mention the twin planes and twin directions for bcc, fcc and hcp metals.
Descriptive Questions 5.1. What are point defects? Explain, in detail, the different types of point defects with suitable sketches. 5.2. What is dislocation? Explain with suitable sketches, the edge and screw dislocations. Distinguish between edge and screw dislocations. 5.3. What are surface defects? Explain with suitable sketches the different types of surface defects. 5.4. What is deformation in metals? Explian different types of deformations? Write about slip and twin boundary.
Exercise 5.1. The following data are measured for Fe. If Fe crystallites in BCC, find the percentage of vacancy in pure iron. Density = 7.87 g m3, lattice parameter = 2.866 Å and molecular weight = 55.85. Determine the angle across a small angle grain boundary in copper, when the dislocations in the boundary are 1000 Å apart. Calculate the fractional vacancy concentration (N/n) of aluminium at 300 K and 800 K (Given that the energy of formation of vacancy for Al is 0.75 eV per atom).
Chapter
6
CLASSIFICATION OF SOLIDS
OBJECTIVES To explain the property of a solid material on the basis of band theory. To study the classification of semiconductor such as intrinsic and extrinsic semiconductor. To explain the arrangement of atoms in intrinsic semiconductor. To explain the structural changes of the extrinsic semiconductor when added with the tri/pentavalent element.
6.1
INTRODUCTION
Most of the devices are made of semiconductors such as silicon and germanium. The applications of semiconductors and their devices are ever increasing in all fields of science and technology. The knowledge on the classification, structures and properties of semiconductors is more essential to identify the right materials for applications. In the following chapters, properties of materials like electrical, magnetic, etc., are studied in detail. Therefore, in this chapter the classification, bonding and structure of solids are discussed.
6.2
CLASSIFICATION OF SOLIDS ON THE BASIS OF BAND THEORY
Based on the energy band structure, the arrangement of electrons and forbidden bands, solid materials are classified into the following three categories: (1) Conductors (2) Insulators, and (3) Semiconductors Let us briefly discuss these materials briefly and elaborate more on semiconducting materials.
Classification of Solids
6.2.1
135
Conductors
Materials which conduct electric current when a potential difference is applied across them are known as conductors. In case of a conductor, the valence band is completely filled, while the conduction band is half filled, as shown in Fig. 6.1. Degeneracy 2p 6 2s
Empty
6N
2
Conduction band (half filled) Forbidden energy gap Valence band (fully filled)
2N 2N
1s
2
(a) Energy level diagram
(b) Energy bands
Fig. 6.1 Conductors–Lithium atom Therefore, when a small potential difference is applied to a solid material, it provides sufficient energy to the electron in the valence band to shift to the conduction band. Thus, the shifting of electrons from the valence band to the unfilled conduction band results in the flow of current in the material. Examples for good conductors are copper, lithium, etc.
6.2.2
Insulators
Solid materials which do not conduct electric current under normal conditions are known as insulators. In insulators, the valence band is completely filled and it has no electron in the conduction band. Further, the forbidden energy gap will be very high when compared with a conductor. The energy band diagram of an insulator (for example, ebonite) is shown in Fig. 6.2. Therefore, the energy required to shift an electron from the valence band, to the conduction band in order make electrical conduction possible, is very high. Hence, it is not possible to provide enough energy by an ordinary electric field. However, one can achieve electrical conduction in an insulator with very high voltage known as breakdown voltage.
Empty conduction band
Forbidden band Eg = 5 eV Energy (eV)
Valence band
Fig. 6.2 Energy bands in insulators
136
Materials Science
6.2.3
Semiconductors
Semiconductors (for example, silicon or germanium) are materials whose electrical conductivity lies between that of conductors and insulators. The conductivity of semiconductors is in the order of 104 to 104 mho m1. The magnitude of the forbidden energy gap of a semiconductor lies in between the forbidden energy gap of insulators and conductors, as shown in Fig. 6.3.
Conduction band (contains few electrons at room temperature)
Eg 1 eV
Energy (eV)
Valence band (with few holes at room temperature)
Fig. 6.3 Energy bands in semiconductors Semiconducting materials, whether elemental, compound or oxide, are crystalline solids in nature. Well known semiconductors, such silicon and germanium, are elemental semiconductors, while gallium arsenide (GaAs), cadmium sulphide (CdS), etc., are known as compound semiconductors. Some of the oxide semiconductors are Bi2O3, Te2O3, ZnO3, Cu2O, etc. Let us discuss the different types of semiconductors and their applications in detail.
6.3
CLASSIFICATION OF SEMICONDUCTORS
Semiconductors are of two types and are classified on the basis of the concentration of electrons and holes in the materials: (1) Pure or intrinsic semiconductors, and (2) Doped or extrinsic semiconductors Let us discuss the above two types of semiconductors in detail.
6.3.1
Pure or Intrinsic Semiconductors
Highly pure semiconductors are called intrinsic semiconductors, which means that the concentration of electrons must be equal to the concentration of holes. In order to understand the electrical conducting property in a semiconducting material, let us first consider the arrangement of atoms in a material, say, silicon (or germanium). Both germanium and silicon have four valence electrons as shown in Fig. 6.4.
Classification of Solids
Electron
Si
137
Si
Si
Si
Si
Fig. 6.4 Twodimensional arrangement of atoms in silicon at T = 0 K Let us consider the crystal arrangement of silicon (or germanium). Silicon atom is represented by a circle, while the valence electron is marked by black dots. The central silicon atom is surrounded by four valence electrons constituting a covalent bond between two atoms, due to the sharing of valence electrons. If we consider the crystal structure at 0 K, all the valence electrons are engaged in forming covalent bonds with the neighbours. Therefore, no free electron is available. At this stage, the material does not conduct current due to the lack of mobile charges, i.e., at 0 K, the material behaves as an insulator. Electrical conduction can be more lucidly explained by considering the energy level diagram of silicon at 0 K as shown in Fig. 6.5. At 0 K, the valence band is completely filled and there is no empty space in the valence band. Therefore, electrons can not shift from the valence band to the conduction band through the forbidden gap. The shifting electrons is not possible even for a large applied field strength at 0 K.
Conduction band
Eg
Energy (eV)
Valence band
Fig. 6.5 Energy band diagram of silicon at T = 0 K However, the thermal energy is sufficient to liberate an electron from the valence band at room temperature. When the temperature of the intrinsic semiconductor is raised, the atoms in silicon vibrate in their mean position. This provides sufficient energy to the electrons due to which the backing of the covalent bonds take place as shown in Fig. 6.6. The broken electron is now said to be a free electron. When an electrical field is applied, the free electron acquires sufficient energy and shifts from the valence band to the conduction band. This results in the creation of a hole in the valence band as shown in Fig. 6.7. The free electrons move in the conduction band, while the holes move in the valence band. Thus, electrons and holes move opposite to each other as shown in Fig. 6.7.
138
Materials Science
Si
Si
Si
Si
Si
Fig. 6.6 Two dimensional arrangement of atoms in silicon at T > 0 K When a potential difference is applied across a silicon/germanium crystal, the electric force experienced by the electrons and holes are opposite. Thus, due to the opposite charges, the movement of electrons and holes give rise to an electric current in the same direction. The conductivity of germanium is higher than silicon due to its lower energy gap. Electron
Conduction band
Hole
Energy (eV)
Valence band
Fig. 6.7 Energy band diagram of silicon at T > 0 K
6.3.2
Extrinsic Semiconductors
The application of intrinsic semiconductors is restricted due to its low conductivity. In electronic devices, high conducting semiconductors are more essential. The concentration of either electrons or holes in a semiconductor is essential. The concentration of either electrons or holes in a semiconductor is increased depending upon the requirements in the electronic devices. This can be carried out simply by adding impurities (one atom in 107 host atoms) to the intrinsic semiconductors. The process of adding impurity to the intrinsic semiconductors is known as doping. The doped semiconductor is known as extrinsic semiconductor. The concentration of electrons and holes are not equal in an extrinsic semiconductor. Extrinsic semiconductors are classified into two categories based on the concentration of the charge carriers namely,
Classification of Solids
139
(1) ntype semiconductors, and (2) ptype semiconductors (1) ntype semiconductors When a pentavalent atom such as arsenic (antimony, bismuth, phosphorus) is added as a dopant to the tetravalent silicon atom, the arsenic atom will occupy one site of the silicon atom. Thus, out of five free electrons in arsenic, four electrons make covalent bonds with the four neighbouring silicons atoms and the fifth one is loosely bound to the silicon atom, as shown in Fig. 6.8. Si
Si
As
Si
Energy level (eV)
Conduction band
Donor level Valence band
Si (a) With free electrons
(b) Energy at donor level
Fig. 6.8 Doping in ntype semiconductors The energy required to ionise the fifth electrons is very less and hence, the thermal energy of the material shifts the free electrons to the conduction band. Each arsenic atom contributes one free electron to the crystal and hence, it is called a donor impurity. In this type of semiconductor, the concentration of charge carriers (i.e., electrons) is more than that of holes. Therefore, these semiconductors are called ntype semiconductors. In an ntype semiconductor, electrons are the majority current carriers while holes are the minority current carriers. (2) ptype semiconductors Instead of a pentavalent atom, the addition of a trivalent atom indium (In) to the tetravalent silicon atom, occupies the crystal site of the silicon atom as shown in Fig. 6.9. Si
Si
In
Si
Energy level (eV)
Conduction band
Acceptor level
Valence band Si (a) With vacancy
(b) Energy at acceptor level
Fig. 6.9 Doping in ptype semiconductors
140
Materials Science
The three valence electrons in indium make covalent bonds with the three neighbouring silicon atoms, whereas the fourth bond has an empty space known as hole due to the deficiency of one electron. Therefore, when a trivalent atom is added to silicon, it creates a hole in the valence band. The dopant (indium) accepts an electron from the neighbouring silicon atom to form a covalent bond and hence, it is called an acceptor. The hole in the valence band moves freely and hence, the current flows through the material. This type of electrical conduction will take place only when the dopant valency is less than that of the parent atom. Such semiconductors are called ptype semiconductors. In a ptype semiconductor, holes are the majority current carrier and electron are the minority current carriers.
6.4
ELEMEMENTAL AND COMPOUND SEMICONDUCTORS
Semiconductors are those materials which have resistivity between a metal and an insulator. In semiconductors, the conduction band and the valence band is separated by an energy gap in the order of 1 eV. Some semiconductors such as Si and Ge are made up of only one type of atoms. These semiconductors are said to be elemental semiconductors. Some semiconductors like GaAs, InP, InSe, CdS, CdSe, etc., are made up of two different materials. They are binary semiconductors. A semiconductors made up of two or more than two different types of atoms is said to be a compound semiconductors. In a semiconductor, the electrical conductivity is due to the movement of the electrons and holes. The equation for the conductivity of a semiconductor is (6.1)
s = neme + pe mh
where n is the concentration of electron, p the concentration of hole and, me and mh are the mobilities of electron and hole, respectively. The energy gap of Si at room temperature is 1.1 eV and that of Ge is 0.72 eV. The properties of Si and Ge are listed in Table 6.1.
Table 6.1
Physical Properties of Si and Ge
Property
Ge
Si
Eg (eV) Nc (cm3) Nv (cm3) ni (cm3) me (cm2V1s1) mh (cm2V1s1) Density (gm cm3) Atomic weight Atomic number er
0.72 1.04 ¥ 1019 6 ¥ 1018 2.4 ¥ 1013 3900 1900 5.32 72.6 32 16
1.1 2.8 ¥ 1019 1.04 ¥ 1018 1.45 ¥ 1010 1350 450 2.33 28.1 14 11.9
GaAs is a semiconductor of group III and group V in the periodic table. It is one of the mostly studied semiconducting material. It has a direct band gap of 1.42 eV at room temperature. The gallium arsenide
Classification of Solids
141
devices are nearly 2.5 times faster than Si devices and the noise of the GaAs devices is low. Since the cost of a GaAs device is nearly 10 times greater than that of a Si devices and the density of GaAs is high, it is not possible to materialise GaAs for device applications. Table 6.2 lists the energy gap of some groups IV, group II–VI and groups III–V semiconductors. Consider the semiconductors with one element common such as ZnS, ZnSe and ZnTe. From Table 6.2, is found that the energy gap decreases with the increase in atomic weight. Some compound semiconductors, like GaP, InP, InAs and InSb, belonging to groups III–V of the periodic table are important. Generally, compound semiconductors are slightly ionic in character. This ionic character increases as we go from group III–V to II–VI elements.
Table 6.2
Energy Gap of Some Semiconductors
Semiconductor Group IV Diamond Si Ge Group II–VI ZnS ZnSe ZnTe Group III–V InP InAs InSb
Eg (eV) 5.3 1.11 0.72 3.5 2.8 0.85 1.27 0.33 0.18
ZnO, ZnS, ZnSe, CdS, CdTe, CdSe and HgS are some of the group II–VI compound semiconductors, while PbS, PbSe and PbTe are some of the group II–VI compound semiconductors. Some ternary alloys such as AlxGa1x As or quaternary alloys such as Alx Ga1x As y Sb1y are mostly used in device applications. GaAs, GaAs1xPx are mostly used for opto electronic devices such as LEDs. AlxGa1x As is also used in Modulation Doped Filled Effect (MODFET) transistor.
6.5 CRYSTAL STRUCTURE AND BONDING IN Si AND Ge Most of the semiconductors crystallise in diamond structure. The crystal structure of a diamond lattice is shown in Fig. 6.10. Atoms in a diamond lattice have four nearest neighbours. The structure of diamond can be considered as two face centered cubic lattice. Silicon and germanium are covalent crystals. The total number of electrons in germanium is 32 and in silicon is 14. When germanium and silicon atoms occupy the diamond lattice, each of this atom gets attracted by four of its nearest neighbour as shown in Fig. 6.11. The diamond lattice
142
Materials Science
structure has been referred to as the basic lattice structure in silicon and germanium, and also for many semiconductors. Thus, covalent bonds are formed between silicon or germanium atoms in the diamond lattice. The model shown in Fig. 6.11 is employed for visualising either the missing atom or broken bond or free electron.
Fig. 6.10 Diamond Structure Ge
Ge
Si
Ge
Ge
Si
Si
Ge
Si
(a) Germanium
(b) Silicon
Si
Fig. 6.11 Crystal Structure
6.6
APPLICATIONS
The applications of semiconductors are wide and varied. Some of the major applications are as follows. (1) Solid state diodes The combination of a ptype and an ntype semiconductor forms a p–n junction. The p–n junction is known as a solid state diode and is used in electronic devices such as televisions, radios, amplifiers, etc. (2) Most of the electronic devices are made by using semiconductors like silicon, germanium, etc. (3) Ferroelectricdoped oxide glasses are used as barrier layer capacitor due to their high permittivity and conductivity.
Classification of Solids
143
Key Points to Remember Solids are classified based on energy band structure, arrangement of electrons and forbidden bands such as conductors, insulators and semiconductors. In conductors, the valence band is completely filled while the conduction band is halffilled. Solid materials which do not conduct electric current under normal condition are known as insulators. In insulators, the valence band is completely filled and there are no electrons in conduction band. Three different types of semiconductors are elemental, compound and oxide semiconductors. Semiconductors are classified into two types namely, pure or intrinsic and doped or extrinsic semiconductors. In intrinsic semiconductors, the carrier concentration of electrons and holes are equal. These semiconductors are highly pure semiconductors. Doping is the process of adding impurity to an intrinsic semiconductor. Doped semiconductors are known as extrinsic semiconductors. Extrinsic semiconductors are two types namely ntype and ptype. In ntype semiconductors, electrons are majority current carriers while in ptype semiconductors, the holes are majority current carriers. When a dopant with valency higher than the parent atom is doped, then the resultant semiconductors is known as ntype semiconductors. When a dopant with valency lower than the parent atom is doped, then the resultant semiconductor is known as ptype semiconductors. A solar cell is nothing but a pn junction diode based on the principle of photoelectric effect and it converts light into electrical energy.
Solved Problems Example 6.1 Calculate the wavelength of light emitted by an LED with band gap of energy 1.8 eV. Given Data: Bandgap of given LED is Eg = 1.8 eV = 1.8 ¥ 1.609 ¥ 1019 = 2.8962 ¥ 1019 J Solution:
We know that, wavelength emitted from given LED is l=
hc Eg
144
Materials Science
Substituting the values, we get =
6.626 ¥ 1034 ¥ 3 ¥ 108 2.8962 ¥ 1019
= 6.863 ¥ 107 m The wavelength of light emitted from given LED is 6.863 mm. Example 6.2 Calculate the band gap energy of GaAsP semiconductor whose output wavelength is 6715Å. Given Data: The wavelength of greenlight from mercury lamp = 6715 ¥ 1010 m. Solution:
We know that, band gap is Eg =
hc l
Substituting the values, we get =
6.626 ¥ 1034 ¥ 3 ¥ 108 6751 ¥ 1010
= 2.944 ¥ 1019 J = 2.495 ¥ 1018 or,
=
2.944 ¥ 1019 1.6 ¥ 1019
= 1.8 eV The band gap of the given GaAsP is 1.8 eV.
ObjectiveType Questions 6.1. In conduction, the valence band is ____________ while the conduction band is ____________ filled. 6.2. In conducting materials, the flow of current is due to shifting of ____________ from valence band to conduction band. 6.3. In insulators, ____________ band is completely filled and does not have any ____________ is conduction band. 6.4. Examples for insulators ____________. 6.5. The forbidden gap energy of an insulator is ____________ eV. 6.6. Examples of semiconductors ____________, ____________. 6.7. The conductivity of semiconductor is in the order of ____________ ohm1 m1. 6.8. Give an example for compound semiconductors ____________, ____________. 6.9. Give two examples for oxide semiconductors ____________, ____________. 6.10. In intrinsic semiconductors, the concentration of electrons and holes are not equal. (True / False) 6.11. Give any two examples for intrinsic semiconductors ____________, ____________ .
Classification of Solids
6.12. 6.13. 6.14. 6.15. 6.16. 6.17.
145
The valence electron for silicon is ____________. The conductivity of semiconductors depends on energy gap. (True / False) The majority current carrier is ntype semiconductor is ____________. ____________ is the majority current carrier is ptype semiconductors. Give any two examples for pentavalent atoms ____________, ____________. ____________ and ____________ are examples for trivalent atom.
Answers 6.1. 6.4. 6.7. 6.10. 6.13. 6.16.
completely, half carbonite 104 to 104 False True arsenic antinony
6.2. 6.5. 6.8. 6.11. 6.14. 6.17.
electrons 5 GaAs, GaP silicon, germanium electrons Indium Boron
6.3. 6.6. 6.9. 6.12. 6.15.
valence, electron silicon, germanium Bi2O3, Te2O3 4 holes
Short Questions 6.1. 6.2. 6.3. 6.4. 6.5. 6.6. 6.7. 6.8. 6.9. 6.10. 6.11. 6.12. 6.13. 6.14. 6.15. 6.16. 6.17.
What is a semiconductor? Define a conductor. What is meant by an insulator? Draw the energy level diagram of a conductor. Draw the energy level diagram of an insulator. Draw the energy level diagram of a semiconductor. State the properties of semiconductors. What is meant by an intrinsic semiconductor? What is an extrinsic semiconductor? Distinguish between intrinsic and extrinsic semiconductor. What are elemental, compound semiconductors? Give two examples. Explain the crystal structure of germanium and silicon. Mention any four advantages of semiconductors. What is meant by doping? Define ptype and ntype semiconductor. Explain ntype semiconductor. What are the advantages of semiconducting materials?
Descriptive Questions 6.1. Explain with a neat sketch the intrinsic and extrinsic semiconducting materials. 6.2. What is an energy band diagram? Explain the energy diagram for and extrinsic semiconducting materials. 6.3. Write notes on the following: (a) Intrinsic semiconductors (b) Extrinsic semiconductors
Chapter
7
ELECTRON THEORY OF SOLIDS
OBJECTIVES To understand the electrical conduction in materials. To explain the conductivity of a material using free electron theory. To derive the equation for electrical conductivity of a solid using free electron theory. To derive the equation for thermal conductivity of a material and hence, derive the Wiedemann–Franz law. To verify Ohm’s law. To discuss the limitations of classical free electron theory.
7.1
INTRODUCTION
In solids, electrons in the outermost orbit of atoms determine its electrical properties. Electron theory is applicable to all solids, both metals and nonmetals. In addition, it explains the electrical, thermal and magnetic properties of solids. The structure and properties of solids are explained employing their electronic structure by the electron theory of solids. There are three main stages for development of this theory, namely, classical free electron theory, quantum free electron theory and zone theory. The first theory was developed by Drude and Lorentz in 1900. According to this theory, metal contains free electrons which are responsible for the electrical conductivity and metals obey the laws of classical mechanics. In 1928, Sommerfield developed the quantum free electron theory. According to Sommerfield, the free electrons move with a constant potential. This theory obeys the quantum laws. Bloch developed the Brillouin zone or Band theory in 1928. According to this theory, free electrons move in periodic potential provided by the lattice. This theory is known as band theory of solids. Let us discuss in the following headings, electrical and thermal conductions, their relationship, and the advantages and drawbacks of classical free electron theory.
Electron Theory of Solids
147
7.2 ELECTRICAL CONDUCTION When an electronic potential difference is applied across materials, it conducts electricity. Electrical conductivity is defined as the quantity of electricity flowing through a material per unit area per unit time maintained at unit potential gradient. The material with this property is called a conducting material. The most important property of a material is electrical resistance, and it is used to characterise the electrical properties of the material. Let R be the resistance of the material. A and l are the area and length of the material, respectively. Therefore, the resistivity of the material is Resistivity (r) = Resistance ¥
Area Length r=R
or,
A l
Wm
(7.1)
The reciprocal of the electrical resistivity is known as electrical conductivity (s), i.e.,
s=
=
1 r l 1 l = W 1m1 R A RA
(7.2)
The electrical conductivity of a material depends only on the presence of free electrons or conduction electrons. These free electrons move freely in the metal and do not correspond to any atom. This group of electrons is also called electron gas.
7.3 CLASSIFICATION OF CONDUCTING MATERIALS Based on the electrical conductivity, conducting materials are classified into three major categories, namely, (1) Zero resistivity materials (2) Low resistivity materials, and (3) High resistivity materials (1) Zero Resistivity Materials The material which conducts electricity at zero resistance is known as a zero resistivity material. Superconducting materials like alloys of aluminium, zinc, gallium, nichrome, nibium, etc., conduct electricity almost at zero resistance below the transition temperature. The above superconducting materials are perfect diamagnets. The applications of these materials are energy saving in power systems, superconducting magnets, memory storage, etc.
148
Materials Science
(2) Low Resistivity Materials The resistivity of high electrical conductivity materials is very low. The electrical conductivity of metals and alloys like silver, and aluminium is very high, of the order of 108 W1 m1 . Low resistivity materials are used as resistors, conductors, electrical contacts, etc., in electrical devices. In addition, these materials are also used in electrical power transmission and distribution lines, winding wires in motors and transformers. (3) High Resistivity Materials Generally, materials with high resistivity will have low temperature coefficient of resistivity. For example, tungsten, platinum, nichrome, etc., have high resistivity and low temperature coefficient of resistance. High resistivity materials are used in the manufacturing of resistors, heating elements, resistance thermometers, etc.
7.4
CLASSICAL FREE ELECTRON OR DRUDE― LORENTZ THEORY OF METALS
Very high electrical and thermal conductivity are the outstanding properties of metals. The positive ion cores and the valence electrons are the charge carriers in metals and hence, good conductivity means the presence of a mobile charge carrier. The observed high conductivity due to conduction by the drift ion cores is difficult to understand. If this happens, then conductivity must increase with increase in temperature. Hence, it may be concluded that mobile charges in metals are valence electrons. The classical free electron theory reveals that the free electrons are fully responsible for electrical conduction.
7.4.1
Postulates of Classical Free Electron Theory
The free electrons, or electron gas, available in a metal move freely here and there during the absence of an electronic field similar to the gas molecules moving in a vessel as shown in Fig. 7.1. These free electrons collide with other free electrons or positive ion cores or the walls of the container. Collisions of this type are known as elastic collisions. The total energy of an electron is assumed to be purely Kinetic Energy (KE).
Fig 7.1 Absence of the field—Free electron On the other hand, suppose an electric field is applied to the material through an external arrangement as shown in Fig. 7.2. The free electrons available in the metal gain some amount of energy and are directed to move towards a higher potential. These electrons acquire a constant velocity known as drift velocity . The velocity of the electron obeys the Maxwell–Boltzmann studies.
Electron Theory of Solids
149
Free electrons
E
Fig. 7.2 Presence of field—free electron
Drift Velocity It is defined as the average velocity acquired by the free electron in a particular direction during the presence of an electric field.
Relaxation Time The relaxation time is defined as the time taken by a free electron to reach its equilibrium position from its disturbed position, during the presence of an applied field. t=
l
(7.3)
where l is the distance travelled by the electron.
7.5 EXPRESSION FOR ELECTRICAL CONDUCTIVITY AND DRIFT VELOCITY In order to obtain the expression for electrical conductivity, the velocity of the electron in the conducting material is obtained by two methods. In the first method, the velocity of the electron is obtained without considering the collision of free electrons. In the second method, the collision of free electrons is taken into account for obtaining the velocity. Thus, the current density behaviour of a conducting material is studied under the above two approaches to obtain the expression for electrical conductivity. Consider a conductor which is subjected to an electric field of strength E as shown in Fig. 7.3. Consider that n is the concentration of the free electrons; m, the mass and e, the electric charge of the electron in the conductor. According to Newton’s second law of motion, the force F acquired by the electrons is equal to the force exerted by the field on the electrons. Free electrons
E
Fig. 7.3 Metal—conduction
150
Materials Science
Therefore, the equation of motion
F = ma = eE
or,
a=
Acceleration
(7.4)
e E m
Integrating Eq. (7.4), we get The velocity of the electron
n=
eE t +C m
(7.5)
where C is an integration constant, and is obtained by applying the boundary conditions. During the absence of the electric field, the average velocity of the electron is zero, i.e., when
t = 0, v = 0
Substituting the above boundary condition in Eq. (7.5), we get C = 0 Substituting the value of C in Eq. (7.5), we get Velocity of the electron
v=
eE t m
(7.6)
According to Ohm’s law, the current density in a conductor J=
I A
(7.7)
Therefore, the charge dq flowing through this area A in time dt is dq = e n Av dt dq = I = enAv dt
(7.8)
where I is the current flowing through the conductor with an area of crosssection A. Substituting the value of I from Eq. (7.8) in Eq. (7.7), we get J = –nev
(7.9)
Substituting the value of n from Eq. (7.6) in Eq. (7.9), we get J=
ne2 E t m
(7.10)
It is clear from Eq. (7.10) that the current density is directly proportional to the applied field E. When the field increases, the current density also increases, and it reaches infinity when the field is applied for a long period. However, in actual practice, J never becomes infinity. Rather, it remains constant beyond a certain field strength. This is due to the presence of collisions of free electrons which is not taken into account for obtaining the current density.
Electron Theory of Solids
151
Due to the collision of free electrons, a frictional force acts on the electrons. The frictional force experienced by the electron = m /t r
(7.11)
where is the drift velocity of the electron and t r the relaxation time between any two successive collisions during the presence of an electron field. Therefore, equation of motion m
d m = eE + dt tr
(7.12)
Rearranging Eq. (7.12), we get tr
or,
d È eEt r ˘ + ˙ = Í dt Î m ˚
d  dt = tr È eEt r ˘ Í m + ˙ Î ˚
(7.13)
Integrating Eq. (7.13), we get È e E tr ˘ t + ˙ = + ln B ln Í Î m ˚ tr
(7.14)
where ln B is an integration constant. Simplifying Eq. (7.14), we get e E tr + = Be m
–t/t r
(7.15)
In order to obtain the value of the integration constant, consider the boundary condition, when t = 0, = 0. Therefore, Eq. (7.15) can be written as B=
Substituting the Eq. (7.16) in Eq. (7.15), we get
=
eE tr m
(7.16)
e E t r –t/t r [e – 1] m
(7.17)
Substituting the value of < v > from Eq. (7.17) in Eq. (7.9), we get The current density
J=
ne2 t r E [1 – e–t/t r] m
(7.18)
J=sE The current density is proportional to the electric field intensity E and a constant s, known as electrical conductivity.
152
Materials Science
Therefore, electrical conductivity
s=
ne2 t r [1  e–t/t r] m
(7.19)
Equation (7.19) shows that the conductivity of the material is directly proportional to E and it reaches a maximum value within 1014 s (since t r is of the order of 1014 s). Beyond the limit, it remains as constant. Therefore, the steady statevalue of the electrical conductivity and drift velocity of the electron are Electrical conductivity
and drift velocity
s =
ne2 t r m
(7.20)
=
e E tr m
(7.21)
Resistivity (r) We know that the resistivity of a material is the reciprocal of electrical conductivity. Therefore, the resistivity r= =
1 s m ne2 t r
(7.22)
Mobility (me )
We know that from Eq. (7.21), the average velocity of electrons =
i.e.,
(7.23)
µ E
or, where
etr E m
etr is the proportionality factor known as mobility me. m etr me = m
(7.24)
The mobility of a charge carrier is defined as the average velocity of the charge carrier per unit applied electric field intensity.
Mean Free Path (l) The average distance travelled by an electron between any two successive collisions is known as the mean free path. i.e,
l = v tr
where v is the root mean square velocity of the electron.
(7.25)
Electron Theory of Solids
153
7.6 THERMAL CONDUCTIVITY Thermal conductivity (K) of a material is equal to the amount of heat energy (Q) conducted per unit area of crosssection per second to the temperature gradient (dT/dx). i.e.,
Q µ dT dx
or,
Q= K
Therefore, thermal conductivity
K =
dT dx
Q (dT dx )
(7.26)
In solids, the conduction takes place both by available free electrons and thermally excited lattice vibrations known as phonons. Therefore, the total conductivity is Ktotal = Kelectrons + Kphonons
(7.27)
where phonons are the energy carriers for lattice vibrations.
Metals In case of metals, the concentration of free electrons is very high. Therefore, electrons, in addition to thermal vibrations, absorb and transport thermal energy. Hence, the thermal conductivity of a metal is due to the free electrons. (Kelectron >> Kphonon. ), Ktotal = Kelectrons
(7.28)
Insulators In insulators, the thermal conductivity is due to atomic or molecular vibration of the lattice, i.e,
Ktotal = Kphonons
(7.29)
Semiconductors The thermal conductivity is due to both electrons and phonons. Therefore,
Ktotal = Kelectrons + Kphonons
(7.30)
7.7 EXPRESSION FOR THERMAL CONDUCTIVITY Consider a uniform rod HC with the temperature of the hot end H as T1 and the temperature of the cold end C as T2, as shown in Fig. 7.4. Heat is flowing from the hot end H to the cold end C. Let A be the crosssectional area which is at a distance equal to the mean free path l of the electrons between the two ends H and C. The kinetic energy of the electrons at the hot end H is greater than that of the electrons at the colder end C.
154
Materials Science
2l T1
l
T2
l
H
O
C
Fig. 7.4 Thermal conductivity Let Q be the amount of heat flowing through the rod from the end H to C whose length is 2l. Therefore, the heat conducted
or,
Qa
A(T1  T2 ) t 2l
Q=
KA (T1  T2 )t 2l
(7.31)
where K is the coefficient of thermal conductivity; A, the area of crosssection; t, the time for conduction and 2l, the length of the rod. Therefore, the thermal conductivity per unit area per unit time K=
Q2l A (T1  T2 ) t
(7.32)
Let n be the number of available conduction electrons and v be the root mean square velocity of the electrons. Let us assume that the available free electrons in the metal have an equal probability to move in all the six possible directions. Therefore, an average of 1/6 nv electrons can travel in any one direction. We know that the free electrons are assumed to be free moving gas molecules. The average kinetic energy of an electron at the hot end H of temperature T1 =
3 kB T1 2
(7.33)
where kB is the Boltzman constant. Similarly, the average kinetic energy of an electron at the cold end C of the temperature T2 =
3 kB T2 2
(7.34)
The number of electrons crossing the area at A per second, =
1 nv 6
(7.35)
\ The heat energy transferred per unit area per unit time from the hot end H to the cold end C is = number of electrons ¥ average KE of electrons moving from H to C =
1 3 nv kB T1 6 2
Electron Theory of Solids
=
1 n v kB T1 4
155
(7.36)
Similarly, the heat energy transferred across A per second from C to H =
1 3 n v kBT1 6 2
=
1 n v kB T1 4
(7.37)
\ The resultant heat energy transferred from H to C across A per second, Q=
We know that, temperature gradient
nv kB ( T1  T2 ) 4
dT T1  T2 = dx 2l
(7.38)
(7.39)
Substituting the values of Q and temperature gradient from Eq. (7.38) and (7.39) in Eq. (7.32), we get Thermal condition
K =
n( v / 6) (3 / 2) kB (T1  T2 ) ( T1  T2 ) / 2l
or,
K =
( T  T2 ) 2 l 1 nv kB 1 ( T1  T2 ) 4
(7.40)
K =
1 nv kB l 2
(7.41)
Simplifying the above equation, we get
We know from the classical free electron theory, the electronic specific heat capacity of the metal is Ce =
3 R 2
(7.42)
where R is the gas constant and is equal to n kB. Substituting the R value in Eq. (7.41), we get Thermal conductivity K =
1 Ce v l 3
(7.43)
Thermal conductivity of a metal is determined either by using Eq. (7.41) or Eq. (7.43), depending on the available data.
7.8 WIEDEMANN–FRANZ LAW The ratio between the thermal conductivity and electrical conductivity of a metal is directly proportional to the absolute temperature of the metal when the temperature is not too low,
156
Materials Science
i.e.,
K µT s K =L sT
(7.44)
where K/s T is a constant known as Lorentz number. The value of L is equal to 2.44 ¥ 108 W W K2 at 293 K. We know that Thermal conduction
Electrical conduction \
K=
1 nv kB l 2
ne2t r m K 1 / 2nvkB l = s ( ne2 t r / m) s=
=
mvkB l 2e2 t r
(7.45)
(7.46) (7.47)
(7.48)
Substituting l = v t r in the above equation, we get K mv2 kBt r = s 2e2t r
(7.49)
K k 3 = kB T B s 2 e2
(7.50)
Simplifying the above equation, we get
We know that kinetic energy of an election is 1/2 mv2 = 3/2 kB T. Therefore,
Lorentz number
K 3 kB2 = sT 2 e2 L=
3 kB2 ¥ 2 e2
(7.51)
Substituting the values of kB and e in Eq. (7.51), we get Lorentz number
L=
3(1.38 ¥ 1023 )2 2(1.6 ¥ 1019 )2
= 1.11 ¥ 108 W W K2
(7.52)
We observe that the theoretical value of the Lorentz number is only onehalf of the experimental value (= 2.44 ¥ 108 W W K2). The observed discrepancy is due to the failure of the classical theory to give the correct value for the thermal conductivity of metals. In order to rectify the discrepancy, the
Electron Theory of Solids
157
concept of quantum theory has been used to obtain the expression for thermal conductivity. According to the quantum theory, the expression for thermal conductivity is modified by considering the electronic specific heat as,
We know that Lorentz number,
K=
n p 2 kB2 T t r 3m
L =
K sT
L =
n p 2 kB2 T t r m ¥ 3m ne2 t r T
(7.53)
Substituting the values of K and s, we get or,
(7.54)
2
Lorentz number
=
p 2 È kB ˘ 3 ÍÎ e ˙˚
Substituting the values of kB, e and p in Eq. (7.54), we get L = Lorentz number
p 2 (1.38 ¥ 1023 )2 3(1.6 ¥ 1019 )2
= 2.44 ¥ 108 W W K2
(7.55)
Equation (7.55) gives the correct value of the Lorentz number and is in good agreement with the experimental value. Thus, it confirms that the Wiedemann–Franz law is verified using the quantum theory. Further, it supports that Wiedemann–Franz law is not applicable for low temperature.
7.9 VERIFICATION OF OHM’S LAW The classical free electron theory is used to verify Ohm’s law. In order to verify the same, consider that the steadystate current density can be written from Eq. (7.19) as J=
ne2 t r E m
(7.56)
Similarly, the steadystate conductivity from Eq. (7.20), is s=
ne2 t r m
(7.57)
Compare Eqs. (7.56) and (7.57), one can write J= s E
(7.58)
158
Materials Science
We know that the current density J = I/A, the conductivity s = 1/r, and the electric field intensity E = V/d, Therefore, Eq. (7.58) is given by I 1 V = A r d or, We know that, r =
Ê rdˆ I V= Á Ë A ˜¯
(7.59)
rd A
(7.60)
RA and hence, d R=
Substituting the above value in Eq. (7.59), we get V= I R
(7.61)
Equation (7.61) states the Ohm’s law. It is clear from the above equation that Ohm’s law is verified employing classical free electron theory.
7.10
CLASSICAL FREE ELECTRON THEORY: ADVANTAGES AND DRAWBACKS
Even though the classical free electron theory is the first theory developed to explain the electrical conduction and thermal conduction of metals, it has many practical applications. The advantages and disadvantages of the classical free electron theory are as follows.
Advantages a. b. c. d.
It It It It
explains the electrical conductivity and thermal conductivity of metals. explains the Wiedemann–Franz law. verifies Ohm’s law. is used to explain the optical properties of metals.
Limitations a. b. c. d. e.
It fails to explain the electric specific heat and the specific heat capacity of metals. It fails to explain superconducting properties of metals. It fails to explain new phenomena like photoelectric effect, compton effect, blackbody radiation, etc. It fails to explain electrical conductivity of semiconductors or insulators. The classical free electron model predicts the incorrect temperature dependence of s. According to the classical free electron theory, s = ne2tr /m. f. It fails to give a correct mathematical expression for thermal conductivity. g. Ferromagnetism could not be explained by this theory. h. Susceptibility has greater theoretical value than the experimental value.
Electron Theory of Solids
159
Key Points to Remember The three main theories developed for metals are the classical free electron theory, quantum free electron theory and zone or band theory. The classical free electron theory is a macroscopic theory and it obeys classical laws. The quantum free electron theory is a microscopic theory and it obeys quantum laws. Zone theory is a macroscopic theory and is based on the energy bands of solids. Electrical conductivity is defined as the quantity of electricity flowing through the material per unit area per unit time maintained at unit potential gradient. ne2t r The electrical conductivity s = where n is the number of electrons per unit; e, the m charge; m, the mass and t r , the relaxation time. The mobility of a charge carrier is defined as the average velocity of the charge per unit applied electric field intensity. me =
et r m
The mean free path is the average distance travelled by the electron between any two successive collisions l = v t r . The thermal conductivity of a metal Ktotal = Kelectrons + Kphonons Thermal conductivity of an insulator Ktotal = Kphonons The coefficient of thermal conductivity is defined as the ratio of the heat energy transferred across unit area of crosssection in one second to the temperature gradient. K=
Q 2l A (T1  T2 ) t
The thermal conductivity of a metal K =
1 n v kB l 2
The thermal conductivity of a metal in terms of electronic specific heat 1 K = Ce v l 3 The Wiedemann–Franz law states that the ratio between thermal conductivity and electrical conductivity of a metal is directly proportional to absolute temperature is not too low K µT s Lorentz number
L=
K sT
Ohm’s law is verified using the classical free electron theory.
160
Materials Science
Solved Problems Example 7.1 The following data are given for copper: (i) Density = 8.92 ¥ 103 kg m3, (ii) Resistivity = 1.73 ¥ 108 W m, and (iii) Atomic weight = 63.5. Calculate the mobility and the average time collision of electrons in copper obeying classical laws. Given Data:
Solution:
The resistivity of copper
r = 1.73 ¥ 108 W m
The atomic weight of copper
z = 63.5
The density of copper is
d = 8.92 ¥ 103 kg m3
We know that, the carrier concentration =
Avogadro’s number ¥ Density Atomic weight
Substituting the values, we get i.e.,
n = 6.023 ¥ 1026 ¥
8.92 ¥ 103 63.5
n = 8.46 ¥ 1028 m3 The conductivity of copper is,
s= =
1 r 1 1.73 ¥ 108
= 5.78 ¥ 107 W1 m1 ne2t m Rearranging the above equation, we get We know that conductivity is
s=
sm ne2 Substituting the value s, m, n and e, we get 5.78 ¥ 107 ¥ 9.11 ¥ 1031 = 8.46 ¥ 1028 ¥ (1.6 ¥ 1019 )2 t=
We know that,
t = 2.43 ¥ 1011 s.
Mobility
m=
5.78 ¥ 107 s = 8.46 ¥ 1028 ¥ 1.6 ¥ 1019 ne
m = 4.27 ¥ 103 m2 V1 s1 The mobility of electrons in copper is 4.27 ¥ 103 m2 V1 s1 .
Electron Theory of Solids
161
Example 7.2 Sodium metal with bcc structure has two atoms per unit cell. The radius of sodium atom 0
is 1.85 A . Calculate its electrical resistivity at 0° C, if the classical value of mean free time at this temperature is 3 ¥ 1014 s. Given Data: = 1.85 A∞
The radius of the sodium atom
tr = 3 ¥ 1014 s
Mean free time of sodium at 0ºC Solution:
4
For bcc structure, lattice constant is given by a =
a=
Therefore,
ne =
Density of electrons
3
r
4 ¥ 1.85 ¥ 1010
= 4.27 ¥ 1010 m
3 Number of atoms per unit cell Volume (a3 )
where number of atoms per unit cell is 2 for bcc structure. \ ne =
Therefore,
2 ( 4.27 ¥ 1010 )3
ne = 2.57 ¥ 1028 m3
r =
We know that resistivity
m ne2 t
\ Substituting the value, we get r=
9.11 ¥ 1031 (2.57 ¥ 1028 ) ¥ (1.6 ¥ 1019 )2 ¥ (3 ¥ 1014 ) r = 4.616 ¥ 108 W m
Therefore, the resistivity copper is 4.616 ¥ 108 W m . Example 7.3 Calculate the electrical resistivity of sodium at 0oC. It has 25.33 ¥ 1027 electrons per unit volume and has a mean free time of 3.1 ¥ 1014s. Given Data: Number electrons per unit volume
n = 25.33 ¥ 1027
Mean free time of the electron
tr = 3.1 ¥ 1014
162
Materials Science
Solution:
We know that, the electrical resistivity of sodium metal is r=
m ne2t r
where m and e are the mass and charge of electrons, respectively. Substituting the value of n, tr, m and e, we get =
25.33 ¥ 1027
9.11 ¥ 1031 ¥ (1.6 ¥ 1019 )2 ¥ 3.1 ¥ 1014
= 4.532 ¥ 1036 W m The electrical resistively of sodium at 0°C is 4.532 ¥ 1036 W m. Example 7.4 The relaxation time of conduction electrons in a material is 3 ¥ 1014s. If the density of electrons is 5.8 ¥ 1028 per m3, calculate the resistivity of the material and mobility of the electron. Given Data:
Solution:
Number of force electrons per unit volume
n = 5.8 ¥ 1028 m3
The relaxation time of conduction electrons
tr = 3 ¥ 1014 s.
We know that, the electrical resistivity of the metals is given by r=
m ne2 t r
Substituting the value of n, tr, mass of electron and charge of electron, we get r=
5.8
¥ 1028
9.11 ¥ 1031 ¥ (1.6 ¥ 1019 )2 ¥ 3.4 ¥ 1014
= 1.804 ¥ 108 W m Therefore, the electrical conductivity of the material is 1.804 ¥ 108 W1 m1 . We also know that, the mobility of electron is me =
et r m
Substituting the value of e, tr and m, we get =
1.6 ¥ 1019 ¥ 3.4 ¥ 1014 = 5.9715 ¥ 103 9.11 ¥ 1031
Therefore, the mobility of the electron in a metal is 5.97 ¥ 103 m2 v1s1 .
Electron Theory of Solids
163
Example 7.5 A uniform silver wire has a resistivity of 1.54 ¥ 108 ohm m at room temperature. For an electric field along the wire of 1 volt/cm, compute the average drift velocity of an electron assuming that there is 5.8 ¥ 1028 conduction electrons/m3. Also calculate the mobility. Given Data:
Solution:
The resistivity of the silver
= 1.54 ¥ 108 ohm m
Electric field along the wire
= 100 v m1
The carrier concentration of electron
= 5.8 ¥ 1028 m3
We know that, the mobility of the electron m =
s 1 (or ) ne r ne
Substituting the values of n, e and r, we get m=
=
1.54 ¥
108
1 ¥ 5.8 ¥ 1028 ¥ 1.6 ¥ 1019
1 = 6.9973 ¥ 103 142.912
The mobility of the electrons in silver is 6.9973 ¥ 103 m2 v1s1 The drift velocity
vd = m E vd = 6.9973 ¥ 103 ¥ 100
Therefore, drift velocity (vd) = 0.69973 The drift velocity of the electron in silver is 0.69973 m s1. Example 7.6 The density of silver is 10.5 ¥ 103 kg m3, assuming that each silver atom provides one conduction electron. The conductivity of silver at 20ºC is 6.8 ¥ 107 W1 m1. Calculate the density and mobility of electron in silver with atomic weight of 107.9 ¥ 103 kg m3. Given Data:
Solution:
The density of silver
= 10.5 ¥ 103 kg m3
The conductivity of silver at 20ºC
= 6.8 ¥ 107 W1 m1
The atomic weight of silver
= 107.9 ¥ 103 kg m3
We know that, the number of atoms present per m3 = Avogadro’s number ¥
Density Atomic weight
164
Materials Science
= 6.023 ¥ 1026 ¥
10.5 ¥ 103 107.9
= 5.86 ¥ 1028 atoms/m3 As each silver atom contributes one electron, the density of electrons is 5.8 ¥ 1028 atoms/m3. We know that the conductivity is given by s = nem m= \
6.8 ¥ 107 s = ne 5.86 ¥ 1028 ¥ 1.609 ¥ 1019
m = 0.72 ¥ 102 m2 V s1 Therefore, the mobility of electron is 0.72 ¥ 102 m2 V s1 .
Example 7.7 The thermal and electrical conductivities of Cu at 20oC are 390 W m1 K1 and 5.87 ¥ 107 W1 m1, respectively. Calculate the Lorentz number. Given Data:
Solution:
Electrical conductivity of copper
s = 5.87 ¥ 107 W1 m1
Thermal conductivity of copper
k = 390 W m1 k1
Temperature
T = 293 K
We know that, the Lorentz number is L=
K sT
Substituting the values of K, s and T, we get =
390 5.87 ¥ 107 ¥ 293
= 2.26756 ¥ 108 W W K 2 Therefore, the Lorentz number is 2.267 ¥ 108 W W K2. Example 7.8 Calculate the electrical and thermal conductivities for a metal with relaxation time of 1014 second at 300 K. Also, calculate the Lorentz number using the above result. (Density of electrons = 6 ¥ 1028 m3.) Given Data: The relaxation time
t r = 1014 s
The temperature
T = 300 K
The electron concentration
n = 6 ¥ 1028 m3
Electron Theory of Solids
Solution:
165
We know that the electrical conductivity is s=
ne2t r m
Substituting the values of n, e, tr and m, we get =
6 ¥ 1028 ¥ (1.6 ¥ 1019 )2 ¥ 1014 9.1 ¥ 1031
= 1.6879 ¥ 107 Therefore, the electrical conductivity is 1.6879 ¥ 107 W1 m1. We know that the thermal conductivity k=
np 2 k 2BT t r 3m
Substituting the values, we get =
6 ¥ 1028 ¥ p 2 (1.38 ¥ 1023 )2 ¥ 300 ¥ 1014 3 ¥ 9.1 ¥ 1031
= 123.927525 W m1 k1 We know the thermal conductivity is 123.92 W m1 k1. Lorentz number is
L=
k sT
Substituting the corresponding value in the above equation, we get =
123.927525 = 2.44737 ¥ 108 1.6879 ¥ 107 ¥ 300
The Lorentz number is 2.4474 ¥ 108 W W K2. Example 7.9 The density and atomic weight of Cu are 8900 kg m3 and 63.5. The relaxation time of electrons in Cu at 300 K is 1014 s. Calculate the electrical conductivity of copper. Given Data:
Solution:
Density of copper
= 8900 kg m3
Atomic weight of Cu
= 63.5
Relaxation time
= 1014 s
We know that the concentration of free electrons Avogadro’s constant ¥ Denstiy ¥ Number of free electrons per atom n= Atomic weight
166
Materials Science
Substituting the values, we get =
6.022 ¥ 1023 ¥ 8900 ¥ 103 63.5
= 8.44 ¥ 1028 Since the number of free electrons per atom in copper is 1, the electrical conductivity ne2t r s= m 8.44 ¥ 1028 ¥ (1.6 ¥ 1019 )2 ¥ 1014 = 9.1 ¥ 1031 The electrical conductivity is 2.374 ¥ 107 Ohm1 m1. Example 7.10 The resistivity of a piece of silver at room temperature is 1.6 ¥ 108 W m. The effective number of conduction electrons is 0.9 per atom and the Fermi energy is 5.5 eV. Estimate the mean free path of the conduction electrons. Calculate the electronic relaxation time and the electronic drift velocity in a field of 100 V m1. The density of silver is 1.05 ¥ Ê m ˆ =1 . 104 kg/m3 Á Ë m * ˜¯ Given Data: The resistivity of the silver piece at room temperature
r = 1.6 ¥ 108 W m
The effective number of conduction electrons for atom
= 0.9
Fermi energy of the silver piece
= 5.5 eV = 5.5 ¥ 1.60 ¥ 1019 = 8.8 ¥ 1019 J
Solution:
We know that the conductivity
1 s= r 1 1.6 ¥ 108
=
= 6.25 ¥ 107 The conductivity of the silver piece is 6.25 ¥ 107 W1 m1
n = 6.023 ¥ 1023 ¥
1.05 ¥ 104 107.9 ¥ 103
= 5.86 ¥ 1028 m3 We know that the relaxation time t =
sm ne2
Electron Theory of Solids
167
Substituting the values, we get =
6.25 ¥ 107 ¥ 9.11 ¥ 1031 5.86 ¥ 1028 ¥ (1.603 ¥ 1019 )2
t = 3.78 ¥ 1014 Therefore, the relaxation time is 3.78 ¥ 1014 s l = ct
The mean free path is given by
= 3 ¥ 108 ¥ 3.78 ¥ 1014 l = 1.134 ¥ 105 m We know that, the drift velocity is
vd =
sE ne
Substituting the values, we get
vd =
6.25 ¥ 107 ¥ 100 5.86 ¥ 1028 ¥ 1.6 ¥ 1019
= 0.66 ms1 Therefore, the drift velocity of electrons in the silver piece is 0.66 m s1 Example 7.11 A copper wire has a resistivity of 1.7 ¥ 108 W m at room temperature of 300 K. If the copper is highly pure, find the resistivity at 700˚C. Given Data: The resistivity of copper wire at room temperature r = 1.7 ¥ 108 W m. Solution:
We know that
r µ T1/2 1/ 2
i.e.,
T r1 = 11/ 2 T2 r2 r2 =
r1 T11/ 2 T21/ 2
By rearranging the above equation, we get r2 = r1
T11/ 2 T21/ 2
Substituting the value of r 1, T1 and T2, we get r2 = 1.7 ¥ 108 ¥
(700 + 273)1/ 2 3001/ 2
The resistivity of the copper wire is 3.0616 ¥ 108 W m.
168
Materials Science
Example 7.12 A conduction wire has a resistivelity of 1.54 ¥ 108 W m at room temperature. The Fermi energy for such a conductor is 5.5 eV. There are 5.8 ¥ 1028 conduction electrons per m3. Calculate (i) The relaxation time and the mobility of the electrons. (ii) The average drift velocity of the electrons when the electric field applied to the conductor is 1 V cm1. (iii) The velocity of an electron with Fermi energy. (iv) The mean free path of the electrons. Given Data: The resistivity Fermi energy
r = 1.54 ¥ 108 W m EF = 5.5 eV = 5.5 ¥ 1.609 ¥ 1019 = 8.8495 ¥ 1019 J
Concentration of electrons
n = 5.8 ¥ 1028 m3
Solution: (i) We know that the relaxation time a tr =
m r ne2
Substituting the value of r, EF, n and e, we get tr =
9.1 ¥ 1031 1.54 ¥ 108 ¥ 5.828 ¥ (1.6 ¥ 1019 )2
= 3.97972 ¥ 1014 s Therefore, the relaxation time is 3.98 ¥ 1014. We know that the mobility of the electrons is m= m=
et r m 1.6 ¥ 1019 ¥ 3.97972 ¥ 1014 9.1 ¥ 1031
= 6.9973 ¥ 103 The mobility of the electrons is 6.99 ¥ 103 m2 V1 s1. (ii) We know that the drift velocity of the electrons. vd =
et r E m
Electron Theory of Solids
Substituting the value of e, tr , E and m in the above equation, we get m=
1.6 ¥ 1019 ¥ 3.98 ¥ 1014 ¥ 1 ¥ 102 9.11 ¥ 1031
= 0.69973 The drift velocity of the electrons is 0.69973 m s1. (iii) We know that the Fermi velocity is vF = =
2EF m 2 ¥ 5.5 ¥ 1.6 ¥ 1019 =1.3907 ¥ 106 m s1 9.1 ¥ 1031
Therefore, the Fermi velocity is 1.39 ¥ 106 m s1. We also know that the mean free path l = vFtr = 1.3907 ¥ 106 ¥ 3.97972 ¥ 1014 = 5.5346 ¥ 108 The mean free path is 5.535 ¥ 108 m.
ObjectiveType Questions 7.1. 7.2. 7.3. 7.4. 7.5. 7.6. 7.7. 7.8. 7.9.
____________ is the macroscopic theory. Quantum free electron theory is a macroscopic theory and it obeys ____________ law. Zone theory is based on ____________ of solids. The reciprocal of electrical resistivity is known as ____________. The unit for electrical resistivity is ____________. The free electrons in a metal are known as ____________. Electrical conductivity of lowresistivity materials is in the range of ____________. Examples for highresistivity materials are ____________, ____________ and ____________. According to Newton’s second law of motion (a) F = ma2 (b) F = ma 2 2 (c) F = m a (d) F = ma 7.10. The electrical conductivity of a metal is (a) s =
ne2 t r m2
(b) s =
ne2 t r2 m2
(c) s =
ne2 t r m
(d) s =
ne t r m2
169
Materials Science
170
7.11. The resistivity of a material
7.12. 7.13. 7.14. 7.15.
(a) r =
m ne2 t r
(b) r =
m ne t r
(c) r =
m ne2 t r2
(d) r =
m2 ne2 t r
The The The The
mobility of the electron me = ____________ thermal conduction in a metal is equal to Ktotal = ____________ thermal conduction for an insulator is Ktotal = ____________ coefficient of thermal conductivity K is equal to
(a)
1 2 n v kB l 2
(b)
1 2 2 n v kB l 2
(c)
1 2 nv kB l 2
(d)
1 nv kB l 2
7.16. According to Wiedemann–Franz law (a)
K µ T2 s
(b)
K µT s
(c)
K = T2 s
(d)
K µT2L s
7.17. Ohm’s law is verified using the classical free electron theory. (True/False) Answers 7.1. 7.4. 7.7. 7.10. 7.13. 7.16.
Classical free electron Electrical conductivity 108 (c) Kelectron (b)
7.2. 7.5. 7.8. 7.11. 7.14. 7.17.
quantum W1 m1 Tungsten, Platinum, nichrome (a) Kphonon True.
Short Questions 7.1. 7.2. 7.3. 7.4. 7.5.
What is meant by electrical conductivity? Define electrical conductivity. What is meant by conductivity materials? Define density of states and sketch the same for a metal? What are the main theories developed for metals?
7.3. 7.6. 7.9. 7.12. 7.15.
energy bands electron gas (b) e tr / m (d)
Electron Theory of Solids
7.6. 7.7. 7.8. 7.9. 7.10. 7.11. 7.12. 7.13. 7.14. 7.15. 7.16. 7.17. 7.18. 7.19. 7.20. 7.21. 7.22. 7.23. 7.24. 7.25. 7.26. 7.27.
171
What is meant by free electrons? What is classical free electron theory? Mention any two important features of quantum free electron theory of metal. Define electric collision. What are the sources of resistance in metals? Mention the postulates of free electron theory. Define relaxation time. Distinguish between relaxation time and collision time. Define mean free path. Define the mobility of electrons. Define drift velocity. Distinguish between drift velocity and thermal velocity of an electron. Define coefficient of thermal conductivity. Define electrical conductivity. Distinguish between thermal and electrical conductivity. State Wiedemann–Franz law. What is meant by Lorentz number? What are the similarities between the electrical and thermal conductivity? Verify Ohm’s law using classical free electron theory. Mention the application of classical free electron theory. What are the advantages of classical electron theory? What are the drawbacks of classical free electron theory?
Descriptive Questions 7.1. What are the postulates of free electron theory? Drive an expression for electrical conductivity based on free electron theory. 7.2. Derive an expression for electrical conductivity in a material in terms of mobility of electrons and hence obtain Wiedemann–Franz law. 7.3. Define electrical and thermal conductivity and deduce the expression for the same. 7.4. Deduce Wiedemann Franz law classically and quantum mechanically. 7.5. Describe the classical free electron theory and deduce Lorentz number. Also, discuss the merits and demerits of classical free electron theory.
Chapter
8
STATISTICS AND BAND THEORY OF SOLIDS
OBJECTIVES To To To To To To To
8.1
derive the Fermi Dirac statistics for the energy states. study the probability of occupation of electrons. explain the density of states in metal or semiconductors. study the effect of temperature on Fermi energy function. study the Band theory of solids and origin of band gap. study the KronigPenney model and Brillouin zone of solids. study the effect of temperature and impurity on electrical properties of metals.
INTRODUCTION
The classical free electron theory could not explain specific heat capacity, electronic specific heat, etc. But they are well explained using quantum free electron theory. On the other hand, quantum free electron theory fails to explain the distinction among metals, semiconductors and insulators, the positive value of Hall Effect and some transport properties. All the above failures are overcome by the energy band theory of solid. The band theory of solids is used to explain the band structure and the electrical properties of solids. The outcome of quantum mechanics, Pauli’s exclusion principle and Bohr’s atom model are results of the band theory of solids. The statistics mainly used to derive the velocity and the energy distribution of particles is of three types namely, (i) MaxwellBoltzmann statistics, (ii) BoreEinstein statistics, and (iii) FermiDirac statistics. The Maxwell – Boltzmann statistics deals with particles having no spin (Eg., gaseous particles). The BoseEintein statistics explains the particles like photon having integral spins, while the particle with half integral spin was dealt by the FermiDirac statistics. Examples for FermiDirac statistics are the particles like electrons which have half integral spin and hence, these particles are known as Fermi particles or Fermions. The FermiDirac statistics, Fermi energy, density of states and band theory of solids are briefly discussed in this chapter.
8.2
FERMIDIRAC STATISTICS
The distribution of energy states in a semiconductor is explained by FermiDirac statistics since it deals with the particles having half integral spin like electrons. Consider that the assembly of electrons as
Statistics and Band Theory of Solids
173
electron gas which behaves like a system of Fermi particles or Fermions. The Fermions obey FermiDirac statistics, i.e., Pauli’s exclusion principle. Therefore, the probability function f (E) of an electron occupying an energy level E is given by f (E) =
1
(8.1)
1 + exp ÈÎ( E  EF ) / KT ˘˚
where EF is known as Fermi energy, K the Boltzmann constant and T the absolute temperature. In Eq. (8.1), the probability function f (E) lies between 0 and 1. Hence, there are three possible probabilities namely, f (E) = 1 f (E) = 0 f (E) = 0.5
100 % probability to occupy the energy level by electrons. No probability to occupy the energy levels by electrons and hence, it is empty. 50 % probability of finding the electron in the energy level.
A detailed explanation for the above three cases are given by considering the temperature dependence of Fermi distribution function and its effects on the occupancy of energy level by electrons is shown in Fig. 8.1. E
EF
E
E
EF
EF
N/2
0
Distance (a) Distribution of electrons in conduction band at 0 K
f(E )
1
(b) Fermi Dirac distribution function at 0 K
N(E ) (c) Electron distribution function
Fig. 8.1 FemiDirac distribution function
Case I
Probability of occupation at T = 0 K and E < EF
Substituting the above condition in Eq. (8.1), we get f (E) = = Therefore,
1 1+ e 1 =1 1
f (E) = 1
(8.2)
Equation (8.2), clearly indicates that at T = 0 K, the energy level below the Fermi energy level EF is fully occupied by electrons leaving the upper levels vacant. Therefore, there is a 100 % probability that the electrons to occupy energy level below Fermi energy. Generally, a single energy band namely, conduction band diagram as shown in Fig. 8.1(a) is used to characterise the conductors.The conduction bands have more energy levels than free electrons. Figure 8.1(a) indicates that conduction band is
174
Materials Science
filled up to a certain energy level marked as EF, while the energy levels above the highest filled level is empty. Fermi energy level is defined as the upper most filled energy level in a conduction band at 0 K. In other words, the highest energy level occupied by an electron in a conductor at 0 K is the Fermi energy level.
Case II Probability of occupation at T = 0 K and E > EF Substituting the above condition in Eq. (8.1), we get 1 1+ e
f (E) = =
or, Therefore,
1 1 1
=
=0
f (E) = 0
(8.3)
Equation (8.3) clearly indicates that at T = 0 K, the energy levels above the Fermi energy level EF is unoccupied, i.e., vacant. Therefore, there is a 0 % probability for the electrons to occupy the energy level above the Fermi energy level. Figure 8.1(b) shows that the variation of f (E) for different energy values is a step function.
Case III Probability of occupation at T = 0 K and E = EF Substituting the above condition in Eq. (8.1), we get f (E) =
or, Therefore,
1 1+ e0
=
1 1+1
=
1 = 0.5 2
f (E) = 0.5 or 1/2
(8.4)
Equation (8.4) clearly indicates that at T = 0 K, there is a 50 % probability for the electrons to occupy Fermi energy level. Therefore, the Fermi energy level is defined as the energy level at any temperature, the probability of electron is 50 % or ½. Similarly, it is also defined as EF the average energy occupied by the electrons which participate in conduction process in a conductor at a temperature above 0 K.
Case IV At high temperature (T > 0 K ), i.e., KT >> EF or T = At higher temperature, electrons are excited above the Fermi energy level which is vacant. Therefore, most of the electrons are lying in the deep conduction band, without any disturbance. Since, the energy KT is not sufficient to make any transition to an unoccupied level. This energy is sufficient to make a jump to higher level to those electrons which lie in the energy level adjunct to Fermi level. At higher temperatures, the electrons lose the quantum mechanical properties and the traditional classical Boltzmann distribution function.
Statistics and Band Theory of Solids
8.2.1
175
Density of States
The energy distribution of electrons in a metal or semiconductor is determined using Fermi–Dirac statistics. The nx, ny, nz are quantum numbers used to construct the point in the sphere. ny z
Octants
D
Quadrant
dR
E A x
B
R
y
C
nx
Hemisphere
nz
(a) Division of a Sphere
(b) Octant
Fig. 8.2 Density of States The ability of a metal to conduct electricity depends on the number of quantum states and the available energy levels of the electrons. Therefore, the determination of energy states for the electrons is essential. The numbers of quantum states present in a metal between the energy interval E and E + dE per unit volume is known as density of states. Density of states Z(E) =
No. of quantum states present between E and E + dE Volume of the specimen
(8.5)
Consider that the sphere is further divided into number shells as shown in Fig. 8.2(a). Therefore, each shell is represented by a set of quantum numbers (nx, ny and nz) and will have an associated energy. Let E be the energy of the point which is same for all points present on the sphere. Therefore, the radius of the sphere with energy E is n2 = nx2 + ny2 + nz2
(8.6)
Consider that the unit volume represents one energy state. Therefore, number of energy states in a sphere of radius n is =
4 3 pn 3
(8.7)
Equation (8.7) represents the total volume of the sphere. We know that the quantum number nx, ny, nz takes only the positive integral values and hence, one has to take only one octant in the sphere, i.e., 1/8 of the total volume of the sphere. Therefore, every states available within one octant of the sphere of radius n and its energy E is =
1 È4 3˘ pn ˙ 8 ÍÎ 3 ˚
(8.8)
176
Materials Science
Similarly, the energy states available within one octant of the sphere of radius n + dn and its energy E + dE is =
1 È4 3˘ p ( n + dn ) ˙ Í 8 Î3 ˚
(8.9)
Therefore, the number of energy states available within the sphere of radius n and n + dn is obtained by finding the energy difference between the two energy levels namely E and E + dE. N(E) d(E) = =
1 È4 1 È4 3˘ ˘ p ( n + dn ) ˙  Í p n3 ˙ Í 8 Î3 ˚ ˚ 8 Î3 1 Ê 4p ˆ È 3 3 Á ˜ ( n + dn )  n ˘˚ 8Ë 3 ¯ Î
Expanding (n + dn)3, we get p 3 n + dn3 + 3n 2 dn + 3ndn 2  n3 6
(
N(E) d(E) =
)
(8.10)
Simplifying the above Eq. (8.10) using (a + b)3 = a3 + b3 + 3a2b + 3ab2, we get N(E) d(E) =
p dn3 + 3n 2 dn + 3ndn 2 6
(
)
Neglecting the higher powers of dn, i.e., dn2 and dn3, we get N(E) d(E) =
p 3n 2 dn 6
(
)
Simplifying the above equation, we get
or,
N(E) dE =
p 2 n dn 2
(8.11)
N ( E ) dE =
p n (ndn) 2
(8.12)
Consider a cubic metal piece with cube edge l. Therefore, the energy of electron within the cube is E=
n2h2 8ml 2
Rearranging the above equation, we get n2 =
8ml 2 E h2
(8.13) 1/ 2
È 8ml 2 E ˘ n =Í 2 ˙ Î h ˚
or,
The value of ndn is obtained by differentiating Eq. (8.13) 2
i.e.,
2ndn = 8ml E 2
h
(8.14)
Statistics and Band Theory of Solids
ndn =
or,
8ml 2 dE 2h 2
177
(8.15)
Substituting the value of n and ndn from Eqs. (8.14) and (8.15) in Eq. (8.12), we get N(E)dE =
p Ê 8ml 2 E ˆ 2 ÁË h 2 ˜¯
1/ 2
Ê 8ml 2 ˆ ÁË 2h 2 ˜¯ dE
Simplifying the above equation, we get N(E)dE =
p Ê 8ml 2 ˆ 4 ÁË h 2 ˜¯
3/ 2
E1/ 2 dE
(8.16)
where l3 is the volume of the metal piece. According to Pauli’s exclusion principle, we know that two electrons with opposite spin occupy each state. Therefore, the number of energy states available for electron occupancy is p Ê 8m 2 ˆ N(E)dE = 2 ¥ Á 2 ˜ 4Ë h ¯
3/ 2
E1/ 2 dE
(8.17)
Equation (8.17) is the effective number of energy states in a volume l3 with energy between E and E + dE. The number of available energy states per unit volume l3 = 1. We know that, Z(E) d(E) =
Density of states
N (E) d (E) V
Substituting the value of N(E) d(E) and l = 1, in the above equation, we get Density of states
Z(E) dE =
p Ê 8m ˆ Á ˜ 2 Ë h2 ¯
3/ 2
E1/ 2 dE
(8.18)
Equation (8.18) is the density of energy states, i.e., charge carrier in the energy interval E and E + dE. One can determine the carrier concentration in the metals and semiconductors using the above equation.
8.3 CARRIER CONCENTRATION (FREE ELECTRON DENSITY) IN METALS The concentration of the carrier nc, i.e., number of electrons per unit volume in the given energy levels E and E + dE is obtained by integrating the product of the density of states and the probability of occupancy f (E). nc = Ú Z ( E ) f ( E ) dE
Therefore,
(8.19)
Substituting the values of Z(E) and f (E) in the above equation, we get nc = Ú
4p 1 (2m)3/ 2 E1/ 2 dE ( E  EF )/ KT 3 h 1+ e
Equation (8.20) gives the carrier concentration in the given energy level E + dE.
(8.20)
178
Materials Science
8.4
8.4.1
EFFECT OF TEMPERATURE ON FERMI ENERGY FUNCTION Determination of Fermi Energy at 0 K
In metals, at 0 K, the electrons occupy up to the Fermi level EF. Therefore, f (E) = 1 for energy levels between E = 0 and E = EF. Substituting the above values in Eq. (8.20), we get 4p (2m)3/ 2 E1/ 2 dE h3
nc = Ú
The evaluation of integration in the above equation gives the concentration of electrons in a band in terms of Fermi energy level EF. At T = 0, EF = EFo, i.e., EFo is the highest energy level occupied by the energy at T = 0 K. The above integration is valid only E < EFo. Therefore, integrating the above equation at T = 0 K, we get Ê 2ˆ EFo = h ÊÁ 3n ˆ˜ ÁË 8m ˜¯ Ë p ¯
2/3
(8.21)
EFo = B n2/3
or,
B=
where,
Ê h2 ÁË 8m
e
(8.22)
ˆ Ê 3ˆ ˜¯ ÁË p ˜¯
2/3
is a constant and is equal to 5.85 ¥ 1038 J.
Equation (8.22) is used to determine the highest energy level, i.e., Fermi energy level (EFO) occupied by an electron at T = 0 K by knowing the value of the carrier concentrations. The value of EFO for few important metals is given in Table 8.1.
Table 8.1
Highest Energy Level EFO at 0 K
Metals
Values of n (¥ 1028 m3)
EFO
Cu
8.491
7.06
Zn
13.153
9.45
Al
18.066
11.68
Mean Energy of Electron at T = 0 K Consider that Eave is the average energy of the electron at 0 K, Therefore, 1 EF o Eave = Ú N ( E ) dE E n o Substituting the values of N(E)dE in the above equation, we get Eave =
1 EF o 4p (2m)3/ 2 E1/ 2 E dE Ú n o h3
(8.23)
Statistics and Band Theory of Solids
=
or,
EF o 1 4p (2m)3/ 2 Ú E 3/ 2 dE 3 nh o
179
(8.24)
Integrating the term, we get Eave = =
or,
1 4p 2 5/ 2 (2m)3/ 2 EFO 3 5 nh 1 4p 2 3/ 2 EFO (2m)3/ 2 EFO 3 nh 5
Substituting the values of EFO from Eq. (8.21) in the above equation, we get Eave
2/3 1 4p 2 Ê h 2 Ê 3n ˆ ˆ = ( 2 m) 3/ 2 Á ÁË ˜¯ ˜ 3 5 Ë 2m 8p nh ¯
3/ 2
EFO
(8.25)
1 4p 2 h3 Ê 3n ˆ ( 2 m) 3/ 2 Á ˜ EFO 3 5 (2m)3/ 2 Ë 8p ¯ n h
(8.26)
Rearranging the above equation, we get Eave =
Simplifying the above equation, we get 3 Eave = EF o 5
(8.27)
Equation (8.27) gives the average Fermi energy values occupied by electrons at 0 K. It is clear that Fermi energy of solids depends on density of electrons in the solid.
8.4.2 Fermi Energy of Electrons at Nonzero Temperature (T > 0 K) When the temperature increases, i.e., T > 0 K and hence (E  EF) >> KT. Therefore, the Fermi–Dirac distribution function can be written as, f (E) = e  ( E  EF )/ KT for E  EF > KT Therefore, the carrier concentration of electrons n=
top of theband
Ú
f ( E ) N ( E ) dE
(8.28)
o
Substituting the value of f (E) and N(E) in the above equation, we get n=
a 4p 3/ 2 2m ) Ú E1/ 2 e  ( E  EF )/ KT dE 3 ( h o
(8.29)
Substituting the value of n from the above equation (8.28) in Eq. (8.29), we get Eave =
1a  ( E  EF )/ KT dE Ú E N (E) e no
(8.30)
180
Materials Science
Fermi energy at any temperature is obtained by evaluating the above equation, EF (T ) = EFo
i.e.,
È p 2 È kT ˘ 2 ˘ Í1 Í ˙ ˙ ÍÎ 12 Î EFO ˚ ˙˚
(8.31)
and Eavg (T ) =
È 5p 2 È kT ˘ 2 ˘ 3 EFo Í1 Í ˙ ˙ 12 Î EFO ˚ ˙ 5 ÍÎ ˚
(8.32)
Equations (8.31) and (8.32) show that Fermi energy level decreases with increase in temperature, while average energy increase with increase in temperature. Thus, the variation in Fermi energy level with temperature is very small and hence, it is neglegiable.
8.5
SIGNIFICANCE OF FERMI ENERGY
Fermi energy levels are used to explain the flow of electrons when two metals are in contact, ptype and ntype semiconductors and Seebeck effect. Let us discuss briefly about the significance of Fermi energy levels in the following heading:
8.5.1
Metal – Metal Contacts
Consider two different metals namely, platinum (Pt) and molybdenum (Mo), respectively with work function 5.36 eV and 4.17 eV. The work function of Pt is higher than Mo which gives rise to higher Fermi energy level in Mo than Pt. When these metals are brought in contact as shown in Fig. 8.3, the electrons from the higher energy level flows into lower energy level, i.e., Mo to Pt. Therefore, the inner surface of Pt at the PtMo metal contact region becomes more negative while the inner surface of Mo becomes positive. The flow of electrons takes place until two energy levels are equal. As a result, a contact potential is developed across the PtMo contact region which is equal to 1.16 eV (5.36–4.2eV). The developed contact potential stops the further flow of electrons from Mo to Pt metals. Pt
Mo
Pt
Mo
EF EF
Electrons Electrons
Electrons 
+ + Electrons + +
EF
Fig. 8.3 PtMo metals contact Contact Potential Similarly, the flow of electrons and holes in pn junction semiconductor are explained using the Fermi energy levels. When a pn junction is formed, there is a difference in the Fermi energy levels between
Statistics and Band Theory of Solids
181
the ptype and ntype semiconductors. As a result, there is a flow of electrons from ntype to ptype and there is a flow of holes from ptype to ntype semiconductors. The transfer of electrons and holes take place until the Fermi levels in both the semiconductors reach the same level.
8.5.2
Seebeck Effect and Thermocouple
Consider that the two ends of the metal are kept at two different temperatures, say 273 K and 373 K as shown in Fig. 8.4. Therefore, in view of the difference in the temperatures between the two ends, flow of electrons from hot end to cold end starts. Therefore, more electrons are accumulated at the cold end and hence, it becomes more negative when compared to the hot end. Therefore, it develops a potential difference between the two ends of the metal, which is known as seebeck effect. One can use the seebeck effect to measure the thermo emf across the metals which are kept at different temperatures using the thermocouple. Metal 373 K
273 K
Fig. 8.4 Seebeck effect Consider two copper wires having the same Fermi energy levels are connected at their ends. One end of the wire is kept as cold end, i.e., at 273 K while the other end is kept as hot end, i.e., at 373 K. A voltmeter connected across the hot and cold ends as shown in Fig. 8.5(a) is used to measure the thermo emf generated between the ends. There is no flow of electrons between the hot and cold ends, since the same copper wire is used having the same Fermi energy levels. Therefore, there is no thermo emf across the ends and hence, voltmeter does not show any deflections. Cu
Cromel
Cu 373 K
Alumel
273 K
373 K
V
273 K
V (b)
(a)
Fig. 8.5 Thermocouple On the other hand, when two different metals having different Fermi energy levels say, Cromel (eV) and Alumel (eV) metals are connected and kept at two different temperatures, it generates an emf as shown in Fig. 8.5(b). Therefore, electrons flow from hot to cold end and hence, the voltmeter shows a deflection. The cromelalumel metal connects act as a thermocouple and is known as Ktype thermocouple. The thermocouples are obtained by connecting two different materials having different Fermi levels. The different types of thermocouples and the materials used are given in Table 8.2.
182
Materials Science
8.6
EFFECTIVE MASS OF AN ELECTRON
Consider the influence of an external field E on the electron when it is in a vacuum as shown in Fig. 8.6(a). The external field results in an increase in the force acquired by electron. According to Newton’s law of motion, the force acquired by the electron is F = ma. Let Fext be the force experienced by the electron when an external field is applied. Therefore, the acceleration of the electron a=
Fext m
(8.33) Electron
Ion
Vacuum
e E (a) Vacuum
E (b) Crystal
Fig. 8.6 Electron under the influence of an electric field On the other hand, when an external electric field E is applied to the crystal (Fig. 8.6(b)), the electron in the crystal acquires force both due to the external and internal fields. The field which exists in a crystal due to the periodic arrangement of atoms or ions is known as internal field. Let Fint be the internal field available in the crystal. Therefore, the acceleration exerted by the electron a=
Fext + Fint m
(8.34)
One cannot measure the internal force experienced by the electrons directly. Therefore, another mathematical expression is used to determine the acceleration exerted by the electron by considering the internal force into the system and replacing the mass of an electron as the effective mass (m*) of the electron as, a=
Fext m*
(8.35)
In Eq. (8.35), the effective mass (m*) of the electron incorporates all the internal forces that exist in the crystal. The behaviour of effective mass is same as that of classical mechanics. The effective mass of some of the important metals are shown in Table 8.2. Metals like Cu and Ag show that their effective mass is nearly equal to the mass of the electrons. The effective mass of electron in different metals are displayed in Table 8.2.
Expression for the Effective Mass Consider an electric field of strength E is applied to the crystal. The force exerted by the electron in the crystal is F = eE = ma
(8.36)
Statistics and Band Theory of Solids
183
Table 8.2 Effective Masses of Electrons in Different Metals Metals
me* / m
Cu Ag Au Bi K Li Na Ni Pt Zn
1.010 0.990 1.100 0.047 1.120 1.280 1.200 28.000 13.000 0.850
According to quantum concept, the electrons behave as a wave and hence, the group velocity is vg =
dw dk
(8.37)
where w is the angular frequency and k the wave vector or wave number and its value is equal to 2p/l. We know that the energy of the electron E = hw
(8.38)
Differentiating the above equation, we get dE = h dw dw = dE / h
or,
Substituting the value of dw in the above equation, we get the group velocity as vg =
1 dE h dk
(8.39)
The acceleration exerted by the electron is obtained by differentiating the above equation wrt, The acceleration exerted by the electrons or,
a= a=
dv g dt
=
1 d Ê dE ˆ Á ˜ h dt Ë dk ¯
1 d 2 E dk h dk 2 dt
(8.40)
One can determine the energy gained by the electron by considering the E – k diagram of the conduction band as shown in Fig. 8.7. When an electric field is applied, the electron gains energy and hence, it moves from one k value to another k value in the E – k diagram. The accelerated electron coincides with lattice vibration and hence, random scattering of electrons takes place. The scattered electron takes into another k value as shown in Fig. 8.7. Thus, the group velocity of the electron is determined from the gradient of the E – k diagram. Let Fext be the external force acting on the electron by the application of external field. The distance moved by the electron when it acquires energy externally is dt. Therefore, the energy gained by the electron
184
Materials Science
E
k4 k3
k1 k2
k
Fig. 8.7 Ek diagram of conduction band dE = Fext vg dt
(8.41)
Rearranging the above equation, we get Fext =
1 dE vg dt
(8.42)
Substituting the value of Vg from Eq. (8.39) in the above equation, we get Fext = h
dk dt
dk = Fext h dt
or, Substituting the value of
(8.43)
dk from Eq. (8.43) in Eq. (8.40), we get dt Fext a= 1 2 2 Èd E ˘ h Í 2˙ Î dk ˚
(8.44)
Comparing the value of a with a = F/m, we get F = m
Fext Èd E ˘ h Í 2˙ Î dk ˚ 2
1
=
Fext m*
(8.45)
2
1
Èd2E ˘ where m* = h 2 Í 2 ˙ known as the effective mass of the electron and it depends on the E – k diagram. Î dk ˚ Consider an E – k diagram for a valance band which is downward concave as shown in Fig. 8.7. The effective mass of an electron, which is at the top of the valance band is negative. The negative sign of the effective mass indicates that the electrons are deaccelerating by the application of the external field. Generally, the effective mass of a crystal depends on curvature (d2E / dk2), on the E – k diagram. Thus, the E – k diagram of the crystal depends on the nature of bonding and the symmetry of the crystal structure. Cyclotron resonance method is generally used to determine the effective mass of the crystal.
Statistics and Band Theory of Solids
185
8.7 CONCEPT OF HOLE One can explain the concept of hole by plotting a graph between energy of an electron energy E and wave vector k known as Ek diagram as shown in Fig. 8.8. In Fig. 8.8(a), all the states in both bands b and b’ are filled by electron and hence, there is no vacancy state. On the other hand, in Fig. 8.8(b) all the states are not filled in band b while there is a vacancy or empty state of an electron in band b. The absence of an electron or empty state is known as a hole. (1) We know that the total wave vector in a filled energy band is zero. Let k be the wave vector of an electron in the band b and k be the wave vector of an electron in band b'. In Fig. 8.8(a), all the states are filled and hence, the total wave vector in a filled energy band is zero. However, in Fig. 8.8(b), there is one extra wave vector in band b' since there is an empty state in band b. This empty state or space is known as hole and its wave vector is kh. Therefore, the wave vectors of the hole and electrons are equal in magnitude but opposite in nature, i.e., kh = ke. E
E b
b'
k
k
b
b'
k
k
(a) Filled states
(b) Empty state
Fig. 8.8 E – k diagram of valence band (2) The wave vectors of hole and electrons are equal and opposite in magnitude. Therefore, the electron which is missing in the valence band is excited to conduction band. (3) The charge for a hole is positive, i.e., e+, while the charge of an electron is negative, i.e., e. (4) The energy of hole and electrons are equal but opposite in magnitude, i.e., eh (kh) = ee ( ke) =  ee (ke). (5) When an electric field is applied to a band, the negatively charged electrons move opposite to the field direction (Fig. 8.9). On the other hand, the positively charged holes move with same velocity as that of electron in the same direction of the field, i.e., vh = ve E(¨ E )
E k A
B
C D E FG
H
E k
CD E FG B H A
k A
B
C D E FG
H
Fig. 8.9 Motion of a hole—Applied field (6) The effective mass of an electron at the top of the valence band is negative, while it is positive for hole due to its opposite charge as that of electron.
186
Materials Science
(7) The equation of the motion of an electron is h
dke =  e ( E + ve x B ) dt
(8.46)
Similarly, the equation for motion of a hole is h
dkh = e ( E + vh x B ) dt
(8.47)
(8) The equation for the current density for an electron is J =  neV
(8.48)
Similarly, the equation for current density of a hole is J = neV
8.8
(8.49)
BAND THEORY OF SOLIDS – ORIGIN OF ENERGY GAP
The quantum free electron theory of metals assumes that the free electrons known as conduction electrons are fully responsible for the conduction mechanism. The above theory explains phenomena like specific heat capacity, electrical conductivity, thermal conductivity, electrodynamics of metals, photoelectric effect, compton effect, etc. However, it fails to explain many other physical properties. This model fails to explain the distinction between metal, semiconductor and insulator. Similarly, it fails to explain the positive values of the Hall coefficient. Therefore, the band theory of solids was proposed to overcome the failures of quantum free electron theory. In order to explain the band theory of solids, cyclic or periodic boundary conditions is used to explain the free electrons. Consider the onedimensional periodic arrangement of positively charged ions inside a crystal as shown in Fig. 8.10. The motion of the free electrons inside the positively charged ion core is shown in Fig. 8.10(a). Therefore, the wave function of the electron is y (x) = Ae
jkx
(8.50)
where k is the wave vector and A the amplitude. +
+
+
+
+
+
+
+
+
+
+
+
+
+
+
+
(a) Motion of electron PE A
B
C
D
E
a (b) Potential energy variation
Fig. 8.10 Onedimensional periodic potential
Statistics and Band Theory of Solids
187
The potential energy of the freely moving electron at the positive ion site inside the crystal is zero while it is maximum at the middle. On the other hand, outside the crystal, the potential energy is infinite. Therefore, the potential energy of the moving electrons varies periodically with same period as that of crystal as shown in Fig. 8.10(b). Therefore, momentum (p) and energy (E) of the moving electron is 2 hk and È( hk ) / 2m ˘ , respectively. Î ˚ When an electron moves in a periodic potential it undergoes similar effects such as reflection and diffraction as that of an ordinary wave. The electrons which satisfies the Bragg’s condition for reflection during its motion in a periodic potential takes k vector. A
B
C
D
E
a
Fig. 8.11 Reinforcement of electron waves Consider the arrangements of atoms in a periodic potential as shown in Fig. 8.11. Let us consider that electrons are moving along the positive xdirection in the periodic potential. When the electron wave incident on atom A, a part of the wave gets reflected back for a while, the remaining part of the wave gets transmitted through it. Similarly, when a part of the transmitted wave is incident on atom B, a part of the wave gets reflected back while a part is transmitted through it and this process continues. All the reflected electron waves from atoms A, B, C etc., are reinforced when it satisfies the Bragg’s condition. Therefore, the formation of standing wave pattern takes place due to reinforcement of waves when the path difference between the reflected waves from atoms A and B is 2a. Therefore, interference patterns is obtained when 2a = nl
(8.51)
where n is an integer and it takes the value 0, 1, 2, 3, etc., and l the wave length. We know that wave vector k = 2p/l. Substituting the k value in the above equation, we get p (8.52) a Equation (8.41) indicates that the standing wave patterns are formed due to the reinforcement of reflected beams whose wave vector is in the order of p/a. Wave vector k = n
Therefore, the equation for the wave function of the travelling wave is y+(x) = A e jkx
(8.53)
Similarly, the wave function for the reflected wave is y(x) = A ejkx
(8.54)
We know that the formation of the standing wave pattern takes place only when wave function y+(x) and y(x) are reinforced. It is clear from Eqs. (8.53) and (8.54), the reinforcement takes places in two different ways namely, y1(x) = y+(x) + y(x)
(8.55)
y2(x) = y+(x)  y(x)
(8.56)
188
Materials Science
Substituting y+(x) and y(x) from Eqs. (8.55) and (8.56) respectively in the above equations, we get y1(x) = Ae jkx + Ae jkx = A cos
np x a
(8.57)
y2(x) = Ae jkx  Ae jkx = A sin
np x a
(8.58)
Let r(y) be the probability density function or charge density of the standing wave pattern. Therefore, the probability density for the above two standing waves are 2
r(y1) = y 1 = A2 cos 2 2
r(y2) = y 2 = A2 sin 2
np x a
(8.59)
np x a
(8.60) r1(y1) r2(y2)
Fig. 8.12 Piling of energy by charge density The energies associated with standing wave of the above two wave functions are used to determine the energy gap.
Brillouin Zones The energy of an electron moving in a periodic potential is limited within allowed regions or zones. One can determine the energy gap by finding the difference in the potential energies of the electrons piled with two different waves functions namely y1(x) and y2(x). Figure 8.12 shows the piling of standing waves y1(x) and y2(x). The wave function y1(x) piles the maximum energy of the electrons at the positive ion cores. Therefore, the wave function y1(x) gives the potential energy of the standing wave. On the other hand, the wave function y2(x) piles the energy of the electrons at the middle of the positive ion cores. Thus, it increases the potential energy of the wave function than potential energy of the standing wave. Therefore, the difference between the potential energies of the electrons piled by these two wave functions y1(x) and y2(x) gives the energy gap i.e., Energy of electron We know that wave vector
E=
( hk ) 2 2m
k = ± n (p/a).
(8.61) (8.62)
The relationship between the energy and wave number for a onedimensional lattice is obtained by plotting a graph between total energy E and wave vector k as shown in Fig. 8.13. Figure 8.13 demonstrates the origin of energy gap in electron energy at the Brillouin zone boundaries. The energy and wave vector graph shows discontinuities in the energy band at k = ± p/2, ± p ... etc. It is clear from Fig. 8.13 that electron has an allowed energy value in the region or zone between k =  p/a and k = +p/a. This zone is known as first Brillouin zone. Similarly, energy value that lies between the band k =  p/a to k = pa
Statistics and Band Theory of Solids
189
E
Second First First Second Brillouin Brillouin Brillouin Brillouin Zone Zone Zone Zone
Band
Energy
2V1
Energy gap
Forbidden energies
Band Es –k
–2p/a
–p/a
O
Energy gap
2V1 Ec
2p/a
k
Allowed energies
Band
p/a
Fig. 8.13 Energy gap—Brillouin zone boundaries and k = +p/a to k = +p a is known as second Brillouin zone. The break between the first and second Brillouin zones is called as forbidden region or forbidden band or forbidden zone. One can also define the higher order Brillouin zones.
Energy Gap One can determine the band gap energies by considering the interaction of the electron with the periodic potential of the lattice. Consider that an electron beam is incident in a twodimensional arrangement of lattice system as shown in Fig. 8.14. The incident electron gets reflected both at k = ± p/a and 2p k= ± . When k = ±p/a, the electron gets reflected from planes [0 1] and [1 0], while it gets reflected a 2p . from plane [1 1] when k = ± a k1 k3 k2
[1 0]
[0 1] a
a 2 a
[1 1]
Fig. 8.14 Reflection of wave vectors by [0 1] and [1 1] planes
190
Materials Science
We know that k sin q = ±
np a
(8.63)
In order to determine the energy gap in the crystal lattice, the interaction of electron in all possible directions is to be considered. The minimum and maximum energy value in each band depends on the crystal direction. Therefore, the energy of the electron as a function of the crystal direction is shown in Fig. 8.15. For the [1 0] plane, E1 is the maximum energy value while E2 is the minimum energy value. However, for the [1 1] plane, E1’ is the maximum energy value which is higher than E1 and E2’ is the lower energy value which is lower than E2. Therefore, the energy gap E2’ E1’ is low when compared to E2  E1.
Band
Second Brillouin zone
Energy gap
Band
First Brillouin zone
Band
Second Brillouin zone
k1[1 0]
Energy gap
E
Band
k
p/a (a) [1 0] plane
First Brillouin zone
k3[1 1] 2/pa
(b) [1 1] plane
Fig. 8.15 E—k diagram
8.8.1
Classification of Materials
The overlapping of the first and second Brillouin zone in a crystal lattice is shown in Fig. 8.16. The overlapping of the first Brillouin zone of [1 0] electron over the second Brillouin zone of [1 1] electron results a continuous distribution of energy. Therefore, electron finds any energy (Fig. 8.16(a)) and hence, the material is a metal. Similarly, the first Brillouin zone of [1 0] direction overlap with the first Brillouin zone
Statistics and Band Theory of Solids
191
which of [1 1] direction which results in an energy gap as shown in Fig. 8.16(b). Thus, the electron does not find any energy in between the bands and hence, the material is known as semiconductor or an insulator. Eg2
Band
Band
Eg1 Band
Gap
+
Eg2
Band
[1 0]
Band Eg1
= Band
[1 1]
Band [1 0]
(a) Semiconductor or insulator of metal
Band +
Band =
Eg1
Eg
Band
Band
[1 1] (b) Metal
Fig. 8.16 Classification of materials
8.9 THE KRONIGPENNEY MODEL The periodic potential for the motion of electron inside the crystal is uniform. The above conclusion is arrived based on the free electron theory. On the other hand, according to KronigPenney model, the periodic potential for the motion of electron inside a crystal is not uniform; rather it has variable potential energy due to the presence of immobile lattice ions in a crystal. A graphical representation of potential energy for an electron in a one dimensional solid is shown in Fig. 8.17. One can infer from Fig. 8.17 that the electron acquire a maximum potential energy at the middle of any two ions while it acquires minimum potential energy at the position of the ions.
Potential energy
v
a
(ion)
x distance
Fig. 8.17 Potential energy of the electrons as a function of distance in a one dimensional crystal Kronig and Penney replaced the graphical model shown in Fig. 8.17 by another figure, Fig. 8.18 to represent the potential energy of the electron in a periodic lattice. Figure 8.18 show the periodic potential in a onedimensional solid. The periodicity is (a+b). The important salient features of this simplified potential barriers of electrons are (i) same period as that of lattice, and (ii) minimum potential at the position of ions and the maximum potential at the middle of any two ions. The potential energy of the electron is obtained by solving the Schrödinger’s equation with a periodic potential.
192
Materials Science
V Vo
region region 1 2 –(a+b)
–b
0
a
a+b
X
Fig. 8.18 Periodic potential of electron in a onedimensional solids – KronigPenney model The time independent Schrödinger equation for an electron in a onedimensional solid is 
h2 d 2y + ( E  V ( x )) y = 0 2m dx2
(8.64)
where V(x) is the periodic potential due to the lattice. One can obtain the wave function associated with this model by solving Eq. (8.64) with its limit V(x) = V0 /2 and V(x) = V0 /2 seperately. Bloch’s theorem is used to solve the Schrödinger equation with the above two limitations. Therefore, the solution to the Eq. (8.17) is y ( x ) = uk ( x ) eikx
(8.65)
where uk (x) is a periodic function, i.e., it has the same periodicity as that of the lattice. The periodic function uk (x) satisfies the following condition: uk (x) = uk (x + a)
(8.66)
where k refers to the given state of electron. It is clear that the solutions to the Schrödinger’s equation in a periodic potential are the plane waves, i.e., eikx. These planes waves are modulated by the function uk(x). The periodic function uk(x) has the same periodicity as that of the lattice, which states the Bloch’s theorem. In view of various mathematical steps involved in the evaluation of Schrödinger’s equation, let us take the final equation for discussion. i.e.,
cos ka = P
sin a a + cos a a aa
(8.67)
where
P=
ma V0 w h2
(8.68)
and
a=
2mE h
(8.69)
It is easy to discuss the periodic potential of electrons in a solid by drawing a graph between a a and sin a a (P + cos a a) as shown in Fig. 8.19. aa
Statistics and Band Theory of Solids
193
The righthand side of Eq. (8.67) is plotted as a function of a a for given P value. The resultant graph is an oscillating curve as shown in Fig. 8.19 consisting of both positive and negative values. The amplitude of the curve decreases with increase in a a values. The lefthand side of equation consists of cosine function with a limitation of +1 to –1. These two limits of cosine functions are represented as horizontal lines in Fig. 8.19. The curve which lies within the limits of +1 and 1, satisfies the equation Eq. (8.67), while the curve lies outside the limits of +1 and 1 are not satisfying the conduction. Thus, the shaded position of the curve is not valid. Therefore, the curve which lies within the distance of +1 to 1 is in the allowed ranges of a a and hence, it is marked as dark as shown in Fig. 8.19. The important observation made from the above results on the energy of electrons in a periodic potential is as follows. (1) The electron possesses energies within certain bands and there is no energy outside the bands. Thus, the energy bands are separated by a forbidden energy range known as energy gaps. (2) An increase in the width of allowed bands with increase in aa value. The width of any particular band decreases with increase in P value, i.e., binding energy of electrons.
P
sin aa + cos aa aa
+1 aa –1 –3p
–2p
–p
0
p
2p
3p
sin a a Fig. 8.19 A plot of ( P a a + cos a a) as a function a a
Case (i) When P is large When P is large the allowed regions of electron becomes very narrow. In addition, the curve is very steep and its lies between minimum and maximum values of cos ka, i.e., from +1 to 1. Therefore at P =
or sin a a = 0.
i.e., a a= np Substituting the value of a in the above equation, we get 2mE a = np h
Simplifying the above equation, we get
or,
E=
n2p 2 h2 2ma2
E=
n2 h2 8ma2
(8.70)
194
Materials Science
Equation (8.70) gives the energy levels of an electron in a potential well of width a. It is clear from the above equation that the electrons are independent to each other. In addition, every atoms is confined to a similar atom through an infinite potential barrier.
Case (ii) When P = 0
When P = 0, cos ka = cos aa
i.e., k = a Substituting the value of a in the above equation, we get 2mE h
k= Simplifying the above equation, we get
or,
E=
( hk )2 2m
E=
p2 2m
(8.71)
Equation (8.71) represents the energy of the free electron. One can cover the whole range of the electrons from free electron to bound electron by varying the values of p between 0 and a.
Case (iii) When P = ±1 For an allowed region, the value of cos ka ranges from +1 to 1. cos ka = ±1 ka = np
i.e.,
k=
or,
np a
(8.72)
Thus, the discontinuity in electron energy occurs at an interval of n i.e.,
k =±
p , while n = 1, 2, 3…. a
p 2p 3p ,± , ± ,...., a a a
(8.73)
Equation (8.73) is used to obtain the energy of the electron E as a function of k. The dispersion curve p drawn between E and k consist of discontinuities at k = ± n , where n = 1, 2, 3…. as shown in Fig. 8.20. a
Energy gap E Energy band Energy gap –2p/a
–p/a
p/a 2p/a
Energy band
k
Fig. 8.20 Energy as a function of k
Statistics and Band Theory of Solids
195
The dispersion curve is used to determine the behaviour of electron in a periodic potential. The knowledge on the change in energy of electron in a crystal helps to understand the electron transport properties in that crystal.
8.10 BRILLOUIN ZONE According to KronigPenney model, the energy of electron in a solid contains discontinuities at certain value of k, while at k space the energy varies continuously. The kspace is the space in which three components of k values of electrons are represented graphically along x, y and z axis. Thus, the kspace is used to draw the boundaries to represent the continuous variation of energies. The zones which lie within the boundaries of Kspace are known as Brillouin zones. One can represent the Brillouin zones for one, two and threedimensional cases sepreately as given below.
8.10.1 Brillouin Zone in One Dimension The arrangement of atoms in onedimensional kspace is shown in Fig. 8.23. We know that in one dimensional case, the value of k is
k=
np a
(8.74)
where a is the lattice parameter of the crystal and n an integer. The value of n = ±1, ±2, ±3,…, etc. a 1st Zone
–2p/a
–p/a
+p/a
0
+2p/a
2nd Zone
Fig. 8.21 Brillouin zone – One dimension Substituting n = ± 1 in Eq. (8.74), we get k =±
p a
(8.75)
i.e., the region lies between k = p/a and k = –p/a is known as first Brillouin zone. Similarly, substituting n = ± 2 in Eq. (8.74), we get
k =±
p a
(8.76)
i.e., the regions lies between k = 2p/a and k = –2p/a except the first Brillouin zone are known as second Brillouine zone. The first and second Brillouin zones are represented graphically in Fig. 8.21.
196
Materials Science
Similarly, substituting n = ± 3 in Eq. (8.74), we get k = ±3
p a
(8.77)
i.e., the regions lies between 3p/a and 3p/a other than the first and second Brillouin zones are known as third Brillouin zones. Therefore, When the value of k lies between p/a £ k £ p/a, one can get the first Brillouin zone. When the value of k lies in between 2p/a £ k £ p/a and p/a £ k £ 2p/a, one can get the second Brillouin zone. When the value of k lies in between 3p/a £ k £ 2p/a and 2p/a £ k £ 3p/a, one can get the third Brillouin zone.
8.10.2
Brillion Zones in Two Dimensions
Let us consider the motion of an electron in a twodimensional square lattice. The equation for the wave vector in case of a twodimensional lattice is
n1kx + n2 k y = ( n12 + n22 )
np a
(8.78)
where n1 and n2 are the integers, respectively along x and y axis. The n represent the order of the Brillouin zone. It can takes the value like 1, 2, 3, etc. One can obtain the first Brillouin zone by substituting the values for n1 and n2. When n1 = ±1 and n2 = 0 in Eq. (8.78), we get kx = ±(p/a)
(8.79)
Similarly, when n1 = 0 and n2 = ±1 in Eq. (8.78), we get ky = ±(p/a)
(8.80)
Therefore, the square bounded by the lines kx = ±p/a and ky = ±p/a represents the first Brillouin zone. The square ABCD in Fig. 8.24 is the first Brillouin zone for a twodimensional square lattice. Similarly, one can obtain the second Brillouin zone by substituting the values for n1 and n2 in Eq. (8.78). When n1 = +1 and n2 = +1 in Eq. (8.78), we get kx + ky = 2p/a
(8.81)
When n1 = +1 and n2 = 1 in Eq. (8.78), we get kx  ky = 2p/a
(8.82)
Similarly, for other values of n1 and, we get For n1 = 1 and n2 = 1 kx + ky = 2p/a
(8.83)
Statistics and Band Theory of Solids
197
and n1 = l and n2 = 1 kx  ky = 2p/a
(8.84)
The Eqs. (8.81) to (8.84) are the set of four lines at 45∞ to both kx and ky axis and passes through the ±2p/a. These intercepts are represented as E, F, G and H in Fig. 8.24. The area of the second Brillouin zone is in between the square EFGH and ABCD. Similary, the third Brillouin zone is obtained by substituting n1 = 0, ±1 and ±2 and n2 = 0, ±1 and ±2 in Eq. (8.78) with n = 3 and graphically shown in Fig. 8.24. E
B
A p a ky
H
kx
–p a
–2p a
F –2p a
p a
–p a
1st Zone 2nd Zone 3rd Zone
D
C
G
Fig. 8.22 The first three Brillouin zones for a twodimensional lattice It is an interesting observation to note that the first Brillouin zone is square, while the second Brillouin zone is obtained by adding a triangle to each face of the square. Similarly, the third Brillouin zone is obtained by adding a triangle to each face of the second Brillouin zone.
8.10.3 Brillouin Zones in Three Dimensions The equation for k vectors in three dimension lattice is
kx n1 + k y n2 + kz n3 =
p 2 ( n1 + n22 + n32 ) a
(8.85)
One can obtain the first Brillouin zone by substituting the value of n1, n2 and n3. When n1 = ±1 and n2 = n3 = 0, we get
kx = ±
p a
(8.86)
ky = ±
p a
(8.87)
When n2 = ±1 and n1 = n3 = 0, we get
198
Materials Science
When n1 = n2 = 0 and n3 = ±1, we get
kz = ±
p a
(8.88)
The graphical representation of kx, ky and kz values give cube structure. One can obtain the second Brillouin zone by adding a pyramid to each face of the cube. Similarly, the third Brillouin zones are obtained by adding a pyramid to each face of the second Brillouin zone.
8.11
EXPLANATION OF BAND GAP
One can explain the origin of the energy gap by considering the formation of energy bands in solids. We know that, the concentration of the atoms in the gaseous medium is less and/or loosely packed when compared to concentration of the solid medium. The interatomic distance in the gaseous state is very large and hence, the interaction of any two atoms in gaseous state is very weak. On the other hand, in the interatomic distance in the solid state is very large and hence, leads to a strong interaction between any two atoms in solid materials. Thus, in solids, the interaction of the atoms is overlapped with each other. Therefore, the continuously energy state formed. This continuum state is separated into two different bands namely valance band and conduction band through an energy gap. This gap is known as forbidden gap or energy gap. The difference between the metals, semiconductor and insulators are explained by band gap. The band structure for the metal, semiconductor and insulator are shown in Fig. 8.23. The comparison between the metal, semiconductor and insulator are given in Table 8.4.
Valence band (a) Conductor
Large energy gap
Valence band
Conduction band Band energy
Overlap
Conduction band Band energy
Band energy
Conduction band
(b) Insulator
Small energy gap Valence band
(c) Semiconductor
FIg. 8.23 Bang gap
Table 8.4 Comparison Between Metal, SemiConductor and Insulator Sr. No
Conductors
Semiconductors
Insulators
1.
The valance band is completely filled.
At room temperature, few electrons are filled.
The valence band is completely filled.
2.
The forbidden energy gap is zero.
The forbidden energy gap is ~1 The forbidden energy gap in the order of few MeV which is or 2 eV which is very small when compared to an insulator. higher than semiconductor.
3.
Electrons are loosely bound to the nucleus.
Electrons are not tightly bound to the nucleus.
4.
It will conduct electricity It will conduct electricity at normal condition. partially at normal condition.
Electrons are tightly bound to the nucleus. It will not conduct the electricity at normal condition.
Contd.
Statistics and Band Theory of Solids
199
Table 8.4 (Continued) Sr. No
Conductors
Semiconductors
Insulators
5.
The resistivity of conductor is very small and it is in the order of few mill ohm m.
The resistivity of semiconductor is very less and it is in the order of 0.5 to 103 ohm m.
The resistivity of an insulator is very high and it is in the order of 107 to 1012 ohm m.
6.
Example for conductor Example for semiconductor are Example for insulator are are copper lithium, gold, silicon, germanium, gallium ebonite, glass, rubber, glass silver, etc. Arsenide, cadmium sulphate, etc. fibre, porcelain, etc.
Generally, the band gap in semiconductor is classified into types.
8.11.1
DIRECT BAND GAP SEMICONDUCTORS
In a semiconductor, a direct band gap means that the minimum of the conduction band lies directly above the maximum of the valence band in the EK space. In a direct bandgap semiconductor, electrons at the conductionband minimum can combine directly with holes at the valenceband maximum, while conserving momemtum (Fig. 8.24). The energy of the recombination across the band gap will be emitted in the form of a photon of light. This is radiative recombination which is also called spontaneous emission. E X L
Eg
Photon K
(a) Direct band gap
Fig. 8.24 Direct band gap The example for a direct bandgap semiconductor is gallium arsenide which is commonly used in laser diodes.
8.11.2
INDIRECT BAND GAP SEMICONDUCTORS
Not all semiconductor materials have the minimum of the conduction band above the top of the valence band in the EK band structure. These materials are known as indirect semiconductors. The examples are Si, Ge, etc. Indirect band gap is a band gap in which the minimum energy in the conduction band is shifted by a kvector relative to the valence band. The kvector difference represents a difference in momentums (Fig. 8.25).
200
Materials Science
E L X
DE
Photon Ephoton Eg –DE
Eg
Photon h K
(b) Indirect band gap
Fig. 8.25 Indirect band gap Semiconductors that have an indirect band gap are inefficient at emitting light. This is because any electrons present in the conduction band quickly settle into the energy minimum of that band. Electrons in this minimum require some source of momentum allowing them to overcome the offset and fall into the valence band. Photons have very little momentum compared to this energy offset. Since the electrons cannot rejoin the valencc band by radiative recombination, conduction band electrons last quite some time before recombining through less efficient means. The indirect (nonradiative) recombination takes place at point defects or at grain boundaries in Si. If the excited electrons are prevented from reaching these recombination places, they will fall back into the valence band by radiative recombination. The absorption of light at an indirect gap is much weaker than at a direct one. As in the emission process, both the laws of conservation of energy and of momentum must be observed. The only way to promote an electron from the top of the valence band to the bottom of the conduction band is to simultaneously emit (or absorb) a phonon that compensates for the missing momemtum vector. However, such a combined transition has a much lower probability. The absorption of an indirect band gap material usually depend more on temperature than that of a direct band gap material, because at low temperatures phonons are not available for a combined process. From Fig. 8.25, we have Eg = hg + Ephonon
(8.89)
where Ephonon is the energy of a phonon and hg is the energy of the emitted photon. Let us consider the difference between direct and indirect bandgap semiconductors.
Table 8.5
Difference Between Direct and Indirect Bandgap Semiconductors
Sr. No
Direct bandgap semiconductor
1.
As shown in the band diagram, the minimum energy of conduction band and maximum energy of valence band are have the same value of wave vector.
Indirect bandgap semiconductor As shown in the band diagram, the minimum energy of the conduction band and maximum energy of the valence band having different values of wave vector.
Contd.
Statistics and Band Theory of Solids
201
Table 8.5 (Continued) Sr. No
Direct bandgap semiconductor
Indirect bandgap semiconductor
2.
An electron from the conduction band can recombine with a hole in the valence band directly emitting a light photon of energy hg.
An electron from the conduction band can recombine with a hole in the valence band indirectly through traps. Here, there is emission of photon along with phonon. The emission of phonon leading to the rise of temperature of the material.
3.
Lifetime (i.e., recombination time) of charge carriers is very less.
Lifetime of charge carriers is more.
4.
Due to emission of light photon during recombination of charge carriers, these are used to fabricate LEDs and laser diodes.
Due to longer lifetime of charge carriers, these are used to amplify the signals as in case of diodes and transistors.
5.
These are mostly from the compound
These are mostly from the elemental semiconductors.
6.
Examples: In P, Ga As
Examples: Si, Ge
8.12 CONDUCTIVITY OF COPPER AND ALUMINUM Material properties like electrical conductivity are widely used to select the materials for wide range of applications. Even though, copper and aluminum are monovalent metals, the resistivity of copper is higher than aluminum, i.e., the electrical conductivity of Cu (5.88 ¥ 107 W1m1) at room temperature is lower than that of aluminum (6.21 ¥ 107 W1m1). We know that the electrical conductivity of a metal is, s=
ne 2t r m
(8.90)
where n is the concentration of electrons and tr the relaxation time, m is the mobility of the electrons and is equal to m = e t r /m. Therefore, Electrical conductivity s = ne m
(8.91)
Table 8.6 displays some of the electrical properties of Cu and Al. The important properties of pure Cu such as, highest conductivity next to silver, good mechanical strength, fairly resistant to corrosion and formability into wires or strips or rolled sheets help to use for many electrical applications. The addition of metals like Fe (0.2% ) or As (0.3%) reduces the electrical conductivity to nearly 50%. In view of the high resistivity of aluminum (1.6 times greater) than Cu, it replaces the Cu for many industrial applications. Manganin is an alloy of Cu, Ni and Manganese. Constantan is an alloy of Cu and Ni. It has constant resistance over a wide temperature range. For contact materials operating at high currents alloys of Cu like CuWNo is used. Solders, which are alloys having lower melting points than the metals to be connected. Alloys like SnPbCd (melting point 145–180°C) and CuZn alloy (hard solder) (melting point 825 – 860°C) are used for soldering.
202
Materials Science
Table 8.6 Electronic Properties of Cu and Al Metal
s
(W1
m1)
n (m1)
m* / me Lattice Constant (a) A°
EF eV
me (m2 / voltsec.)
Cu
5.88 ¥ 107
8.5 ¥ 1028
1.01
3.61
7.00
4.3 ¥ 103
Al
6.21 ¥ 107
5.85 ¥ 1028
0.99
4.05
11.8
7 ¥ 103
8.13
EFFECT OF TEMPERATURE AND IMPURITY ON ELECTRICAL RESISTIVITY OF METALS (MATTHIESSEN’S RULE)
We know that the resistivity of the metals is due to the scattering of the conduction electrons. The resistivity of the metal is divided into two components namely ideal and residual resistivity. Generally in metals, the scattering takes place in the mechanism which results in the component of resistivity namely rph and ri. When the electrons are scattered by lattice vibration, i.e., phonons free from all defects give rise to ideal resistivity rph. The ideal resistivity is temperature dependent. On the other hand, when the electrons are scattered by the presence of the impurities and imperfection like dislocation vacancies, grain growth and boundaries, give rise to residual resistivity. The residual resistivity is independent of temperature and hence, the remaining does not need to be zero even at T = 0 K. Therefore, the resistivity of a metal is Resistivity of metal r = rph + ri
(8.92)
Equation (8.87) is known as Matthiessen’s rule. According to Matthiessen’s rule, the total resistivity of a metal is the sum of resistivity due to phonons scattering which depends on temperature and the resistivity due to the scattering by impurities which is independent of temperature. Assume that there is no scattering mechanism, r ph =
m ne 2t ph
(8.93)
Similarly, if there is no scattering by lattice vibration ri =
m ne 2t i
(8.94)
Substituting the rph and ri in Eq. (8.65), we get
or,
r=
m m + 2 2 ne t ph ne t i
r=
m Ê 1 1ˆ + ˜ 2 Á ne Ë t ph t i ¯
(8.95)
Statistics and Band Theory of Solids
203
Equation (8.90) is used to explain the effect of temperature and impurities on electrical resistivity of metals. The temperature dependent resistivity of metal expects the superconducting metal is shown in Fig. 8.17. At low temperature, the amplitude of lattice vibration is very small and hence, the scattered electrons are also very less. Thus, it results in a larger tph and hence, the rph is almost equal to zero. Therefore, the total resistivity of the metal is equal to r = ri
(8.96)
Resistivity (r)
It is clear from the Eq. (8.91), that the resistivity of a metal has a residual resistivity ri at T = 0 K as shown in Fig. 8.17. On the other hand, when the temperature increases, the amplitude of lattice vibration increases and hence, the scattering of electrons by the lattice also increases. Therefore, the resistivity of lattice vibration is added to total resistivity (rph + ri) and hence, a linear increase in resistivity with increases in temperature is observed at low temperature as shown in Fig. 8.17.
r = rc + rph rphdT rph re (Scattering by impurity)
Temperature T
Fig. 8.26 Temperature dependent resistivity of metal At high temperatures, the scattering effects due to phonons overcome the effect due to scattering and impurities which give rise to the resistivity which depends on lattice vibration only. As a result, at higher temperature, the resistivity of metals which depends purely on lattice vibrations varies exponentially than at lower temperature. Similarly, at low temperature, the resistivity of metal depends on lattice vibration and residual resistivity and hence, shows a linear variation with temperature. In a pure metal, the scattering of electrons takes place only due to lattice vibrations. But in case of impure metals, the scattering of electrons is both due to the lattice vibrations and impurity scattering. Therefore, the mean free time of electrons for impure metals is of two components namely, (i) the mean free time due to lattice vibration, and (ii) the mean free time due to impurity atoms. The total mean free time is given by, 1 1 1 = + t tT t I
(8.97)
204
Materials Science
where tT is the mean free time due to thermal scattering (i.e., lattice vibrations) and tI the mean free time for electrons due to impurity scattering. The drift mobility (md) is also written as, 1 1 1 = + md mT m I
(8.98)
where mT is the mobility of electrons due to thermal scattering and mI the mobility of the electrons due to impurity scattering. The electrical resistivity of an impure metal is written as, 1 1 1 = + r ne mT ne m I
(8.99)
r = rT + r I
(8.100)
where rT is the resistivity of the metal due to thermal scattering and rI the resistivity of metal due to impurity scattering. The resistivity of the metal due to thermal scattering is known residual resistivity rR. Hence, the resistivity of an impure metal is r = rR + rI
(8.101)
Equation (8.97) is known as Matthiessen’s rule.
8.14
HIGH RESISTIVITY MATERIALS
Generally, high resistivity materials are used for variety of applications such as heat elements, resistors and resistance thermometers.
8.14.1
Heating Elements
Heating elements are made in the form of coil to permit thermal expansion and contraction during heating and cooling respectively. The properties like melting point, resistivity and oxidation resistance of heating elements are high. On the other hand, properties like thermal expansion and electric modulus are low. The low thermal expansion and electric modulus are required to reduce the fatigue in the heating elements due to the repeated heating and cooling.
8.14.2
Resistors
The high resistivity materials are used for resistor applications. It requires low value of temperature coefficient of resistance and thermoelectric potential. However, the materials should have high resistance to atmospheric corrosion and also a stable resistance.
Statistics and Band Theory of Solids
205
8.14.3 Resistance Thermometers The properties of the materials required for resistance thermometers are high temperature coefficient of resistance with an excellent sensitivity. The high resistivity materials are classified into two categories namely high resistivity metals and alloys.
High Resistivity Metals and Alloys Examples for high resistivity metals are tungsten and platinum, while nichrome, manganin, constantan, kanthal, alumel and cromel are examples for high resistivity alloys. The properties of high resistivity metals are given in Table 8.7. Similarly, the chemical compositions, properties and their applications, of high resistivity alloys are given in Table 8.8.
Table 8.7 Metal Tungsten
Properties of High Resistivity Metals Properties
Heavy metal
Applications Filament materials in electrical bulbs
Quickly oxidisation in inert atmosphere. Density ~19290 kg m–3 Specific gravity ~ 19.6 Melting point ~ 3683 K Resistivity ~ 5.5 ¥ 10–8 W m Tensile strength ~ 3.45 GPa Platinum
Whitish metal with more ductility than silver, gold and copper
Jewellry products
It has fcc structure
Resistance thermometer
It is very ductile and malleable
Resistance wires
Electrical conductivity is 16 % equal to copper
Thermocouples
Oxidised even at high temperature
Standard weights
Specific gravity ~ 21.45
Laboratory dishes
Melting point ~ 2027 K Resistivity ~ 10.5 ¥ 10–8 W m Temperature coefficient of resistivity ~ 3.93 ¥ 103 K1 Hardness (annealed) ~ 45 Brinell Tensile strength ~117 MPa.
Manganin
Constantan 55 % Cu 45 % Ni
Kanthal
Alumel
Cromel
2.
3.
4.
5.
6.
Maximum working temperature ~ 1366 K
Maximum working temperature ~ 1400 K Resistance ~ 116 ¥ 10–8 W Temperature coefficient of resistivity ~ 0.58 ¥ 10–3 K–1
80 % Ni 20 % Cr
High oxidation resistance High ductility and resistant to sulfuric acid Resistivity ~ 139 ¥ 10–8 W m Temperature coefficientresistivity ~ 30 ¥ 10–6 K–1 Maximum working temperature is 1573 K Tensile strength ~ 813 MPa with elongation of 1216 %
High resistivity High ductility High corrosion resistance Low temperature coefficient of resistance High thermoelectric effect with either copper or ferrous Tensile Strength ~ 965MPa Maximum working temperature ~ 773K
Good resistance to atmospheric corrosion Higher ductility Tensile strength ~ 482 MPa Maximum working temperature ~ 343K Resistivity ~ 48 ¥ 10–8 Wm Temperature coefficient of resistivity is 20 ¥ 10–6
Higher ductility Resistance ~ 108 ¥ 10–8 Wm Temperature coefficient of resistance ~ 100 ¥ 10–6 K–1. Maximum Working temperature ~ 1573 K.
Properties
94 % Ni 2.5 % Mn 0.5 % Fe Balanceother elements
69 % Fe 23 % Cr 6 % Al 2 % Co
8085 % Cu1215 % Mn 25 % Ni
80 % Ni 20 % Cr
Nichrome
1.
Composition
Alloy
Sr. No
Thermocouples
Thermocouples
Heating element in heaters and furnace
Thermocouple Rheostats Starters for electrical instruments
Coil Shunt wires in electrical instruments Spring sheet
Heating element in heaters and furnace
Applications
Table 8.8 Composition, Properties and Applications of High Resistivity Alloys
206 Materials Science
Statistics and Band Theory of Solids
207
Key Points to Remember The particles like electrons with half integral spin obey Fermi–Dirac statistics. Particle like electrons with half integral spin are known as Fermi particles or Fermions. The probability function of an electron occupying an energy level E is given by f (E) =
1 1 + exp ÈÎ( E  E ) / KT ˘˚
Fermi energy level is the uppermost energy level in a conduction band at 0 K. At T = 0 K and E > EF, the levels above Fermi levels is unoccupied, i.e., vacant. The probability of electron to occupy the energy level above the Fermi energy level is zero at T = 0 K and E > EF. 50 % or ½ % is the probability for electrons to occupy Fermi energy level at T = 0 K and E = EF. The number of quantum states present in a metal between any internal E and E + dE per unit volume is known as density of states. To study the Krong–Penny model for the motion of an electron. To understand the origin of Band structure and Brillouin zones. Density of states Z(E) =
No. of quantum states present between E and E + dE Volume of the specimen
The average volume of Fermi energy level Eave = 3/5 EFO. The Fermi level in Mo is higher than that of Pt, since the work function in Mo is low. The electrons in Mo, which are in higher energy levels flow into Pt when Pt and Mo are brought into contact. The Seebeck effect is used to measure the thermo emf using a thermocouple. 1 2 2 Ê d Eˆ The effective mass of the electron is given by m* = h Á 2 ˜ Ë dk ¯
The negative effective mass actually represents the electron is deaccelerating due to the applied field. The quantum free electron theory explains the specific heat capacity of metals, electrical conductivity, thermal conductivity, electronic specific heat capacity, electrodynamics of metals, photoelectric effect, Compton effect, etc. But it fails to explain distinction between metal, semi metal, semiconductor and insulator. According to the Energy band theory of solids, the free electrons are moving in a periodic potential produced by positive ion cores. The band electrons are treated as weakly perturbed by the periodic potential. The band which lies between k = 0 and k = ±p/2 is known as the first Brillouin zone. The band which lies between k = ±p/2 and k = ±p is known as second Brillouin zone. In a pure metal the scattering of electrons takes place only due to lattice vibrations. But in the case of impure metals, the scattering of electrons is both due to the lattice vibrations and impurity scattering.
208
Materials Science
Solved Problems Example 8.1 Calculate the Fermi energy of the following metals:
r (g
cm3)
Mat
Cu
Zn
Al
8.96
7.14
2.70
63.55
65.38
27.0
Given Data: For Cu Density of Cu
= 8.96 ¥ 103 kg m3
Atomic weight of Cu
= 63.55
For Zn Density of Zn
= 7.14 ¥ 103 kg m3
Atomic weight of Zn
= 65.38
For Al
Solution:
Density of Al
= 2.7 ¥ 103 kg m3
Atomic weight of Al
= 27.0
(i) For Cu The concentration of electrons in Cu n= =
Density ¥ Avogadro’s constant ¥ No. of free electrons per atom Atomic weight
8.96 ¥ 103 ¥ 6.022 ¥ 1026 63.55
= 8.4905 ¥ 1028 m3 Fermi energy at 0 K, Ê h 2 ˆ Ê 3n ˆ EFO = Á Á ˜ Ë 8me ˜¯ Ë p ¯
2/3
Substituting the values of h, n and m in the above equation, we get Ê (6.626 ¥ 1034 )2 ˆ Ê 3 ¥ 8.4905 ¥ 1028 ˆ 2 / 3 =Á ˜ ˜¯ ÁË 8 ¥ 9.1 ¥ 1031 ˜¯ ÁË p = 1.129729 ¥ 1018 J = 7.0608 eV.
Statistics and Band Theory of Solids
(ii) For Zn
The concentration of electrons in Zn n=
=
r NA ¥ No. of free electrons/atom M at 7.14 ¥ 103 ¥ 6.022 ¥ 1026 ¥ 2 65.38
= 13.152976 ¥ 1028 m3 Fermi energy at 0 K, Ê h 2 ˆ Ê 3n ˆ EFO = Á Á ˜ Ë 8me ˜¯ Ë p ¯
2/3
Substituting the values of h, n and m in the above equation, we get Ê (6.626 ¥ 1034 )2 ˆ Ê 3 ¥ 13.153 ¥ 1028 ˆ 2 / 3 =Á ˜ ˜¯ ÁË 8 ¥ 9.1 ¥ 1031 ˜¯ ÁË p = 1.51252397 ¥ 1018 J = 9.45 eV. (iii) For Al
The concentration of electrons in Al n=
r NA ¥ No. of free electrons/atom M at
2.7 ¥ 103 ¥ 6.022 ¥ 1023 ¥ 3 27 = 18.066 ¥ 1028 m3
=
Fermi energy at 0 K, Ê h 2 ˆ Ê 3n ˆ EFO = Á Á ˜ Ë 8me ˜¯ Ë p ¯
2/3
Substituting the values of h, n and m in the above equation, we get Ê (6.626 ¥ 1034 )2 ˆ Ê 3 ¥ 18.066 ¥ 1028 ˆ 2 / 3 =Á ˜ ˜¯ ÁË 8 ¥ 9.1 ¥ 1031 ˜¯ ÁË p = 1.8689 ¥ 1018 J = 11.68 eV. The Fermi energy of Cu is 7.0608 eV. The Fermi energy of Zn is 9.45 eV. The Fermi energy of Al is 11.68 eV.
209
210
Materials Science
Example 8.2 Calculate the density of states for Cu at the Fermi level for T = 0 K, if (m*/m) = 1.01. Given Data:
Solution:
Temperature
=0K
The effective mass of electron in Cu
= 1.01 Z(E) = g E1/ 2 / 2
The density of states is given by
l = 6.82 ¥ 1027 m3 eV3/2
where Fermi energy at 0 K,
Ê h 2 ˆ Ê 3n ˆ EFO = Á Á ˜ Ë 8me ˜¯ Ë p ¯
2/3
Substituting the values of h, n and m in the above equation, we get Ê (6.626 ¥ 10  34) 2 ˆ Ê 3 ¥ 8.4905 ¥ 1028 ˆ =Á ˜¯ p Ë 8 ¥ 9.1 ¥ 1031 ˜¯ ÁË
2/3
= 1.129729 ¥ 1018 J = 7.0608 eV. The value of EF for Cu is 7.0608 eV. Therefore, Z(E) = g EF 1/ 2 / 2 = 3.39 ¥ 1027 ¥
7.0608
= 9 ¥ 1027 m3 The density of states for Cu at the Fermi level for T = 0 K is 9 ¥ 1027 m3. Example 8.3 The resistivity of Ni at 200 º C is 69 nWm. If 80% Ni is alloyed with 20% chromium, the resistivity changes to 1120 nWm. Find the Nordheim’s coefficient. Given Data: Resistivity of Ni = 63 nWm Resistivity of Cr = 129 nWm Resistivity of 80% Ni + 20% Cr = 1120 nWm Solution:
The resistivity of alloy from Nordheim’s relation is rI = C ¥ (1  X) Where X is the atomic fraction of the solute atom. Here, X = 0.8 therefore rI = C X (1X) 1120 ¥ 109 Wm = C ¥ 0.8 (10.8)
Statistics and Band Theory of Solids
C=
211
1120 ¥ 109 0.8 ¥ 0.2
= 7 ¥ 106 The Nordheim’s coefficient is 7 ¥ 106 Wm. Example 8.4 Calculate the conductivity of Al at 25º C using the following data. Density of Al = 2.7 g cm3, atomic weight of Al = 27, and relaxation time of 1014 s. Given Data:
Solution:
Density of Al
= 2.7 ¥ 103 Kg m3
Atomic weight of Al
= 27
Relaxation time
= 1014 s
The number of electron available per m3 in Al, n= =
rN A ¥ No. of free electrons per atom M at 2.7 ¥ 103 ¥ 6.022 ¥ 1026 ¥ 3 27
= 18.066 ¥ 1028 m3 Conductivity of Al,
n=
=
ne 2t r m
(
)
2
18.066 ¥1028 ¥ 1.6 ¥ 1019 ¥1014 9.11 ¥ 1031
= 5.0823 ¥ 107 ohm m. The conductivity of Al is 5.0823 ¥ 107 ohm m. Example 8.5 Use Fermi distribution function to obtain the value of F (E) for EEF = 0.01 eV at 200 K. Given Data: The difference between energy level to Fermi level EEF = 0.01 eV = 0.01 ¥ 1.6 ¥ 1019 J = 1.6 ¥ 1021 J Temperature Solution:
T = 200 K
We know that the Fermi distribution function F (E) =
1 1+ e
( E  EF )/ kT
212
Materials Science
Substitution the value of EEF and T, we get =
1 1 + e(1.6¥10
21
)/(1.38¥1023 ¥ 200 )
=
1 1 + e0.5797
= 0.3589 The Fermi distribution function for energy E is 0.3589. Example 8.6 Calculate Fermi energy and Fermi temperature in a metal. Fermi velocity of electron in the metal is 0.86 ¥ 106 m s1. Given Data:
Solution:
Velocity of electron
v = 0.86 ¥ 106 m s1
Mass of electron
m = 9.1 ¥ 1031 kg
Electronic charge
e = 1.6 ¥ 1019 C
Boltzmann’s constant
k = 1.38 ¥ 1023 J K1
We know that the Fermi energy 1 EF = mv 2 2 Substituting the values, we get 1 = ¥ 9.11¥1031 ¥ 0.86 ¥106 2 = 3.368 ¥ 1019 J We also know that the Fermi temperature TF =
EF k
Substituting the value, we get =
3.368 ¥1019 1.38 ¥1023
= 2.43 ¥ 104 K Therefore, the Fermi temperature TF is 2.43 ¥ 104 K. Example 8.7 Calculate the number of states lying in an energy interval of 0.01 eV above the Fermi level for a crystal of unit volume with Fermi energy EF = 3.0 eV. Given Data: Mass of electron Energy interval Planck’s constant Fermi energy
m = 9.1 ¥ 1031 kg DE = 0.01 eV h = 6.63 ¥ 1034 Js EF = 3.0 eV
Statistics and Band Theory of Solids
Solution:
Let us take E1 is ground state, E1 = 3.0 eV
i.e.,
= 3.0 ¥ 1.6 ¥ 1019 E1 = 4.8 ¥ 1019 J E2 = E1 + DE
E2 is given by
= (3.0 + 0.01) eV = 3.01 ¥ 1.6 ¥ 1019 J E2 = 4.816 ¥ 1019 J Number of status per unit volume lying between E1 and E2 is given by 4p (2m)3/ 2 E1/ 2 dE 3 E1 h
E2
n=Ú
Here density of status Z (E) is unity E2 4p (2m)3/ 2 Ú E1/ 2 dE 3 h E1
=
Integrating the above equation, we get E2
È2 ˘ 4p = 3 ( 2 m) 3/ 2 Í ( E ) 3/ 2 ˙ h Î3 ˚E
1
Simplifying the above equation, we get E2
È2 ˘ 4p ( 2 m) 3/ 2 Í ( E ) 3/ 2 ˙ h3 3 Î ˚E
=
1
=
4p 2 (2m)3/2. ÈÎ E23/ 2  E13/ 2 ˘˚ h3 3
Substituting the value, we get =
(
4p ¥ 2 ¥ 9.1¥1031
(6.63 ¥ 10 )
34 3
)
3/ 2 3/ 2 2 ¥ ÈÎ ÈÎ(4.816)3/ 2  (4.8)3/ 2 ˘˚ ¥1019 ) ˘˚ 3
= 3.74 ¥ 1055 ¥ (1.108 ¥ 1030) = 4.14 ¥ 1025 The number of states lying between the energy level is 4.14 ¥ 1025.
213
214
Materials Science
Example 8.8 Fermi temperature of a metal is 24600 K. Calculate the Fermi velocity. Given Data: Fermi temperature of the metal TF = 24600 K m = 9.11 ¥ 1031 kg
Mass of an electron Solution:
We know that, the Fermi velocity is 2kTF m
vF = Substituting the values, we get =
2 ¥ 1.38 ¥ 1023 ¥ 24600 9.11 ¥ 1031
= 0.8633 ¥ 106 m s 1 The Fermi velocity vF is 0.8633 ¥ 106 m s1. Example 8.9 Free electron density of aluminum is 18.10 ¥ 1028 m3. Calculate its Fermi energy at 0 K. Planck’s constant and mass of free electron are 6.62 ¥ 1034 J s and 9.1 ¥ 1031 kg. Given Data:
Solution:
Electron density of aluminum
n = 18.10 ¥ 1028 m3
Planck’s constant
h = 6.62 ¥ 1034 J s
Mass of electron
m = 9.1 ¥ 1031 kg
We know that the Fermi energy at 0 K Ê 3n ˆ EF0 = Á c ˜ Ë 8p ¯
2/3
h2 2m
Substituting the given values, we get Ê 3 ¥ 18.10 ¥ 1028 ˆ =Á ˜¯ 8 ¥ 3.14 Ë
2/3
= 1.8689 ¥ 1018 J =
1.8689 ¥1018 1.6 ¥1019
= 11.68 eV The Fermi energy at 0 K is 11.68 eV.
¥
(6.62 ¥ 1034 ) 2 2 ¥ 9.1 ¥ 1031
Statistics and Band Theory of Solids
215
Example 8.10 The free electron density of aluminum is 18.10 ¥ 1028 m3. Calculate its Fermi energy at 0 K. Planck’s constant and mass of free electron are 6.62 ¥ 1034 J s and 9.1 ¥ 1031 kg. Given Data: Electron density of aluminum n = 18.10 ¥ 1028 m3 Planck’s constant h = 6.62 ¥ 1034 J s Mass of electron m = 9.1 ¥ 1031 kg Solution:
We know that the Fermi energy at 0 K, EFO
Ê 3n c ˆ = ÁË ˜ 8p ¯
2/3
h2 2m
Substituting the given values, we get
Ê 3 ¥ 18.10 ¥ 1028 ˆ = Á ˜ 8 ¥ 3.14 Ë ¯
2/3
¥
(6.62 ¥ 10 34 )2 2 ¥ 9.1 ¥ 10 31
= 1.8689 ¥ 1018 J =
1.8689 ¥ 10 18 1.6 ¥ 10 19
= 11.68 eV The Fermi energy at 0 K is 11.68 eV. Example 8.11 Calculate the temperature at which there is 1 % probability that a state with 0.5 eV energy above the Fermi energy is occupied. Given Data: The difference between energy level to Fermi level E  EF = 0.5 eV = 0.5 ¥ l.6 3 l019 J = 8.0 ¥ l020 J Probability = 0.01 Solution:
We know that the Fermi distribution function, f (E) =
1 1+ e
( E  EF )/ kT
Substitution the value of E  EF and f (E) in the above equation, we get 0.01 =
1 1+ e
( 3.2 ¥10 21 )/(1.38 ¥10 23 ¥T )
1 =
1+ e
5797 / T
216
Materials Science
Rearranging the above equation, we get e
5797 T
=
1 1 0.01
= 99 Taking the natural logarithm on both sides, we get 5797 = ln 99 T T=
or,
5797 ln 99
= 1261.1 K Therefore, temperature at which there is 1% probability that a state with 0.5 eV energy occupied above the Fermi energy level is 1261.1 K. Example 8.12 Show that occupation probability at E = EF + DE is equal to nonoccupation probability at E = EF  DE. Solution:
To be proved The probability of occupation of the energy level EF + DE = The probability of nonoccupation energy level E ¥ EF  DE.
Proof:
We know that the probability function f (E) for an electron occupying an energy level E f (E) =
1 1 + exp( E  E f ) / KT
(8.98)
Therefore, the probability function f (E) for an electron occupying an energy level E = (EF + DE) f ( E ) EF +DE =
1 1 + exp( DE ) / KT
(8.99)
Similarly, the probability function f (E) of an electron occupying an energy level just below the Fermi level E ¥ (EF  DE) f ( E ) EF DE =
1 1 + exp( DE ) / KT
(8.100)
Probability of absence = 1  Probability of presence Therefore, the probability of nonoccupation = 1  probability of occupation = l  f (E)
(8.101)
Substituting the f (E) value from Eq. (8.75), in the above equation, we get The probability of nonoccupation =
1 1 + exp( DE ) / KT
Statistics and Band Theory of Solids
217
Therfore, the probability of nonoccupation electron for an energy state (EF  DE) = 1
1 1 + exp[( DE ) / KT ]
Consider that eDE/KT = x and hence, eDE/KT = 1/x. The above equation can be written as, 1 The probability of nonoccupation = 1 1+ x 1 = 1or, 1+ x 1+ x  x = 1+ x Simplifying the above equation, we get 1 1+ x Therefore, the probability of nonoccupation at energy level =
E F  DE =
1 1 + exp( DE ) / KT
(8.102)
Equations (8.78) and (8.79) are equal and it shows that the probability of occupation at EF + DE is equal to the probability of nonoccupation at EF  DE. Thus, the given problem is proved. Example 8.13 Show that the sum of the probability of occupancy of energy at DE below the Fermi level and that at E above the Fermi level is unity. Solution:
To be proved Probability of an electron occupying + Probability of an electron below = 1 above the Fermi energy occupying the Fermi energy f (E)(EF + De) + f (E) (EF  De) = 1
Proof:
We know that the probability function f (E) of an electron occupying an energy level E f (E) =
1 1 + exp( E  E f ) / KT
(8.103)
Therefore, the probability function f (E) of an electron occupying an energy level just above the Fermi level (EF + DE) is f ( E )( EF + DE ) is =
1 1 + exp( DE )/ KT
(8.104)
Similarly, the probability function f (E) of an electron occupying an energy level just below the Fermi level (EF  DE) f ( E )( EF  DE ) is =
1 1 + exp(DE )/ KT
(8.105)
218
Materials Science
Substituting eDE/KT = x and eDE/KT = 1/x, in Eq. (8.104), we get 1 x +1 1 = (1 / x ) + 1
f ( E )( EF +DE ) = f ( E )( EF DE )
Substituting the values of f (E) (EF + DE) and f (E) (EF  DE) in Eqs. (8.104) and (8.105) in the above equation, we get 1 1 + =1 1+ x Ê 1ˆ 1 + ÁË ˜ x¯ Rearranging the above equation, we get 1 x + =1 1+ x 1+ x 1+ x =1 1+ x
1=1 Therefore, the sum of the probability of occupancy of energy of the occupied states above and below the Fermi levels is equal to unity. Example 8.14 The Fermi level in potassium is 2.1 eV. What are the energies for which the probabilities of occupancy at 300 K are 0.99, 0.01 and 0.5? Given Data: The Fermi energy EF = 2.1 eV Temperature T = 300 K Solution:
We know that the Fermi distribution function, f (E) =
1 1 + e( E  EF )/ KT
(8.106)
Rearranging the above equation, we get E  EF e KT
=
1 1 f (E)
Taking the natural logarithm on both sides of the above equation, we get Ê 1 ˆ E  EF = ln Á 1 KT Ë f ( E ) ˜¯ Simplifying the above equation, we get Ê 1 ˆ E = E F + KT ln Á  1˜ Ë f (E) ¯
(8.107)
Statistics and Band Theory of Solids
219
The first term in the above equation is in eV, while the second term is in joule. To convert the second term into electron volts, it is divided by the charge of electron, i.e., 1.9 ¥ 1019. Substituting the values of K, T, EF and f (E) = 0.99 in the above Eq. (8.110), we get Therefore,
E = 2.1 +
1.38 ¥ 10 23 ¥ 300 1.6 ¥ 10
19
Ê 1 ˆ ln Á 1 Ë 0.99 ˜¯
The energy for the probability of occupying of 0.99 is 1.98 eV. Substituting the values of K, T, EF and f (E) = 0.01 in Eq. (8.110) and dividing the second term by l.9 ¥ l019, we get E = 2.1 +
1.38 ¥ 10 23 ¥ 300 1.6 ¥ 10 19
Ê 1 ˆ ln Á 1 Ë 0.01 ˜¯
The energy for the probability of occupying of 0.01 = 2.219 eV Substituting the values of K, T, EF and f (E) = 0.5 in Eq. (8.110) and dividing the second term by 1.9 ¥ l019, we get E = 2.1 +
1.38 ¥ 10 23 ¥ 300 1.6 ¥ 10 19
Ê 1 ˆ ln Á 1 Ë 0.5 ˜¯
The energy for the probability of occupying of 0.5 is 2.1 eV. Therefore, the energies for the occupying of electrons at 300 K for the probability of 0.99 is 1.98. The energies for the occupying of electrons at 300 K for the probability of 0.01 are 2.22. The energies for the occupying of electrons at 300 K for the probability of 0.5 are 2.1. Example 8.15 Calculate the probability of an electron occupying an electron level of 0.02 eV above the Fermi level at 200 K and 400 K in a metal. Given Data: The difference between energy level to Fermi level E  EF = 0.02 eV = 0.02 ¥ l.6 ¥ l019 J = 3.2 ¥ 1021 J Temperature T = 200 K and 400 K Solution:
We know that the Fermi distribution function, f (E) =
1 1+ e
( E  EF )◊ KT
(8.111)
Substituting the values of E  Ef and T = 200 K in the above equation, we get =
1 1+ e
( 3.2 ¥10 21 )/(1.38 ¥10 23 ¥ 200 )
220
Materials Science
1 =
1 + e1.1594
= 0.2387 The Fermi distribution function for the given energy at 200 K is 0.2387. Substituting the values of E = EF and T = 400 K in Eq. (8.111), we get = =
1 ( 3.2 ¥10 21 )/(1.38 ¥10 23 ¥ 400 )
1+ e 1
1 + e 0.5797
= 0.3589 The Fermi distribution function for the given energy at 400 K is 0.3589. Therefore, the Fermi distribution function for the given energy at 200 K is 0.2387. The Fermi distribution function for the given energy at 400 K is 0.3589. Example 8.16 Calculate the Fermi energy in eV for a metal at 0 K, whose density is 10500 kg m23, atomic weight is 107.9 and has one conduction electron per atom. Given Data: Density of the metal ¥ 10500 kg m23 Atomic weight of metal ¥ 107.9 Solution:
We know that the concentration of electrons in metal n=
Density ¥ Avogadro’s constant ¥ No. of free electrons per atom Atomic weight
Substituting the values in the above equation, we get 1 ¥ 10500 ¥ 6.022 ¥ 1026 = 107.9 = 5.861 ¥ 1028 m3 We know that Fermi energy at 0 K, Ê h2 ˆ E Fo = Á ˜ Ë 8me ¯
Ê 3n ˆ ÁË ˜¯ p
2/3
Substituting the values of h, n and m in the above equation, we get Ê (6.626 ¥ 10 34 ) ˆ =Á ˜ Ë 8 ¥ 9.1 ¥ 1031 ¯
Ê 3 ¥ 5.861 ¥ 1028 ˆ Á ˜ p Ë ¯
2/3
Statistics and Band Theory of Solids
221
= 8.8173 ¥ l0218 J = 5.510 eV Therefore, the Fermi energy of the given metal is 5.5 eV. Example 8.17 Calculate the probability of an electron occupying an electron level of .02 eV above the Fermi level at 300 K and 1000 K in a metal. Given Data: The difference between energy level to Fermi level E  EF = 0.2 eV = 0.2 ¥ l.6 ¥ l019J = 3.2 ¥ 1020J Solution:
We know that the Fermi distribution function, 1 f (E) = 1 + e( E  EF )/ KT
(8.112)
Substituting the values of E  EF and T = 300 K in the Eq. (8.112), we get =
1 1+ e
( 3.2 ¥10 20 )/(1.38 ¥10 23 ¥ 300 )
1 =
1 + e 7.7294
= 0.004394 The Fermi distribution function for given energy at 300 K is 0.004394. Substituting the values of E  EF and T = 1000 K in Eq. (8.112), we get = =
1 ( 3.2 ¥10 20 )/(1.38 ¥10 23 ¥100 )
1+ e 1
1 + e 2.3188
= 0.089 The Fermi distribution function for the given energy at 1000 K is 0.089. Therefore, the Fermi distribution function for given energy at 300 K is 0.004394. The Fermi distribution function for the given energy at 1000 K is 0.089. Example 8.18 Find the electron density for a metal with a Fermi energy of 3 eV. Given Data: Fermi level at 0 K, EF0 = 3 eV = 3 ¥ 1.6 ¥ 1019 J = 4.8 ¥ 1018 J
222
Materials Science
Solution:
We know that Fermi energy at 0 K, Ê h2 ˆ EF 0 = Á ˜ Ë 8me ¯
Ê 3n ˆ ÁË ˜¯ p
2/3
Substituting the values of h, EF0 and m in the above equation, we get Ê (6.626 ¥ 10  34)2 ˆ 4.8 ¥ 10 19 = Á ˜ Ë 8 ¥ 9.1 ¥ 10  31 ¯
Ê 3ˆ ÁË ˜¯ p
2/3
( n) 2 / 3
= 5.8437 ¥ l038 ¥ n2/3 Rearranging the above equation, we get Ê 4.8 ¥ 10 19 ˆ n=Á ˜ Ë 5.8457 ¥ 10 38 ¯
3/ 2
= 2.36 ¥ 1028 The number of freeelectron concentration in metal is 2.36 ¥ 1028 m3. Therefore, the Fermi energy at 0 K is 5.8437 ¥ 1038 ¥ n2/3. The number of free electrons concentration in metal is 2.36 ¥ 1028 m3. Example 8.19 The Fermi energy in silver is 5.5 eV at 0 K. Calculate the number of free electrons per unit volume and the probability of occupation for an energy of 5.6 eV in silver at the same temperature. Given Data: Fermi level at 0 K EF0 = 5.5 eV = 5.5 ¥ l.6 ¥ l019 J = 8.8 ¥ 1019 J Temperature T = 0 K Solution:
We know that Fermi energy at 0 K, Ê h2 ˆ Ê 3n ˆ 2 / 3 EF 0 = Á ˜Á ˜ Ë 8me ¯ Ë p ¯ Substituting the values of h, EF0 and mass of electron m in the above equation, we get Ê (6.626 ¥ 10 34 )2 ˆ Ê 3 ˆ 2 / 3 2 / 3 8.8 ¥ 10 19 = Á ˜ Á ˜ ( n) Ë 8 ¥ 9.1 ¥ 10 31 ¯ Ë p ¯ = 5.8437 ¥ 1038 ¥ n2/3 Rearranging the above equation, we get Ê 8.8 ¥ 10 19 ˆ n=Á ˜ Ë 5.8437 ¥ 10 38 ¯ = 5.844 ¥ l028
3/ 2
Statistics and Band Theory of Solids
Therefore, the concentration of free electrons in silver is 5.844 ¥
1028
223
m3.
It is clear from the above observation that at T ¥ 0 K, the probability of occupation of energy is E = 5.6 eV, which is greater than EF , i.e., E > EF. Therefore, the probability of electrons to occupy the energy level above the Fermi energy level is zero, i.e., f (E) = 0. Example 8.20 The relaxation time of conduction electrons in copper is 2.6 ¥ 104 s. If the copper has a resistivity of 1.6 ¥ 108 W and the Fermi energy 7 eV. Find the charge carrier density and Fermi velocity. Given Data: Fermi level at 0 K EF0 = 7e V = 7 ¥ 1.6 ¥ 1019 J = 1.12 ¥ l018 J Solution:
We know that Fermi energy at 0 K, Ê h2 ˆ EF 0 = Á ˜ Ë 8me ¯
Ê 3n ˆ ÁË ˜¯ p
2/3
Substituting the values of h, EF0 and m in the above equation, we get Ê (6.626 ¥ 10 34 )2 ˆ Ê 3 ˆ 2 / 3 2 / 3 1.12 ¥ 10 18 = Á ˜ Á ˜ ( n) Ë 8 ¥ 9.1 ¥ 10 31 ¯ Ë p ¯ = 5.8437 ¥ 1038 ¥ n2/3 Rearranging the above equation, we get Ê 1.12 ¥ 10 18 ˆ n=Á ˜ Ë 5.8437 ¥ 10 38 ¯
3/ 2
= 8.39 ¥ 1028 Therefore, the number of freeelectron concentration in copper is 8.39 ¥ 1028 m3. We know that thermal velocity of free electrons in copper is Vth =
2 EF m
Substituting the values of k, T and m in the above equation, we get Vth =
2 ¥ 1.12 ¥ 10 18 9.11 ¥ 10 31
= 1.568 ¥ l06 m s1 The thermal velocity of the free electrons in copper is 1.568 ¥ 106 m s1. Therefore, the number of freeelectron concentration in copper is 8.39 ¥ 1028 m3. The thermal velocity of the free electrons in copper is 1.568 ¥ 106 m s1.
224
Materials Science
ObjectivesType Questions 8.1. Probability function f(E) for an electron is 1 (a) f (E) = 1 exp ÈÎ E  E f / KT ˘˚
(
(c) f (E) =
(
1
)
(b) f (E) =
)
(d) f (E) =
1+ exp ÈÎ E  E f / KT ˘˚
(
1
)
1+ exp ÈÎ E f  E / KT ˘˚
(
1
)
1 exp ÈÎ E f  E / KT ˘˚
8.2. Fermi energy level is the ______ energy level in a conduction band at 0 K. 8.3. Electrons occupy the Fermi energy level fully and leave vacant above EF at T = 0 K, when (b) E = EF (a) E + EF (c) E > EF (d) E < EF 8.4. Fermi level is ______ at T = 0 K, E < EF 8.5. Zero percent probability is the probability for the electrons to occupy the energy level above the Fermi energy level at T = 0 K and (a) E + EF (b) E = EF (c) E > EF (d) E < EF 8.6. Electrons occupy 50% or ½ of the Fermi energy level at ______ and ______ 8.7. Density of states is equal to (a)
No. of quantum states present between E and E < dE Volume of the specimen
(b)
No. of quantum states present between E and E > dE Volume of the specimen
(c)
No. of quantum states present between E and E  dE Volume of the specimen
(d)
No. of quantum states present between E and E + dE Volume of the specimen
8.8. The concentration of free electrons in metal is equal to (a) Ú
4p (2m)3/ 2 E1/ 2 dE h3
(b) Ú
4p (2m)3/ 2 E 1/ 2 dE h3
(c) Ú
4p (2m)3/ 2 E 5/ 2 dE h3
(d) Ú
4p (2m)3/ 2 E 3/ 2 dE h3
8.9. The value of Fermi energy level at T = 0 K Ê h 2 ˆ Ê 3n ˆ (a) EFo = Á ˜ Á ˜ Ë 8m ¯ Ë p ¯
2/3
Ê h 2 ˆ Ê 3n ˆ (b) EFo = Á ˜ Á ˜ Ë 8m ¯ Ë p ¯
2/3
Ê h 2 ˆ Ê 3p ˆ = Á ˜Á ˜ Ë 8m ¯ Ë n ¯
2/3
Ê h 2 ˆ Ê 3m ˆ = Á ˜Á ˜ Ë 8p ¯ Ë n ¯
2/3
(c) EFo
(d) EFo
Statistics and Band Theory of Solids
8.10. The average energy of the electrons at T = 0 K (a) Eave = 5/3 EFO (b) Eave = 1/3 EFO (c) Eave = 1/5 EFO (d) Eave = 3/5 EFO 8.11. Average Fermi energy level of electrons at nonzero temperature Eave (T) is equal (a) 5/3 EFO (b) 1/3 EFO (c) 3/5 EFO (d) 3/4 EFO Answers 8.1. (c) 8.5. (c) 8.9. (b)
8.2. Upper most filled 8.6. T = 0 K, E = EF 8.10. (d)
8.3. (d) 8.7. (d) 8.11. (b)
8.4. Vacant 8.8. (a)
Short Questions 8.1. Write the mathematical expression for the FermiDirac statistics and explain all the terms. 8.2. What is Fermi level and Fermi energy? 8.3. Explain the distribution of electrons at 0 K based on the quantum theory. 8.4. Draw Fermi distribution curve for 0 K and at any temperature T K. 8.5. Define the density of states. 8.6. What do you mean by quantisation of momentum? 8.7. Show that an electron’s momentum in a potential well is quantised. 8.8. Deduce an expression for Fermi energy in terms of concentration of electrons at 0 K. 8.9. Obtain an expression for Fermi energy at T < 0 K. 8.10. Explain the significance of Fermi energy in thermo emf measurements. 8.11. Explain the significance of Fermi energy in metalmetal contacts. 8.12. Write the expression for carrier concentration of metal. 8.13. What is meant by effective mass of an electron? 8.14. 8.15. 8.16. 8.17. 8.18. 8.19. 8.20. 8.21. 8.22.
Explain the electrical conductivity of Cu. What is a hole? What is meant by Brillouin Zone? Illustrate the first, second and third Brillouin zones for a two dimensional square lattice. Based on band theory of solids, explain the nature of conductor and semiconductors. Based on band theory of solids, explain the nature of insulator and semiconductors. Explain the significance of Brillouin zones with the reference to any cubic lattice. Why was the band theory of solids proposed? Explain the occurrence of energy gap in semiconductor.
225
226
Materials Science
Descriptive Questions 8.1. Derive a mathematical expression for density of states. 8.2. Write short notes on the following: 1. FermiDirac distribution 2. Fermi energy at T = 0 K and T > 0 K. 3. Significance of Fermi energy 8.3. What is meant by effective mass of an electron? Derive an expression for the effective mass of an electron. 8.4. What is hole? List out the properties of a hole. 8.5. Write the short notes on onedimensional and twodimensional Brillouin zones. 8.6. Discuss the KrongPenny model for the motion of an electron in a periodic potential. 8.7. Draw the Brillouin zone for twodimensional square lattice of length a. 8.8. Write a note about the high resistivity of metals and alloys.
Exercises 8.1. Evaluate the Fermi energy of alkali metals Li, Na and K using the following data: Density (kg m3) Atomic weight 8.2. Determine the electrical Density of Cu Atomic weight of Cu Relaxation time of Cu
Li
Na
K
534
971
860
6.939
22.99
39.202
conductivity of Cu at 25ºC using the following data. = 8960 Kg m3 = 63.55 = 1014 s.
Chapter
9
PHASE DIAGRAM
OBJECTIVES To study the classification of alloys. To understand the principle and process methods of metal and alloys. To understand the phase diagram. To explain the characteristics of metals and alloys using the phase diagram. To study the applications of metals and alloys.
9.1 INTRODUCTION Metals used for specific industrial applications are metal alloys and not pure metals. All the industrial applications are made possible due to their varied and excellent physical and chemical properties. The different composition of the metal alloys are used to obtain the required properties to meet the design requirements on an engineer. Generally, alloys are made by mixing two or more metals or metal and nonmetals employing proper metal process method. The properties of alloys such as less ductility, high strength, low conductivity, corrosion resistance, hardness, etc., makes alloys different from pure metals. Therefore, the knowledge on the structural, chemical, mechanical, electrical and magnetic properties of material is essential. Thus, the characteristics properties of any alloys can be studied through systematic representation of graph known as phase diagram. In this chapter, metal and alloys, its classification, characteristics properties and its applications using the phase diagram are discussed briefly with a view to understand the engineering materials.
9.2 CLASSIFICATION OF METAL ALLOYS The metallic materials are further classified into ferrous and nonferrous materials. The materials which contain ferrite or iron atoms as the principle constitutes are known as ferrous metals. On the other hand, metals which do not contain any ferrous or iron atoms are known as nonferrous metals. The ferrous materials are magnetic in nature, while the nonferrous materials are nonmagnetic materials. The atoms
228
Materials Science
are arranged in periodic or regular manner and hence, nonferrous materials are crystalline in nature. The most common structure of the materials are face centered, body centered and closely packed hexagonal structure. The general classification of metal alloys is shown in Fig. 9.1. Metal and Alloys
Ferrous
Steel
Low Alloy
Low Carbon
Nonferrous
Cast Iron
High Alloy
Medium Carbon
Gray Iron
High Carbon
Ductile Iron
White Iron
Copper and its alloys
Malleable Iron
Alulminium and its alloys
Magnesium Titanium and and its alloys its alloys
Fig. 9.1 Flowchart for the classification of metal alloys
9.3
FERROUS ALLOYS
Ferrous alloys are important engineering materials used for different applications. The major constituent present in the ferrous alloys is iron. Due to their excellent mechanical and physical properties, versatility, simple process and easy availability, it finds wide applications in industries. The main disadvantage of ferrous alloys is resistance to corrosion. Ferrous alloys are further classified into two categories namely steels and cast irons.
9.3.1
Steels
Based on the carbon content, steels are classified into low carbon, medium carbon and high carbon steels. Ironcarbon steels contain many alloys with different components. The mechanical and physical properties of ironcarbon alloys are changed depending on the required applications through the addition of different compositions of alloying elements and heat treatments.
Low Carbon Steels The major quantities of steel produced in the market are low carbon steels. The low carbon steel contains less than 0.25 wt % of carbon as an additional element. The microstructure of low carbon steel is made up of ferrite and pearlite. The important properties of low carbon steels are high ductility, high toughness,
Phase Diagram
229
machineability and weldability. One can process ironcarbon alloys through a simple process method at low cost. The excellent mechanical properties of this alloy leads to important applications like automobile body component, structural component in building construction, industrial and house hold applications. Some of the important low carbon steels, their properties and applications are given in Table 9.1.
Table 9.1 Mechanical Properties and Applications of Low Carbon Steels ASTM number
Tensile Yield strength Ductility % EL strength MPa MPa in 50 mm (2 in.)
Typical applications
1010
325
180
28
Automobile panels, nails and wire
1020
380
205
25
Pipe and structures
A36
400
220
23
Bridges and buildings
A516 Grate 70
485
260
21
Lowtemperature pressure vessels
A440
435
290
21
Structures that are bolted or riveted
A633 Grade E
520
380
23
Structures used at low ambient structural temperatures
A656 Grade 1
655
552
15
Truck frames and railway cars
Medium Carbon Steels The constituent of carbon in medium carbon steel lies between 0.25 and 0.60 wt %. One can improve the mechanical properties of these alloys by proper heat treatments. The hardenabilities of these alloys are very low and hence, it can be improved using suitable quenching rates. The strength of medium carbon steels are improved with the addition of elements like nickel, chromium and molybdenum. The strength of heat treated medium carbon steel alloys is more than the low carbon alloys. These alloys are used to manufacture high strength structural components like rotating wheels, railways tracks, crankshafts, etc. Some of the important medium carbon steel alloys, their properties and applications are given in Table 9.2.
Table 9.2 Mechanical Properties and Applications of Medium Carbon Steels AISI UNS number number
Tensile strength MPa
Yield strength Ductility [%EL in MPa 50 mm (2 in.)]
Typical applications
1040
G10400
605 – 780
430 – 585
33 – 19
Crankshafts, bolts
1080a
G10800
800 – 1310
480 – 980
24 – 13
Chisels, hammers
1095a
G10950
760 – 1280
510 – 830
26 – 10
Knives, hacksaw blades
4063
G40630
786 – 2380
710 – 1770
24 – 4
Springs, hand tools
4340
G43400
980 – 1960
895 – 1570
21 – 11
Bushings, aircraft tubing
6150
C61500
815 – 2170
745 – 1860
22 – 7
Shafts, pistons, gears
Materials Science
230
High Carbon Steels High carbon steels contains the maximum carbon contents, i.e., 0.60 to 1.4 wt %. When compared to low and medium carbon steels, the high carbon steels are hard and strongest. The high carbon steels exhibit least ductile properties. The high carbon steels are used for many industrial applications under hardened and tempered conditions. In order to make more hardened carbide components, alloying elements like chromium, vanadium, tungstan and molybdenum are added. Most of the cutting tools and dies are made by means of using high carbon steels with any one of the alloying elements. The composition and applications of high carbon steels with different alloying elements are shown in Table 9.3.
Table 9.3 Composition and Applications of High Carbon Steel with Different Alloying Element AISI number
UNS number
Ml
Composition (wt %)
Typical applications
C
Cr
Ni
Mo
W
V
T11301
0.85
3.75
0.30 max
8.70
1.75
1.20
Drills, saws; lather and planer tools
A2
T30102
1.00
5.15
0.30 max
1.15
—
0.35
Punches, embossing dies
D2
T30402
1.50
12
0.30 max
0.95
—
O1
T31501
0.95
0.50
0.30 max
—
0.50
S1
T41901
0.50
1.40
0.30 max 0.50 max
W1
T72301
1.10 0.15 max 0.20 max 0.10 max 0.15 max 0.10 max Blacksmith tools, woodworking tools
9.3.2
Stainless Steel
2.25
1.10 max Cutlery, drawing dies 0.30 max Shear blades, cutting tools 0.25
Pipe cutters, concrete drills
The major disadvantage of steels namely corrosion resistance is overcome by stainless steels (SS). The addition of elements like chromium (Cr), nickel (Ni) and molybdenum (Mo) to steels improve their corrosion resistance in different environmental conditions. For example, 11 wt % of chromium is required to improve the corrosion resistance of stainless steel. Based on the microstructure, the stainless steels are classified into three classes namely, martensitic stainless steel, ferritic stainless steel and austenitic stainless steel. The precipitationhardening treatment is used to obtain high strength and corrosion resistant of stainless steels. The mechanical properties and high corrosion resistance of stainless steel leads to an excellent applications both at ambient and elevated temperatures. The properties of martensitic, ferritic and austenitic stainless steels are different due to their microstructural constituent present. For example, martensitic and ferritic stainless steels are magnetic in nature. The important applications of martensitic, ferritic, and austenitic stainless steels along with precipitation hardening of steels are given in Table 9.4.
0.20 C, 25 Cr, 1.5 Mn
0.08 C, 19 Cr, 9 Ni, 2.0 Mn
0.03 C, 17 Cr, 12 Ni, 2.5 Mo, 2.0 Mn
0.15 C, 12.5 Cr, 1.0 Mn
0.70 C, 17 Cr, 0.75 Mo, 1.0 Mn
446
304
316L
410
440A
177PH 0.09 C, 17 Cr, 7 Ni, 1.0 Al, 1.0 Mn
0.08 C, 11.0 Cr, 1.0 Mn, 0.50 Ni, 0.75 Ti
Composition (wt %)
409
AISI number
Precipitation hardened
Annealed Q and T 1450
725 1790
485 825
485
Annealed
Annealed Q and T
515
515
380
Tensile strength MPa
Annealed
Annealed
Annealed
Condition
1310
415 1650
275 620
170
205
275
205
Yield strength MPa Ksi
1–6
20 5
20 12
40
40
20
20
Ductivity [%EL in 50 mm (2 in.)]
Mechanical properties
Springs, knives, pressure vessels
Cutlery, bearings, surgical tools
Rifle barrels, cutlery, jet engine parts
Welding construction
Chemical and food processing equipment, cryogenic vessels
Valves (high temperature), glass molds, combustion chambers
Automotive exhaust components, tanks for agricultural sprays
Application
Table 9.4 Composition, Properties and Applications of Martensitic, Ferritic, Austenitic and Precipitationhardening Stainless Steel
Phase Diagram 231
F10008
F32800 ¸ 3.53.8 C, 2.0–2.8 Si, Ô Ô F34800 ˝ 0.05 Mg, > ni, where ni is the intrinsic carrier concentration. At very low temperatures, all the valence bands are completely occupied by the electrons and the donor carriers. Therefore, no electron is available in the conduction band for the electrical conduction. This is depicted in Fig. 10.6(a). T < TS
TS < T < T1
T < T1
Conduction band
Conduction band
Conduction band
EF Eg
As
+
As
+
As
+
Donor level
As
+
As
+
As
+
As
EF
+
As
+
As
+
EF
EF
Valence band
Valence band
Valence band
(a) At T = T1
(b) At T = T2
(c) At T = T3
Fig. 10.6 Concentration of electrons at different temperatures: (a) At a very low temperature, (b) At a temperature, which is sufficient to excite donor electron, and (c) At a temperature, which is sufficient to excite valence electrons If the temperature is increased gradually, some of the donor electrons are ionised and their electrons are excited to the conduction band, as shown in Fig. 10.6(b). At room temperature, all
Transport Properties of Semiconductors
259
the donor electrons are excited to the conduction band. If the temperature is further increased, there is no increase in concentration of electrons in the conduction band, since the electrons in the conduction band require a minimum energy of DE = Ec  Ev, which is greater than the ionisation energy [DEi = Ec  Ed ( Ti ) When the temperature becomes sufficient to liberate electrons from the valence band, the concentration of electrons in the conduction band increases very sharply. The reason is, at this temperature more and more number of electrons get liberated and they are excited to the conduction band. This region is said to be the intrinsic range.
260
Materials Science
If a plot is drawn between ln (n) and 1/T, a curve as shown in Fig. 10.7 is obtained. The three regions can be distinctly seen in Fig. 10.7. Since there is a sharp increase in the concentration of electrons at high temperature, concentration is given as Ê  Eg ˆ n µ T3/2 exp Á Ë 2kT ˜¯
(10.68)
In(n)
Intrinsic slope = –Eg/2k
Ts
Extrinsic
ln(Nd)
Ti
Ionization slope = –DE/2k
ni(T ) 1/T
Fig. 10.7 A plot of ln (n) versus 1 for ntype semiconductor T
This shows that there is a domination of the exponential part over T 3/2 in the high temperature region. In the extrinsic region, n ª ND and is practically independent of temperature. The temperature dependence of the intrinsic concentration of Si, Ge and GaAs are shown in Fig. 10.8. From the slope of this curve, one can determine the band gap of the semiconducting materials. 300 K
873 K
1018 1015
Ge
2.4 × 1013 cm–3
Si
1.45 × 1010 cm–3
1012 n 109 GaAs
2.1× 106 cm–3
106 103 1
2 103 (K–1)
3
4
Fig. 10.8 Temperature dependence of intrinsic concentration of Si, Ge and GaAs
Transport Properties of Semiconductors
261
10.8.2 Variation of Drift Mobility with Temperature The drift mobility varies with two distinctly different temperature variations. At high temperature region, the drift mobility is limited by scattering from lattice vibrations. At high temperature, m a T 3/2, i.e., the mobility decreases with an increase in temperature. At low temperature, the scattering of electrons by ionised impurities is the major mobility limiting mechanism and m µ T 3/2. The mobility is given by the expression, m=
et r me*
(10.69)
where e is the charge of the electron, tr is the mean free time, and me* the effective mass. The mean free time is given by tr =
1 Svth N s
(10.70)
where S is the surface area of the scatterer, vth is the mean speed of the electrons and Ns is the number of scatterer per unit volume. The surface area of the scatterer is pr2. As the temperature increases, the amplitude of the lattice vibration also increases. Therefore, r2 µ T behaviour is observed. The mean speed of the electron is obtained using the relation, 1 mvth2 = 3 k BT 2 2 vth µ T1/2
i.e.,
(10.71)
Thus, the mean free time is given as tr =
1 1 1 µ µ 3 1 2 (p r )vth N s T (T ) T 2 2
t µ T 3/2
i.e.,
(10.72)
i.e., at high temperature, the drift mobility varies with T 3/2. At low temperature, the ionised impurity scattering is dominant over thermal scattering. Consider that at a low temperature, an electron is scattered by an ionised impurity, such as As+. As an electron is scattered by an ionised impurity, the magnitude of the kinetic energy of the electron is less than the potential energy. i.e., KE < PE. Therefore, the PE is given by PE =
e2 4p e 0e r rc
The critical radius corresponding to the electron, when it is just scattered, is rc which is when KE ª PE(rc).
262
Materials Science
3 e2 kBT = 2 4p e rc
Therefore,
e
KE =
1 m v2 2 e
KE > PE KE ª PE rc
As+
KE > PE
Fig. 10.9 Scattering of an electron by an ionised impurity e2 6p k BT e
i.e.,
rc =
The surface area,
p e4 S = pr2 = (6k T e p ) 2 B 1 T2
(10.73)
1 T (T 1/ 2 ) N I
(10.74)
Sµ
i.e., From Eqs. (10.70), (10.71) and (10.73), we get t1 µ
2
where NI is the concentration of ionised impurities. The ionised impurity scattering limited mobility from Eq. (10.69) can be written as, t1 µ
T 3/ 2 NI
(10.74)
Equation (10.74) shows that the drift mobility due to impurity scattering is directly proportional to T3/2. The combined drift mobility using Mathiessen's rule can be written as, 1 1 1 = + md mI mL
(10.75)
where md , mL and ml are the drift mobility, the mobility due to lattice scattering and the mobility due to impurity scattering, respectively. The variations of drift mobility with temperature and doping concentration are shown in Figs. 10.10 and 10.11, respectively.
Transport Properties of Semiconductors
263
Total scattering 1 m 1 mD
Lattice scattering (phonon) ª T 3/2
Impurity scattering ª T 3/2
T
Fig. 10.10 A plot of ÊÁ 1 ˆ˜ versus temperature (T) Ë md ¯
Drift mobility (md)(cm2V–1s–1)
2000 1000
Holes
Electrons
50 1015
1018 1016 1017 1019 Dopant concentration, cm–3
1020
Fig. 10.11 Variation of drift mobility with doping concentration in Si for electrons and holes
10.8.3 Variation of Conductivity with Temperature The variation of electrical conductivity with temperature has three distinct regions namely, (i) ionisation range, (ii) extrinsic range, and (iii) intrinsic range. The variation of ln (s) versus (1/T) is shown in Fig. 10.12. In the ionisation range, the concentration of carriers is given by 1
È  ( EC  ED ) ˘ Ê1 ˆ2 n = Á N C N D ˜ exp Í ˙ Ë2 ¯ 2kT Î ˚
(10.76)
Materials Science
log (n)
log(s)
Resisitivity
264
Logarithmic Scale
Intrinsic
Semiconductor
Metal
T Extrinsic Ionization
Lttice scattering
m µ T 3/2
log(m)
m µ T 3/2 Impurity scattering 1/T Low temperature
High temperature
Fig. 10.12 Variation of conductivity, concentration and mobility with temperature and the electrical conductivity is also proportional to the concentration of carriers; it dominates the temperature dependence of conductivity. In the intrinsic region, the conductivity is given by sI = nie(me + mh) In the above equation, the intrinsic concentration varies with temperature and hence, the conductivity also varies with temperature. In the extrinsic region, the concentration of carriers is n ª Nd for ntype material and the conductivity varies with the temperature dependence of the drift mobility. The temperature dependence of conductivity, concentration and mobility are shown in Fig. 10.12.
10.9
10.9.1
VARIATION OF FERMI LEVEL WITH TEMPERATURE IN EXTRINSIC SEMICONDUCTOR
ntype Semiconductor
The Fermi level for an ntype semiconductor is given by Ê E + ED ˆ kT È N D ˘ EF = Á C ln Í ˙ ˜¯ + Ë 2 2 Î NC ˚
(10.77)
Transport Properties of Semiconductors
265
Ê E + ED ˆ Substituting T = 0 K in the above equation, we get EF = Á C ˜¯ . This shows that in an ntype Ë 2 semiconductor, the Fermi level lies in between the conduction band and the donor level at zero degree Kelvin. As the temperature increases from 0 K, the Fermi level falls. At higher temperature, it falls below the donor level and hence, it approaches the centre of the forbidden gap. The Fermi level lying at the middle of the energy gap at very high temperature shows that the material is behaving as an intrinsic semiconductor. As the donor concentration is increased, the Fermi level will move up. The variation of Fermi level with temperature is shown in Fig. 10.13. Ec Ef ED
ND = 1024 mND = 1021 m3
E
EF
EV T
500 K
Fig. 10.13 Variation of Fermi level in an ntype semiconductor with temperature
10.9.2
ptype Semiconductor
The Fermi level in a ptype semiconductor is given by Ê E + EV ˆ kT È NV ˘ EF = Á A ln Í ˙ ˜+ Ë 2 ¯ 2 Î NA ˚
(10.78)
The variation of Fermi level with temperature in a ptype semiconductor is shown in Fig. 10.14. As Ê E + EV ˆ T = 0 K, the above equation reduces to EF = Á A ˜ i.e., the Fermi level lies at the middle of Ë 2 ¯ the acceptor level and the valence band at 0 K. If the temperature is increased, the Fermi level rises. If the temperature is sufficiently high, the Fermi level increases above the acceptor level. At very high temperature, it lies at the middle of the energy gap. This shows that at very high temperatures, the ptype material behaves as an intrinsic material. As the acceptor concentration is increased, the Fermi level shifts downwards as shown in Fig. 10.14.
266
Materials Science
Ec
E
EF
NA = 1021/m–3 NA = 1024/m–3
EA
EV T
500 K
Fig. 10.14 Variation of Fermi level with temperature in a ptype material
Key Points to Remember In semiconductors, electrons and holes are the charge carriers for conductors. In semiconductors, all the states in the valence band are occupied while in the conduction band, they are empty at 0 K. Fermi distribution function 1 Ê EF  EC ˆ 1  exp Á Ë RT ˜¯ The concentration of electrons in the conduction band of a semiconductor is equal to f (E) =
Ê E  EC ˆ n = Nc exp Á F Ë RT ˜¯ The concentration of holes in the valence band of a semiconductor is equal to Ê E  EF ˆ p = Nv exp Á V Ë RT ˜¯ The concentration of intrinsic carrier concentration in an intrinsic semiconductor is Ê Eg ˆ ni = Ao T3/2 exp Á Ë 2 KT ˜¯ In an intrinsic semiconductor, when the effective mass of holes and electrons are equal, then Fermi energy level lies at the middle of energy gap, EF =
EC + EV 2
Transport Properties of Semiconductors
267
A semiconductor doped with acceptor impurities has more positive charges and is known as a p type semiconductor. A semiconductor doped with donor impurities is known as an ntype semiconductor. In an ntype semiconductor, the Fermi energy level lies at the middle of the donor level and the lower energy level of the conduction band, EC + ED 2 In a ptype semiconductor, the Fermi energy level lies at the middle of the top of the valence band and the acceptor energy level, i.e.,
i.e.,
EF =
EF =
EV + E A 2
When a transverse magnetic field is applied to a current carrying conductor in the zdirection, an electric field is induced in a direction perpendicular to both the current and magnetic field. This phenomenon is known as Hall effect. The Hall voltage developed on the specimen is equal to V H = E H ¥ d, where EH is the electric field intensity due to Hall effect and d, is the thickness of specimen. 1 1 1 According to Mathiessen, the combined drift mobility is equal to m = m + m , where ml and mL d l L are the mobility due to impurity scattering and lattice scattering.
Solved Problems Example 10.1 Calculate the intrinsic carrier concentration, intrinsic conductivity and resistivity of Ge at 300 K using the following data: me = 0.4 m2 V1 s1, mh = 0.2 m2 V1 s1, Eg = 0.7 eV, me* = 0.55 m0, and mn* = 0.37 m0. Given Data: T = 300 K
Temperature
Solution:
Electron mobility
me = 0.4 m2 V1 s1
Hole mobility
mh = 0.2 m2 V1 s1
Band gap
Eg = 0.7 eV
Electron effective mass
me* = 0.55 m0
Hole effective mass
mh* = 0.37 m0
The intrinsic concentration is given by Ê 2p kT ˆ ni = 2 Á 2 ˜ Ë h ¯
3/ 2
È  Eg ˘ (mh* me* )3/ 4 exp Í ˙ Î 2kT ˚
268
Materials Science
Ê 2p ¥ 1.38 ¥ 1023 ¥ 300 ˆ = 2Á ˜¯ (6.626 ¥ 1034 ) 2 Ë
3/ 2
(0.55 ¥ 0.37)3/ 4 ¥ (9.1 ¥ 1031 )3/ 2
È  0.7 ¥ 1.6 ¥ 1019 ˘ exp Í ˙ 23 Î1.38 ¥ 10 ¥ 300 ˚ = 1.352 ¥ 1013 m3 s = ni e (me + mn)
The intrinsic conductivity
= 1.298 ¥ 106 r = 1/s
The intrinsic resistivity
= 0.77 ¥ 106 The intrinsic concentration
ni = 1.352 ¥ 1013 m3
The intrinsic conductivity
s = 1.298 ¥ 106 W1 m1
The intrinsic resistivity
r = 0.77 ¥ 106 W m.
Example 10.2 A ntype Si wafer has been doped uniformly with antimony (Sb) atoms and the doped Si has the donor concentration of 1016 per cm3. Calculate the Fermi energy with respect to the Fermi energy in intrinsic Si (For Si, ni = 1.45 ¥ 1010 cm3). Solution:
Doping of Sb converts Si into ntype material with Nd = 1016 cm3. For Si, ni = 1.45 ¥ 1010 cm3 Nd > ni Therefore, we have
Nd = 1016 cm3
For intrinsic Si,  ( EC  EFi ) ˘ ni = Nc exp ÈÍ ˙ kT Î ˚
(10.79)
Nd = Nc exp È  ( EC  EFd ) ˘ Í ˙ kT Î ˚
(10.80)
For doped Si,
Dividing Eq. (10.79) by Eq. (10.80), we get Nd È ( E  EFi ) ˘ = exp Í Fd ˙ ni kT Î ˚ EFd  EFi = kT ln
Ê Nd ˆ = 0.348 eV ÁË n ˜¯ i
The Fermi energy with respect to EF in intrinsic Si = 0.348 eV.
Transport Properties of Semiconductors
269
Example 10.3 Find the resistance of an intrinsic germanium rod which is 1 cm long, 1 mm wide and 1 mm thick at 300 K. For germanium ni = 2.5 ¥ 1019 /m3 , me = 0.39 m2 V1 s1 , mh = 0.19 m2 V1 s1 at 300 K. Given Data: ni = 2.5 ¥ 1019 /m3
Intrinsic carrier concentration Electron mobility,
me = 0.39 m2 V1 s1
Hole mobility
mh = 0.19 m2 V1 s1 l = 1 ¥ 102 m
Length of the rod Solution:
We know that the electrical conductivity of an intrinsic semiconductor (Germanium) is s = ni e ( me + m h ) Substituting the values, we get = 2.5 ¥1019 ¥1.6 ¥1019 ¥ (0.39 + 0.19) = 2.32 Therefore, the resistance, l sA where A is area of crosssection and given by product of width and thickness. R =
Substituting the given values, we get R =
1 ¥ 102 = 4310 W 2.32 ¥ (1 ¥ 103 ¥ 1 ¥ 103 )
The resistance of germanium is 4310 W. Example 10.4 The intrinsic carrier density is 1.5 ¥ 1016 m3. If the electron and hole mobilities are 0.13 and 0.05 m2 V1 s1, calculate the electrical conductivity. Given Data:
Solution:
Carrier concentration,
ni = 1.5 ¥ 1016 m3
Electron mobility,
me = 0.13 m2 V1 s1
Hole mobility,
mh = 0.05 m2 V1 s1
We know that the electrical conductivity is s = n1e [ m e + m h ]
270
Materials Science
Substituting the values, we get = 1.5 ¥ 1016 ¥ 1.6 ¥ 1019 [0.13 + 0.05] = 4.32 ¥ 104 W1 m1 The electrical conductivity of the intrinsic semiconductor is 4.32 ¥ 104
W1 m1 .
Example 10.5 Find the intrinsic resistivity of Ge at room temperature of 300 K if the carrier density is 2.15 ¥ 1013/cm3 Given Data:
Solution:
Mobility of electron
m e = 3900 cm 2 V 1 s 1
Mobility of hole
m n =1900 cm 2
Carrier density
ni = 2.15 ¥ 1013 cm3
We know that the conductivity of Ge is s i = e( me + m h )ni Substituting the values, we get = 1.6 ¥ 1019 ¥ (3900 + 1900) ¥ 2.15 ¥ 1013 = 1.6 ¥ 1019 ¥ 5800 ¥ 2.15 ¥ 1013 = 2.32 ¥ 102 ohm1 cm1 We also know that the intrinsic resistivity ri =
1 si
Substituting the values, we get =
1 2.32 ¥ 102
ri = 43 W cm. Example 10.6 In a ptype germanium ni = 2.1 ¥ 1019 m3 and density of boron is 4.5 ¥ 1023 atoms m3. The electron and hole mobilities are 0.4 and 0.2 m2V1s1, respectively. What is its electrical conductivity before and after the addition of boron atoms? Given Data: Carrier concentration
ni = 2.1 ¥ 1019 m3
Electron mobility
m e = 0.4m 2V 1s 1
Hole mobility
m h = 0.2 m 2 V 1 s 1
Density of boron is equal to density of hole
p = 4.5 ¥ 1023 m3
Transport Properties of Semiconductors
Solution:
271
We know that the conductivity of the Ge is s = n1e( m e + m h ) Substituting the values, we get = 2.1 ¥ 1019 ¥ 1.6 ¥ 1019 (0.4 + 0.2) = 2.016 W1m1 After doping with boron, the electrical conductivity due to extrinsic (ptype) semiconductor is s p = pe mp Substituting the values, we get = 4.5 ¥ 1023 ¥ 1.6 ¥ 1019 ¥ 0.2 = 1.44 ¥ 104 W 1m 1 Therefore, the electrical conductivity of boron doped semiconductor is 1.44 ¥ 10 4 W 1 m1 .
Example 10.7 Find the resistance of a 1 cm3 pure Si crystal. What is the resistance when the crystal is doped with arsenic with a doping concentration of 1 in 109 (Given: n = 5 ¥ 1028 m3, ni = 1.45 ¥ 1013 m3, me = 1.35 m2 V1 s1, mh = 0.45 m2 V1 s1). Given Data:
Solution:
Atomic concentration in Si
= 5 ¥ 1028 m3
Intrinsic concentration (ni)
= 1.45 ¥ 1013 m3
Electron mobility (me)
= 1.35 m2 V1 s1
Hole mobility (mh)
= 0.45 m2 V1 s1
The intrinsic conductivity is si = ni e (me + mh) = 4.18 ¥ 106 W1 m1 The resistivity is
r = 1/s = (RA/L) = 2.39 ¥ 105 W m
Therefore, the resistance is R = L/sA = 2.39 ¥ 107 W If the crystal is doped with 1 in 109 arsenic, then the donor concentration is given by Nd =
N si 5 ¥ 1028 = = 5 ¥ 1019 m3 9 10 9 10
272
Materials Science
The concentration of hole is
(
2 1.45 ¥ 1016 p = Ni = 5 ¥ 1019 Nd
)
2
= 4.2 ¥ 106 m3
Therefore, the conductivity is s = neme = Nd e me = 10.8 W1 m1 R = L/sA = 9.26 W
The resistance is Example 10.8
Mobilities of electrons and holes in a sample of intrinsic Ge at 300 K are 0.36 m2 V1 s1 and 0.17 m2 V1 s1, respectively. If the resistivity of the specimen is 2.12 W m, compute the forbidden energy gap for Ge, me* = 0.5 m0 and mh* = 0.37 m0. Given Data:
Solution:
Temperature
T = 300 K
Resistivity
r = 2.12 W m
Electron mobility
me = 0.36 m2 V1 s1
Hole mobility
mh = 0.17 m2 V1 s1
The conductivity is given by s = 1/r =
1 = 0.471698 W1 m1 2.12
The conductivity is also given by s = ni e (me + mh) ni =
s 0.471698 = 1.6 ¥ 1019 (0.36 + 0.17) e ( me + m h )
= 5.56247 ¥ 1018 The intrinsic concentration of carriers is given by Ê  Eg ˆ ni = (NC NV)½ exp Á Ë 2k BT ˜¯ where,
2p k BT ˆ NC = 2 ÊÁ Ë h 2 ˜¯
3/ 2
(m )
* 3/ 2 e
Ê ˆ 23 = 2 Á 2p ¥1.38 ¥10 ¥2300 ˜ ÁË ˜¯ 6.626 ¥1034
(
= 8.852 ¥ 1024
)
3/ 2
(0.5 ¥ 9.1¥10 )
31 3/ 2
Transport Properties of Semiconductors
NV = 2 ÊÁ 2p k BT ˆ˜ Ë h2 ¯
3/ 2
273
(m )
* 3/ 2 h
Ê ˆ 23 = 2 Á 2p ¥1.38 ¥10 ¥2300 ˜ ÁË ˜¯ 6.626 ¥1023
(
3/ 2
(0.37 ¥ 9.1¥10 )
31 3/ 2
)
= 5.635 ¥ 1024 The energy gap of an intrinsic semiconductor is given by È ( N C NV )1/ 2 ˘ ˙ Eg = 2kT ln Í ni ÍÎ ˙˚ = 2kT ¥ 14.054 Eg = 0.727 eV The band gap of Ge is 0.7 eV. Example 10.9 For an intrinsic semiconductor with a gap width Eg = 0.7 eV, calculate the concentration of intrinsic charge carriers at 300 K assuming that m = m *e = m0 (rest mass of electron). Given Data: m0 = m* = 9.1
Reset mass of electron, Planck’s constant
h = 6.62
¥ 1034 Js
Boltzmann’s constant,
k = 1.38
¥ 1023 JK1
Eg = 0.7 eV
Bandgap energy
Solution:
¥ 1031 kg
¥ 1019 C
Electronic charge
e = 1.6
Temperature,
T = 300 K
We know that the intrinsic carrier concentration Ê 2 p me* k T ˆ ni = 2 ¥ Á ˜¯ h2 Ë
3 2
e
 Eg / 2 k T
Substituting the values, we get Ê 2 ¥ 3.14 ¥ 9.1 ¥ 1031 ¥ 1.38 ¥ 1023 ¥ 300 ˆ = Á ˜¯ (6.626 ¥ 1034 ) 2 Ë È  Eg ˘ = 2.5087 ¥ 1025 exp Í ˙ Î KT ˚
3
2
È  Eg ˘ exp Í ˙ Î KT ˚
274
Materials Science
= 2.5087 ¥
1025
È 0.7 ¥ 1.6 ¥ 1019 ˘ exp Í ˙ 23 Î 2 ¥ 1.38 ¥ 10 ¥ 300 ˚
= 2.5087 ¥ 1025 ¥ 1.335 ¥ 106 = 33.49 ¥ 1018 Therefore, the carrier concentration of an intrinsic semiconductor is = 33.49 ¥ 1018 m3. Example 10.10 The energy gap of silicon is 1.1 eV. Its electron and hole mobilities at room temperatures are 0.48 and 0.013 m2V1s1. Evaluate the carrier concentration and its electrical conductivity. Given Data:
Solution:
Energy gap,
Eg = 1.1 eV
Electron mobility,
me = 0.48 m2V1s1
Hole mobility,
mh = 0.013 m2 V1s1
Temperature,
T = 300 K
Boltzmann’s constant
k = 1.38 ¥ 1023 JK1
We know that the intrinsic carrier concentration Ê 2 p me* k T ˆ (  Eg / 2 k T ) ni = 2 Á ˜¯ e h2 Ë Substituting the given values, we have Ê ˆ 31 23 2 ¥ 3.14 ¥ 9.1 ¥ 10 ¥ 1.38 ¥ 10 ¥ 300 ˜ ni = 2 ¥ Á 34 2 Á ˜ 6 626 ¥ 10 . Ë ¯
(
32
)
Ê 2.3626 ¥ 1050 ˆ ni = 2 ¥ Á Ë 4.39038 ¥ 1067 ˜¯
32
Ê 1.76 ¥ 1019 ˆ ¥ exp Á Ë 828 ¥ 1023 ˜¯
= 2 ¥ [5.3942 ¥ 1016]3/2 ¥ exp
(21.256)
= 2 ¥ 1.2528 ¥ 1025 ¥ 5.8697 ¥ 1010 ni = 1.4707 ¥ 1016 m3 We know that the electrical conductivity, s i = ni e ( m e + m n )
19
Ê 1.1 ¥ 1.6 ¥ 10 ˆ ¥ exp Á 23 Ë 2 ¥ 1.38 ¥ 10 ¥ 300 ˜¯
Transport Properties of Semiconductors
275
Substituting the values, we get = 1.4707 ¥ 1016 ¥ 1.6 ¥ 109 (0.48 + 0.013) si = 1.160 ¥ 103 W1 m1 Therefore, the electrical conductivity of silicon is 1.160 ¥ 103 W1 m1. Example 10.11 For a silicon semiconductor with a band gap of 1.12 eV, determine the position of the Fermi level at 300 K if me* = 0.12m0 and mh* = 0.28m0 . Given Data:
Solution:
Band gap,
Eg = 1.12 eV
Effective mass of electron
me* = 0.12m0
Effective mass of hole
mh* = 0.28m0 .
Temperature
T = 300 K
We know that the Fermi energy is EF =
Eg 2
+
Ê m* ˆ 3 kT log e Á h* ˜ 4 Ë me ¯
Substituting the values, we get EF =
Ê 0.28 m0 ˆ 1.12 3 ¥ 1.38 ¥ 10 23 ¥ 300 log e Á + 2 4 ¥ 1.6 ¥ 10 19 Ë 0.12 m0 ˜¯
= 0.56 +
3 ¥ 0.0258 ¥ log e 2.333 4
= 0.56 + 0.01935 ¥ 0.8473 = 0.56 + 0.016 = 0.576 eV Therefore, the Fermi energy silicon at 300 K is 0.576 eV. Example 10.12 Suppose that the effective mass of holes in a material is four times that of electrons. At what temperature would the Fermi level be shifted by 10% from the middle of the forbidden energy gap? Given Eg = 1 eV. Given Data: Energy gap
Eg = 1 eV = 1.6 ¥ 1019 J
At temperature T
mh* / me* = 4
276
Materials Science
Solution:
We know that the Fermi energy is EF =
Ê m* ˆ Ec + Ev 3 kT + log Á h* ˜ 2 4 Ë me ¯
For 0 K, EF is lies between the band gap. Hence, EF is given by EF = Ev + 0.5 eV ( Ev + 0.5) ¥ 1.6 ¥ 10 19 =
Ec + E v 2
[\T = 0]
Let Fermi level shift by 10% at temperature T, i.e., 0.1 eV. i.e.,
( Ev + 0.6 ) ¥ 1.6 ¥ 1019 =
Ev + E0 3 k T + log 4 2 4
Subtracting the above equation, we get 0.16 ¥ 1019 =
3k T log 4 4
Simplifying, we get T =
=
4 ¥ 0.16 ¥ 1019 3 ¥ 1.38 ¥ 1023 ¥ log 4 0.6408 ¥ 1019 = 116 K 5.739 ¥ 1023
Therefore, the temperature at watch Fermi level is shifted 10% is 116 K. Example 10.13 The following data are given for an intrinsic Ge at 300 K. Calculate the conductivity of the sample (Given: ni = 2.4 ¥ 1019 m3, me = 0.39 m2 V1 s1, mh = 0.19 m2 V1 s1) Given Data:
Solution:
Intrinsic concentration
ni = 2.4 ¥ 1019 m3
Electron mobility
me = 0.39 m2 V1 s1
Hole mobility
mh = 0.19 m2 V1 s1
The intrinsic conductivity is si = ni e (me + mp) = 2.4 ¥ 1019 ¥ 1.6 ¥ 1019 (0.39 + 0.19) = 2.22 W1 m1 The conductivity of Ge at 300 K
si = 2.22 W1 m1.
Transport Properties of Semiconductors
277
Example 10.14 In an ntype semiconductor, the Fermi level lies 0.3 eV below the conduction band at 300 K. If the temperature is increased to 330 K, find the new position of the Fermi level. Solution:
The concentration of carrier electrons at 300 K is given by È ( E  EF 300 ) ˘ Ni300 = NC exp Í C ˙ kT Î ˚
(
(i)
)
È 0.3 ¥1.6 ¥1019 ˘ ˙ = NC exp Í k ¥ 300 ÍÎ ˙˚ È  ( EC  EF 300 ) ˘ Ni330 = NC exp Í ˙ kT Î ˚
(ii)
Taking NC300 ª NC330 from Eqs. (i) and (ii), we get È 0.3 ¥1.6 ¥1019 ˘ È  EC  EF 300 ˘ exp Í ˙ = exp Í ˙ k ¥ 300 Î k ¥ 330 ˚ Î ˚ E  EF 300 0.3 = C 300 330 EC  EF330 = 0.33 eV At 330 K, the Fermi energy level lies 0.33 eV, below the conduction band. Example 10.15 The conductivity of Ge at 20 °C is 2 W1 m1. What is its conductivity at 40 °C? Eg = 0.72 eV. Solution:
The conductivity is given by s1 = ni e (me + mm) È 2p kT ˘ ni = 2 Í 2 ˙ Î h ˚
where
3/ 2
È  Eg ˘ (me m p )3/ 4 exp Í ˙ Î 2kT ˚
At 20 °C and 40 °C È 2p k ¥ 293 ˘ ni20 = 2 Í ˙˚ h2 Î
3/ 2
È 2p k ¥ 313 ˘ ni40 = 2 Í ˙˚ h2 Î
3/ 2
Ê  Eg ˆ (me m p )3/ 4 exp Á Ë 2k ¥ 293 ˜¯
(iii)
Ê  Eg ˆ (me m p )3/ 4 exp Á Ë 2k ¥ 313 ˜¯
(iv)
278
Materials Science
Dividing Eq. (iii) by Eq. (iv), we get ni 40 Ê 313 ˆ = Á Ë 293 ˜¯ ni 20
3/ 2
È Eg Ê 1 1 ˆ˘ exp Í ÁË ˜ ˙ = 2.743 Î 2 k 293 313 ¯ ˚
si20 = ni20 e(me + mm)
i.e.,
si40 = ni40 e(me + mm) s i 20 n = i 20 s i 40 ni 40
i.e.,
si40 = si20
ni 20 = 2 ¥ 2.743 ni 40
= 5.486 W1 m1 The conductivity of Ge at 40 °C is 5.486 W1 m1. Example 10.16 The energy gap of Si is 1.1 eV. The average electron effective mass is 0.31 m, where m is the free electron mass. Calculate the concentration in the conduction band of Si at RT, T = 300 K. Assume that EF = Eg/2. Given Data: Energy gap of Si
= 1.1 eV
Effective mass of electron
= 0.31 m
Temperature
= 300 K EF = Eg/2
Solution:
For Si, the intrinsic concentration is given by È 2p kT me* ˘ ni = 2 Í ˙ 2 Î h ˚
3/ 2
È  ( EC  EV ) ˘ exp Í ˙ 2kT Î ˚
Substituting the given values, we get È 2p ¥ 1.38 ¥ 1023 ¥ 300 ¥ 0.31 ¥ 9.1 ¥ 1031 ˘ ni = 2 Í ˙ (6.626 ¥ 1034 ) 2 Î ˚
3/ 2
È  Eg ˘ exp Í ˙ Î 2kT ˚
È 1.1 ¥ 1.6 ¥ 1019 ˘ ni = 4.32166 ¥ 1024 exp Í ˙ 23 Î 2 ¥ 1.38 ¥ 10 ¥ 300 ˚ = 2.5367 ¥ 1015 electrons per m3 The intrinsic concentration of Si at 300 K is 2.5367 ¥ 1015 electrons per m3.
Transport Properties of Semiconductors
279
Example 10.17 The Hall coefficient and conductivity of Cu at 300 K have been measured to be 0.55 ¥ 1010 m3 A1s1 and 5.9 ¥ 107 W1 m1, respectively. Calculate the drift mobility of electrons in copper. Given Data:
Solution;
Hall coefficient of Cu
=  0.55 ¥ 1010 m3 A1 s1
Conductivity of Cu
= 5.9 ¥ 107 W1 m1
Temperature
= 300 K
Drift mobility =  RH s  = 0.55 ¥ 1010 ¥ 5.9 ¥ 107 = 3.2 ¥ 103 m2 V1 s1 The drift mobility is given by, m d = 3.2 ¥ 103 m2 V1 s1
Example 10.18 Using the electron drift mobility from the Hall effect measurement (md = 3.2 ¥ 103 m2V 1s 1), calculate the concentration of conduction electrons in copper, and determine the average number of electrons contributed to the free electron gas per copper atom in a solid (Given: s = 5.9 ¥ 107 W1 m1) Solution:
The conductivity of an ntype semiconductor is given by s = nem Therefore,
ni =
s em
ni =
5.9 ¥107 1.6 ¥1019 ¥ 3.2 ¥ 103
Substituting the value, we get
= 1.15 ¥ 1029 m3 The concentration of free electron in pure Cu, n=
Avogadro’s constant ¥ Density ¥ Number of free electrons per atom Atomic weight =
6.022 ¥ 1023 ¥ 8900 ¥ 1¥ 103 63.5
= 8.44 ¥ 1028 electrons per m3.
280
Materials Science
The average number of electrons contributed per Cu atom =
Concentration of electrons in an ntype semiconductor Concentration of electrons in pure Cu atom
=
1.15 ¥1029 = 1.36 8.44 ¥ 1028
Therefore, the average number of electrons contributed per Cu atom is one. Example 10.19 Find the Hall coefficient and electron mobility of germanium for a given sample (1 cm length, 5 mm breadth, 1 mm thickness). A current of 5 milliamperes flows from a 1.35volt supply and develops a Hall voltage of 20 nillivolts across the specimen in a magnetic field of 0.45 Wb/m2. Given Data: Current through the specimen
Solution:
I = 5 ¥ 103 A
Voltage across the specimen
V = 1.35 V
Length of the sample
L = 1 ¥ 102 m
Breadth of the sample
b = 5 ¥ 103 m
Thickness of the sample
t = 1 mm or 1 ¥ 103 m
Area of the sample
a = 5 ¥ 106 m2
Hall voltage
Vy = 20 ¥ 103
Magnetic field
H = 0.45 Wb m2
We know that the resistivity of the Ge sample is Ra l
r =
V 1.35 = I 5 ¥ 103 Substituting the values of R = V/I, we get S =
Va lI
1.35 ¥ 5 ¥ 106 = 0.135 W m 5 ¥ 103 ¥ 1 ¥ 102 We know that the Hall field, is r =
Ey =
Vy Thickness
Transport Properties of Semiconductors
=
20 ¥ 103 1 ¥ 103
= 20 Vm 1 Current density given by, Jx =
Current Area of crosssection
Substituting the values, we get J =
5 ¥ 103 5 ¥ 106
= 1 ¥ 103 Am 2 Ey 1 = ne HJ x =
20 0.45 ¥ 103
= 0.044 m3 C 1 We know that the Hall coefficient is RH =
3p 1 ¥ 8 ne
Substituting the values, we get =
3 ¥ 3.14 ¥ 0.044 8
= 0.0524 = 0.0524 m3 C 1 We know that the electron mobility is me = =
RH r 0.0524 = 0.39 0.135
= 0.39 m 2 V 1 s 1 \ Therefore, the mobility of the Ge sample is 0.39 m 2 V 1 s 1 .
281
282
Materials Science
Example 10.20 A 2.0cm wide and 1.0mm thick copper strip is placed in a magnetic field with B = 1.5 weber / m2 perpendicular to the strip. Suppose a current of 200 A is set up in the strip. What Hall potential difference would appear across the strip? Given N = 8.4 ¥ 1028 electrons/m3. Given Data: Ix = 200 A
Current flowing
Hz = 1.5 Wb m2
Applied magnetic field
Solution:
Number of electrons per unit volume
n = 8.4 ¥ 1028 electrons m3
Thickness of the strip
d = 1.0 ¥ 103 m
Ix HZ net Substituting the values, we get
Hall potential, Vy =
Vy =
200 ¥ 1.5 8.4 ¥ 10 ¥ 1.6 ¥ 1019 ¥ 1.0 ¥ 103 28
= 2.2 ¥ 105 = 22 ¥ 106 Therefore, the Hall potential difference appearance between the ship is 22 m v. Example 10.21 The Hall coefficient of a specimen of a doped silicon is found to be 3.66 ¥ 104 m3/C. The resistivity of the specimen is 8.93 ¥ 103 W m. Find the mobility and density of the charge carriers? Given Data: Hall coefficient of the specimen RH = 3.66 ¥ 104 m3 C1 r = 8.93 ¥ 103 W m
Resistivity of the specimen Solution:
We know that the carrier concentration is
nh =
1 RH e
Substituting the values, we get =
1 3.66 ¥104 ¥1.6 ¥1019
= 1.708 ¥ 1022 m3 The carrier concentration of silicon doped specimen is 1.708 ¥ 1022 m3 We also know that, the mobility of carrier is mn =
RH r
Transport Properties of Semiconductors
283
Substituting the values, we get
mh =
3.66 ¥ 104 8.93 ¥ 103
mh = 0.04099 m2 V1 s1 The mobility of silicon doped specimen is 0.04099 m2 V1 s1. Example 10.22 An ntype semiconductor specimen has Hall coefficient RH = 3.66 ¥ 1011 m3 A1 s1. The conductivity of the specimen is found to be 112 ¥ 107 W1 m1. Calculate the charge carrier density ne and electron mobility at room temperature. Given Data: RH = 3.66 ¥ 1011 m3 A1 s1
Hall coefficient
s = 112 ¥ 107 W1 m1
Conductivity Solution:
The Hall coefficient is given by RH =
\
n=
=
3p 1 8 ne 3p 1 8 RH e 3p 1 8 3.66 ¥ 1011 ¥1.6 ¥1019
= 2 ¥ 1029 m3 For ntype semiconductor, s = neme me = s/ne me =
112 ¥107 1.6 ¥1019 ¥ 2 ¥ 1029
= 0.035 m2 V1 s1 The concentration of electrons is 2 ¥ 1029 m3. The electron mobility at room temperature = 0.035 m2 V1 s1.
284
Materials Science
Example 10.23 A current of 50 A is established in a slab of copper, 0.5 cm thick and 2 cm wide. The slab is placed in a magnetic field B of 1.5 T. The magnetic field is perpendicular to the plane of the slab and to the current. The free electrons concentration in Cu is 8.4 ¥ 1028 m3. What will be the magnitude of the Hall voltage across the width of the slab. Given Data:
Solution:
Current
I = 50 A
Magnetic field
B = 1.5 T
Thickness of the slab
t = 0.5 ¥ 102
Width of the slab
d = 2 ¥ 102
Concentration of electrons
N = 8.4 ¥ 1028 m3
The Hall voltage is given by VH =
BI new
Substituting the value, we get =
1.5 ¥ 50 8.4 ¥ 1028 ¥ 1.6 ¥ 1019 ¥ 2 ¥102
= 2.79 ¥ 107 The Hall voltage is 2.79 ¥ 107 V. Example 10.24 Find the relaxation time of conduction electrons in a metal of 1.54 ¥ 108 W m resistivity, if the metal has 5.8 = 1028 conduction electrons per m3. Given Data:
Solution:
The resistivity of the metal
= 1.54 ¥ 108 W m
The carrier concentration of electron
= 5.8 ¥ 1028 m3
We know that, the relaxation time t r =
sm ne
2
=
m r ne 2
Substituting the values of r, m, n and e in the above equation, we get tr =
9.1 ¥ 10 31 1.54 ¥ 10 8 ¥ 5.8 ¥ 1028 ¥ (1.6 ¥ 10 19 )2
= 3.97972 ¥ 1014 s Therefore, the relaxation time for the electron in the metal is 3.98 ¥ 1014 s.
Transport Properties of Semiconductors
285
Example 10.25 A certain conductor has electron concentration of 5.9 ¥ 108 m3. Calculate the mobility of the charge carrier. Given conductivity is 6.22 ¥ 10 W1 m1 . Given Data:
Solution:
The conductivity of the metal
s = 6.22 ¥ 107 W1 m1
The carrier concentration of electron
n = 5.9 ¥ 1028 m3
We know that the mobility of the electron m =
s ne
Substituting the values of n, e and s in the above equation, we get m=
6.22 ¥ 107 5.9 ¥ 1028 ¥ 1.6 ¥ 10 19
= 6.5889 ¥ 103 Therefore, the mobility of the electrons in silver is 6.59 ¥ 1023 (m2 v1s1). Example 10.26 There are 1020 conduction electrons per m3 in a material having a resistivity of 0.1 W m. Find the charge mobility and electrical field needed to produce a drift velocity of 1 m per second. Given Data:
Solution:
The resistivity of the metal
= 0.1 W m
The carrier concentration of electron
= 1020 m3
The drift velocity
= 1 m s1
We know that the mobility of the electron m =
1 r ne
Substituting the values of n, e and r in the above equation, we get 1 m= 20 0.1 ¥ 10 ¥ 1.6 ¥ 10 19 = 0.625 The mobility of the electrons in a material is 0.625 m2v1s1 We know that the drift velocity vd = mE vd m Substituting the values, we get E=
=
1 0.625
= 1.6 Therefore, the mobility of the electrons in material is 0.625 m2v1s1 The electric field is 1.6 V m1.
286
Materials Science
Example 10.27 A certain conductor has electron concentration of 5.9 3 1028 m3. Calculate the mobility of the charge carrier. Given conductivity is 6.22 3 10 W21 m21 . Given Data:
Solution:
The conductivity of the metal
s 5 6.22 3 107 W21 m21
The carrier concentration of electron
n 5 5.9 3 1028 m3
s ne Substituting the values of n, e and s in the above equation, we get
We know that the mobility of the electron m =
6.22 ¥ 107
m=
5.9 ¥ 1028 ¥ 1.6 ¥ 10 19 5 6.5889 3 1023
Therefore, the mobility of the electrons in silver is 6.59 3 1023 m2 v21s21). Example 10.28 There are 1020 conduction electrons per m3 in a material having a resistivity of 0.1 W m. Find the charge mobility and electrical field needed to produce a drift velocity of 1 m per second. Given Data: 5 0.1 W m
The resistivity of the metal
The carrier concentration of electron 5 1020 m3 5 1 m s21
The drift velocity Solution:
1 r ne Substituting the values of n, e and r in the above equation, we get
We know that the mobility of the electron m =
m=
1 0.1 ¥ 10
20
¥ 1.6 ¥ 10 19
5 0.625 The mobility of the electrons in a material is 0.625 m2v21s21 We know that the drift velocity vd 5 mE E=
vd m
Substituting the values, we get 1 = 1.6 0.625 Therefore, the mobility of the electrons in material is 0.625 m2v21s21 =
The electric field is 1.6 V m21
Transport Properties of Semiconductors
287
Example 10.29 Calculate the mobility of electrons in copper assuming that each atom contributes one free electron for conduction. Resistivity 5 1.73 ¥ 108 W m, Atomic weight = 63.5 and Density 5 8.92 ¥ 103 kg m3. Avogadro’s number is 6.025 ¥ 1023/mole. Given Data:
Solution:
The resistivity of the copper
r = 1.73 ¥ 108 W m
The atomic weight of the copper
z = 63.5
The density of the copper is
d = 8.92 ¥ 103 kg m3
We know that the carrier concentration = Avogadro ¢s number ¥ Density Atomic weight Substituting the values in the above equation, we get 8.92 ¥ 103 63.5 3 m
i.e., n = 6.023 ¥ 1023 ¥ n = 8.46 ¥ 1025
We know that the the relaxation time is, s =
1 r
1 =
1.73 ¥ 10 8
= 5.78 ¥ 107 V1m1 Similarly, we know that the relaxation time is t =
ms ne 2
Substituting the values of s, m, n and e in the above equation, we get =
5.78 ¥ 107 ¥ 9.11 ¥ 10 31 8.46 ¥ 1025 (1.6 ¥ 10 19 )2
t = 2.43 ¥ 1011 s s ne Substituting the values of s, n and e in the above equation, we get
We know that mobility m =
5.78 ¥ 107 =
8.46 ¥ 1025 ¥ 1.6 ¥ 10 19
m = 4.27 m2 V1s1 The mobility of electrons in copper is 4.27 m2 V1s1 Therefore, the conductivity of copper is 5.78 ¥ 107 W1 m1 The mobility of electrons in copper is 4.27 m2 V1s1.
288
Materials Science
Example 10.30 A uniform silver wire has a resistivity of 1.54 ¥ l08 ohmm at room temperature. For an electric field along the wire of 1 volt/cm, calculate the average drift velocity and mobility of electron assuming that there is 5.8 ¥ 1028 conduction electrons/m3. Given Data:
Solution:
The resistivity of silver
= 1.54 ¥ 108 ohm m1
Electric field along the wire
= 100 V m1
The carrier concentration of electron
= 5.8 ¥ 1028 m3 s ne 1 = rne
We know that the mobility of the electron m =
Substituting the values of n, e and r in the above equation, we get m=
=
1 1.54 ¥ 10
8
¥ 5.8 ¥ 1028 ¥ 1.6 ¥ 10 19
1 = 6.9973 ¥ 10 3 142.912
The mobility of the electrons in silver is 6.9973 ¥ 103 m2 V1s1 Similarly, we know that the drift velocity vd = m E Substituting the values of m, and E in the above equation, we get vd = 6.9973 ¥ l03 ¥ 100 The drift velocity (vd ) = 0.69973 Therefore, the drift velocity of the electron is silver is 0.69973 m s1. Example 10.31 For a metal having 6.5 ¥ 1028 conduction electrons per m3, find the relaxation time of the conduction electrons if the metal resistivity is 1.43 ¥ 108 ohm m. Given Data: = 1.43 ¥ 108 W m = 6.5 ¥ 1028 m3
The resistivity of the metal The carrier concentration of electron Solution:
We know that the relaxation time tr = =
sm ne 2
m r ne 2
Transport Properties of Semiconductors
289
Substituting the values of r, m, n and e in the above equation, we get tr =
9.1 ¥ 10 31 1.43 ¥ 10 8 ¥ 6.5 ¥ 1028 ¥ (1.6 ¥ 10 19 )2
= 3.828 ¥ l0l4 s Therefore, the relaxation time for electrons in the metal is 3.83 ¥ l014 s. Example 10.32 Calculate the freeelectron concentration, mobility and drift velocity of electrons in an aluminum wire of 5m length and a resistance of 60 m W if it carries a current of 15 A assuming that an aluminum atom contributes 3 free electrons for conduction. Data given for aluminum: resistivity = 2.7 ¥ 108 W m, atomic weight = 26.98 and density = 2.7 ¥ 103 kg m3. [VTU MQP] Given Data: The resistance of aluminum
R = 60 m W m
The resistivity of aluminum
r = 2.7 ¥ 108 W m
Current in the wire
I = 15 A
Length of the aluminum wire
L=5m
Number of free electrons per atom
m=3
The density of the aluminum
D = 2.7 ¥ 103 kg m3 = 26.98
The atomic weight of the aluminum Solution:
We know that the concentration of free electrons n=
No. of free electrons ¥ N A ¥ 103 ¥ Density Atomic weight
Substituting the values in the above equation, we get =
3 ¥ 6.023 ¥ 1023 ¥ 103 ¥ 2.7 ¥ 103 26.98
= 1.808 ¥ l029 s ne 1 = rne
We know that the mobility of the electron m =
Substituting the values of n, e and r in the above equation, we get m=
1 2.7 ¥ 10
8
¥ 1.808 ¥ 1029 ¥ 1.6 ¥ 10 19
= 1.2803 ¥ 103 The mobility of the electron in aluminum is 1.2803 ¥ 103 m2v1s1
290
Materials Science
We know that the drift velocity vd = m E Substituting E = IR /L, we get IR L Substituting the values of I, R, L and m in the above equation, we get vd = m
vd =
1.2803 ¥ 10 3 ¥ 15 ¥ 60 ¥ 10 3 5
= 2.3 ¥ l04 m s1. The drift velocity of the electron in aluminum is 2.3 ¥ 104 m s1. Therefore, the free electron concentration in aluminum is 1.808 ¥ 1029 m3. The mobility of the electron in aluminum is 1.2803 ¥ 103 m2v1s1. The drift velocity of the electron in aluminum is 2.3 ¥ 104 m s1. Example 10.33 Calculate the drift velocity and thermal velocity of conduction electrons in copper at a temperature 300 K, when a copper wire of 2 m length and a resistance of 0.02 W carries a current of 15 A given the mobility of free electrons in copper is 4.3 ¥ 103 m2v1s1. Given Data:
Solution:
The resistance of the copper
R = 0.02 W m
Current in the wire
I = 15 A
Mobility of free electrons
m = 4.3 ¥ 103 m2v1s1
Length of the copper wire
L=2m
Temperature
T = 300 K
We know that the voltage drop across the wire V = IR Substitute the values of I and R, in the above equation, we get V = 15 ¥ 0.02 V = 0.3 V We know that the electric field in the metal E =
V L
Substituting the values of V and d in the above equation, we get =
0.3 2
= 0.15 V m1 We know that the drift velocity of the electron in the metal is vd = E ¥ m
Transport Properties of Semiconductors
291
Substituting the values of E and m, in the above equation, we get = 0.15 ¥ 4.3 ¥ l03 = 0.645 ¥ 103 m s1 The drift velocity of the free electrons in copper is 0.645 mm s1. We know that the thermal energy of the free electron in metal is Eth = Therefore, thermal velocity of free electrons in copper is Vth =
1 3 mVth2 = KT 2 2
3kT m
Substituting the values of k, T and m, in the above equation, we get Vth =
3 ¥ 1.381 ¥ 10 23 ¥ 300 9.11 ¥ 10 31
= 1.168 ¥ 105 m s1 The thermal velocity of the free electrons in copper is 1.168 mm s1. Therefore, the drift velocity of the free electrons in copper is 0.645 mm s1. The thermal velocity of the free electrons in copper is 1.168 mm s1.
ObjectiveType Questions 10.1. In a semiconductor all the states at 0 K in valence band are ________. 10.2. All the states at 0 K in the conduction band of a semiconductor are empty. (True/False) 10.3. The value of concentration of electrons in the conduction band is equal to Ê E  EC ˆ (a) n = Nc exp Á F Ë kT ˜¯
Ê E + EC ˆ (b) n = Nc exp Á F Ë kT ˜¯
Ê  E + EC ˆ (c) n = Nc exp Á F ˜¯ Ë kT
Ê E + EC ˆ (d) n = Nd exp Á F Ë kT ˜¯
10.4. The concentration of holes in the valence band is equal to Ê E + EF ˆ (a) p = Nv exp Á V Ë 2kT ˜¯
Ê E  EF ˆ (b) p = Nv exp Á V Ë 3kT ˜¯
Ê E + EF ˆ (c) p = Nv exp Á V Ë kT ˜¯
Ê E  EF ˆ (d) p = Nv exp Á V Ë kT ˜¯
292
Materials Science
10.5. The intrinsic carrier concentration in an intrinsic semiconductor is equal to Ê Eg ˆ Ê Eg ˆ (a) ni = Ao T3/2 exp Á (b) ni = Ao T3/2 exp Á ˜ Ë 3kT ¯ Ë 3kT ˜¯ Ê Eg ˆ (c) ni = Ao T3/2 exp Á Ë 2kT ˜¯
Ê Eg ˆ (d) ni = Ao T3/2 exp Á Ë 2kT ˜¯
10.6. The the Fermi energy level in an intrinsic semiconductor is equal to ________. 10.7. In an intrinsic semiconductor, the concentrations of electrons and holes are not equal. (True/False) 10.8. The thermal excitation energy produced by an electron in extrinsic semiconductors at room temperature is equal to ________. 10.9. The acceptor energy level for Ge lying above the valence band is equal to ________. 10.10. In ntype semiconductors, the value of Fermi energy level is equal to (a) EF =
EC + EV 2
(b) EF =
EC + ED 2
(c) EF =
EC + E A 2
(d) EF =
EC  ED 2
10.11. The concentration of electrons in an ntype semiconductor is equal to È 2p me * kT ˘ Ê E  EF ˆ (a) n = ( N D )1/ 2 2 Í exp Á D 2 ˙ Ë kT ˜¯ h Î ˚ È 2p me * kT ˘ Ê E + EF ˆ (b) n = ( N D )1/ 2 2 Í exp Á D 2 ˙ Ë kT ˜¯ h Î ˚ È 2p me * kT ˘ Ê E  EF ˆ (c) n = (2 N D )1/ 2 2 Í exp Á D 2 ˙ Ë kT ˜¯ h Î ˚ È 2p me * kT ˘ Ê E + EF ˆ (d) n = (2 N D )1/ 2 2 Í exp Á D 2 ˙ Ë kT ˜¯ h Î ˚ 10.12. The Fermi energy level in a ptype semiconductor is equal to EV + E A E  Ec (b) EF = V 2 2 EV + EC EV  E A (c) EF = (d) EF = 3 2 10.13. The carrier concentration in a ptype semiconductor is equal to 10.14. The mobility of charge carrier is s = ________. 10.15. The hall voltage of a specimen is equal to (a) VH = EH/d (b) VH = EH × d (a) EF =
(c) VH = 2EH/d
(d) VH = 2EH × d
Transport Properties of Semiconductors
293
10.16. According to Mathiessen’s rule, combined drift mobility is equal to (a)
1 2 1 = m d ml m L
(b)
1 2 1 = + m d ml m L
(c)
1 1 1 = m d ml m L
(d)
1 1 1 = + m d ml m L
10.17. In semiconductors, the electrical conductivity is proportional to concentration of carrier. (True/False) Answers 10.1. Occupied 10.3. (a) 10.5. (d) 10.7. False 10.9. 0.01 eV 10.11. (c) 3/ 4 1 10.13. ( 2 N a ) 2 È 2p M h kT ˘ exp ÊÁ EV  E A ˆ˜ Í h2 ˙ Ë 2kT ¯ Î ˚ 10.15. (b)
10.2. True 10.4. (d) EV + EC 10.6. 2 10.8. 0.025 eV 10.10. (b) 10.12. (a) 10.14. n e μ 10.16. (d)
10.17. True
Short Questions 10.1. 10.2. 10.3. 10.4. 10.5. 10.6. 10.7. 10.8. 10.9. 10.10. 10.11. 10.12. 10.13. 10.14. 10.15. 10.16. 10.17. 10.18. 10.19.
What is meant by Fermi level? What is meant by Fermi temperature? Distinguish between the intrinsic and extensic semiconductor? State mass action law. What is an intrinsic semiconductor? What is an extrinsic semiconductor? What is an ntype semiconductor? What is a ptype semiconductor? What is meant by donor energy level? What is meant by acceptor level? Write down the expression for carrier concentration for a ptype semiconductor. Write down the expression for carrier concentration for a ntype semicondictor? Define the term conductivity of a semiconductor. Define the term mobility of a semiconductor. What is Hall effect? Explain the origin of Hall effect. What is Hall coefficient? What is meant by Hall voltage? Mention the applications of Hall effect.
294
Materials Science
Descriptive Questions 10.1. (a) Derive the expressions for concentration of holes in a valence band and that of electrons in a conduction band for an intrinsic semiconductor. (b) Deduce an expression for intrinsic concentration using mass action law. 10.2. Deduce the mathematical expressions for the concentration of electrons and hole in the conduction band and valence band for an intrinsic semiconductor respectively and hence show that the Fermi level lies at the middle for an intrinsic semiconductor. 10.3. Obtain an expression for the conductivity of an ntype semiconductor and hence explain the determination of energy gap. 10.4. Derive an expression for Fermi level in ntype semiconductor and hence obtain an expression for carrier concentration of an ntype semiconductor. 10.5. Derive an expression for Fermi level in a ptype semiconductor and hence obtain an expression for concentration of hole in a ptype semiconductor. 10.6. (a) What is Hall effect? (b) Obtain an expression for Hall coefficient. (c) Explain the experimental technique used to find Hall coefficient. (d) List the advantages of Hall effect. 10.7. Write briefly about the temperature dependence of carrier concentration and Fermi level in an extrinsic semiconductor.
Exercises 10.1. Calculate the intrinsic conductivity of Si at 300 K. me = 0.135 m2 V–1 s–1 mh = 0.048 m2 V–1 s–1 Eg = 1.11 eV me* = 0.26 m0 mn* = 0.39 m0 10.2. Calculate the intrinsic carrier concentration of GaAs at 300 K. Given that the electron effective mass is 0.07 m, the hole effective mass is 0.56 m and its energy gap is 1.4 eV. 10.3. The resistance of a CdSe crystal is 10 W cm at 300 K. Find its resistance at 350 K. The band gap of CdSe is 1.74 eV. 10.4. The resistance of a semiconductor at different temperatures is given below. T (K)
r (W m)
300 340 380 420 450
89 165 365 1012 9658
Find the band gap of that semiconducting material. 10.5. SnSe is a ptype semiconductor. Its Fermi level lies just 0.2 eV above the valence band at 300 K. Find the position of the Fermi level at 370 K.
Chapter
11
MECHANICAL PROPERTIES
OBJECTIVES To understand mechanical properties and their applications in engineering materials. To understand stress, strain, elastic modulus and Poisson’s ratio. To explore the knowledge on the merits of hardness. To explain various types of tests like tensile, compression, impact, fatigue and creep tests. To discuss the various factors affecting mechanical properties. To explore the strengthening mechanism to improve mechanical properties. To define fracture mechanism.
11.1 INTRODUCTION The properties possessed by a material can be classified into the following types namely, physical, mechanical, electrical, chemical and thermal properties. Therefore, before selecting a material for a particular application, one has to know about its various properties. Hence, the study of properties of materials is a must for the selection of materials. The term mechanical property can be defined as the ability of the material to resist any deformation due to externally applied load. A material may have a number of mechanical properties. Some of the important mechanical properties are elasticity, plasticity, ductility, brittleness, malleability, weldability, castability, hardness, toughness, stiffness, resilience, creep endurance and strength. In this chapter, mechanical properties, their measurements and strengthening mechanisms are discussed to improve the mechanical properties and fracture.
296
Materials Science
11.2
MECHANICAL PROPERTIES AND THEIR MEASUREMENTS
The property exhibited by a material when it is subjected to an external load is known as mechanical property. Most of the above properties are defined based on the behaviour of the materials due to the application of stress. In the following section, let us study the definition for some of the mechanical properties. (1) Stress Consider a load is applied to a material. Due to the application of the load, a force is acting on the material. Therefore, there are some changes in the dimension of the material. An internal force known as a restoring force is acting and that force resists the changes taking place in the material. The restoring force acting per unit area of crosssection is known as stress and it is measured in N m2. It is given by the relation Stress =
Restoring force (or) applied force Area of cross section of the material
(11.1)
(2) Strain Consider a load is applied to a material. Due to the application of load, there are some changes in the dimension of the material. The ratio of the change in dimension to the actual dimension is known as strain. Therefore, Strain =
Change in dimension Actual dimension
(11.2)
The change in dimension of the material may represent either the change in length or volume or shape. Depending on the change in dimension, strain is classified into three types; linear strain, bulk strain and shear strain. Strain has no unit. (3) Modulus of elasticity Within the elastic limit, the ratio of stress to strain is a constant and this constant is known as modulus of elasticity. Depending upon the strain, there are three different types of modulus of elasticity namely, Young’s (Y), Bulk (K) and Rigidity (h) modulus. The above modulus are defined as, Young’s modulus = Bulk modulus =
Linear stress Linear strain
Bulk stress Bulk strain
Rigidity modulus =
Shear stress Shear strain
(11.3) (11.4) (11.5)
The unit for Young’s, Bulk and Rigidity modulus is N m2. (4) Poisson’s ratio When a wire is stretched, the length of the wire will increase. At the same time, the wire will become thinner, i.e., there is a decrease in the crosssection of the wire. The ratio of change in diameter to the original diameter of the wire is known as lateral strain. The ratio of the change in length to the original length of the wire is known as linear strain. The ratio of lateral strain to linear strain is known as Poisson’s ratio. It is denoted by the letter s and it has no unit. Poisson’s ratio =
Lateral strain Linear strain
(11.6)
Mechanical Properties
s=
Dd/d Dl/l
297
(11.7)
Dl Dd is the lateral strain and the linear strain. l d (5) Stress – Strain diagram The relation between stress and strain can be represented diagrammatically by plotting a curve between stress and strain. The plot is obtained by taking the strain in the x axis and the stress in the y axis. The stressstrain diagram is shown in Fig. 11.1.
where
Upper yield point Ultimate stress
Stress
Fracture Lower yield point Elastic limit Limit of proportionality
Strain
Fig. 11.1 Stress – Strain diagram (6) True strain and true stress The stress and strain used so far are known as conventional or engineering stress and strain. When a load is applied to a material, within the elastic limit, consider there is a change in the length of the material due to the application of the load. Thus, the change in length produces some change in the thickness or diameter of the material. The decrease in the diameter of the material within the elastic limit is not appreciable. Therefore, it is neglected. But in the plastic region, the change in the thickness or diameter of the material is not a negligible quantity. Therefore, in order to take into account the change in the diameter of the material in the plastic region, the terms, true strain and true stress are introduced. True stress (S*) is defined as the ratio of the load on the specimen to the instantaneous crosssectional area supporting the load. It is expressed as, S *=
P Ai
(11.8)
where Ai is the instantaneous crosssectional area corresponding to the load P. It is measured in N m2. True strain is defined as the ratio of the change in linear dimension to the instantaneous value of the dimension. e=Ú
Lf L0
Lf dL = Ln L L0
(11.9)
Equation (11.9) is known as natural or true strain. True stress and strain are used in plastic region of the material, whereas engineering stress and strain are used in elastic region.
298
Materials Science
The relation between conventional linear strain and true strain are obtained as follows. Conventional strain,
e=
Lf DL L f  L0 = = 1 L0 L0 L0
and true strain,
e = Ln
Lf L0
(11.10)
(11.11)
From Eq. (11.10) and Eq. (11.11), we get e = Ln (1 + e)
(11.12)
True strain and conventional strain are identical up to a strain value of 0.1. (7) Elasticity Consider a material is subjected to a load. There is a change in the dimension of the material due to the application of the load. When the load is removed, the material will regain its original shape. One can observe that up to a certain value of the load, the material is able to regain its original shape or dimension whenever there is an increase (or) decrease in the load. Beyond that value, it is not able to regain its original dimension. The region in which a material is capable of regaining its dimension is known as elastic region. The property, in which there is some change in dimension due to the load and regaining of the actual shape when the load is removed, is known as elastic property or elasticity of the material. Within the elastic limit, the material obeys the Hooke’s law. (8) Plasticity Consider a load is applied to the material beyond the elastic limit. The deformation produced in the material due to the application of load beyond the elastic limit is not recoverable. The region that lies above the elastic region is known as plastic region. The property exhibited by the material in the plastic region is known as plasticity. (9) Ductility The property of the material that allows it to be drawn into wires or elongated before rupture takes place is known as ductility. (10) Tensile strength The tensile strength is the maximum conventional stress that can be withstood by the material. (11) Hardness The resistance offered by the material to the permanent deformation of the surface is known as hardness of the material. (12) Impact strength The impact strength is the maximum strength offered by a material when there is a dynamic load applied to it. (13) Strength The property of the material that can withstand external force without rupture is known as strength. (14) Toughness The ability of the material to withstand stress without fracture is known as toughness. In another way, it is defined as the ability to absorb energy in the plastic state. (15) Stiffness Stiffness is the ability of the material to resist deformation. (16) Malleability The ability of a material to be deformed under the action of compressive stress is known as malleability. (17) Resilience Resilience is defined as the energy per unit volume required to deform the material up to the elastic limit. (18) Brittleness The property of a material that produces fracture without any appreciable deformation due to the application of an external load is known as brittleness. (19) Creep The time dependent deformation of a material due to the application of a constant load is known as creep.
Mechanical Properties
299
(20) Endurance The property of a material that can withstand varying load (of the same or opposite nature) is known as endurance. (21) Weldability The capacity of a metal to be joined or welded readily with other metals in order to perform satisfactorily in the fabricated structure is known as weldability. (22) Castability The property of metal which is cast into forms is known as castability. (23) Machinability It is the property of a material which helps to machine the cutting tools. In the following section, hardness, tensile, compression, impact, creep and fatigue tests are discussed in detail.
11.2.1 Hardness Measurement The term hardness represents the resistance to deformation. In case of metals, hardness represents the measure of resistance to permanent or plastic deformation. The term hardness is related to the strength of the material. Therefore, a design engineer often needs the value of the hardness of the material. There are different types of hardness measurements namely, scratch hardness, indentation hardness and rebound or dynamic hardness. The different methods used to measure the hardness of the materials are discussed in the following sections: (1) Moh’s Hardness Moh’s hardness is mostly used by mineralogists. It is one of a scratch hardness. This hardness number is assigned by scratching one material by another. If a material is able to scratch another material, then it is given a higher hardness number. The mineralogists have arranged 11 different minerals and correspondingly assigned the hardness number as 1, 2, 3,… 10 as shown in Table 11.1. The hardness number of the softest material talc is assigned as 1 (scratch hardness 1) and diamond is given the scratch hardness number 10. The other elements are given scratch hardness number from 2 to 9. The Moh’s hardness number for different materials are listed in Table 11.1. For most of the engineering materials, the Moh’s hardness number lies between 4 and 8. The interval in the Moh’s hardness number is not widely spaced in the high hardness range.
Table 11.1 Moh’s Hardness Number for Different Materials Material
Moh’s Hardness Number
Talc
1
Gypsum
2
Calcite
3
Fluorite
4
Apatite
5
Orthoclase (or) feldspar
6
Quartz
7
Topaz
8
Corundum
9
Diamond
10
300
Materials Science
(2) Relation for Hardness The term hardness represents the resistance offered by the material to deformation such as abrasion or wear, cutting, machining, crushing or scratching. From the stressstrain curve, one can infer that the modulus of elasticity represents the resistance offered by the material to deformation. In mathematical form it can be written as, Y=
SL el
(11.13)
where Y is the Young’s modulus, SL the linear stress and e the linear strain. The linear stress is given by, Force F = Area A
(11.14)
Change in length l  l0 = Actual length l0
(11.15)
SL = and the linear strain is, e = l
where l is the increased length and lo the actual length. The volume of the material is equal to the product l A0 of length and area. For a constant volume, . Therefore, the linear strain can be written as, = l0 A e=
A l 1= 0 1 l0 A
(11.16)
Substituting the value of linear strain and linear stress from Eqs. (11.15) and (11.16) in Eq. (11.13), we get Y=
F F = A A Ê ˆ 0A A Á 0  1˜ Ë A ¯
(11.17)
The hardness of a material is determined using indenters. The area of contact of the indenter and the depth of penetration of the indenters depend on the force applied and the shape of the indenter. Therefore, the hardness of the material can be expressed in terms of force and area of contact. Based on the above relation, the hardness of a material can be expressed by the load and the corresponding area of contact, i.e., H=
Applied load (kg) P = 2 Surface area of impression (mm ) A
(11.18)
where P is the applied load and A the area of contact. (3) Brinells Hardness Tester The Brinells hardness tester is one of the oldest and mostly acceptable hardness testing methods, developed by JA Brinell in 1900. The hardness measurement is based on the principle of making an indentation using a 10 mm diameter spherical steel ball by applying a constant load of 3000 kg for a period of 10 to 15 seconds. For the soft metals, a load of 500 kg is used to produce an indentation and to avoid deep indentation. Similarly, for a hard metal, a tungsten carbide spherical ball is used to minimise distortion of the indenter instead of a steel ball. The hardness of a
Mechanical Properties
301
material is given by load / area and it has a unit of kg mm2. Even though, the Brinell hardness has a unit of kg mm2, it is represented by a number called Brinell Hardness Number (BHN). Consider a specimen is indented by an indenter as shown in Fig. 11.2. Let D be the ball diameter in mm, d the diameter of impression in mm, P the applied load in kg mm2 and t the depth of impression in mm. The Brinell hardness can be obtained using the relation, HB =
Applied load (kg) P = 2 Surface area of impression (mm ) A
(11.19)
where A is the area of contact between the ball and the indentation and P the applied load. From the geometry of Fig. 11.2, the area of contact A is equal to pDt, where D is the diameter of the ball and t the depth of impression. The depth of impression can be determined from the property of the circle, i.e.,
d d . 2 2
(Dt) t =
(11.20)
Indenter O D/2 P d/2
D/2 d/2 t
Q Specimen
d
Fig. 11.2 Brinell indentation
(Dt) d/2
d/2 t
Fig. 11.3 Depth of impression – determination Rearranging Eq. (11.20), we get t2  Dt +
d2 =0 4
(11.21)
Equation (11.21) is a quadratic equation. The solutions for this quadratic equation can be written as
and
t=
+ D + D2  d 2 2
(11.22)
t=
+ D  D2  d 2 2
(11.23)
302
Materials Science
Equation (11.22) will give a depth greater than D/2 and it shows that the depth of penetration is greater than D/2. The depth of penetration is less than D/2, hence Eq. (11.22) is not a solution to Eq. (11.21). Therefore, Eq. (11.23) is the only solution for Eq. (11.21). Substituting the values of A and t in Eq. (11.15), we get P È + D  D2  d 2 ˘ pDÍ ˙ 2 ÍÎ ˙˚ 2P HB = p D ( D  D2  d 2 )
HB =
i.e.,
(11.24)
Equation (11.24) is used to find the hardness of a material using Brinell hardness tester. The schematic representation of a Brinell hardness testing machine is shown in Fig. 11.4. The specimen under test is placed over the base plate and a suitable load is applied using hydraulic loading process. The applied load is measured using the Bourden gauge. After indenting for 10 s, the load is removed and indentation is measured. The area of indentation is measured by measuring the depth of impression using the Brinell microscope. The hardness is determined using Eq. (11.24).
Load Device
Plunger Indentor Specimen Base Plate Anvil Hnad Wheel
Fig. 11.4 Schematic diagram of a Brinell hardness tester – Hydraulic loading In order to obtain an accurate value of Brinell Hardness Number for a material, the value of P must lie between 0.25 and 0.5D. This is achieved by keeping P/D2 as a constant. Therefore, by maintaining the value (P/D2) as a constant, different diameter of impressions is obtained. The constant value (P/D2) maintained for steel is 30 and that of Cu alloy is 10.
Limitations Following are the limitations of the Brinell Hardness Number test: a. It is not suitable for surface hardened components. b. If the impression is large, it may initiate a crack.
Mechanical Properties
303
c. Generally, a steel ball is used to measure the hardness of the materials up to 450 BHN and for the materials having hardness greater than 450 BHN, tungsten carbide ball is used up to 600 BHN. There is a possibility in the variation of the hardness value measured by these indenters due to the use of indenters. (4) Vicker’s Hardness Test The Vicker’s hardness test is also based on the principle of the impression made by a square based pyramid made of diamond as the indenter. The Vicker’s hardness is the ratio of the load applied to the surface area of the pyramidal indentation. The Vicker’s hardness number is given by, P (11.25) A where P is the load applied and A the surface area of contact. In this hardness measurement, the load is varied from 1 to 120 kg. Further, there is no need to change the indenter as in case of Brinell hardness tester since diamond is used an indenter. The Vicker’s hardness number is equal to load applied per unit area. The unit for the VHN is kg mm–2. However, it is represented as Diamond Hardness Number (DHN) or Vicker’s Hardness Number (VHN). VHN =
The area of pyramidal impression can be calculated using the relation, S A=4L (11.26) 2 where L is the length of a side and S the slant height of the impression. From Fig. 11.5(a), D = 2L. Substituting the value of L in Eq. (11.26), we get A=
2D S
(11.27)
D
L
D S
136°
L (a) Indenter
(c) Perfect indentation
D  Diagonal L  Length of a side S  Slant height of impression
(b) Indentation in Vicker’s hardness tester
(d) Pin cushion indentation (due to sinking)
Fig. 11.5 Geometry of indenter and indentation
(e) Parallel indentation (due to ridging)
304
Materials Science
The angle of indenter is 136°. Therefore, the angle of indentation is also 136°. The surface area of contact is, S=
L 2 sin (a / 2)
(11.28)
where a is the angle of the indenter. Therefore, S=
The area of contact is given by, A =
D2
L D/ 2 = 2 sin 68∞ 2 sin 68∞
(11.29)
D2
(11.30)
= 2 sin 68∞ 1.854
Substituting the value of A from Eq. (11.30) in Eq. (11.25), we get VHN =
1.854 P D2
(11.31)
where P is the load applied in kg and D the average of two diagonal lengths of the impression in mm. The schematic representation of a Vicker’s hardness testing machine is shown in Fig. 11.6. After loading the specimen, a varying load is applied through the pedal from 1 kg to 120 kg. The diagonal lengths of the impression are measured using a microscope. Vicker’s Hardness Number is determined using Eq. (11.25). Vicker’s hardness testing machine is more accurate and versatile. For clear focusing, viewing and accurately measuring the diagonal length, a high degree of polishing of the metal surface is required.
Start of the test
Minor load applied
Major load applied
Major load removed
End of the test
Fig. 11.6 The Rockwell indentation procedure
Advantages Vicker’s hardness test has the following advantages: a. It is suitable for hard materials. b. Micro hardness test can be carried out by varying the load from 1 to 1000 g. One can determine the hardness value of the micro constituents from the micro hardness test. c. The impressions produced by different loads are geometrically similar and hence no need to decide on correct load.
Mechanical Properties
305
(5) Rockwell Hardness Tester The Rockwell hardness tester is based on the principle of the depth of penetration which is inversely proportional to the hardness of the material. The sample under test is loaded in the loading frame. The dial has two pointers. Initially, the first pointer is given a minimum load of 10 kg. An impression is made on the specimen. Then, the second pointer is given some higher load (major load) at the same position in which the minor load was applied. The indenter is removed and then, the hardness of the sample is measured from the reading dial. The Rockwell hardness measuring instrument consists of different scales such as B scale and C scale. The B scale is used to measure the hardness of a soft material using a steel ball from RH0 to RH100 (RH refers to Rockwell hardness). The C scale is used to measure the hardness greater than RH100 using a diamond cone indenter for hard materials. Therefore, the hardness of the material is, RH = h 
t 0.002
(11.32)
where h is a constant and t the depth in mm.
Advantages Rockwell hardness test has the following advantages: a. The apparatus is easy to handle and the readings are noted directly from the reading dial. b. A small size impression is made before using a larger load and hence, the uneven surface in the specimen is avoided. c. It is useful for quality control, when a large number of samples is used. d. The testing process is very fast.
Limitations Following are some of the drawbacks of the Rockwell hardness test: a. More than one scale is used to find the hardness of the material. Hence, there is a chance of error in the measurement. b. The scale varies from 1 to 100. Therefore, the scale is a contracted one. c. It is not possible to directly convert the Rockwell Hardness Number into Brinell Hardness Number or Vicker’s Hardness Number. d. It is not as accurate as Vicker’s hardness test, particularly when measuring the hardness of materials having small differences. (6) Rebound Hardness Rebound hardness is based on the principle of the hardness of a material which is directly proportional to the height of the rebound of a diamond tip hammer that falls on the material. A standard diamond tip hammer is made to fall on the material from a standard height. The hammer will make a surface indentation at the spot and it will rebound to a certain height. When the hammer is made to fall on a hard material, the surface impression produced is low and the height of rebound is more. By measuring the height of rebound one can determine the hardness of the material. The Shore’s scleroscope is an apparatus used to measure the rebound hardness. The Brinell Hardness Number is related to the rebound hardness measured by Shore’s scleroscope using Beeching’s formula applicable for steel and is written as follows: S = 0.118 B + 8, and S = 0.1 B + 15, when S is more than 55. The hardness number is used to correlate with other properties of the materials. Following are some of the uses of the hardness test: a. The Brinell Hardness Number is related to the tensile strength using the relation, Tensile strength (MPa) = 3.45 BHN.
306
Materials Science
b. The hardness number is used to correlate with wear resistance. A material used to grind ore or crush should be very hard. c. The hardness number is used to compare materials, to study about the behaviour of material, heat treatment, quality control and so on.
11.2.2
Tensile Test
The tensile test is used to study the strength of a material when it is subjected to a tensile load. A load which tends to pull apart the two ends of an object as shown in Fig. 11.7 is said to be a tensile load. The tensile test is carried out in a Universal Testing Machine (UTM). Load
Object
Load
Load
Fig. 11.7 Application of tensile stress to a specimen The material under test is usually round, square or rectangular. For metals, if sufficient thickness of the material is obtained, the material is machined in such a way that its central portion is thin compared to the outer edges. The UTM has provision to hold the samples with pin end, threaded end and shouldered end. The materials with different type of ends are shown in Fig. 11.8. Distance between shoulders Reduced section Diameter Gauge length Overall length
Shouldered end
Thread end
Pin end
Fig. 11.8 Sample used for tensile test The block diagram of a tensile testing machine is shown in Fig. 11.9. The material is fitted in the UTM in between the upper adjustable cross head and lower load sensitive cross head. One can apply load to the material by moving the lower load sensitive cross head step by step. The load reading is noted from the load scale. An extensometer fitted in the apparatus is used to measure the increase
Mechanical Properties
307
in length in the region marked as gauge length. The load is applied until the material gets fractured. From the data, a stressstrain diagram is drawn. The typical curve obtained for mild steel and medium carbon steel is shown in Fig. 11.10. Load scale
Hydrolic press Main piston
Fixed cross head Movable cross head Specimen
Oil pump
Fig. 11.9 Block diagram of a tensile testing machine E F
Stress
C B A
D Local necking
Plastic range Elastic range Strain
Fig. 11.10 Stress– Strain curve for mild steel or medium carbon steel From the strainstress curve, the following mechanical properties are obtained for the specimen under test. (1) Engineering Stress It is obtained by taking the ratio of applied load (P) to the original area of crosssection of the specimen (A0). Engineering stress, S =
P A0
(11.33)
(2) Engineering Strain Engineering strain is the ratio between elongation and the original gauge length (L0) Engineering strain, e =
L  L0 L0
(11.34)
One can determine the materials properties such as proportional limit and elastic limit using the stressstrain curve.
308
Materials Science
a. Proportional limit: The proportional limit is a point in stress – strain curve in which the curve deviates from linearity, i.e., the deviation from the relation, Stress = Young’s modulus × Strain. b. Elastic limit: The elastic limit is the region in which Hooke’s law is perfectly obeyed. In another way, it is defined as a point in which the plastic region starts.
Stress
(3) Yield Strength The stress at which the slip becomes noticeable and significant is known as yield strength. It is also defined as the stress required to produce a small value of plastic deformation. In case of mild steel, a sharp yield point is produced. In such a case, the lower value of the yield point is taken as the yield strength. In certain materials, there are no sharp edges. In such cases, a line parallel to the lower portion of the curve is drawn. The point of intersection gives the yield point. It is known as offset yield strength. It is represented in percentage, such as 0.1%, 0.2% or 0.5% offset yield strength. A material having high yield strength is selected for application or one must apply a force that produces stress which is below the yield strength.
0.2% offset yield strength Strain
Fig. 11.11 Yield strength determination from stressstrain curve (4) Modulus of Elasticity The modulus of elasticity or Young’s modulus is the slope of the stressstrain curve in the elastic region. Modulus of elasticity, E =
S e
(11.35)
where S is the mechanical stress and e the mechanical strain. The modulus is a measure of the stiffness of the material. A stiff material with a high modulus of elasticity maintains its size and shape even under an elastic load. (5) Tensile Strength or Ultimate Tensile Strength The ultimate tensile strength is the ratio of the maximum load applied to the original area of crosssection of the material. The tensile strength is the stress at which necking begins in ductile materials. The tensile strength is not relatively important as compared to yield strength. But it is used to estimate the other properties that are very important to measure. Tensile strength is an easily measurable quantity and it is also available in handbooks. (6) Percentage Elongation The percentage elongation is the ratio of increase in length to the original length of the specimen. Percentage elongation = =
Increase in length ¥ 100 Original length Lf  L0 ¥ 100 L0
where L0 and Lf are the original length and gauge length after fracture, respectively.
(11.36)
Mechanical Properties
309
(7) Ductility The percentage elongation or percentage reduction in area gives the value of ductility. It is measured after the specimen gets fractured. Percentage reduction in area =
A0  Af ¥ 100 A0
(11.37)
Similarly, A0 and Af are the actual area of crosssection and area of crosssection at fracture, respectively. Ductility measures the amount of deformation that a material can withstand without breaking. Ductility is important to both designers and manufacturers. A manufacturer needs a ductile material, since it can be shaped into a complicated form. A designer needs a material having at least a little value of ductility because the material deforms when a large stress is applied.
s
(8) Resilience Resilience is defined as the energy per unit volume required to deform the material up to the elastic limit. The shaded area shown in the stress strain curve (Fig. 11.12) up to the elastic limit gives the value of resilience.
Resilience
e
Fig. 11.12 Resilience determination using stressstrain curve
s
(9) Toughness Toughness is defined as the ability to absorb energy in the plastic state. The total shaded area (Fig. 11.13) in the plastic region of the stressstrain curve gives the value of toughness. The tensile test is also used to find whether the material is brittle or ductile by observing the appearance of fracture.
e
Fig. 11.13 Toughness determination using stressstrain curve
11.2.3 Compression Test The compression test is used for brittle material such as concrete. The specimen under test is loaded in a UTM and a compressive load is applied step by step and the corresponding deformation is measured using
310
Materials Science
compressometers. Using the compression test, one can draw a loaddeformation curve for the specimen under test. The compressive test of commonly used brittle materials such as grey cast iron and concrete is shown in Fig. 11.14. One can determine the ultimate stress and stress at the proportional limit by using the loaddeformation curve (FIg. 11.15).
Fig. 11.14 Compressive stress applied to a specimen
Stress
Stress
Concrete
Strain (a) Concrete
Grey cast iron
Strain (b) Grey cast iron
Fig. 11.15 Loaddeformation curve
11.2.4
Impact Test
During the working of a material, certain materials may undergo suddenly a heavy load. In order to understand the ability of the material to withstand heavy load, the impact test is carried out. It is used to study the brittleness of the material. The impact test measures the energy absorbed for fracture and it gives the impact strength of the material. Generally, the notched specimen is used for impact strength measurements. Two different methods are used for the impact strength measurements, namely, Charpy test and Izod test. The specimen used for the Charpy test has a dimension of 11 mm ¥ 11 mm ¥ 55 mm with a Vnotch, 45° angle, 2 mm deep and 0.25 mm root radius as shown in Fig. 11.16. The Charpy impact test apparatus is shown in Fig. 11.17. The notched specimen is placed on the horizontal beam. A heavy swinging pendulum of mass 16 kg and velocity 4.9 m s1 is made to strike on the specimen from a standard height. The specimen gets fractured due to the applied load. The ductile material becomes brittle due to the presence of notched specimen. This is known as notch
Mechanical Properties
Scale
180°
Point of Support
90°
90°
R
Pointer
a b
Hammer
O
311
Stand
Angle of raise
Specimen
Anvil
Angle of fall W
Striking edge W
Fig. 11.16 Charpy and Izod test  impact test specimen sensitivity. From this test, one can directly measure from the calibrated dial, the energy absorbed for fracturing the specimen in Newton meter. For Izod tests, a specimen of dimension 11 mm ¥ 11 mm ¥ 75 mm is fixed using vice and the other end is free. A Vnotch of 2 mm depth and angle 45° is produced at a distance of 28 mm from the free end. By striking the edge of the free end using a swinging pendulum, the energy for fracture is determined.
Advantages Following are some of the advantages of impact test: a. One can determine the impact strength of the material. b. By examining the fractured surface, one can identify whether the material is brittle or ductile or a combination of both. c. By measuring the impact test over a range of temperatures, the ductilebrittle transition temperature can be determined. The temperature at which a material changes from ductile to brittle is known as transition temperature. 10 mm
Striking hammer
28 mm
55 mm 40 mm
10 mm
75 mm
22 mm
Anvil 10 mm Striking edge (a) Specimen for Charpy test
10 mm (b) Specimen for Izod test
Fig. 11.17 Schematic diagram of an impact testing machine – Charpy test
312
Materials Science
11.2.5
Fatigue Test
Fatigue test is the fracture of the material, when it is subjected to a cyclic load for a long period of time. Rotating shafts, aircraft wings, and connecting rods are some examples of the structural and machine components subjected to cyclic loading. A simple fatigue testing machine is shown in Fig. 11.18. The specimen is connected to an electric motor through a shaft. The specimen gets rotated when the electric motor rotates. A counter is used to measure the number of revolution made by the electric motor. A dead load is applied to the machine using ball bearings. Specimen Ball bearing
Shaft
Rotter support
Flexible coupling Electric motor Revolution counter Rotter support
W
Fig. 11.18 Moore fatigue testing machine
Stress
The ball bearings relieve the machine from bending moment that is applied to the shaft. The specimen rotates due to the applied cyclic stress (sinusoidal stress). The number of cycles that the specimen can withstand without fracture is determined. The minimum stress at which a specimen can withstand without fracture, whatever may be the number of cyclic stress is known as endurance limit. Below the endurance limit, the specimen does not undergo fracture for repeated stresses. From this test, the endurance limit and the number of cycles, a material can withstand for a particular stress can be determined.
Endurance limit Strain
Fig. 11.19 S – N Curve The following other results are also obtained from fatigue test: a. Fatigue life: The number of cycles a material can withstand to a particular stress is known as fatigue life. b. Fatigue limit: The stress below which no fatigue failures occur is known as fatigue limit. c. Fatigue strength: The stress required to produce failure by fatigue is known as fatigue strength. In aluminium alloys, the fatigue strength is based on 500 million cycles.
Mechanical Properties
313
11.2.6 Creep Test Certain materials undergo failure when they are subjected to a constant load for a long period of time. This failure is known as creep. Creep fracture mostly occurs at elevated temperatures. Creep failure is one of a time dependent failures occurring in the materials at elevated temperatures. The components in furnace plant, boiler plant, turbine blades, and high temperature engine components undergo creep fracture. The schematic representation of a creep testing machine is shown in Fig. 11.20. The specimen is kept inside a furnace at an elevated constant temperature for a long period of time, and a constant load is also applied at the same time. The percentage of elongation of the material is measured by measuring the strains using strain gauge or optical extensometer for different times. Then, the creep curve is drawn by plotting the percentage of elongation against time as shown in Fig. 11.21. From Fig. 11.21, the region OA represents the percentage elongation produced by applying the load at room temperature. If the same load is applied at elevated temperature, the material experiences the initial percentage elongation OC and it is shown in Fig. 11.21. If the same is applied at a constant elevated temperature, the curve takes a path of CDEF. In the initial region CD, the strain is decreasing and it is known as primary creep. In the region DE there is a straight line portion, revealing that the strain varies linearly. The portion DE is known as the secondary creep. In the region EF, there is a sudden variation of strain. This region is known as tertiary creep. After the portion F, the material undergoes fracture. The creep test is carried out for four or five specimens at different constant temperatures and loads. Elongation versus time is plotted for each specimen.
Furance shell Insulation Heating Element Specimen
Weight Bar
Fig. 11.20 Schematic representation of a creep testing machine
314
Materials Science
Elongation(%)
Primary creep
Secondary creep
Tertiary creep F E
D C A O
B (At room temperature) Time(Min)
Fig. 11.21 Creep behaviour of carbon under constant applied stress
11.2.7
Factors Affecting Mechanical Properties
The various factors that affect the mechanical properties of a material are as follows: (1) (2) (3) (4)
Grain size Temperature Heat treatment, and Atmospheric exposure
(1) Grain size The metals having grains of small size are known as fine grained metals. The metals having large sized grains are known as coarse grained metals. The coarse grained materials have higher hardenability, high creep strength at high temperature and better forging properties. The fine grained metals have high tensile strength and low ductility, more resistance to cracking and fine surface finishes. The fine grained metals are work hardened. (2) Effect of temperature of the material:
High temperature produces the following effect on the mechanical properties
a. Yield stress, ultimate tensile strength, stiffness and fracture stress of many materials decreases with the increase in temperature. b. Creep takes place at high temperature. c. Changes in the structural properties take place at high temperature, and d. Toughness of steel is reduced and embrittlement of steel occurs at high temperatures. Low temperature produces the following effects on the mechanical properties of the materials: a. The nonferrous materials exhibit better properties than ferrous materials when their temperature is below 111oC. b. The ductility and toughness of Ni, Cu and Al are retained, while their tensile strength increases at low temperatures and c. The creep resistance of metal increases with decrease in temperature. (3) Heat treatment Heat treatment is an operation that involves the heating of the material to the required temperature followed by cooling at suitable rates. Heat treatment produces the following changes in the mechanical properties of the material: a. Improves machinability b. Relieves internal stresses produced during work hardening, forging, castings of the material c. Improves corrosion resistance
Mechanical Properties
315
d. Modifies crystal structure, either coarse grained or fine grained e. Improves surface hardenability, and f. Improves mechanical properties (4) Effect of atmospheric exposure Atmospheric exposure affects the mechanical properties of the material. The exposure of the material to wet air for a considerable period of time produces an oxide layer over the material. Iron rusts in the presence of humid air. The tensile strength and fatigue life are generally affected due to the oxide film. Metals like Al, Cr, Ni and stainless steel are not affected by atmospheric exposure. When these materials are exposed to the atmosphere containing sulphur dioxide and hydrogen sulphide, their properties are tarnished.
11.3 STRENGTHENING MECHANISM TO IMPROVE THE MECHANICAL PROPERTIES 11.3.1 Introduction Pure metals are good electrical and thermal conductors. But their mechanical strength and hardness are very low. Therefore, the metals are rarely used in pure state. The material having good strength can be prepared by alloying the element. For example, the coppernickel alloy has a strength that is greater than that of pure copper. The presence of dislocations reduces the strength of the materials. The dislocations lead to slip and hence, the strength gets reduced. The strength of the materials can be increased so as to meet the industrial requirements. There are several methods used to increase the strength of the materials. Some of the methods used to strengthen the materials are as follows. (1) Grain size strengthening (2) Work hardening or strain hardening or cold working (3) Precipitation hardening (4) Solid solution strengthening (5) Diffusion hardening, and (6) Heat treatment hardening
11.3.2 Grain Size Strengthening Polycrystalline materials consist of a number of grain boundaries. Grain boundaries act as barriers to slip motion. Therefore, by increasing the grain boundary area one can minimise or prevent the slip motion. If slip motion is minimised or prevented, then the strength of the materials gets increased. In case of fine grained materials, the grain boundary area gets increased and hence, the strength of the material gets increased. The relationship between the grain size and the tensile strength can be written as, s = so + kd1/2
(11.38)
where s is the yield stress, d the average grain diameter, k the locking factor which measures the effect of grain boundary and s0 the friction stress which represents the overall resistance offered by the crystal to dislocation movement. Eq. (11.38) is known as HallPetch relation.
316
Materials Science
The effect of grain size on tensile strength and ductility for annealed 7030 brass is shown in Fig. 11.22. The grain size reduction is achieved by introducing impure particles into the liquid. Addition of such particles in metals is called grain refinement or inoculation. The addition of 0.02% to 0.05% of titanium and 0.01% to 0.03% of boron to aluminium alloys, addition of aluminium to steel results in reducing the grain size and hence, the strength gets increased. 100
80 tensile strength
420
60
ductility
280
140
40
Elongation in %
Tensile strength (MPa)
560
20 0
0.05
0.1
0.15
0.2
Grain size (mm)
Fig. 11.22 Variation of tensile strength and ductility with grain size for 70–30 brass
11.3.3
Cold Working
The strength of the ductile material can be increased and hence, the ductility decreases due to mechanical working of the materials fairly at low temperatures. The mechanical process like rolling, forging, drawing, extrusion, stretch forming and bending are used to increase the strength of the materials. Thus, it leads to an increase in the strength of the materials and it is known as work hardening or strain hardening or cold working. Cold working means the deformation of the metal below the recrystallisation temperature. During cold working, the number of dislocations increases, causing the metal to be strengthened. The amount of deformations produced due to cold working is defined using the percentage of cold work. Percentage of cold work =
A0  Af ¥ 100 A0
(11.39)
where A0 is the original crosssectional area of the metal and Af the final crosssectional area after deformation. Generally in cold worked materials, the mechanical properties such as yield and tensile strength are found to increase while the ductility decreases. The effect of cold work on the mechanical properties of Cu is shown in Fig. 11.23. (1) Applications Following are some of the applications of cold work: a. The mechanical properties such as tensile and yield strength gets increased. b. The cold working of metals prevents oxidation.
Mechanical Properties
317
c. It is an inexpensive method of producing large number of small parts. d. Ductility, electrical conductivity and corrosion resistance are decreased due to cold working. e. It produces an excellent surface finish. 100 90
600 tensi
Strength (MPa)
ength
le str
400
60
yield strength
% elongation 30
200 ductility
0
20
40 60 80 Percent cold work
100
Fig. 11.23 Effect of cold work on the mechanical properties of copper (2) Limitations
Following are some of the disadvantages of cold working:
a. It introduces residual stresses during the deformation. This may be harmful or beneficial to the metals. b. It produces textures or preferred orientations that cause an anisotropic behaviour in the metals. c. It requires greater energy to deform the cold worked material. d. It increases recrystallisation temperatures.
11.3.4 Solid Solution Strengthening A solid solution is a solid phase that is obtained by mixing any two metals in liquid state and allowed to solidify. A solid solution has uniform composition everywhere. The addition of liquid copper with liquid nickel and solidifying the liquid by allowing it to cool to room temperature is known as coppernickel solid solution. This process is also called alloying. When a solid is mixed with another solid in liquid states, solid solutions are formed readily. During this process, solvent and solute atoms have similar size and electron structures. The solid solutions are two types, namely (1) Substitutional solid solution, and (2) Interstitial solid solution (1) Substitutional solid solution A substitutional solid solution is formed when the solute and the solvent atoms are of comparable size. For example, consider copper and zinc. the atomic radii of copper and zinc are respectively 1.278 Å and 1.332 Å and both have 28 sub valence electrons. When zinc is mixed with copper, copper atoms are replaced by zinc. The solution of copper and nickel is an another example for substitutional solid solution. The substitutional solid solutions are of two types namely, ordered substitution solid solution and random substitution solid solution. Let us discuss the above solid solutions in detail in the following section:
318
Materials Science
a. Ordered substitution solid solution: The ordered solid solution is formed when the solute atoms occupy similar lattice points in the solvent matrix and it is shown in Fig. 11.24(a). This ordered solid solution is generally produced at low temperatures due to low thermal agitation.
(a) Ordered
(b) Random
(c) Interstitial
Fig. 11.24 Solid solutions b. Random substitution solid solution: A solid solution containing a random arrangement of solute atoms in a solvent material, when there is a mixing of two materials is shown in Fig. 2.24(b). When zinc is added to copper, zinc atoms easily replace the copper atoms randomly resulting in the formation of random substitutional solid solutions. If the solid solution is slowly cooled, there is a rearrangement of atoms and hence, a definite ordering of atoms takes place. (2) Interstitial solid solution The interstitial solid solution is formed, when the size of the solute atom is comparable with interstitial space of the solvent atoms. The interstitial solid solution is shown in Fig. 2.24(c). In the interstitial solid solution, the solute atoms are accommodated in the intermediate positions of the solvent atoms. Carbon atoms dissolved in iron, constitute an interstitial solid solution. The formation of copper nickel solid solution has a strength that is greater than that of pure copper. Addition of less than 40% of Zn to copper strengthens the CuZn alloy than that of pure Cu. (3) Effects of solid solution strengthening The following properties are observed in solid solution strengthened materials: a. The yield strength, tensile strength and hardness of the alloy increases than that of the pure metals. b. The ductility decreases, than that of the pure metals. But in CuZn alloy both ductility and strength increases. c. Electrical conductivity of the alloy gets reduced. d. The creep resistance increases at elevated temperatures.
11.3.5
Precipitation Hardening
Precipitation hardening is a process of strengthening the material by heating the specimen to solution treatment temperature and maintaining it in that temperature for 30 minutes to 1 hour followed by quenching in hot or cold water and ageing at room temperature or at an elevated temperature. It is also called age hardening. Certain alloys such as Al4% Cu alloy and a number of copper base alloys such as ZrCu, CrCu and BiCu display an age hardening response. Let us explain the process of age hardening with reference
Mechanical Properties
319
to Al – 4% Cu alloy. The Al rich end of the phase diagram of AlCu alloy is shown in Fig. 11.25. The eutectic temperature of Al – 4% Cu alloy is 821 K. The solvus line indicates the solid solubility of Cu in Al. The a phase of Al – 4% Cu alloy is rich in Al. The Al – 4%Cu alloy is solution treated above the solvus temperature Ts, in the a phase region. Then, it is suddenly quenched into a cooling liquid such as water. Quenching the alloy at room temperature reduces the formation of supersaturated solution of a phase. This solid solution is unstable and it forms precipitates of CuAl2 and hence, there is a formation of a + d solid solution. The q solid solution is CuAl2. During the formation of precipitates of CuAl2, some intermediates with fine particle sizes of about 100 to 500 Å are formed. The formation of fine particles increases the strength of the alloys. The fine particle precipitation occurs within a period of few days. This process is called natural ageing. The fine particle precipitation can also be formed by heating the specimen in the temperature range of 393 K to 453 K. At the ageing temperature, the atoms are able to diffuse into short distances.
liquidus line, L 700
eutectic point 548°C
temperature (°C)
600 a
400
Ts
solidus line
solution treatment
1
500
a+L
solvus line
300 3 200 100
a+q age
Quench 2
4
6
8
10
wt % of Cu
Fig. 11.25 Al rich end of AlCu phase diagram The Vicker’s Hardness Number is plotted against the aging time at room temperature aged Al4% Cu specimen at 453 K. Fig. 11.26 shows that the maximum hardness is obtained within a short time. It is inferred from Fig. 11.26 that the hardness decreases, if the aging time is increased beyond the maximum value. It is said to be over ageing. Generally, all the materials are not age hardenable. For age hardening of an alloy, the following conditions must be satisfied: a. The alloy should have single phase on heating above the solvus line and on cooling it should have two phases. b. The alloy must be quenchable. c. The matrix should be relatively soft and ductile, and the precipitate should be hard and brittle. d. The precipitate must form a coherent structure with matrix structure.
320
Materials Science
180 °C Vickers hardness number
80 60 Ov er
40
ag e
in
g
20 0 1
2
3
4
5
6
7 Ageing time (Days)
Fig. 11.26 Precipitation hardening behaviour in Al – 4% Cu alloy
11.3.6
Diffusion Hardening
Diffusion hardening is the process of strengthening the materials by diffusing either carbon or nitrogen or both into the surface of the material. This type of surface hardening produces very hard and wearresistive outer surface and the inner core is more ductile and tougher. The surface hardening by means of diffusion of carbon and/or nitrogen by diffusing them into the surface of steel is also known as thermochemical treatment. The different types of diffusion hardening of steels are as follows: (1) Carburising (2) Nitriding (3) Cyaniding, and (4) Carbonitriding (1) Carburising Carburising is a process of increasing the strength of the steel by diffusing carbon atoms by thermochemical treatment. It is carried out in the temperature range 1173 K to 1203 K and the surface layer is enriched with 0.7 to 0.9% of carbon. The hardness of the surface of the steel varies with the carbon content. The variation of Vicker’s Hardness Number with carbon content for alloyed and nonalloyed steels is shown in Fig. 11.27. There are three different types of carburising, namely pack carburising, liquid carburising and gas carburising. a. Pack Carburising: The steel component to be heat treated is packed in a heat resistance box with 80% granular coal and 20% BaCO3 energiser. The container is heat treated at 1203 K for 6 to 8 hours. During heat treatment, the diffusion of carbon takes place due to the following reactions: The decomposition of BaCO3 produces CO as, BaCO3 Æ BaO + CO2
(11.40)
CO2 + C Æ 2CO
(11.41)
Mechanical Properties
9
321
9 NiCr steel
8
8
7
7
6
6
5
5 0.4
0.6
0.8 Carbon, wt % (a) Alloyed steel
1.0
0.4
0.6 0.8 1.0 Carbon % (in wt) (b) Nonalloyed steel
Fig. 11.27 Variation of VHN with carbon content for alloyed and nonalloyed steel Then the CO reacts with steel and it produces carburised steel, i.e., Fe+2CO Æ Fe(C) + CO2
(11.42)
The term case depth represents the thickness of the hardened surface. The case depth at a particular temperature is given by, Case depth = k t
(11.43)
where t is time and k a constant. The case depth obtained using this method is nearly 1 mm to 2 mm. b. Liquid Carburising: In liquid carburising, the steel is placed in a bath of molten alloys of cyanide that contains carbon. The bath temperature is maintained between 1118 K and 1173 K. The bath contains sodium cyanide or potassium cyanide, sodium and potassium chloride and barium chloride. The BaCl2 acts as an activator. The reactions are as follows: 2NaCN + BaCl2 Æ Ba[CN]2 + 2NaCl
(11.44)
Ba[CN]2 + Fe Æ Fe(C) + BaCN2
(11.45)
The heat transfer is very fast and hence, the heating time is very low. The case depth obtained is nearly 0.08 mm. c. Gas Carburising: The gas carburising is carried out in a gaseous atmosphere. The carburising gaseous atmosphere is produced from liquids such as methanol, isopropanol or gaseous hydrocarbons such as propane and methane. The gas carburising temperature varies from 1143 K to 1223 K. In the carburising temperature, CH4 decomposes into carbon and hydrogen, i.e., CH4 + Fe Æ Fe(C) + 2H2 The decomposed carbon reacts with steel and hence, hardens the surface.
(11.46)
322
Materials Science
(2) Nitriding Nitriding is a process of diffusing nitrogen into the surface of steel and hence, hardening the steel. It is carried out below 863 K. The portions that are not to be nitrided are covered with a tin coating produced by electrolysis. The tin coatings prevent the passage of nitrogen into the steel. Before nitriding, the machining and grinding process should be finished. The dissociation of anhydrous ammonia gas at 823 K produces nitrogen and hydrogen. This nitrogen diffuses into the surface of the steel, i.e., 2NH3 Æ 2 [N]Fe + 3H2
(11.47)
The time required for nitriding of steel varies from 21 to 100 hours. The hardness achieved is 900 to 1100 VHN and for a case depth of 0.5 mm the time required for nitriding is 100 hours. (3) Cyaniding Cyaniding is a process of diffusing the carbon and nitrogen in liquid atmosphere. In cyaniding, the steel is immersed in a liquid cyanide bath which permits both carbon and nitrogen to diffuse into steel. The bath temperature varies from 1173 K to 1233 K. The basic reactions are, 2NaCN + O2 Æ 2 NaCNO
(11.48)
2NaCNO + O2 Æ Na2CO3 + CO + 2N
(11.49)
2CO Æ CO2 + C
(11.50)
The carbon and nitrogen diffuse into the steel and produce wear resistant steel. The bath containing 8% of NaCN, 82% of BaCl2 and 10% of NaCl produces a case depth of 0.5 to 2 mm at 1223 K for a period of 1.5 to 6 hours. This method has an advantage of high heat transfer coefficient and low distortion in pieces because of liquid bath and uniform temperature. (4) Carbonitriding Carbonitriding is a process of diffusing carbon and nitrogen in the gaseous atmosphere. For this, a gaseous mixture of ammonia and a carburising gas is used. The carburising is carried out at 1073 K to 1143 K. The gas mixture contains about 15% of NH3, 5% of CH4 and 80% of neutral carrier gas. Carbon and nitrogen diffuses into the steel. The diffusion of nitrogen increases the hardenability than that of carbon. The case depth obtained is nearly 0.05 – 0.75 mm. To avoid cracking, the steel is quenched in oil after carburising followed by tempering. The hardness obtained is nearly 850 VHN.
11.3.7
Heat Treatment Hardening
The process of heating and cooling the materials such as steel to obtain the required mechanical properties is known as heat treatment. The different heat treatment processes used for steel are as follows. (1) Annealing (2) Normalising (3) Hardening or quenching (4) Tempering (5) Austempering and martempering, and (6) Case or surface hardening The heat treatment process involves heating the specimen into the required temperature and cooling it in various media at different rates of cooling, so as to produce new phases. Due to the variation of cooling process, there is a phase transformation of steel. This phase transformation in steel increases the hardness of steel.
Mechanical Properties
323
11.4 FRACTURE
11.4.1 Introduction The breaking of a specimen into two or more than two parts due to the application of stress is known as fracture. Fracture occurs due to excessive plastic deformation, excessive wear, corrosion, repeated application of cyclic stress and so on. Fracture is an undesirable engineering problem since it produces numerous unwanted effects. The fracture of an axle in an automobile causes accident. The fracture of a turbine shaft in a power station produces power failures. Therefore, one must know about the different types of fractures, reason for causes of fracture and the methods used to minimise or to avoid fracture. The different types of fractures are as follows: (1) Brittle fracture (2) Ductile fracture (3) Fatigue fracture, and (4) Creep fracture The different types of fracture mechanisms and their characteristics are discussed in detail in the following section.
11.4.2 Brittle Fracture The brittle fracture occurs suddenly without any indication of crack or fracture in the materials. This fracture occurs without any plastic deformation. The brittle fracture is a dangerous one, since it occurs without any warning. In the brittle materials, the rate of propagation of crack is very rapid. If the two broken pieces are joined together appropriately, one can get the original shape of the material. The fractured surface is shiny or looks like a polished surface and it is flat. This is because the brittle fracture occurs due to the separation of grains along specific crystallographic planes known as cleavage planes. In bcc iron, (100) planes are the cleavage planes. The brittle fracture of the materials occurring when a tensile stress is applied is shown in Fig. 11.28. Following are the characteristics of brittle fractures: (1) It occurs suddenly without any warning. (2) It occurs with little or no plastic deformations. (3) The rate of propagation of the crack is very fast. (4) The fractured surface is shiny and flat and (5) It occurs along the cleavage planes. Generally, bcc metals and hcp polycrystalline metals are brittle whereas many fcc metals are ductile.
324
Materials Science
stress
stress
Fig. 11.28 Brittle fracture
11.4.3
Mechanism of Brittle Fracture or Griffith Theory of Brittle Fracture
The theoretical value of the stress required to produce a brittle fracture varies from Y/5 to Y/30, where Y is the Young’s modulus of the material. But in practice, the brittle materials fracture at stresses much lower than the theoretical value. The fracture stress for glass is about 50 MN m2, which is nearly equal to Y/1000 for glass. Similarly, the alloys of iron and nitrogen have fracture stress of 5 MN m2, which is nearly equal to Y/40,000. This shows that the brittle fracture occurs at a lower value than the theoretical value. Griffith first proposed the explanation for the brittle fracture. According to him, the brittle fracture is initiated due to the presence of small cracks in the brittle materials. The crack occurs due to several reasons, such as surface scratch, and collection of dislocations during solidification of the material. Consider a brittle material is subjected into tensile stress. Due to the application of the tensile stress, the material elongates. During the elongation of the material, some form of energy is stored in the material. This energy is known as elastic strain energy. As the material elongates, the elastic strain energy increases. At the same time, due to the application of the tensile stress, the crack present in the material grows in size. Due to the growth of the material, the surface energy of the material increases. As the size of the crack is large, the elastic strain energy does not increase due to the presence of the crack. The tensile stress does not pass from one portion to the other portion of the material through the crack. Therefore, the elastic strain energy is released by the material, when the size of the crack is of sufficient size. According to Griffith, the brittle fracture is initiated when the elastic strain energy stored is equal to the surface energy of the crack. Consider a brittle material has an elliptical crack of length, 2C as shown in Fig. 11.29. Consider a tensile stress of S is applied to the material. The maximum stress present at the tip of the crack is given by, Sm = 2S
L P
(11.51)
Mechanical Properties
325
where P is the radius of the curvature at the tip and S the applied stress perpendicular to the length 2L. The brittle fracture is initiated when the elastic strain energy released is just equal to the increase in the surface energy of the crack. The elastic strain energy released per unit volume is given by, Elastic strain energy released, UE = strain field per unit volume × area × width s 2L
s
Fig. 11.29 Model for Griffith fracture theory The elastic strain field per unit volume is S 2/2E, the area of the crack is pL2 and consider the width is unity. Therefore, the elastic strain energy is UE =
S2 pS 2 L2 ¥ pL2 ¥ 1 = 2E 2E
(11.52)
The strain field will be properly integrated from infinity to get the actual strain energy. The actual strain energy is twice the value of Eq. (11.52). Let the surface energy per unit area be g. The surface energy for a crack of length 2C and width unity is, Us = g ¥ 2L ¥ 1
(11.53)
The total surface energy is obtained by multiplying Eq. (11.53) by 2, because the crack has two surfaces. Therefore, the total surface energy is Us = 2 ¥ 2g L = 4g L
(11.54)
According to Griffith, the crack will propagate if the change in the elastic strain energy per unit length is equal to the change in the surface energy per unit length. Therefore, dUE dUs = dL dL d Ê p S 2 L2 ˆ d = ( 4g L) dL ÁË E ˜¯ dL
(11.55)
326
Materials Science
2p S 2 L = 4g E i.e.,
S=
2g E pL
(11.56)
Eq. (11.56) is known as the Griffith equation. It gives the tensile stress necessary to initiate the brittle fracture in a material. According to Eq. (11.56), the tensile stress required to initiate the brittle fracture is directly proportional to the square root of the Young’s modulus of the material and inversely proportional to the square root of the length of the material. The Griffith’s theory is applicable to brittle material such as glass. In case of crystalline materials, this theory has to be slightly modified to take into account the plastic deformation that occurs.
11.4.4
Ductile Fracture
The ductile fracture occurs in materials after some plastic deformation. The ductile fracture is shown in Fig. 11.30. The application of tensile stress to a ductile material increases the plastic deformation and hence, the material gets strain hardened. The strain hardening increases the strength of the material. The strength acquired by strain hardening compensates the decrease in crosssectional area and it introduces neck in the material. The neck formation introduces triaxial state of stress in the material. After this, there are three successive events involved in the formation of ductile fracture. Stress
Stress
Fig. 11.30 Ductile fracture The first event is the formation of cavities or voids at the place in which necking is formed, since at the necking portion the stress is concentrating. The second event involved is the linking of all cavities so as to form a larger cavity or crack. The crack propagates perpendicular to the direction of tensile stress. The third event involved is the propagation of crack by shearing in a direction approximately 45° to the tensile axis. This will produce a cup and cone type fracture. The various stages of ductile fracture formation is shown in Fig. 11.31.
Mechanical Properties
327
Cone cup
(a)
(b)
(c)
(d)
Fig. 11.31 Various stages of ductile fracture The ductile fractured surface appears dull when viewed with the naked eye. If the ductile fractured surface is viewed using a scanning electron microscope, the surface has dimpled appearance. The ductile fracture occurs with some plastic deformation. The rate of propagation of the ductile fracture is low. The pure materials have more ductility.
Difference Between Brittle and Ductile Fracture The ductile and brittle fractures have the following differences: Sr. No
Brittle Fracture
Ductile Fracture
1.
It occurs with no or little plastic deformation. It occurs with large plastic deformation.
2.
The rate of propagation of the crack is fast.
The rate of propagation of the crack is slow.
3.
It occurs suddenly without any warning.
It occurs slowly.
4.
The fractured surface is flat.
The fractured surface has rough contour and the shape is similar to cup and cone arrangement.
5.
The fractured surface appears shiny.
The fractured surface is dull when viewed with naked eye and the surface has dimpled appearance when viewed with scanning electron microscope.
6.
It occurs where micro crack is larger.
It occurs in localised region where the deformation is larger.
11.4.5 Fatigue Fracture Ductile materials, when they are subjected to a large number of varying loads or fluctuating loads, undergo fracture at stresses much below the static fracture stress. This type of fracture is said to be fatigue fracture. The examples for the materials that undergo varying loads are rotating shafts, gears, springs, connecting rods and aircraft wings, etc.
328
Materials Science
The plot for steel and Al alloy drawn between the stress (S) applied to the materials and the number of cycle (N) the load applied is shown in Fig. 11.32. The curve drawn between stress and the number of cycles is known as SN curve. The SN curve for steel shows that there is a minimum stress below which there is no fracture. This minimum value of stress below which the specimen can withstand for any number of stress reversal is known as endurance limit. The curve shows that steel has a definite endurance limit. The Alalloys do not show a welldefined endurance limit. In such cases one can define a quantity known as fatigue strength or fatigue limit. The fatigue limit is the stress value at which the materials undergo fracture for a specified number of stress cycles (say 106 cycles). 800 steel
Stress (MPa)
600
400 endurance limit
Al alloy
200
0 104
105
106
107
108
109
No of cycles (log N)
Fig. 11.32 A plot of stress versus applied load for steel and aluminium
Factors Affecting Fatigue Fractures Following are the factors which affect the fatigue fractures: a. At low temperature, the fatigue strength is high. The fatigue strength decreases with increase is temperature. b. Corroding atmosphere reduces fatigue. This can be minimised using surface treatments such as coatings, castings, carburising and nitriding. c. Fatigue failure takes place due to surface imperfections such as surface irregularities and machining marks. d. The stress concentration points like notches, screw threads and machining undercuts increases the fatigue failures.
Prevention of Fatigue Fracture The fatigue fracture of a material can be minimised and hence, its lifetime can be increased by increasing its fatigue resistance by the following methods: a. The stress concentration is eliminated by avoiding sharp corners with good design of materials. b. The surface treatments such as nitriding, carburising, coatings, etc., are used to prevent the corrosion of the materials thereby the life time of the materials can be increased. c. The surface irregularities should be removed by polishing and hence, the fatigue resistance of the material can be increased.
Mechanical Properties
329
11.4.6 Creep Certain materials are subjected to a constant load for a long period of time; there may be development of strain and hence, lead to fracture of the material. This type of fracture is known as creep. Constant load is applied to certain materials such as turbine blade, pressure vessel for high temperature chemical processes, aircraft, timber beam in the roof of buildings and lead coverings in telephone cables. If the load is applied in these materials for a longer period of time, the creep fracture is produced. Creep is one of the time dependent fractures occurring in materials. Creep can also be defined as a time dependent permanent deformation produced in the material. (1) Different stages in creep curve The creep curve is drawn between the percentage of elongation and the time as shown in Fig. 11.33. In Fig. 11.33, OA represents the instantaneous percentage of elongation produced, when the load is applied at room temperature. The percentage of elongation produced at elevated temperature is represented as OP. There are three different stages of creep curve namely, a. Primary creep, b. Secondary creep, and c. Tertiary creep Tertiary creep S
6
Secondary creep
Elongation in %
Primary creep R
4 Q
2 P A
(at room temperature)
0
B
Time (min)
Fig. 11.33 Creep curve a. Primary creep: The application of a constant load to the material produces strain. The percentage of elongation produced in the material work hardens or strain hardens the material. In the primary region, PQ, the percentage of elongation is very high compared to the strength produced due to the work hardening of the material. b. Secondary creep: The straight line portion QR of the creep curve is known as secondary creep. In the secondary creep region, the strain hardening just balances the percentage of elongation in the material. The structural observations show that polygonization is an important recovery process during the secondary creep stage. c. Tertiary creep: In the tertiary creep stage, the creep rate increases with time until fracture. The percentage of elongation is rapid in this stage.
330
Materials Science
(2) Effect of temperature and stress in creep The increase of either temperature or stress to the material increases the strain. This increase in strain increases the possibility of creep fracture. The variation of creep with the increase in temperature and for a constant stress is shown in Fig. 11.34(a). The creep curve for different stresses, where s1>s2>s3>s4 at a constant temperature is shown in Fig. 11.34(b).
T1
s1 T2
s2
T3 Strain
Strain
s3
T4 T1 > T2 > T3 > T4 > Time (a)
s4 s1 > s2 > s3 > s4 > Time (b)
Fig. 11.34 Variation of creep with (a) temperatures and (b) stresses (3) Mechanism of creep Creep is a high temperature phenomenon. Many materials deform due to the following mechanism when they are strained: a. Dislocation climb, b. Vacancy diffusion, and c. Grain boundary sliding The temperature, stress and strain rate are responsible for these mechanism. a. Dislocation climbs: It is the process of the movement of dislocation line to climb up or down. The dislocation climb occurs at high temperatures. The dislocation move perpendicular to the slip plane due to temperature. This movement of dislocation induces creep. b. Vacancy diffusion: The migration of vacancy from one side of a grain boundary to another side is known as vacancy diffusion. The movement of vacancy for a longer period of time results in creep. c. Grain boundary sliding: In polycrystals, the sliding of grain boundaries causes creep at high temperatures. Sliding of grain boundaries produces vacancy and hence, ductile materials lose their ability and creep occurs. (4) Factors affecting creep The factors that affect creep are given below. a. Creep is a high temperature process. Therefore, temperature plays a major role in the creep fracture. b. Creep resistance depends on grain size of the material. A coarse grained material exhibits better creep resistance than a fine grained material. c. Chemical reactions affect creep rate. The chemicals used as lining materials in furnaces affect the creep rate.
Mechanical Properties
331
Key Points to Remember Stress is defined as the restoring force acting per unit area of crosssection. The ratio of change in dimension to actual dimension is known as strain. Young’s modulus is the ratio of the linear stress to the linear strain. Rigidity modulus is the ratio of the bulk stress to the bulk strain. Bulk modulus is the ratio of the shear stress to the shear strain. Poisson’s ratio is defined as the ratio of lateral strain to linear strain. Within the elastic limit, the ratio of stress to strain is a constant and this constant is known as modulus of elasticity. Elasticity is defined as the change in dimension due to the load and regaining the actual shape when the load is removed. Hardness is defined as the ratio of the applied load to the suppressed area of impression. The resistance offered by the material to the permanent deformation of the surface is known as hardness of the material. The different types of hardness are Moh’s hardness, Brinell hardness, Vicker’s hardness, Rockwell hardness and Rebound hardness. 2P Brinell hardness of the material is HB = where P is the applied load, D p D ( D  D2  d 2 ) the diameter of the ball and d the depth of impression. 1.854 P Vicker’s hardness of the material is VHN = , where P is the load applied in kg and D2 D the average of two diagonal lengths of the impression in mm. t Rockwell hardness of the material is RH = h , where h is a constant and t the depth in mm. 0.002 S Modulus of elasticity is E = , where S is the mechanical stress and e the mechanical strain. e
Fatigue failure is the fracture of the material, when it is subjected to a cyclic load for a longer period of time. The temperature at which a material changes from ductile to brittle failure is known as transition temperature. The heat treatment of the material improves mechinability, corrosion resistance, surface hardenability and mechanical properties. Polymer material consists of number of grain boundaries. The relationship between the grain size and the tensile strength is s = s0 + kd1/2 where s is the yield stress, d the average grain diameter, k the locking factor which measures the effect of grain boundary and s0 the friction stress which represents the overall resistance offered by the crystal to dislocation movement. The deformation of the metal below the recrystallisation temperature is known as cold working. The breaking of a specimen into two or more than two parts due to the application of stress is known as fracture. The four different types of fracture are brittle, ductile, fatigue and creep. The ability of the material to withstand stresses without fracture is known as toughness. The property of the material that produces fracture without any appreciable deformation due to the application of an external load is known as brittleness. The time dependent deformation of a material due to the application of a constant load is known as creep. The stress required to produce failure by fatigue is known as fatigue strength.
332
Materials Science
Solved Problems Example 11.1 Calculate the stress produced in an aluminium alloy test piece of 10 mm diameter when subjected to a load of 2000 kg axially along the bar. Given Data: Load applied = 2000 kg Diameter of the test piece = 10 mm Solution:
Stress =
Force 2000 ¥ 9.8 = = 249.5 MPa = 249.5 MN m2. area p ¥ 0.0052
The stress produced in an aluminium alloy is 249.5 MN m2. Example 11.2 A Ti bar 9.4 mm in diameter with a gauge length of 50 mm is pulled in tension to failure. After failure, the gauge length is 53.75 mm and the diameter is 8.8 mm. Calculate the % elongation and % reduction in area. Given Data: Diameter of the bar before failure = 9.4 mm Gauge length of the bar before failure = 50 mm Diameter of the bar after failure = 8.8 mm Gauge length of the bar after failure = 53.75 mm Solution:
Percentage elongation =
l f  lo lo
¥100 =
Percentage reduction in area =
53.75 ¥ 103  50 ¥ 103 ¥ 100 = 7.5% 50 ¥ 103
Ao  Af Ao
2
¥ 100 =
2
p ( 4.7 ¥ 103 )  p ( 4.4 ¥ 103 ) 2
p ( 4.7 ¥ 103 )
¥ 100
= 12.358%. The percentage elongation is 7.5 % and the percentage reduction in area is 12.36%. Example 11.3 Estimate the Brinell hardness number of steel having a tensile strength of 937 MPa. Given Data: Tensile strength of steel = 937 MPa. Solution:
Tensile strength (in MPa) = 3.45 ¥ Brinell Hardness Number Brinell Hardness Number = Tensile strength (in MPa)/3.45 =
937 = 271.59 3.45
The Brinell Hardness Number is 271.59.
Mechanical Properties
333
Example 11.4 A 10 mm indenter is used to find the Brinell hardness test of steel plate with a load of 3000 kg. A 2.2 mm impression is measured on the surface of the alloy. Calculate the Brinell Hardness Number, the tensile strength and the fatigue limit of steel plate. Given Data: Load applied = 3000 kg, Diameter of the indenter = 10 mm Diameter of the impression = 2.2 mm The Brinell Hardness Number, HB =
Solution:
2P p D ( D  D2  d 2 )
2 ¥ 3000
=
(
p ¥ 10 10  102  2.22
)
= 779.5 Tensile Strength (in MPa) = 3.45HB =3.45 ¥ 779.5 = 2689.275 MPa. Fatigue limit = 0.5 ¥ tensile strength = 0.5 ¥ 2689.275= 1344.6375 MPa. The Brinell Hardness Number of steel plate is 779.5. The tensile strength of steel plate is 2689.275 MPa. The fatigue limit of steel plate is 1344. 6375 MPa.
Fill in the Blanks 11.1. 11.2. 11.3. 11.4. 11.5. 11.6. 11.7.
The property exhibited by a material when it is subjected to an external load is known as ________. The restoring force acting per unit area of crosssection is known as ________. The unit for stress is ________. The ratio of the change in dimension to the actual dimension is known as ________. The unit for strain is ________. The region in which a material is capable of regaining its dimension is known as ________. The ratio of the load on the specimen to the instantaneous crosssectional area supporting the load is known as ________. 11.8. Poisson’s ratio is ________. (a)
Dd/d Dl/l
(b)
Dd/d Dl
(c)
Dl/l Dd ¥ d
(d) Dd Dl
11.9. Brinell hardness is obtained using the relation ________. (a) PA (b) P/A (c) A/P (d) P/A2 11.10. In Vicker’s hardness measurement, the load is varied from ________ to ________ kg.
334
Materials Science
11.11. The temperature at which a material changes from ductile to brittle failure is known as ________ temperature. 11.12. ________ material consist of a number of grain boundaries. 11.13. The relationship between the grain size and the tensile strength is ________. 11.14. ________ is a brittle material. 11.15. fcc metals are ________. 11.16. Within the elastic limit, the material obeys ________. 11.17. Moh’s hardness is mostly used by ________. 11.18. The unit for the hardness of a material is ________. 11.19. The methods used for the impact strength measurements are ________ and ________. 11.20. The stress below which no fatigue failure occurs is known as ________. 11.21. Creep takes place at ________ temperature. 11.22. ________ is carried out in the temperature range 1173 K to 1203 K. 11.23. In liquid carburising, the bath temperature is maintained between ________ and ________. 11.24. Nitriding is a process which is carried out below________ K. (a) 863 (b) 864 (c) 865 (d) 866 11.25. The carburising is carried out at ________ and ________. 11.26. The process of heating and cooling the materials is known as ________. 11.27. The ________ fracture occurs suddenly without any indication of crack or fracture in the materials. 11.28. The explanation for the brittle fracture was first proposed by ________. 11.29. ________ is known as the Griffith equation. (a) s =
2g E pL
(b) s =
3g E pL
(c) s =
4g E pL
(d) s =
5g E pL
11.30. ________ material will have more ductility. Answers 11.1. 11.4. 11.7. 11.10. 11.13. 11.16. 11.19. 11.22. 11.25. 11.28.
Mechanical property Strain True stress 1, 120 s = s0 + kd1/2 Hooke’s law Charpy test and Izod test Carburising 1073 K to 1143 K Griffith
11.2. 11.5. 11.8. 11.11. 11.14. 11.17. 11.20. 11.23. 11.26. 11.29.
Stress No unit (a) Transition BCC metals Mineralogist Fatigue limit 1118 K and 1173 K Heat treatment. (a)
Short Questions 11.1. Define the term ‘mechanical property of a material’. 11.2. Mention some mechanical properties of materials.
11.3. 11.6. 11.9. 11.12. 11.15. 11.18. 11.21. 11.24. 11.27. 11.30.
N m2. Elastic region (b) Polycrystalline Ductile kg mm2 High 863 Brittle Pure
Mechanical Properties
11.3. 11.4. 11.5. 11.6. 11.7. 11.8. 11.9. 11.10. 11.11. 11.12. 11.13. 11.14. 11.15. 11.16. 11.17. 11.18. 11.19. 11.20. 11.21. 11.22. 11.23. 11.24. 11.25. 11.26. 11.27. 11.28. 11.29. 11.30. 11.31. 11.32. 11.33. 11.34. 11.35. 11.36. 11.37. 11.38. 11.39. 11.40. 11.41. 11.42. 11.43. 11.44. 11.45.
335
Define stress. What is strain? Define the term ’modulus of elasticity’. What is meant by lateral strain? Define Poisson’s ratio. What is meant by true strain? Explain true stress. Distinguish between elasticity and plasticity. Define the following mechanical properties: (i) hardness, (ii) ductility, (iii) brittleness, (iv) endurance, (v) resilience, (vi) stiffness, and (vii) impact strength. What is Moh’s hardness? Obtain an expression for hardness of a material. Write the expression for hardness and explain the terms. Explain the measurement of Brinell Hardness Number. What are the limitations of Brinell Hardness Testing? Explain the measurement of Vicker’s Hardness Number. Mention the advantages of Vicker’s Hardness Testing. Explain the principle of Rockwell Hardness Testing. What are the limitations of Rockwell Hardness Testing? Mention the advantages of Rockwell Hardness Testing. What do you mean by rebound hardness? Mention the uses of hardness test. What are the mechanical properties obtained for a specimen using a tensile test? Explain tensile test. What is meant by compression test? What is an impact test? Explain the advantages of impact test. Mention the specifications for the Charpy and Izod tests specimen. What are the other results obtained using fatigue test? Mention the factors affecting the mechanical properties of materials. What do you mean by strengthening mechanism of materials? What is grain size strengthening? What is cold working? What are the limitations of cold working? What do you mean by solid solution strengthening? What are the changes obtained in the properties of the materials due to solid solution strengthening? Write about ordered substitution solid solution. What is random substitution solid solution? What is interstitial solid solution? What do you mean by precipitation hardening? What is meant by over ageing? What are the conditions to be satisfied for age hardening? What do you mean by diffusion hardening? Explain the term carburising.
336
Materials Science
11.46. 11.47. 11.48. 11.49. 11.50. 11.51. 11.52. 11.53. 11.54. 11.55. 11.56. 11.57. 11.58. 11.59. 11.60. 11.61. 11.62. 11.63. 11.64. 11.65. 11.66.
What is pack carburising? What do you meant by liquid carburising? What is gas carburising? Explain the process of nitriding. What is meant by cyaniding? What is carbonitriding? What is mean by heat treatment hardening? What do you mean by fracture? What is brittle fracture? Mention the characteristics of brittle fracture. What is ductile fracture? List out the differences between ductile and brittle fracture. What do you mean by fatigue fracture? What is meant by endurance limit? What are the factors affecting fatigue fractures? What are the methods used to prevent fatigue fractures? What is meant by creep? What are the different types of creeps? Explain. What is meant by primary and secondary creep? What do you meant by tertiary creep? What are the factors affecting creep?
Descriptive Questions 11.1. What is hardness of a metal? List out the different types of hardness measurements. Explain with suitable theory, the measurement of Brinell hardness. 11.2. Obtain an expression for hardness. Explain with suitable theory the Vicker’s hardness measurements. 11.3. What is tensile strength? Explain the experimental measurement of tensile strength with suitable sketches. What are the other properties obtained using tensile test measurement. 11.4. Write short note on the following: (i) impact test, (ii) fatigue test, and (iii) creep test. 11.5. Write in detail the different types of strengthening mechanisms used to improve the mechanical properties of materials. 11.6. What is brittle fracture? Derive Griffith criterion for brittle fracture. 11.7. Write short note on the following: (i) ductile fracture, (ii) fatigue fracture, and (iii) creep fracture.
Exercises 11.1. The final gauge length and final diameter of an Al alloy after failure is 38.54 mm and 6.8 mm, respectively. If the initial length and diameter of that Al alloy is 35 mm and 8 mm, respectively. Calculate the ductility of Al alloy. 11.2. A 500 kg load is applied to a 11 mm diameter indenter, producing an impression on a steel plate having a tensile strength of 520 MPa. Estimate the diameter of the impression.
Chapter
12
THERMAL PROPERTIES
12.1 INTRODUCTION The selection of materials for the components requires complete knowledge on the solid materials against thermal effects, i.e., thermal properties. The thermal properties of the solids namely heat capacity, thermal expansion, thermal conductivity, melting point and thermal stresses are essentially required for the design and production engineers. Generally, components are exposed to both low and high temperatures. When a solid material is exposed to heat, it absorbs energy in the form of heat. As a result, the internal temperature of the material is raised and hence, leads to a change in dimension of the solid. The absorbed heat energy is transported from hot region to cooler regions whenever there is a temperature gradient. The heat energy is transferred from hot to cooler region due to lattice vibration in the solids. The lattice vibrations are in turn connected with thermal properties of the solids. In this chapter, a brief discussion on the thermal properties, lattice vibration and its relationship with thermal properties of materials are discussed.
12.2 HEAT CAPACITY Heat capacity is the ability of the solid material to observe heat from the external surroundings, i.e., the energy required to raise unit temperature of the material. When a materials is heated its internal energy increases due to absorption of heat energy. Therefore, the heat capacity c is the fundamental materials property and is given by, c=
dQ dT
(12.1)
where dQ is the quantity of the energy transferred into the body and dT the change in temperature in Kelvin (K) or Celsius (˚C). The magnitude of change in DT is same either in Kelvin (K) or Celsius (˚C). On the other hand, for a material with a basic unit of mass (J Kg1 K1), it is denoted as specific heat c as, c=
q m DT
(12.2)
where q is the amount of heat energy, m the mass (kg) and DT the change in temperature in Kelvin (K) or Celsius (˚C). The specific heat capacity of a solid or liquid is defined as the heat required to raise it unit mass of substance by one degree of temperature.
338
Materials Science
Generally, heat capacity is often denoted for a basis of one mole (for compound) or one gram of atom (for element) of the material. When the material absorbs heat, its total energy E of material increases. Therefore, the total energy E which is sum of potential (Ep) and kinetic (Ek) energy i.e.,
E = Ek + Ep
(12.3)
The increase in potential energy leads to thermal expansion while thermal vibration is produced due to increase in kinetic energy. Generally, the heat capacity or specific heat is measured in two ways based on the environmental condition during the heat transfer. In the first method, the volume of the material is maintained constant, i.e., the specific heat at constant volume (cv). In the second method, the external pressure is maintained constant, i.e., specific heat at constant pressure (cp). The specific heat at constant volume is Ê dQ ˆ cv = Á Ë dT ˜¯ v
(12.4)
The unit for heat capacity per mole of materials is J mol1 K1. One can also represent in terms of per unit mass as J Kg1 K1. Usually, specific heat at constant volume is referred as one mole of a substance. The specific heat capacity of engineering materials at constant pressure is shown in Table 12.1.
Table 12.1 Specific Heat Capacity of Engineering Materials at Constant Pressure at 298 K cp (J Kg1 K1)
Material Metals Aluminum
900
Copper
386
Gold
128
Iron
448
Nickel
443
Silver
235
Tungsten
138
1025 Steel
486
316 Stainless steel
502
Brass
375
Kovar
460
Invar
500
Super Invar
500 Ceramics
Alumina
775
Magnesia
940
Contd.
Thermal Properties
339
Table 12.1 (Continued) cp (J Kg1 K1)
Material Spinal
790
Fused Silica
740
Soda lime glass
840
Borosilicate
850 Polymers
Polyethylene
1850
Polypropylene
1925
Polystyrene
1170
Polytetrafluoroethylene (Teflon)
1050
Phenolformaldehyde phenol Nylon 6,6
1590–1760 1670
In most of solid materials, the difference between cp and cv is very less at room temperature. However, the magnitude of cp is always higher than cv. The specific heat cv depends on temperature. When the temperature is above room temperature, cv ª 3R
(12.5)
where R is the universal gas constant. The value of cv ª 6 Cal mol1 K1 which is known as Dulong and Petit law. The temperature dependence of specific heat cv at low temperature, cv = AT3
(12.6)
Heat Capacity (Cv)
where A is a temperature dependent constant. When the temperature reaches above Debye temperature (qD), the cv value reaches maximum at approximately 3R. The heat capacity as a function of temperature is shown in Fig. 12.1. A sharp rise in the magnitude of cv with increase in temperature is at 0 K. Beyond Debye temperature (qD), the value of cv (~3R) reaches the maximum value. In most of engineering materials like metals, ceramics and polymers, the above energy absorbing mechanism explains the thermal properties approximately. However, the mechanism like atomic vibrations contributes to rise in the energy of the materials. 3R
0 0
Fig. 12.1
qD Temperature (K)
Heat capacity as a function of temperature
340
Materials Science
12.3
THERMAL EXPANSION
We know that solid materials expand during heating and contract during cooling. Generally, solid materials expand equally in all three directions and hence, thermal expansion is known as thermally isotropic. On the other hand, the change in length of the material with rise in temperature is known as linear expansion. Let l0 and lf be the initial and final length of the material at temperature respectively T0 and Tf. The fractional change in length l f  l0 l0
= a L (T f  T0 )
(12.7)
Substituting Dl = lf – l0, l0 = l and DT = Tf – T0, in above equation, we get Dl =a L DT l or
al =
Dl lDT
(12.8)
where aL is a constant known as linear coefficient of thermal expansion. It is one of the important material properties used to study expansion of the solid material due to heating. When a material is alternatively subjected into heating and cooling, it affects its dimension in all directions and hence, leads to a change in volume. Let V be the original volume of the material. Then, the fractional change in volume DV = aV DT V where aV is a constant known as volume coefficient of thermal expansion and DV the change in volume for a change in temperature DT. Therefore, volume coefficient of thermal expansion av =
DV V DT
(12.9)
The linear and volume coefficient of thermal expansion of some materials are listed in Table 12.2. In most of materials, the volume expansion depends on crystallographic directions and hence, it is anisotropic. One can explain the thermal expansion in solids materials by considering the potential energy as a function of interatomic distance. When the solid absorbs heat energy, it increases the thermal vibration of the atom about its equilibrium position. An increase in temperature leads to an increase in average separation distance between the adjunct atoms.
Table 12.2
Linear and Volume Coefficient of Thermal Expansion of Some Materials at 298 K Material
aL (K1)
aV (K1)
23.6
69
19
57
Metals Aluminum Brass
Contd.
Thermal Properties
341
Table 12.2 (Continued) aL (K1)
aV (K1)
17
51
Gold
14.2
42
Iron
11.8
33.3
Lead
1
3
Nickel
13.3
39.9
Silver
19.7
55
Tungsten
4.5
13.5
1025 Steel
12.0
35
316 Stainless steel
16
52
Kovar
5.1
15.2
Invar
1.6
3.6
Super Invar
0.72
2.1
Alumina
7.6
22.4
Magnesia
13.5
39.4
Spinal
7.6
22
Fused Silica
0.4
1.2
Soda lime glass
9.0
26.4
Borosilicate
3.3
9.9
Polyethylene
106198
–
Polypropylene
145180
–
Polystyrene
90150
–
Polytetrafluoroethylene (Teflon)
126216
–
Phenolformaldehyde phenol
122
–
Nylon 6,6
144
–
Polyisoprene
220
–
Material Copper
Ceramics
Polymers
Consider the potential energy as a function of temperature of interatomic distance for a weakly bonded solid material which shows an asymmetric curve as shown in Fig. 12.2(a). At 0 K, the equilibrium interatomic distance for the atom is r0 and it takes a minimum at the potential energy trough of the potential energy curve. When the temperature increases from 0 K to T1, T1 to T2, T2 to T3 and so on, the vibrational energy of the atom increases from E0 to E1, E1 to E2, and so on. Therefore, the increase in vibrational energy increases the interatomic distance from r0 to r1, r1 to r2, and so on. Thus, the observed thermal expansion in case of weakly bonded solid materials exhibit an increase in interatomic separation and hence, the thermal expansion increases with increase in temperature. On the other hand, for a strongly
342
Materials Science
bonded solid, there is no increase in interatomic separation with increase in temperature as observed in Fig. 12.2(a). The potential energy curve is symmetrical as shown in Fig. 12.2(b) and confirms no change in interatomic separation. Therefore, the thermal expansion in case of strongly bonded solid is almost zero.
Interatomic distance r1r2 r3 r4 r5
E5 E4 E3 E2 E1 r0
(a) Weakly bonded – Asymmetric curve
Fig. 12.2
12.3.1
0 Potential energy Vibrational energies
Potential energy Vibrational energies
0
Interatomic distance r3
E3 E2
r2 r1
E1
(b) Strongly bonded – Symmetric curve
Potential energy as a function of interatomic distance
Metals
The linear thermal expansion coefficient of the metals is low and controlled in most of the metal alloys. The magnitude of thermal expansion lies in between ceramics and polymers. The controlled thermal expansion of metal alloys is used for the applications like dimensional stability as a function of temperature.
12.3.2
Ceramics
Generally, ceramics and glasses have strong interatomic bonding energy due to the existence of ionic and covalent types of bonding. Thus, it gives symmetric potential energy and hence, a small increase in interatomic separation with increase in temperature. Therefore, the thermal expansion is very small due to small change in its dimension. The ceramics materials are brittle in nature and experience nonuniform changes in dimension which is known as thermal shock.
12.3.3
Polymers
Generally, polymeric materials experience very large thermal expansion coefficient during heating. The interatomic bonds are weak and hence, the potential energy curve shows an asymmetric nature. The thermal expansion coefficient of polymers is larger than metals and ceramics. The knowledge on thermal expansion coefficient of materials helps to select the materials for specific application.
Thermal Properties
343
12.4 THERMAL CONDUCTIVITY The process of transfer of heat energy from higher temperature to a low temperature region is termed as thermal conductivity. Thermal conductivity is the ability of a material to transfer heat in a solid. Let Q be the quantity of heat flowing through a solid of crosssection area A having a temperature gradient dT/dx, Then, Qa  A
dT dx
or, Q= K A
dT dx
(12.10)
where K is a proportionality constant known as thermal conductivity of the material. The negative sign indicates that heat is flowing from hot to cold end. The unit for K and Q are W m1 K1 and W, respectively. Rearranging Eq. (12.10), we get the thermal conductivity of the metal as K =
Q A ( dT / dx )
(12.11)
Therefore, thermal conductivity of a material is the amount of heat energy (Q) conducted per unit area of crosssection per second to the temperature gradient (dT/dx).
12.4.1 Mechanism of Heat Conduction In solids, the thermal conduction takes place both by available free electron at room temperature and thermally excited phonons due to the temperature gradient. Therefore, the total thermal conductivity of materials (KT) is the sum of thermal conductivity by the free electrons (KE) available in materials and thermal conductivity by the phonons (EP). Phonons are the energy carriers for lattice vibration. i.e., The total thermal conductivity
KT = KE + KP
(12.12)
12.4.2 Metals Pure metals are extremely good conductors of heat. The available large numbers of free electrons (1028 m3) in metals are more efficient for heat transport than phonons. The electrons in metals are not scattered like phonons. Therefore, the heat transport in pure metals is taken care by electrons. Similarly, we know that the free electrons are responsible for electrical conduction. Therefore, in metals, electrons are more responsible for electrical and thermal conduction. Therefore, the total thermal conductivity of a metal depends only on the thermal conductivity by the free electrons. (KE >> KP).
344
Materials Science
i.e.,
KT = KE
(12.13)
Wiedemann – Franz law relates the thermal (K) and electrical (s) conductivity through a single relationship as, L=
K sT
(12.14)
Thermal Conductivity (W m–1 K–1)
where L is a Lorentz’s number and its theoretical value is 2.44 ¥ 108 W W K 2. The Lorentz number is independent of temperature and is common for all metals. The thermal conductivity of any alloys depends on its composition. A typical composition is dependent of thermal conductivity in copper  zinc alloys as shown in Fig. 12.3. The thermal conductivity of some of the important metals, ceramics and polymers is given in Table 12.3.
400 300 200 100 0
Fig. 12.3
Table 12.3
0
10 20 30 40 Composition of Zn (wt. %)
Thermal conductivity of CuZn alloys
Thermal Conductivity of Some of Metals, Ceramics and Polymers at 298 K K (W m1 K1)
Material Metals Aluminum
247
Copper
398
Gold
315
Iron
80
Nickel
90
Silver
428
Tungsten
178
1025 Steel
51.9
316 Stainless steel
15.9
Brass
120
Kovar
17
Contd.
Thermal Properties
345
Table 12.3 (Continued) K (W m1 K1)
Material Invar
10
Super Invar
10 Ceramics
Alumina
39
Magnesia
37.7
Spinal
15.0
Fused Silica
1.4
Soda lime glass
1.7
Borosilicate
1.4 Polymers
Polyethylene
0.460.50
Polypropylene
0.12
Polystyrene
0.13
Polytetrafluoroethylene (Teflon)
0.25
Phenolformaldehyde phenol
0.15
Nylon 6,6
0.24
12.4.3 Insulators In case of insulators, the concentration of free electron is very less. At 0 K, the concentration of free electron is zero. Therefore, the thermal conductivity by the free electron is small (KE ~0). i.e.,
KT = KP
(12.15)
12.4.4 Semiconductors In case of semiconductors, at 0 K, the total thermal conductivity depends only on the thermal conductivity by phonons. At T π 0 K, the total thermal conductivity depends on both phonons and electrons.
12.4.5 Ceramics In case of ceramics materials, there are no electrons for transport of heat energy. Therefore, the total thermal conductivity depends on conductivity of phonons. Even though, the transfer of heat through this mechanism is much lower and slower than insulators. Some selective materials can be served as good thermal insulator. The temperature dependence of thermal conductivity of solids is shown in Fig. 12.4.
346
Materials Science
1,000
100 Graphite
Thermal conductivity, J/(s.m.K)
Bonded SiC Pure dense CeO Pure dense MgO
10 Fireclay refractory
Clearfused silica
Pure dense Al2O3
Dense stabilized ZrO2 1 2,800 °F Insulating firebrick 2,000 °F Insulating firebrick 0.1 Powdered MgO
0.01 0
200 400 600 800 1,000 1,200 1,400 1,6001,800 2,000 Temperature, °C
Fig. 12.4
12.5
Temperature dependence thermal conductivity of some solids
MELTING POINT
The temperature at which a solid state material is transferred into a liquid state is known as melting temperature or melting point (TM). At this melting temperature, the two phases namely, solid and liquid phases coexist. When heat energy is applied to solid materials, it increases its thermal energy and hence, the atoms vibrate about their equilibrium position. A further addition of heat energy results in the braking of atoms at the surface of solid from their equilibrium positions. The internal energy guided by the atoms breaks the chemical bond and hence, the solid gets melted. Therefore, the melting point of any solid material depends on the nature of chemical bond and the quantity of the heat energy required to break the bond. For example, the melting point for a covalent bond solid material is high when compared with ionic and metallic bonds, while the melting point for a molecular point is very low. Thus, the properties of materials depend on bond strength. The properties of materials and their relationship with bond strength are shown in Table 12.4. Similarly, the melting point for some of the common materials is given in Table 12.5.
Thermal Properties
347
Table 12.4 Materials Properties Along with Bond Nature Properties
Nature of Bond Strongly bonded
Weakly bonded
Melting point
High
Low
Elastic modulus
High
Low
Thermal expansion of coefficient
Low
High
Table 12.5 Melting Points for Some Common Metals Materials
Melting point (K)
Copper
1356
Silver
1234
Gold
1336
Zinc
693
Aluminum
873
Lead
600
Lithium
382
Sodium
371
Potassium
337
Carbon
4000
Silicon
1683
Germanium
1210
One can correlate the coefficient of linear thermal expansion (aL) and the melting point (TM) as, aLTM = Constant a LTM = l
(12.16)
where l is a constant and is equal to 0.02, 0.03 and 0.007, respectively for ionic and metals, salts and covalent bonded oxides and glasses. Melting point for a solid material is an important property which helps to understand the materials properties and their applications.
12.6 THERMAL STRESS The stress induced in solid materials due to temperature variation, i.e., thermal gradient is known as thermal stresses. The thermal gradient in a material is developed due to local heating or a combination of dissimilar materials. The knowledge on thermal stresses is more important since it produces fracture or plastic deformation on materials. Consider a bimetallic strip which consists of two different materials as shown in Fig. 12.5. Let aL1 and aL2 be the linear coefficient of expansion for metals A and B, respectively. The coefficient of expansion for metal A is higher than B, i.e., aL1 > aL2. The behaviour of bimetallic during heating and cooling is shown, respectively in Fig. 12.5(a) and (b). The original length L of the strip increases to L1 during heating while it decreases to L2 during cooling. The change in length of strip both during contraction and expansion is due to the free upper end of the strip. On the other hand, there
348
Materials Science
is no change in length at the bottom end, i.e., bottom end, is restricted by a rigid end support. Therefore, thermal stress is induced at the restricted bottom end. Let lT0 and lTf be the changes in the length of the bimetallic strip in its temperature T0 and Tf, respectively. The length of bimetallic strip L1 at temperature T0 is reduced to the length of strip L2 at temperature Tf as, lTf = lT 0 [1 + a (T f  Ti )]
(12.17)
Rearranging the above equation, we get lTf  lT 0 = lT 0a(T f  Ti ) = ±lT 0a DT
(12.18)
where DT is the difference in temperature and is equal to Tf – T0 Rearranging Eq. (12.18), we get lTf  lT 0
= ± a DT
(12.19)
ethermal = ± a DT
(12.20)
lT 0 where (lTf  lT 0 ) / lT 0 is the thermal stress i.e.,
We know that the Young’s modulus E and stress s in a metal are related as s
=E
(12.21)
ethermal Substituting ethermal value from Eq. (12.20) in the above equation, we get (12.22)
s = ± Ea DT
Equation (12.22) is used to determine the thermal stress in a material both during heating and cooling. The thermal stress is induced in a solid material due to temperature gradient across the material during alternate heating and cooling. µ1 > µ2
µ2
L1 > L2
L A
B
A
NORMAL (a) One end is fixed, the other end is free
Fig. 12.5
L2 < L1
B
HEATING (b) Effect of heating
A
B
COOLING (c) Effect of cooling
Bimetallic strip – Thermal stress
Thermal Properties
349
12.7 THERMAL FATIGUE AND THERMAL SHOCK When a material is subjected into alternate heating and cooling, it results in expansion and contraction, respectively. As a result, the material is under thermal fatigue due to which the thermal stress induced in the materials is fluctuating. The unstable thermal stress in the material causes the thermal fatigue failure. Thermal fatigue resistance is the ability of the material to withstand thermal fatigue failure. When there is a sudden and severe change in temperature, a deformation in the material takes place due to the induced high thermal stresses. The deformation in the material due to sudden and severe changes is known as thermal shock. The ability of the material to withstand this effect is known as thermal shock resistance. Examples for high thermal shock resistance materials are graphite, glassceramics and fused silica.
Key Points to Remember The specific heat capacity of a solid or liquid is defined as the heat required to raise it unit mass of substance by one degree of temperature. The specific heat at constant volume is Ê dQ ˆ cv = Á Ë dT ˜¯ v The unit for heat capacity per mole of materials is J mol1 K1. The magnitude of cp is always higher than cv. The temperature dependence of specific heat cv above room temperature is cv ª 3R, where R is the universal gas constant and cv ª 6 Cal mol1 K1 which is known as Dulong and Petit law. The temperature dependence of specific heat cv at low temperature is cv = AT3 where A is a temperature dependent constant. Dl The linear coefficient of thermal expansion is given by al = l DT DV The volume coefficient of thermal expansion is given by a v = V DT The thermal expansion of strongly bonded solid is almost zero. The linear thermal expansion coefficient of the metals is low and the thermal expansion coefficient of polymers is larger than metals and ceramics. Thermal conductivity is the ability of a material to transfer heat in a solid. Thermal conductivity of a material is the amount of heat energy (Q) conducted per unit area of crosssection per second to the temperature gradient (dT/dx). The thermal conductivity of Q the solid is K = A ( dT / dx ) Pure metals are extremely good conductors of heat. Wiedemann – Franz law relates the thermal (K) and electrical (s) conductivity through a single relationship L = K/sT, where L is a Lorentz’s number and its theoretical value is 2.44 ¥ 108 W W K 2. The Lorentz number is independent of temperature and is common for all metals. The temperature at which a solid state material is transferred into a liquid state is known as melting temperature or melting point (TM).
350
Materials Science
At this melting temperature, the two phases namely solid and liquid phases coexist. The melting point for a covalent bond solid material is high when compared with ionic and metallic bonds, while the melting point for a molecular point is very low. The coefficient of linear thermal expansion (aL) and the melting point (TM) are related by a LTM = l ,where l is a constant and is equal to 0.02, 0.03 and 0.007, respectively for ionic and metals, salts and covalent bonded oxides and glasses. Thermal fatigue resistance is the ability of the material to withstand thermal fatigue failure. When there is a sudden and severe change in temperature, a deformation in the material takes place due to the induced high thermal stresses. The deformation in the material due to sudden and severe changes is known as thermal shock.
Solved Problems Example 12.1 A 0.1 m long Alumina furnace tube is heated from room temperature 300 to 1273 K. Assuming the tube is not mechanically constrained calculate the increase in length produced by this heating. [Linear coefficient of thermal expansion for alumina is 8.8 ¥ 106 K1]. Given Data: The length of the alumina rod
Solution:
l0 = 0.1 m
Linear coefficient of thermal expansion for alumina
aL = 8.8 ¥ 106 K1
The difference in temperature
DT = 973 K
We know that, the linear coefficient of thermal expansion is given by al =
Dl l DT
Rearranging the above equation, we get Dl =a L l0 DT Substituting the values of l0, aL and DT, we get Dl = 8.8 ¥ 106 ¥ 0.1 ¥ 973 = 0.856 Therefore, the change in length produced by the heating is 0.856 mm. Example 12.2 A 0.1 m long mullite furnace tube is heated from room temperature (300 K) to 1273 K. Assuming the tube is not mechanically constrained, calculate the increase in length produced by this heating. Assuming that linear coefficient of thermal expansion for mullite is constant over a temperature and is 5.3 ¥ 106 K1. Given Data: The length of the alumina rod Linear coefficient of thermal expansion for mullite The difference in temperature
l0 = 0.1 m aL = 5.3 ¥ 106 K1 DT= 973 K
Thermal Properties
Solution:
351
The change in length produced by the heating is given by Dl =a L l0 DT Substituting the values of l0, aL and DT, we get Dl = 5.3 ¥ 106 ¥ 0.1 ¥ 973 = 0.516 Therefore, the change in length produced by the heating is 0.516 mm.
Example 12.3 Calculate the steady state heat transfer rate (in Jm2s1) through a sheet of copper 10 mm thick if there is temperature drop from 823 K to 773 K across the sheet. Given Data:
Solution:
The thermal conductivity of the copper (at 798 K)
K = 371 J m1 s1K1
The change in temperature
DT = 50˚ C
The change in thickness of the copper’s sheet
Dx = 10 ¥ 103
We know that, the thermal conductivity of the material is given by Q= K A
dT dx
The steady state heat conduction through a sheet of copper is Ê DQ ˆ Ê DT ˆ ÁË ˜ =  K ÁË ˜ ADt ¯ Dx ¯ Substituting the values of K, DT and Dx, we get = 371 ¥
50 10 ¥ 103
= 1.855 ¥ 106 J m2 s1 Therefore, the steady state heat transfer of 10 mm copper sheet is 1.855 ¥ 106 J m2 s1. Example 12.4 Consider an alumina furnace tube constrained of uniform thermal expansion. Calculate the stress that would be generated in the tube if it were heated 1300 K. (aL = 8.8 ¥ 106 K1 and Modulus of Elasticity E = 370 GPa). Given Data: Linear coefficient of thermal expansion for alumina
aL = 8.8 ¥ 106 K1
The difference in temperature
DT= 1300  300 = 973 K
Modulus of Elasticity
E = 370 GPa
352
Materials Science
Solution:
The unconstrained thermal expansion produced by the heating is given by e = aLDT Substituting the values of aL and DT, we get = 8.8 ¥ 106 ¥ 973 = 8.5624 ¥ 103 The compression stress produced by the heating is s = eE Substituting the values of e and E, we get = 8.5624 ¥ 103 ¥ 370 = 3.169 GPa Therefore, the compression stress produced by the heating is 3.169 GPa.
Example 12.5 Calculate the heat flux through a sheet of brass 7.5 mm thick if the temperatures at the two faces are 423 and 323 K. If the area of the sheet is 0.5 m2, calculate the total energy is transmitted per hour. (Thermal conductivity of brass is 120 W m1 K1). Given Data:
Solution:
The thermal conductivity of the brass
K = 120 W m1 K1
The change in temperature
DT = 423 – 323 = 100 K
The change in thickness of the brass’s sheet
Dx = 7.5 ¥ 103 m
The area of the sheet
A = 0.5 m2
We know, that the thermal conductivity of the material is given by Q= K A
dT dx
Substituting the values of K, A, DT and Dx, we get Ê 100 ˆ = 120 ¥ 0.5 ¥ Á Ë 7.5 ¥ 103 ˜¯ = 8 ¥ 105 J s1 The heat conducted through a sheet per hour is = 80 ¥ 105 ¥ 60 ¥ 60 = 2.88 ¥ 109 J h1 Therefore, the heat flux transmitted through a sheet per hour is 2.88 ¥ 109 J h1.
Thermal Properties
353
Example 12.6 The ends of a cylindrical copper rod of 6.4 mm diameter and 250 mm long are mounted between rigid supports. The rod stress face at temperature (293 K). Upon cooling to 233 K, a maximum thermally induced stress of 119 MPa is possible. Calculate the Young’s modulus given thermal expansion of copper as 17 ¥ 106 K1. Given Data: The diameter of the copper rod
= 6.4 ¥ 103 m
The length of the copper rod
= 250 ¥ 103 m
Linear coefficient of thermal expansion for copper
= 17 ¥ 106 K1 DT = 293 – 233 = 60 K
The difference in temperature Maximum thermally induced stress Solution:
=119 MPa
The fractional change in length Dl =a L DT l Substituting the values of aL and DT, we get Dl = 17 ¥ 106 ¥ 60 l = 1.02 ¥ 103 Therefore, the strain produced in the rod is 1.02 ¥ 103. We know that, the Young’s modulus of the rod is given by E=
Stress Strain
Substituting the value of stress and strain, we get E=
119 ¥ 106 1.02 ¥ 103
= 116.7 GPa Therefore, the Young’s modulus of the rod is 116.7 GPa. Example 12.7 Steel of linear expansion coefficient 12 ¥ 106 K1 is used for rail road track. 11.6 meters long rails are laid with a joint space of 5.4 mm allowed in between. What is the maximum temperature that the rails can withstand without undergoing thermal stress? Given Data: The length of the steel rod
l0 = 11.6 m
Linear coefficient of thermal expansion for steel
aL = 12 ¥ 106 K1
The difference in length
Dx = 5.4 ¥ 103 m
354
Materials Science
Solution:
We know that, the linear coefficient of thermal expansion is given by al =
Dl lDT
Rearranging the above equation, we get DT =
Dl la L
Substituting the values of l, aL and Dl, we get DT =
5.4 ¥ 103 11.6 ¥ 12 ¥ 106
= 38.79 K Therefore, the maximum temperature change can withstand without any thermal stress is 38.79 K. Example 12.8 A rod of Aluminum 0.35 m long is heated from 288 K to 358 K while its ends are maintained rigid. What is the magnitude of stress developed? The thermal expansion coefficient and the Young’s modulus of Al are 23.6 ¥ 106 K1 and 69 GPa, respectively. Given Data: The length of the Al rod
= 0.35 m
Linear coefficient of thermal expansion for Al
= 23.6 ¥ 106 K1 DT = 358 – 288 = 70 K
The difference in temperature Young’s modulus of Al rod Solution:
= 69 MPa
The fractional change in length Dl =a L DT l Substituting the values of aL and DT, we get Dl = 23.6 ¥ 106 ¥ 70 l = 1.652 ¥ 103 Therefore, the strain produced in Al rod is 1.652 ¥ 103. We know, that the Young’s modulus of the rod is given by E=
Stress Strain
Rearranging the above equation, we get Stress = E ¥ Strain
Thermal Properties
355
Substituting the value of E and strain, we get E = 69 ¥ 109 ¥ 1.652 ¥ 103 = 0.114 GPa Therefore, the compressive stress produced in Al rod 0.114 GPa. Example 12.9 A brass rod is to be used in application requiring its end to be held rigid. If the rod is stress free at 293 K temperature, what is the maximum temperature to which the rod may be heated exceeding a compressive stress of 172 MPa. Assume a modulus of elasticity of 100 GPa and linear coefficient of thermal expansion is 20 ¥ 106 K1 for brass. Given Data:
Solution:
Linear coefficient of thermal expansion for alumina
aL = 20 ¥ 106 K1
The compressive stress
s = 172 MPa
Modulus of Elasticity
E = 100 GPa
The unconstrained thermal expansion produced by the heating is given by e = aLDT
(i)
The compression stress produced by the heating is s = eE
(ii)
Substituting the values of e from Eq. (ii) in Eq. (i), we get s = a L DT E Rearranging the above equation, we get DT =
s aL E
Substituting the value of s, aL and E, we get =
172 ¥ 106 100 ¥ 109 ¥ 20 ¥ 106
= 86 K i.e.,
Tf – Ti = 86 K
Substuting the value of Ti, we get Tf = 293 + 86 = 379 K Therefore, the maximum temperature at which the rod may be heated without exceeding a compressive stress of 172 MPa is 379 K.
356
Materials Science
Example 12.10 Estimate the amount of heat (in joule) required to raise 2 kg of (a) iron, (b) graphite and (c) polypropylene from room temperature (300 K) to 373 K. (Specific heat capacity of iron, graphite and polypropylene is 444, 711 and 1880 J kg1 K1, respectively). Given Data:
Solution:
The specific heat capacity of iron
= 444 J kg1 K1
The specific heat capacity of graphite
= 711 J kg1 K1
The specific heat capacity of polypropylene
= 1880 J kg1 K1
The change in temperature
DT = 373 – 300 = 73 K
The weight
W = 2 kg
We know, that heat capacity of the solid is C=
q m DT
Rearranging the above equation, we get q = m C DT
(i)
(a) For iron: Substituting the values of m, C and DT, we get q = 2 ¥ 444 ¥ 73 = 64824 J (b) For graphite: Substituting the values of m, C and DT, we get q = 2 ¥ 711 ¥ 73 = 103806 J (c) For polypropylene: Substituting the values of m, C and DT, we get q = 2 ¥ 1880 ¥ 73 = 274480 J The heat energy required to raise temperature 73 K from its temperature of iron, graphite and polypropylene is 64824, 103806 and 274480 J, respectively.
Thermal Properties
357
ObjectiveType Questions 12.1. A metal piece of weight W gms is to be heated uniformly, the amount of heat energy required to raise its temperature by 100 K is given by (a) C ¥ 100/W (b) C ¥ 100 ¥ W (c) C/(100 ¥ W) (d) C ¥ W/100 12.2. The unit for heat capacity per mole of materials is__________. 12.3. When increasing the temperature, the specific heat at constant volume of a solid is___ (a) Constant at very high temperature (b) Constant at very low temperature 3 (c) Varies as T at very high temperature (d) Varies as T3 at very low temperature 12.4. The temperature dependence of specific heat cv at low temperature is directly proportional to __________. (a) Constant at very high temperature (b) Constant at very low temperature (c) Varies as T3 at very high temperature (d) Varies as T3 at very low temperature 12.5. The magnitude of cp is always higher than cv. (True/False) 12.6. The total internal energy of a solid at low temperature is directly proportional ___________. (a) T (b) T2 (c) T3 (d) T4 12.7. Thermal expansion of solids is a direct consequence of ___________ potential versus interatomic distance curve. (Symmetric/Asymmetric) 12.8. The coefficient of thermal expansion is highest in crystals with _____________ bond. 12.9. The rate of transfer of heat energy from one end of a rod to the other end is greater in a _________ (thinner/thicker) rod than a _________ (thinner/thicker). 12.10. Which of the following metals has the highest thermal conductivity? (a) Copper (b) Gold (c) Silver (d) Aluminum 12.11. Among the following materials, which one has the highest thermal expansion coefficient? (a) Fused Silica (b) Nylon (c) Aluminum (d) Brass 12.12. Material most suitable for thermal insulation is __________. (a) Aluminum (b) Alumina (c) Glass (d) Perspex Answers 12.1. (b) 12.5. True 12.9. Thicker, thinner
12.2. J mol1 K1 12.6. (d) 12.10. (c)
12.3. (a) 12.7. Asymmetric 12.11. (b)
12.4. (d) 12.8. Vander Waal’s bond 12.12. (d)
Short Questions 12.1. Define specific heat capacity of solids. 12.2. What do you mean by thermally isotropic solid? 12.3. Sketch and explain the temperature dependence of the specific heat of the solids.
358
Materials Science
12.4. 12.5. 12.6. 12.7. 12.8. 12.9. 12.10. 12.11. 12.12. 12.13. 12.14. 12.15. 12.16. 12.17.
Write the expression for specific heat of solid at constant volume and constant pressure. What is thermal expansion of solids? Write down the equation for thermal expansion of solids and explain the various terms. What do you mean by coefficient of linear expansion of solids? Write down the expression for linear and volume coefficient of expansion of solids and explain the various terms. Sketch and explain the symmetric and asymmetric potential energy curve as a function of interatomic distance. What do you mean thermal conductivity of solid? Write the expression for thermal conductivity of solids? Explain its terms? What is Lorentz’s number? Give its theoretical value. Define the melting point of material. Give an outline about the nature of the properties of the materials with its nature of bond. What is thermal stress? What do you mean by thermal fatigue resistance? What is thermal shock for materials?
Descriptive Questions 12.1. Define the thermal expansion of solids? Obtain the expression for linear and volume coefficient of solids. 12.2. Obtain the expression for thermal conductivity of solids and explain the mechanism of heat conduction through metal and ceramics. 12.3. Write short notes on (i) Melting Point (ii) Thermal Shock and (iii) Thermal fatigue.
Exercises 12.1. A 0.2 m long Alumina furnace tube is heated from room temperature 300 to 1273 K. Assuming the tube is not mechanically constrained calculate the increase in length produced by this heating. [Linear coefficient of thermal expansion for alumina is 8.8 ¥ 106 K1). 12.2. Calculate the steady state heat transfer rate (in J/m2s) through a sheet of copper 10 mm thick if there is temperature drop from 323 K to 273 K across the sheet. (The thermal conductivity of the copper (at 300 K) is 398 J m1 s1K1). 12.3. Consider an alumina furnace tube constrained of uniform thermal expansion. Calculate the stress that would be generated in the tube if it were heated 1273 K. (aL = 8.8 ¥ 106 K1 and Modulus of Elasticity E = 370 GPa). 12.4. A rod of Aluminum 0.50 m long is heated from 298 K to 358 K while its ends are maintained rigid. What is the magnitude of stress developed? The thermal expansion coefficient and the Young’s modulus of Al are 23.6 ¥ 106 K1 and 69 GPa, respectively. 12.5. Steel of linear expansion coefficient 12 ¥ 106 K1 is used for rail road track. 13 meters long rails are laid with a joint space of 6.2 mm allowed in between. What is the maximum temperature that the rails can withstand without undergoing thermal stress?
Thermal Properties
359
12.6. An alumina rod is to be used in application requiring its end to be held rigid. If the rod is stress free at 298 K temperature, what is the maximum temperature to which the rod may be heated exceeding a compressive stress of 172 MPa. Assume a modulus of elasticity of 97 GPa and linear coefficient of thermal expansion is 7.6 ¥ 106 for alumina. 12.7. The specific heat of silicon is 702 J Kg1 K1. How many joules of heat is required for raising the temperature of a silicon chip of volume 6.25 ¥ 109 m3 from room temperature (300 K) to 310 K?
Chapter
13
OPTICAL PROPERTIES OF MATERIALS
OBJECTIVES To understand the various principles and properties of optical materials. To understand the interaction between materials with electromagnetic radiations. To understand the colour centre, trap and exciton. To study the applications of optical materials.
13.1
INTRODUCTION
Optics is the field of science and engineering encompassing the physical phenomena and technologies associated with the generation, absorption, reflection, transmission, manipulation, detection, and utilisation of light. Phenomena like reflection, absorption and emission occur when an electromagnetic wave is incident on the material. Processes like photoemission, photoconductivity, luminescence and stimulated emission takes place due to the adsorption of light by the materials. When light energy is incident on the material, several interactions take place between the electromagnetic radiation and the electrons available in the material. Optical characteristics of the material are explored by studying the interaction of the electrons with the radiation. Therefore, to understand the optical properties of the materials, knowledge on phenomenon such as absorption, reflection, transmission, polarisation, etc., are essentially required. The optical materials used in the field of modern high technology optical device applications are lasers, optical filters, optical memories, photodiodes, electrooptic modulators, photoluminescence, etc. In this chapter, phenomenon such as refractive index, absorption, dispersion, reflection, optical properties and the formation of traps, excitons and colour centers are discussed in detail.
Optical Properties of Materials
361
13.2 FUNDAMENTALS When a light travels from one medium to another, the phenomena such as reflection, refraction, and dispersion takes place. Reflection takes place when light does not pass into the material rather the light bounces at the surface of the material. Refraction occurs when light passes into the material. It is bent towards or away from the normal direction of propagation according to the index of refraction of the material. The normal is a line perpendicular to the surface of the medium. Dispersion occurs when different wavelengths of light are refracted in different amounts, separating the light into its constituent colours. The wave property of light prevents all light from passing directly though a media. As light passes through different medium, a part of it is reflected while the other part is transmitted through it. We know that electromagnetic radiation covers a wide range of frequencies from 104 to 1022 Hz which includes Xray, UV, visible, IR, microwave and radio wave frequencies. The frequency range covered in the electromagnetic spectrum is shown in Fig. 13.1. Similarly, the frequency range of visible spectrum in the electromagnetic radiation is also highlighted. The radiation which falls under the visible light is falling under the visible region that is 4.3 ¥ 1014 to 7.5 ¥ 104 Hz. Even though all the electromagnetic radiations interact with materials, in order to study the optical properties of the materials, the knowledge of visible light in the electromagnetic radiation is essential and is discussed in detail. Energy (eV) Wavelength (m) Frequency (Hz) 10–14 108 1022 106
g Rays XRays
104 102
Ultraviolet Visible Infrared Microwave
100 10–2 10–4 10–6
Radio, TV
10–8 10–10
Fig. 13.1
1020 1018 1016 1014 1012 1010 108 106 104
10–12 10–10
1 angstrom (Å) 1 nanometer (m)
10–8 10–6
Visible spectrum wavelength 0.4 mm Viole Blue 0.5 mm
Yello
1 micrometer (mm) 0.6 mm
10–4
Gree
Oran
1 millimeter (mm) 10–2 100
Red 1 meter (m)
0.7 mm
102 1 kilometer (km) 104
Electromagnetic spectrum  Frequency range
13.2.1 Electromagnetic Radiation According to classical mechanics, the electromagnetic radiation is considered as a wave like nature. The different forms of electromagnetic waves are light, heat, radio waves, Xrays, etc. These waves are at
362
Materials Science
different wavelengths in a wide range of spectrum known as electromagnetic spectrum. The wavelength of all different regions in the electromagnetic spectrum is shown in Fig. 13.1. The wavelength range of all colours in the visible region namely violet, blue, green and red are also given in the same figure. Let l be the wavelength of electromagnetic radiation. Then, the frequency of radiation is n=
c l
(13.1)
where c is the velocity of light (3×108 m s1). According to quantum mechanical concept, the electromagnetic waves can be considered as photons or quanta. Therefore, the energy of photon is E = hn Substitution the value of n in the above equation, we get E=h
c l
(13.2)
Planck’s constant and l the wavelength of incident light.
13.2.2
Interaction of Light with Materials
Consider a monochromatic light of wave length l is incident on a glass material as shown in Fig. 13.2. Let I be the intensity of the incident light. When a light incident at the airglass interface, a part of the light gets reflected back while a part of the light transmitted into the glass materials. The transmitted light in the glass material interacts with atoms, molecules, ions and charged particles present in the materials. As a result, a small part of the transmitted light is observed by the glass materials. When the transmitted light reaches the other end of the glass, it is again transmitted at the glassair interface. Surface normal Incident ray Reflected ray air glass
Reflected ray Transmitted ray
Fig. 13.2
Transmission of Light
Let Ir, Ia and It be the intensity of reflected, absorbed, and transmitted light respectively. Therefore, the intensity of incident light I = Ir+Ia+It
(13.3)
Optical Properties of Materials
363
Dividing the above equation by I, we get I r I a Ie = = =1 I I I
(13.4)
I I Ir , A = a and T = e is known as reflectivity, absorptivity and transmitivity. I I I It is clear from the above discussion that when an electromagnetic radiation, i.e., light is incident on optical materials, the phenomena like scattering, refraction, reflection, transmission, absorption and luminescence takes place due to the interaction of light with electron. where R =
13.2.3 Atomic and Electronic Interactions The interaction between the electromagnetic radiations and the atom, ions or electrons leads to several optical phenomena in materials. The most important interactions are electronic polarisation and electron energy transfer. (1) Electronic polarisation When an electric field is applied to a solid material, the electronic field interacts with electron clouds surrounding each atom. As a result, atoms are shifted through a small distance relative to the nucleus in a direction opposite to the field direction. Thus, it creates a dipole and hence, induces polarisation. The induced polarisation may result in two effects namely, the absorption of energy of the incident radiation and a reduction in the velocity of the light when it passes through the material. In most of the optical materials, the second effect is more dominant and is discussed as refraction. (2) Electron transition One can explain the phenomena of absorption and emission of electromagnetic radiation by considering transition of electron when a light radiation is incident on material. Consider that an electromagnetic light of frequency n is incident on the material. The atoms in the ground state (E1) absorb energy and hence, it is excited to the higher energy state E3. The process of absorption and radiation of electromagnetic radiation is shown in Fig. 13.3. E3
E2 hn hn E1
Fig. 13.3
Electron transition – Absorption and emission
This electron transition is possible only if the energy of the photon is equal to the difference in the energy levels of the filled (E1) and excited states (E3). i.e.,
DE = E3  E1
or,
Energy of photon E = DE = hv
(13.5)
The excited electrons cannot be stable for a long period of time in E3 being as an unstable state. Hence, it will be lifted to a new state known as intermediate whose energy lies between E3 and E1. The electron from intermediate state is returned back to the ground state E1 with the radiation energy hu.
364
Materials Science
13.3
CLASSIFICATION OF OPTICAL MATERIALS
Generally, optical materials are classified into three categories based on the nature of propagation of light namely, (1) Transparent (2) Translucent, and (3) Opaque (1) Transparent Transparent materials are the materials which transmit the light with little absorption and reflection. These materials are transparent in nature and hence, one can view the object through the material. Electrical insulated materials are transparent. Similarly, few semiconducting materials are transparent. (2) Translucent The incident light gets scattered within the materials and hence, the diffused light is transmitted with the other side of the materials. One cannot view the object while viewing through the materials. These materials are known as translucent material. (3) Opaque The material which absorbs the transmission of visible light is termed as opaque. When an electromagnetic radiation in the entire visible spectrum is incident on this material, either it gets reflected or absorbed. Thus, the materials are opaque. Few semiconducting materials also exhibit this opaque nature.
13.4
OPTICAL PROPERTIES OF MATERIALS
Metals are opaque in nature and hence, phenomena like reflection and absorption may take place. However, the nonmetals are transparent to visible light and hence, the phenomena namely refraction and transmission also take place. Therefore, the optical properties associated with metals and nonmetals are used for many practical applications.
13.4.1
Metals and Nonmetals
When a low frequency electromagnetic radiation (like infrared, visible and middle ultraviolet) is incident on the metal, it behaves as an opaque. On the other hand, a high frequency Xray and gray radiations are incident on metals, and hence it behaves as transparent. When a light radiation in the visible spectrum is incident on a metal, the electrons in the filled states absorb energy and hence, emitted into the excited state above Fermi energy level as shown in Fig. 13.4. Thus, energy of the photon is equal to the change in the energy of electrons, i.e., DE. The excited electron emits the excess energy as photon and returns back to the low energy state. When compared to metals, the important phenomena to be studied are refraction and transmission. CB hn VB Metal
Fig. 13.4
Absorptionmetal
Optical Properties of Materials
365
13.4.2 Different Optical Properties (1) Reflection Consider two different transparent medium with refractive index n1 and n2. Let I0 and IR be the intensity of incident and reflected beams. When a transmitting light from the medium I enters the interface of the medium II, a part of the light is scattered. Therefore, the reflectivity of the incident light which is reflected at the interface is R=
IR Io
(13.6)
Consider that the light is incident normal to the interface, then Ê n  n1ˆ R=Á 2 Ë n2 + n 1 ˜¯
2
(13.7)
On the other hand, when the angle of incident light is not normal to the interface between the two medium, then the reflectivity depends on the angle of incidence. Consider two medium namely, air and solid. Let ns be the refractive index of the solid and na the refractive index of the air which is equal to one. Therefore, when light is transmitted from air to solid medium, the reflectivity is Ê n  1ˆ R=Á s ˜ Ë ns + 1¯
2
(13.8)
Equation (13.8) clearly shows that the reflectivity of the solid depends on the refractive index. For example, the reflectivity of silica is 0.05. One can reduce the reflectivity of the glasses by coating a suitable material. One can also reduce the losses due to reflection in lasers and optical instruments by coating a very thin layer of dielectric materials like MgF2. (2) Refraction When a light is transmitted into nonmetals, i.e., transparent material, it results in a decrease in velocity. Therefore, the light rays bent at the interface. Thus, bending of light rays at the interface is known as refraction. Let n be the refractive index of the material. Therefore, the velocity of light in medium u and refractive index are related as n=
c u
(13.9)
where c is the velocity of light in vacuum. We know that one can determine the velocity of vacuum by knowing the permittivity e and permeability µ of the medium. Therefore, the velocity of liquid in a medium u=
1
(13.10)
em Similarly, the velocity of light in the vacuum c=
1 e0 m0
where e0 and µ0 are respectively the permittivity and permeability of free space.
(13.11)
366
Materials Science
Substituting the values of c and u in Eq. (13.6), we get e m
c=
e0 m0 =
(13.12)
er mr
where er (=e/e0) and µr (=µ/µ0) are respectively the dielectric constant and relative magnetic permeability of the material. In most of the transparent materials, µr=1 and hence, Eq. (13.12) can be written as, c=
(13.13)
er
Equation (13.13) clearly shows that the refractive index of the material depends on the dielectric constant of the material. Therefore, the refractive index in turn depends on the dielectric polarisability of the materials. The refractive indexes of some of the transparent materials are given in Table 13.1.
Table 13.1 Refractive Index of Transparent Materials Material
Refractive index
Ceramics Silica glass
1.458
Borosilicate (Pyrex) glass
1.47
Soda–lime glass
1.51
Quartz (SiO2)
1.55
Dense optical flint glass
1.65
Spinel (MgAl2O4)
1.72
Periclase (MgO)
1.74
Corundum (Al2O3)
1.76
Polymers Polytetrafluoroethylene
1.35
Polymethyl methacrylate
1.49
Polypropylene
1.49
Polyethylene
1.51
Polystyrene
1.60
(3) Absorption in metals, insulators and semiconductors The study on the absorption of materials gives information about the band gaps and the energies corresponding to inter and intraband transitions. When the visible light of electromagnetic radiation is incident on a metal, the electrons in the metals are excited into unoccupied energy states just above the Fermi level. Thus, the metal gets absorbed by the incident radiation of light. Therefore, the metals are opaque. Similarly, due to the electron energy band structures, the nonmetallic materials such as insulators are transparent or opaque to visible light. The optical properties of the metals, insulators and semiconductors can be explained with the study of the absorption.
Optical Properties of Materials
367
a. Metals: Consider an electromagnetic light radiation is incident on the metal. Let s be the conductivity of the metal. The incident light propagated through the metal only through a short depth known as skin depth d. The energy of the electron gets attenuated in the material. Therefore, the skin depth Ê 2 ˆ d =Á Ë ncs ˜¯
1
2
(13.14)
where n is the frequency of the incident light, y the magnetic susceptibility. Generally, if any metal is in infrared region, the maximum time required to reduce the energy of the incident light as that of electrons is within 1013 s. A part of energy absorbed by the material within the skin depth region is used to heat the material. The value of the skin depth depends on wavelength of incident light. The value of d for metal is nearly 50 nm. b. Insulators: We know that the energy gap for an insulator is greater than 5 eV. At room temperature, the conduction electron in insulator is zero. Therefore, if light is incident on the insulator, The incident light gets attenuated in a short period, i.e., 104 s. Thus, the time required for attenuation is much less than metal. Therefore, the absorption is possible only in the ultraviolet region. c. Semiconductors: In semiconductors, the transition from the valance band to conduction band is more essential and depends on the forbidden gap and wave length. Therefore, =
hc Eg
(13.15)
where Eg is the band gap of the material. (4) Transmission Consider a material of thickness x as shown in Fig. 13.2. When the light radiation is incident on the material, phenomena like absortion, reflection and transmission may take place. Let I be the incident of light. The light incident on the material gets transmitted through the material and comes out from the other end as, 2
IT = I (1  R ) e b t
(13.16)
where b is the absorption coefficient and R the reflectance of the material. Equation (13.16) clearly shows that the intensity of the transmitted light depends on the material nature, the losses due to reflection and absorption of light. When a light in the visible region is incident on insulators, the electrons in the valance band absorb the energy and hence, make a transition to some impurity levels which lies in the forbidden gap. The above transition is possible either due to radiative or nonradiative process. The phonon generated during the nonradiative process is used to heat the material.
13.5 EXCITONS When light is incident on a semiconductor, the electrons absorb energy and hence, it is excited from the valence band to the conduction band. The excited electron creates a hole in the valence band. Similarly, the excited electrons in the conduction band are also free. The above process is possible only when the energy of the incident photon is higher than band gap energy Eg in the material. The free hole and electron stay very close and are attracted to each other to form a bound state known as exciton. The schematic representation of the bound state of electronhole pair is shown in Fig. 13.5. The bound state electronhole pair is moving around the centre of mass. The formed excitons are weak at low temperature. Therefore, the unstable excitons are dissociated at high temperature. The excitons are electronically neutral and hence, it is not possible to transport any charge using excitons.
368
Materials Science
Conduction Band –
Conduction Band
+ Valence Band
Fig. 13.5
Bound states  Electronhole pair
e
G Lattice atoms
h
Fig. 13.6
Electron MotionExciton
One can demonstrate through a model for exciton by considering the electron and holes as revolving in an orbit with a common center of gravity as shown in Fig. 13.6. The radii of the revolving holes and electrons are inversely proportional to their effective mass. According to the Bohr model, the mass of the electron replaced by reduced mass is mr* =
1 1 + me* mn*
(13.17)
where m *e and m n* are the effective mass of electrons and holes, respectively. Therefore, the binding energy of electronhole, i.e., exciton is Eex = 13.6
mr* 1 2 ( ) me* E f
(13.18)
where Ef is the reached energy. Thus, the energy levels of electron lies at the top of the band gap and below the conduction band. Let Eex be the binding energy of the exciton. Therefore, the energy of the photon is E = hu = Eg – Eex The exciton energy levels are similar to impurity levels of a doped semiconductor.
(13.19)
Optical Properties of Materials
369
13.5.1 Classification of Excitons Generally, excitons are unstable and formed in all crystals. Excitons are two types namely, Frankel and Mott–Wannier excitons. (1) Frankel excitons The excitons which are formed by bounding together the electrons and holes with a short distance less than atomic radius is known as Frankel excitons. Frankel excitons are strongly bound excitons and hence, the hopping of electrons from one atom to the neighboring atoms is possible. (2) Mott–Wannier excitons The bound electron and hole distance is larger than the lattice constant. The excitons formed with larger bound distance between electron and hole is known as Mott–Wannier excitons. Thus, the excitons are formed by weakly bound electron and hole pairs and hence, it behaves like hydrogen atom. The energy spectrum of exciton obtained in Cu2O is shown in Fig. 13.7. The spectrum shows sharp lines which are obtained below the fundamental edge. When impurities are added to the materials, it interacts with excitons and hence, it broadens the sharp peak.
Absorption coefficent a(×104 m–1)
3
Fundamental edge
2
1 0
Fig. 13.7
2.05
2.10 Photon energy (eV)
2.15
Cu2O  Exciton energy spectrum
Properties The important properties of excitons are as follows. a. b. c. d. e. f.
It is an electrically neutral one and hence, it is not possible to transport any charge. It is possible to transport energy through the moment of excitons. Its directional properties and wavelength depends on the possible state of excitons. It is formed only at low temperature. It is unstable and hence, dissociate at high temperatures. It is grouped as an electronhole droplet.
Applications Following are the applications of excitons: a. b. c. d.
It It It It
is is is is
used used used used
to in in to
find the absolute configuration of inorganic complex. polyfluorene blends for application in lightemitting diodes photo acoustic detection. get the ionised energy level and nondegenerate energy levels.
370
Materials Science
13.6
COLOUR CENTRES
The energy band gaps of ionic crystals are wider and hence, it will not absorb any wavelength of light in the visible region. In pure state, the ionic crystals have more transparent nature. However, these crystals are made to absorb certain components of visible light. Under these conditions, the crystal will appear as coloured. Therefore, a colour centre is a lattice defect which absorbs visible light. Generally, colour centres take place in ionic crystals. When a high energy radiation is incident on ionic crystals, the incident radiation damages the crystals and hence, provides colours. For example, a brown colour is produced from quartz after irradiation with neutrons in a reactor. Following are the different methods used to produce the colour centres: (1) The addition of suitable chemical impurities to the crystal. (2) The nonstoichiometric ratio of the components of the crystal. (3) The crystals can be exposed to high energy light like Xrays or gamma rays. (4) The crystal can be bombarded using high energy particles like electrons or neutrons.
13.6.1
Traps
We know that the transitions of electrons in the conduction band to the valence band are by means of either ways namely, radiative or nonradiative recombinations. In radiative recombination, the energy is released in the form of photon of energy hn. On the other hand, in nonradiative recombination process, a phonon is released with energy Er. One can clarify the recombination processes into two ways namely, band to band and defect centre recombination process. The schematic representation of radiative and nonradiative recombination process method is shown in Fig. 13.8. Conduction band
Conduction band hv
Valence band (a) Bandtoband
Fig. 13.8
Er
Valence band (b) Via trap
Recombination – Illustration
In the bandtoband transition, the transition electron from the conduction band recombines with the hole in vacant valence band and hence, it radiates a photon of energy hu. However, in different centers recombination processes, the transition electron from the conduction band is first trapped by a defect centre and then by the hole. Consider that the crystals are having some defect due to the impurity or lattice imperfections. The existence of defects in the crystal leads to a corresponding energy state called as defect state. These defect states are located in forbidden energy gap of the material. These defects are known as traps. The transition electron makes recombination first with these traps and then with the hole in the valence band. The recombination mechanism depends on the energy sites of traps and its nature. Once the electron hole pair is formed, these traps are ready for another recombination process.
Optical Properties of Materials
371
The heat produced during the recombination is used to form the traps or defecting centres in the crystal either by adding the impurity to the materials or transition of electron from conduction band is captured by an impurity level. The second process has high probability of reexisting the electrons in the valance band. Thus, the recombination process produces the traps and trapping centres in the crystal. Figure 13.9 shows the process of trapping and detrapping of electrons by the trapping centres. hv
conduction band
conduction band hv
Valence band
Fig. 13.9
Valence band
Trapping centre
In semiconductors, the recombination process takes place and the electrons are completely transferred into the valence band. On the other hand, in the presence of a trapping centre, initially, the electrons, are transferred from conduction band to temporary state which formed due to traps and then the electron is transmitted to valence band. The second transition leads to recombination process. Thus, the presence of traps in materials reduces the response time and the conduction of the material. The response time of a charge conduction is defined as the time taken by the charge carrier (electrons/holes) to drop to half in steady state value.
13.6.2 FCentres FCentre is the most commonly studied colour centre. One can produce the Fcentre by heating the alkali halide crystals in the excess of alkali metal vapour. The formation of Fcentre in NaCl due to heating in the excess of Na vapour is shown in Fig. 13.10. – Na+ + Cl– electron Negative ion – + – + vacancy – + – + – +
+
Conduction band Fabsorbtion
+ – + – (a) Lattice configuration
Fig. 13.10
Valence band (b) FBand transition
Fcentre
When the NaCl is irradiated, it is splitted into electrons and possible ions by the absorption of excess Na vapour. Thus, it creates a negative ion vacancy in the halide. The negative ion vacancy behaves as a possible charge due to the influence of surrounding positive ions. The negative ion vacancy state is filled by shifting a single valence electron from alkali ion. The diffusion electron is trapped by the same state and hence, the charge neutrality is maintained. Therefore, the trapping of electron in a negative ion vacancy is known as Fcentres. The Fcentres is named from the German word Farbe which means colour.
372
Materials Science
The quantised electron in an orbital motion behaves as a possible charge. The energy levels of quantised electrons lie just below the conduction band in forbidden energy gap. Therefore, when a light radiation is incident on these crystals, electrons are excited from these levels to the excited states with a characteristic absorption band known as Fband. For example, in NaCl, the F band transition occurs at 4650 Å. In this process, the electrons are excited into molten state with the emission of blue colour. The excited electrons return to low energy state by emitting yellow colour. The F band transition in NaCl and the corresponding absorption system for the blue colour is shown in Figs. 13.10a. and (b) and Fig. 13.11. F Centre Optical absorption
Wavelength 4650 Å
Fig. 13.11
Fband transition in NaCl crystal
Let a be the interatomic distance. According to Maxwell, the frequency of Fband absorption is VF =0.5 a2
(13.20)
The different alkali ions and their absorption energies are given in Table 13.2.
Table 13.2 Absorption Energies of Different Alkali Ions Alkali Halides
13.6.3
Energy (eV)
NaCl
2.7
KCl
2.2
KBr
2.0
RbCl
2.0
CsCl
2.0
NaBr
2.3
LiF
5.0
NaF
3.6
KF
2.7
LiBr
2.7
VCentre
When alkali halide crystals are heated with an excess halogen vapour, it creates V centres. The V centres is an analog to F centre, i.e., a hole which is trapped by a positive alkali ion vacancy is called as V centre. For example, a positive ion vacancy is created during the heating of KBr crystal under an excess Br2 vapour. The positive ion vacancy behaves like a negative charge under the influence of negative ions. Therefore, the positive ions vary and are trapped by the blue results in Vcentre as shown in Fig. 13.12.
Optical Properties of Materials
+
–
+
–
+
–
+
–
+
–
+
–
+
–
+
–
+
–
+
–
373
V Centre
Fig. 13.12
Vcentre
An addition of KCl crystal by an Xray radiation with energy of 30 KeV at room temperature produces V and Fcentres. The absorption spectra for the V and Fcenters in KCl crystal are shown in Fig. 13.13.
Absorption coefficent
F
V
Energy (eV)
Fig. 13.13
F and V centre – KCl crystal
13.6.4 M and Rcentres The other colour centers namely, Mcentre and Rcentre are also produced in ionic crystals using any one of the methods as discussed above. A typical colour centre model is shown in Fig. 13.14. +
–
+
–
+
–
+
– V1 + + –
– +
– R2
+ –
–
–
+
–
–
+ v2
+–
+ +
– a +
+
–
–
+
+
–
–
+
+
–
– F – +
+
+
–
+
+ +
–
+
–
+
–
+
R1+
Fig. 13.14
+
– – –
+
+
–
+ – v + 4 + – + – + – + – +
–
+
– –
+ –
+
– +
–
+
–
+
–
+
–
+
– +
–
– –
+
Colour centre model
–
+
374
Materials Science
One can obtain an Mcentre by means of using two adjacent Fcentre. Similarly, Fcentres are also used to form the Rcentre as shown in Fig 13.14.
Applications of Colour centres a. It finds many practical applications in radiation dosimetres, tunable laser and rare earth element lasers. b. It is used to fabricate the high density memory devices. c. It is used to get all the colours in one material.
Key Points to Remember The frequency range of electromagnetic spectrum is 104 to 1022 Hz. The frequency of electromagnetic radiation is g = c/l. The energy of the photon is E = hg. The intensity of the light incident light on a medium is equal to sum of the intensities of reflection, transmission and absorption. The velocity of the light in the medium decreases due to existence of induced polarisation. The optical materials are classified into transparent, translucent and opaque. The transparent materials will transmit the incident light with less absorption and reflection. The light rays are diffused in translucent materials. Opaque materials either reflect or absorb the light. Ê 2 ˆ The skin depth of the material is d = Á Ë uys ˜¯
1
2
The reflectance of the light in the medium is equal to R = ( The wavelength of the emitted radiation by medium is l = The velocity of liquid in a medium is u = The velocity of light in the vacuum is c =
1
ns  1 2 ) ns + 1
hc Eg
.
em 1
.
e0 m0 The refractive index of the medium is n = c/u. 2 The intensity of transmitted light through a medium is IT = I (1  R ) e b t . The bound state electronhole pair is known as exciton. m* 1 The binding energy of the exciton is equal to Eex = 13.6 r ( )2 . me* E f The bound state electronshole pair within shorten distance is known as Fresnel exciton. The bound state electronshole pair within longer distance is known as Mott–Wannier exciton. The lattice defect in the crystal is known as colour centre. The trapping of the Fband adsorption is 0.5 a2. The trapping of electron in a negative ion vacanny is known as Fcentre. The trapping of the hole by positive alkali ion vacanny is known as Vcentre. The defects energy level is located in the forbidden gap is known as traps.
Optical Properties of Materials
375
ObjectiveType Questions 13.1. 13.2. 13.3. 13.4. 13.5. 13.6. 13.7. 13.8. 13.9. 13.10. 13.11. 13.12. 13.13. 13.14. 13.15. 13.16. 13.17. 13.18. 13.19. 13.20. 13.21. 13.22. 13.23. 13.24. 13.25.
The frequency range of electromagnetic spectrum is _______ to _______ Hz. The frequency of electromagnetic radiation is g =_________. The energy of the photon is E __________. The intensity of the light incident light on a medium is ___________ to sum of the intensities of reflection, transmission and absorption. The velocity of the light in the medium _____________ due to existence of induced polarisation. The optical materials are classified into_________, __________ and __________. The transparent materials will ___________ the incident light with absorption and reflection. The light rays are _________in translucent materials. _______ materials either reflect or absorb the light. The skin depth of the material is____________. The reflectance of the light in the medium is equal to________. The wavelength of the emitted radiation by medium is _________. The velocity of liquid in a medium is__________. The velocity of light in the vacuum is___________. The refractive index of the medium is_________. The intensity of transmitted light through a medium is___________. The bound state electronhole pair is known as __________. The binding energy of the exciton is equal to ____________. The bound state electronshole pair within shorten distance is known as __________ exciton. The bound state electronshole pair within longer distance is known as ___________ exciton. The lattice defect in the crystal is known as_________. The trapping of the Fband adsorption is ________. The trapping of electron in a negative ion vacancy is known as__________. The trapping of the hole by positive alkali ion vacancy is known as__________. The defects energy level is located in the forbidden gap is known as_______.
Answers 13.1. 104 to 1022 13.4. equal 13.7. transmit Ê 2 ˆ 13.10. d = Á Ë uys ˜¯ 13.13. u =
13.2. c/l 13.5. decreases 13.8. diffused 1
2
1
Ê n  1ˆ 13.11. R = Á s ˜ Ë ns + 1¯ 13.14. c =
em
1
13.3. = hg. 13.6. transparent, translucent and opaque 13.9. opaque 2
13.12. l =
hc Eg
13.15. n = c/u
e0 m0 2
13.16. IT = I (1  R ) e b t
13.17. exciton
13.18. Eex = 13.6
mr* 1 2 ( ) me* E f
376
Materials Science
13.19. Fresenl 13.22. 0.5 a2 13.25. traps
13.20. Mott–Wannier 13.23. Fcentre
13.21. colour centre 13.24. Vcentre
Short Questions 13.1. 13.2. 13.3. 13.4. 13.5. 13.6. 13.7. 13.8. 13.9. 13.10. 13.11. 13.12. 13.13. 13.14. 13.15. 13.16. 13.17. 13.18. 13.19. 13.20. 13.21. 13.22. 13.23.
Define refractive index. How are optical materials classified? What are significance of optical properties? Explain the dispersion of light waves. What is meant by transparent material? Explain translucent material. Explain how the refractive index and dielectric constant determines the optical properties of the materials. Define dispersion. How one can say that a material is opaque? Explain skin depth. What is meant by traps? What is meant by trapping centre? Explain recombination process. Define excitons. What is meant by Frenkel excitons? Explain Mott–Wannier excitons. What is meant by colour centre? Explain Fcentre. What is meant by radiative recombination? Explain the process of nonradiative recombination. What is meant by Rcentre. Explain Vcentre. How is Vcentre different from Mcentre?
Descriptive Questions 13.1. Explain how the optical properties of the materials are explained using Drude Lowertz by and Maxwell theory. 13.2. What is meant by absorption? Explain the phenomena of absorption of light in metals, insulators and semiconductors. 13.3. Write a note on the following: (a) Traps (b) Excitons (c) Colour centres
Chapter
14
LUMINESCENCE
OBJECTIVES To understand the principle, process, methods, and applications of luminescence. To study the different luminescence phenomena and their properties. To understand the applications of luminescence.
14.1 INTRODUCTION During fundamental absorption, an electron absorbs a photon from the incident beam and jumps from the valence band to the conduction band. Thus, the electrons are excited due to the absorption of energy. The excited electrons can no longer be in the higher energy state and eventually decay back into a lower energy state by emitting radiation. The process of emission of light by a material after absorbing energy other than heat energy, either in the form of light or electric field or high energy electrons, is known as luminescence. Thus, luminescence is the inverse process of absorption. The knowledge about how matter can be induced to emit radiation is essential to understand the principle and operations of different display devices namely, active and passive devices. A detailed discussion on the complete process of luminescence in solid state devices is given in this chapter.
14.2 PRINCIPLE Let E1 and E2 be the energy of the lower and upper energy states, respectively. When a light is incident on the material, due to the absorption of energy, the electrons are excited into a higher energy state E2. The excited electrons can no longer stay in the excited state E2, and they eventually return back to the lower energy state E1, by the emission of radiation of light of energy E given by, E=
hc l
= E2  E1
(14.1)
378
Materials Science
where, h is the Planck’s constant and c the velocity of light. The emitted wavelength ( l) is in band spectrum rather than a single spectrum. Due to the separate group of energy levels E1 and E2, the materials exhibit phosphorescence. The emission of radiation of light (luminescence) from a solid material can be broadly classified based on the luminescence mechanism. (1) Photoluminescence The excitation arises due to the absorption of photon from the source such as infrared, visible, ultraviolet or Xrays. (2) Cathodoluminescence The excitation is due to the bombardment of high energy electron beam. (3) Electroluminescence The excitation is due to the application of either ac or dc electric current as in a pn junction. (4) Thermoluminescence This process occurs at low temperatures. During this process, the carriers are first excited by some means and the electrons are frozen in their trapping states. Upon heating the solid, thermal agitation results in deexcitation of the electrons with the release of radiation.
14.3
PHOTOLUMINESCENCE
Photoluminescence is usually divided into two different categories namely, fluorescence and phosphorescence. If a substance absorbs light by any one of the above mechanisms, it radiates or emits light during excitation or within 108 s after the excitation is removed. This luminescence is known as fluorescence or fast photoluminescence. This phenomena is temperature independent. This property was first observed in fluorspar, i.e., calcium fluoride. Substances like fluorspar, fluorescein, quinine sulphate, uranium oxide, barium platinocyanide, calcite, uranium glass and some fossils exhibit the phenomena of fluorescence. On the other hand, certain substances emit light after the incident radiation is cut off. This property is known as phosphorescence or slow photoluminescence. The time delay between the electron excitation by the incident beam and the emission of light, ranges from 108 s to several minutes or hours or even days. For example, when CdS is illuminated by ultraviolet rays, it emits a pale blue light for about an hour. The action of phosphorescence depends on the impurity ions known as activators present in the material. The impurity ions or activators replace some of the host ions in the crystal lattice. During this process, if the charge of the activators is not identical with that of the host ions, some the activators will enter into the lattice due to the charge of imbalance. As a result, some other impurity atoms with different ionic charges will be introduced, which are known as coactivators. Luminescence materials are broadly classified into characteristic and noncharacteristic materials, based on the existence of luminescence due to the different energy levels of activators and coactivators. In characteristic luminescence, the excitation energy is transferred rapidly in a time less than 108 s to the activator ion. On the other hand, in noncharacteristic luminescent materials, the excitation energy is transferred for a longer time than 108 s.
14.3.1
Fluorescence
In characteristic luminescent materials, the activator ion absorbs energy directly from the incident photon. Thus, the same energy levels are involved for both absorption and emission and hence, the wavelengths
Luminescence
379
are identical. The only difference between the two wavelengths is a shift in emission spectrum towards the red end of the absorption spectrum. This phenomenon is known as Stokes effect. The observed difference in the wavelength can be explained as follows: Let us consider that each charged activator (positively charged) ion is surrounded by six equidistant negatively charged ions (H) at a distance R from the activator, as shown in Fig. 14.1. When the activator is in its ground state, the most probable value of R is R0, as shown in Fig. 14.2, which corresponds to the minimum energy level. The absorption of photon gives rise to a transition from A to B. This transition takes place very rapidly since the ions in the luminescent centre could not have any time to rearrange. The activator at B gives up heat energy to the surroundings by means of vibration and reaches the new position C (i.e., R = R1), as shown in Fig. 14.2. Then, the downward transition takes place from C to D, with the emitted photon having less energy than the absorbed photon. The observed band of absorption or emission of wavelength during the above process is due to the difference in the Rvalue from R0 and R1, respectively, during the absorption and emission processes. The observed difference in R with the corresponding state is due to the oscillation state of the surrounding ions of the activators. H R
H
H
H
H
H H
Fig. 14.1 Characteristic luminescent material assumed impurity site structure
Fig. 14.2 Ion separation as a function of energy—characteristic luminescent material The absorption and emission peak along with the Stokes shift observed in KCl:Ti characteristic luminescence material is shown in Fig. 14.3. The Stokes shift finds commercial applications in fluorescent lamps.
380
Materials Science
Fig. 14.3 Absorption and emission peak, in KCl:Ti characteristic luminescent material Therefore, in characteristic luminescent materials, the excitation and emission of light radiation occurs very rapidly in less than 108 s and hence, this process is known as fast photoluminescence or fluorescence.
14.3.2
Phosphorescence
In noncharacteristic luminescence materials, both activator and coactivator are normally present. The corresponding energy levels for the activators and coactivators are respectively known as hole and electron traps, which are similar to the acceptor and donor energy levels. These energy levels lie in the energy gap in between the conduction and valence bands. The electron–hole generation and recombination process in noncharacteristic luminescent materials are shown in Fig. 14.4. The absorption of energy by the solid, creates an electron–hole pair as shown in Fig. 14.4(a).
Fig. 14.4 Electron–hole generation and recombination process for nonluminescence material Then, the holes are quickly trapped into the acceptor sites (Fig. 14.4(b)). The recombination of electrons with the trapped holes leads to luminescent emission, as shown in Fig. 14.4(c). It is also possible that the trapping of electrons occur at the donor site before recombination, as shown in Fig. 14.4(c). Figure 14.4(d) shows that the trapping of a hole by the acceptor level. The electrons may recombine with a trapped hole as shown in Fig. 14.4(d) and hence, release a luminescent radiation. The time taken by the electron in a trap depends on the depth of the trap below the conduction band (Ec  Ed) and the temperature T.
Luminescence
Therefore, the probability of energy = Q exp[(Ec  Ed)/kT ]
381
(14.2)
where, Q is a constant and is equal to 108 s1. Thus, it is clear from the above discussion that the impurity levels introduced by the activators inside the band gap plays a vital role in determining the emission of light. In this material, the emission of light occurs rather slowly due to the electron–hole recombination which takes place indirectly through the impurity levels. Therefore, this process is known as phosphorescence or slow photoluminescence. The noncharacteristic luminescent materials are used in display applications due to their slow photoluminescence property.
14.4 PHOSPHORS The materials which are used to produce luminescence are known as phosphors. Generally, phosphors absorb the light waves with low wavelengths and spontaneously emit light waves with high wavelengths. For example, the sulphides of calcium, barium, strontium, zinc, etc., with certain added impurities known as activators, emit lights ranging from several minutes to hours or even days. These materials are known as complex phosphors. Complex phosphorous materials exhibit strong phosphorescence and hence, they are used in display applications. The materials and the added impurities along with the emission colours are shown in Table 14.1.
Table 14.1
Phosphors Used in Display Applications
Base materials Zinc sulfide
Activators Silver
Light colours Blue
Yttrium silicate
Cerium
Purple blue
Zinc sulfide
Copper
Green
Gadolium oxysulfide
Terbium
Yellowish green
Zinc orthosilicate
Manganese
Yellowish green
Zinc cadmium sulfide
Silver
Green
Yttrium oxysulfide
Europium
Red
14.5 CATHODOLUMINESCENCE In case of cathodoluminescence, the emission process is same as that of photoluminescence. however, they are different in the actual excitation mechanism. In cathodoluminescence, when a beam of electrons of energy, say EB, greater than 1 keV, strike a solid material, about 10% of the incident electrons will be backscattered. The remaining 90% of the electrons will penetrate into the solid and hence, dislodge the bound electrons from their parent ions. These electrons in turn further generate secondary electrons. At the final stage, these electrons are excited from the top of the valence band (Ec) to the bottom of the conduction band (Ev), by creating an electron–hole pair with minimum energy of the exciting electrons as Eg = (Ec  Ev). During this process, some of the energy, in the form of photon (heat) and lattice vibrations, is wasted. Therefore, the minimum energy required for the above process is Ec 1 3Eg /2. In
382
Materials Science
view of the rapid loss of energy of the primary electrons, the penetration depth or range is less and is given by RC = K EBb
(14.3)
where, EB is the energy of the incident beam, and K and b are the constants depending on the material. It is interesting to note that the efficiency of cathodoluminescence increases with increase in beam voltage. The important requirement of cathodoluminescence is luminescent phosphor, due to its high secondary emission properties. The major application of cathodoluminescence is in cathode ray oscilloscopes and television picture tubes.
14.6
ELECTROLUMINESCENCE
The phosphor particles namely ZnS:Cu are suspended in a nonconducting transparent insulating binding medium of high dielectric constant, as shown in Fig. 14.5. This medium is sandwiched in between two electrodes namely, highly transparent (SnO2) and a metal electrode. As a result, there is no complete conduction path between the two electrodes and hence, deexcitation cannot take place. When an ac voltage is applied between the two electrodes, a short burst of light is emitted for every half cycle for a period of 1023 s.
Fig. 14.5 Electroluminescent device: Construction Even though there are several mechanisms to explain the emission mechanism, the following two are widely accepted. Due to the application of ac voltage, a high electric field is known to exist within the phosphor particle. The existence of the field will lift electrons in the valence band to the same energy state in the conduction band, as shown in Fig. 14.6(a). In the meantime, the other electrons in the conduction band will fill the vacated state by emitting radiation, as shown in Fig. 14.6(b). On the other hand, the electron moving in the electric field may acquire sufficient energy to lift an electron from the valence band to the conduction band, as shown in Fig. 14.7, by creating a hole in the valence band. This hole then moves up into the acceptor state by effectively emptying it for the electrons. The hole in the valence band is filled by a radiative transition of an electron from the conduction band, as shown in Fig. 14.7(c). Both ac and dc devices, containing phosphor materials (such as ZnS:Cu, Mn), were made and their luminescence properties were explained by the Mn21 ions. One can also produce different display colours such as red, green and yellow, by changing the phosphor powders. The commercial application of this
Luminescence
383
technique is poor and is more suitable for matrix addressing due to their high surface area to volume ratio and their electrical voltage characteristics.
Fig. 14.6 Electroluminescence emission: Quantum Mechanical Tunneling
Fig. 14.7 Electroluminescence emission—Avalanche Process
Injunction Electroluminescence When a semiconductor p–n junction or a point contact is forward biased, the radiative emission is known as injunction electroluminescence. In a semiconductor, the injected minority carriers lead to a radiative recombination with the majority carriers across the energy band gap of the material, when it is forward biased, as shown in Fig. 14.8. When the p–n diode is forward biased, the majority carriers from both sides of the material cross the internal potential barrier and enter the other side of the material and become minority carriers, which is known as minority carrier injunction. Then, there will be excess minority carriers and hence, they will recombine with majority carriers to diffuse energy from the junction by radiative emission.
384
Materials Science
The current (I) and voltage (V) relationship for a diode can be written as È Ê eV ˆ ˘ I = I0 Íexp Á  1˙ Ë b kT ˜¯ ˚ Î
(14.4)
where, I0 is the saturation current and b varies between 1 and 2, depending on the semiconductor and temperature.
Fig. 14.8 pn junction: Radiative Recombination This type of recombination in semiconductors occur in three different ways namely, internal transition, recombination via. impurity centers and exciton recombination. The injection electroluminescence has been observed in a number of semiconductors such as silicon (Si), germanium (Ge), cadmium sulphide (CdS), zinc sulphide (ZnS), zinc selenide (ZnSe), zinc telluride (ZnTe), zinc oxide (ZnO), gallium phosphide (GaP), gallium arsenide (GaAs), boron nitride (BN), etc.
14.7
APPLICATIONS
Following are some of the applications of fluorescent materials: a. Fluorescent materials are used in display devices such as CRT, LED, LCD, etc. b. A fluorescent lamp consists of a thin coating of a fluorescent material like magnesium tungstate, zinc silicate, cadmium borate or zinc beryllium silicate. When ultraviolet radiations are made to fall on such type of materials, they absorb the incident radiation and reemit the light having the wavelength in the visible region, and hence, increases the luminous flux. c. When Xrays are made to fall on a glass coated with barium platinocyanide, it produces a fluorescent light. Therefore, it is used as a detector for Xrays. d. The yellowbrown tint of a washed fabric is removed by adding certain fluorescent chemicals with the washing powder. These fluorescent chemicals are used to increase the whiteness of the fabric. e. Fluorescent paints are prepared by adding some fluorescent chemicals to the paints. When they are illuminated by light during the night time, they become visible. f. Watch dials and clocks are coated with certain fluorescent chemicals like radium compounds.
Luminescence
385
Key Points to Remember Luminescence is the process of emission of light by a material after absorbing energy other than heat energy, either in the form of light or electric field or high energy electrons. The energy of emitted radiation is equal to E = hc/l where, h is the Planck's constant, c the velocity of light and l the wavelength of light. In photoluminescence, the excitation arises due to the absorption of photons from the source such as infrared, visible or Xrays. In cathodeluminescence, the excitation is due to the bombardment of high energy electron field. Electroluminescence process takes place due to excitation of either ac or dc electric field. Thermoluminescence takes place at low temperature. Due to the heating of solids, the thermal agitations result in the deexcitation of electrons with release of radiation. Fluorescence is the process of emission of light during excitation or with 10 8 after the excitation is removed. Complex phosphors are the materials which emit light ranging from several minutes to hours or even some days to certain added impurities known as activators. When a semiconductor pn junction or point contact is forward biased, the radiated emission is known as injection electroluminescence.
Solved Problems Example 14.1 Determine the penetration depth of the primary electrons in ZnS for an incident beam energy of 10 keV. Given that K = 1.2 ¥ 104 and b = 0.151. Given Data: The energy of the incident beam, EB = 10 keV K = 1.2 ¥ 104 b = 0.151 Solution:
The penetration depth of the electron Rc = K EBb = 1.2 ¥ 104 (10 ¥ 103 ¥ 1.6 ¥ 1079)0.151 = 0.6998 mm The penetration depth of the electron is 0.6998 mm.
Example 14.2 The difference in energy level between the conduction and the valence band is 0.4 eV. Find the probability of escape per second of a trapped electron at room temperature. Given that kT = 0.025 eV.
386
Materials Science
Give Data: Energy difference, Ec  Ed = 0.4 eV The value of kT = 0.025 eV Solution:
The escape rate per unit time = Q exp  [(Ec  Ed)/kT] = 108 exp (0.4/0.025) = 11.2 s1 Therefore, the luminescent lifetime is nearly 11 s.
ObjectiveType Questions 14.1. 14.2. 14.3. 14.4. 14.5. 14.6. 14.7. 14.8. 14.9. 14.10.
The emission of radiation of light from a solid material is known as _______. The process of emission of light during excitation is known as _______. Examples for the substances which exhibted fluorescence are _______. _______ and _______. In characteristics luminescence materials, the excitation and emission of light radiation occurs very rapidly in less than _______s. _______ materials are used to produce luminescence. The impurity added to improve light radiation is known as _______. Example for activators are _______ , _______ and _______. The energy level for activators is known as _______. Energy trap is the energy level an _______. The current and voltage relationship for a diode is
È Ê eV ˆ ˘  1˙ (a) I = I0 Íexp Á Ë b kT ˜¯ ˚ Î
È Ê eV ˆ ˘ + 1˙ (b) I = I0 Íexp Á Ë b kT ˜¯ ˚ Î
È Ê eV ˆ ˘ (c) I = I0 Í1  exp Á ˙ Ë b kT ˜¯ ˚ Î
È Ê eV ˆ ˘ (d) I = I0 Í1 + exp Á ˙ Ë b kT ˜¯ ˚ Î
14.11. Examples for injection electroluminescence semiconductors are _______ , _______ and _______. 14.12. Fluorescence materials are used in _______, and _______ display devices. 14.13. In cathodeluminescence, the minimum energy of excitation electrons required to create an electron hole pair is equal to (a) Eg = Ec + Ev (b) Eg = (Ec + Ev)/2 (c) Eg = (Ec  Ev)/2
(d) Eg = Ec  Ev
Answers 14.1. Luminescence
14.2. Fluorescence
14.4. 108
14.5. Phosphorus
14.3. Fluorescein, Quinine Sulphate Fluorspar 14.6. Activators
Luminescence
14.7. Calcium, Strontium, Zinc 14.10. (a)
14.8. Hole 14.11. Silicon, Germanium, Cadmium sulphate
387
14.9. Coactivators 14.12. CRT, LED, LCD
14.13. (d)
Short Questions 14.1. 14.2. 14.3. 14.4. 14.5. 14.6. 14.7. 14.8. 14.9. 14.10. 14.11. 14.12. 14.13. 14.14.
What is meant by luminescence? What is lumen? Define the term fluorescence. Define the term phosphorescence. Explain characteristics luminescent materials. Explain noncharacteristic luminescent materials. Define photoluminescence. What is meant by cathodoluminescence? What is meant by electroluminescence? Define thermoluminescence. What is meant by activators? What is meant by coactivators? Explain how a pn junction radiates energy. Mention some of the applications of luminescence.
Descriptive Questions 14.1. What is luminescence? Explain how photoluminescence takes place in characteristic luminescent materials. 14.2. Explain how electroluminescence takes place in phosphor particles. 14.3. What is meant by injunction electroluminescence? Explain how a pn junction diodes emits radiation. 14.4. Write short notes on the following: a. Photoluminescence b. Cathodoluminescence c. Electroluminescence
Exercise 14.1. A pn junction germanium diode operating at 27 ∞C is found to have a saturation current of I0 = 1 mA for an applied forward bias of 0.2 V. Determine the current through the diode.
Chapter
15
DISPLAY DEVICES
OBJECTIVES To study the principle behind LED and different types of LEDs. To explore the possible LED materials and their properties. To understand the principle behind the passive display device, namely, LCD and the classification of LCD devices. To study the characteristic properties of LCD. To compare the relative merits of LED and LCD. To review the applications of display devices.
15.1
INTRODUCTION
Most electronic devices are made of semiconductors such as silicon and germanium. The applications of semiconductors and their devices are ever increasing in all fields of science and technology. Hence, knowledge on the classification, structures and properties of semiconductors has become very essential to identify the right materials for their applications. In the next chapters, electrical properties of materials will be studied in detail. Therefore, in this chapter, the classification, bonding and structure of solids are discussed in the first part; while in the second part, certain applications such as solar cells and display devices are discussed in detail.
15.2
DISPLAY DEVICES
Recent advancements in the field of science and technology require information on the classification, basic principles, working mechanism, performance and applications of different display devices. Display devices are an output unit which give visual representation of data, i.e., display device is a device which produces the information on the screen. Generally, display devices are classified into two different
Display Devices
389
categories namely, active and passive devices. The device which emits radiation on its own is known as an active device. On the other hand, the device which modulates incident radiations to provide necessary display information is known as a passive device. Display devices play an important role in many areas such as electronic instruments, advertisements, healthcare, home products, etc. The principle, operation and applications of both active and passive display devices are given in detail in the following sections.
15.3 ACTIVE DISPLAY DEVICES An active display device is a device which emits its own radiation when required power is given to the device. The examples of active display devices are as follows. (1) Cathode ray tubes, and (2) Light emitting diodes The principle, working and application of light emitting diodes is given briefly in the following heading:
15.3.1 Light Emitting Diode A Light Emitting Diode (LED) is a junction diode which emits light when it is forward biased. The principle behind LED is electroluminescence. The process of injecting electrons and holes into the ntype and ptype materials is known as injection electroluminescence.
Principle Electrons are charge carriers in a semiconductor and they absorb energy when electric energy is applied. The total energy of the charge carrier electrons increases and hence, they are excited to the higher energy state (E2). The excited electrons in the higher energy state stay there only for a few seconds, and after the mean lifetime eventually return back to the ground state energy level (E1). During this process, a spontaneous emission of the radiation of light takes place. The energy of the emitted photon (hn) is equal to the energy of band gap (Eg) of materials, i.e.,
Eg = hn
(15.1)
where, h is the Planck’s constant and n, the frequency of the emitted radiation. Substituting the value of n =
c in Eq. (15.1), we get l Eg =
hc l
(15.2)
where, c is the velocity of light and l, the wavelength of light. Equation (15.2) can be written as l=
hc Eg
Equation (15.3) gives the wavelength of emitted photon.
(15.3)
390
Materials Science
Substituting the values of h = 6.62 ¥ 1034 J s and c = 2.998 ¥ 108 m s1 in Eq. (15.3), we get The wavelength of emitted photon l =
6.62 ¥ 1034 ¥ 2.998 ¥ 108 Eg l=
12400 o A Eg (eV )
(15.4)
Equation (15.4) indicates that the wavelength of emitted photons depends on the energy gap in the semiconductor. Thus, the energy gap of a semiconductor plays a major role in selecting a suitable material for LED applications. The type of material is also an important factor to be considered for material selection.
Operation LED is a forward biased pn junction (Fig. 15.1). When it is forward biased suitably, it emits visible light. During the forward biasing, the charge carriers, namely, electrons and holes, are injected respectively into the anode and cathode regions. The recombination of the charge carriers namely, the electrons from the nside and the holes from the pside, takes place at the junction. During the recombination, the difference in the energy is given up in the form of heat and light radiation, i.e., photons. The energy of light radiation depends on the strength of recombination. Thus, the diode current controls electroluminous efficiency of the LED. The emitted light is very small in intensity and is of the order of microampere range. The emitted light colour depends on the types of materials used. For example, materials like GaAs, GaP and GaAsP are used to produce infrared, red or green, and red or yellow colours.
– –
– –
ptype – – – – – – –
Eg hv
– – +
+ +
+ +
+ +
+ +
– –
ntype – – – – – – –
Ec
+ +
hv +
+ +
+
+
+ +
+
+
+
Ev
+
Fig 15.1 p – n Junction spontaneous emission
15.3.2
LED in Electrical Circuits
The symbol used for LED is shown in Fig 15.2(a). Similarly, a typical forward biased LED circuit and its symbols is shown in Fig. 15.2(b) and (c). The crosssectional view of gallium arsenide phosphide (GaAsP) semiconductor and its symbol is shown in Fig. 15.3. Gallium arsenide is used as substrate to grow a thin layer of n type gallium arsenide phosphate through the epitaxy method. Above the n type layer, a very thin layer of pregion is diffused.
Display Devices
p
n
–
+ (a)
391
+ – (c)
(b)
Fig. 15.2 Light emitting diode Similarly, a very thin layer of pregion is diffused into the epitaxial layer. The anode is laid down on the pregion in the shape of a comb or other similar configurations. In order to allow more central surface area for the light to escape, the provisions for metal oxide connections are given at the outer edge of the player. Light
Photons Metal comb anode pn junction 11.5mm
+ –
+ –
pregion + –
nregion Symbol
Fig. 15.3 Gallium arsenide phosphate semiconductor—sectional view
15.3.3 Types of LEDs LEDs are available as discrete components, packed for specific applications, or as high intensity light source products depending on the applications. (1) Discrete LED The popular standard type LED is in the form of a small round dome epoxy encapsulation. LEDs are also available in a variety of other shapes and sizes. In particular, rectangular, square and triangular LEDs are available for applications like panel indicators. LED components like axial leaded LEDs, bar graph displays, tricoloured RGB LEDs, and surface mount technology components are also available in the market. The salient features of LEDs include low current, high brightness, high voltage, flashing and multicolour variants. (2) Alphanumeric Displays In 1967, LED displays were introduced comprising of seven or more individual LEDs. In most of the electrical appliances and other applications, these types of displays are
392
Materials Science
used. The displays are arranged either by using a multisegment LED display or a dotmatrix LED display. The alphanumeric character is displayed by means of using array LEDs and sevensegment LEDs. The schematic representation of 7 ¥ 5 array and seven segment LED arrangements for the alphanumeric display are shown, respectively in Fig.15.4(a) and (b). In 7 ¥ 5 array LED display, the illuminated points are shown as dark points while nonilluminated points are shown by white points. A typical representation of decimal 5 readout is shown in Fig. 15.4(a). The sevensegment display is energised by applying a potential range from 1.5 to 3.3 V with a constant current of 50 to 100 mA. The above display can produce different colours such as red, blue, green and orange. In most of the display applications, sevensegment displays are commonly used.
(a) 7 ¥ 5 array of LED’s Epoxy encapsulation
Light pipe LED
(b) Sevensegment LED Fig. 15.4 Alphanumeric display (3) LED Clusters and Lights In order to produce brighter and high power lights, groups or clusters of LEDs are used. The total brightness of the group or cluster of LEDs may fail even if there is a breakdown of one or two individual LEDs within the group. However, the application of LED technology is increasing in the market due to high density light yield.
15.3.4
LEDs—Reduction in Reflection Loss
Generally, when an LED emits light, there is a loss of light energy due to reflection losses which arise in LEDs. There are two methods by which one can reduce the loss due to reflection. One way of reducing loss of reflection is by making the LED with a hemispherical dome as shown in Fig. 15.5(a). In this method, the ptype material is used to obtain a hemispherical domelike structure. Thus, the dome forms a semiconductor/air interface. When the light rays strike the semiconductor/air interface at an angle less
Display Devices
393
than the critical angle, they emerge out without any loss. The energy loss is further reduced by replacing the dome by means of plastic encapsulation as shown in Fig.15.5(b). The replacement of semiconductor/ air interface in a hemispherical dome by a plastic/air interface further reduces the loss of energy due to reflection. In most of the commercial LEDs, the plastic encapsulation techniques are employed to improve the brightness of light energy.
Plastic encapsulation p
pn junction
n
Electrical contacts
(a) Hemispherical dome
Electrical contacts
(b) Plastic encapsulation
Fig. 15.5 LEDs— reduction in reflection loss
15.3.5 LED Materials The material selection for the fabrication of LED is essential due to the emission of different colours (wavelength). The emission of light with different colours depends on the semiconductor material. The essential factors such as energy gap, both n and ptype with efficient pathways are to be considered for the fabrication of LEDs. The wavelength of the light emitted depends on the energy gap of the semiconducting material. For example, infrared and far infrared light are emitted by lower band–gap materials, while visible light is emitted by larger band gap (ª2 eV) materials. Due to the high melting point, high resistivity and low structural stability, the high band gap materials have advantages in LED applications than low band gap materials. The commercially available materials for LED applications along with their properties are briefed in the following headings: (1) Gallium Arsenide Gallium Arsenide (GaAs) is an III–V compound semiconductor consisting of the element gallium from column III and the element arsenic from V of the periodic table. It is a direct band gap semiconductor. At room temperature, the band gap energy is 1.44 eV. It has high luminescent efficiencies due to the readily formed pn junction. The mass radiation is due to the band to band transitions. Hence, the emitted radiations are reabsorbed. The efficient diodes are obtained by doping silicon, either as a donor or acceptor. The incorporation of silicon is used to replace either Ga or As depending on the doping. Thus, the main radioactive transition is based on the recombination between conduction band and complete acceptor level. In such a case, the bandtoband transition is not effective due to the insufficient energy of radiation and hence,
394
Materials Science
reabsorption is very low. Generally, the wavelength of light emitted from GaAs LED lies between 910 and 1020 nm. (2) Gallium Phosphate Gallium Phosphate (GaP) is an indirect band–gap semiconductor with Eg = 2.26 eV. These semiconductors are converted into an efficient light emitter by doping impurity in the band gap. Generally, it emits red and green light. There is no bandtoband radioactive transition. Elements such as N and Bi from group V, have the same valence as that of P and are doped. It is useful to get the radioactive recombination rather than forming donor or acceptor states. When the doping concentration of N is greater than 1014 cm3, it results in a shift in the emitted light radiation from 550 nm (green) to 590 nm (yellow). This observed shift in the light radiation is due to the defect level in the band gap. A simultaneous doping of Zn and O in GaP results in light radiation at 640 nm (red). (3) Gallium Arsenide Phosphide Gallium Arsenide Phosphide (GaAs1xPx) is an important semiconductor for LED fabrication due to the change in band gap energy. The band gap energy depends on the composition of x. When the composition is low (x < 0.45), it gives a direct band gap semiconductor, while when it reaches x = 0.45, a change in the direct band gap to indirect band gap takes place. Thus, the energy gap at x = 0.45 is 2.1 eV. One can produce light emission for different colours such as red, orange and yellow by changing the composition of x and the doping content N. (4) Gallium Aluminium Arsenide Gallium Aluminum Arsenide (GaxAl1xAs) is a new semiconductor used for the fabrication of LEDs. The light emitted by these materials lies in between red and near infrared region. The intensity of the light is very high and hence, it is called super bright LEDs. The standard type GaAsP LEDs are replaced by GaAlAs LEDs. The highintensity radioactive emission is due to the formation of ntype Ga0.3Al0.7As and ptype Ga0.6Al0.4As semiconductor by doping Zn. The emission is achieved at 650 nm with high efficiency. The doping of Si with a change in Al composition is possible due to increase in the band gap and hence, emission rate from 870 to 890 nm. (5) Indium Gallium Arsenide Indium Gallium Arsenide (In0.53Ga0.47As) semiconductor is used for fibre optical communications. The light emitted by the LEDs is in the range of 1.1 to 1.6 mm. This wavelength range is more suitable for optical communications since the spectral region of optical fibres lies in the same range. The general characteristic properties of common LED materials are given in Table 15.1.
Table 15.1
Properties of LED Materials
Materials
Band gap type Band gap (eV) Peak wave length (nm)
Colour
GaP:ZnO GaAsP
Indirect Direct
1.78 1.99
700 650
Red Red
GaAsP: N AlGaAs AlGaP AlInGaP GaAsP:N AlInGaP GaP:N GaP SiC GaN
Indirect Direct Direct Direct Indirect Direct Indirect Indirect Indirect Direct
1.95 1.91 2.00 2.08 2.10 2.18 2.20 2.26 2.9 – 3.05 3.5
630 650 620 595 585 570 565 555 480 450
Red Red Red Amber Yellow Yellow–Green Yellow–Green Green Blue Blue
Display Devices
Advantages a. b. c. d. e. f. g.
395
Following are the advantages of LEDs
LEDs are used to produce more light per watt than incandescent bulbs. It is easy to operate than through battery power. LEDs are highly protected as they are built inside solid cases. The lifespan of LEDs is more than 100,000 hours. LEDs light up very quickly. A typical red indicator LED will achieve full brightness within a few microseconds. The response time of LEDs used in communication devices is much faster than normal sources.
15.4 PASSIVE DISPLAY DEVICES Nonemissive display devices are known as passive display devices, i.e., they modify the parameters of light, generated by an external source. The modification may take place in optical parameters such as optical path, path length, absorption, reflection, scattering or a combination of all these parameters. Each modulation will have its own effects. For example, when wavelength is modulated, then the display is coloured. Materials such as liquid crystals, electrophoresis and electrochromium are used to achieve electrooptic effects. Based on the properties of electrooptic materials, one can select the right material for passive display devices. The Liquid Crystal Display (LCD) is widely used due to the variety of modulation effects. The properties of passive display materials are given in Table 15.2. In the following heading, the principle, types, operation and applications are given in detail.
Table 15.2
Properties of Passive Display Materials
Effect
Liquid crystals
Electrophoresis Electrochromism
Hydrodynamic Field effect Operation in transmission
T
T


Operation in reflection
R
R
R
R
Viewing angle
Narrow
Medium
No restriction
No restriction
Operating voltage (V)
15–40
5–10
50–100
1–2
0.002
0.4

0.2
1
0.001
Power consumption continuous 0.1 operation mW cm2 Switching speed 0.05 T  Transmission RReflection
15.4.1 Liquid Crystal Display Liquid crystal is a kind of substance which lies in an intermediate state between a conventional liquid and a solid state. In a restricted temperature range, organic materials exhibit a state of matter known as liquid crystal state. A liquid crystal becomes crystalline solid at low temperature, and at high temperatures, it turns into a clear isotropic liquid. Thus, the properties of liquid crystals are intermediate between liquids and solids. LEDs generate light, while Liquid Crystal Displays do not generate light, rather they reflect light. LCD reflects only a part of the surrounding light, while the other part of the light is absorbed by the display. In view of the above reasons, LCDs are used in lighted areas. LCD displays are used in watches, display boards, TVs, computers and pocket calculators.
396
Materials Science
15.4.2
Principles of LCD
Liquid crystal display is based on two principles namely, polarisation and twisted nematic property of the liquid crystal. (1) Polarisation The process of filtering certain unwanted light wavelengths, employing glass with parallel thin impenetrable black lines, is known as polarisation. When the wavelength of the incident light is parallel to the parallel lines, it will pass through the glass, while the other wavelengths are stopped. Consider two polarised glass sheets are placed one in front of the other with perpendicular polarisation. When light is incident on the glass sheet, it will not pass through it. (2) Twisted Nematic Consider that the liquid crystal is sandwiched between two sheets of polarised glass. The molecules in the liquid crystal arrange themselves in a twisted form. Under this condition, when a light is entering into the first sheet of glass, it comes out of the glass as a polarised light. Thus, the polarised light enters into the twisted form of molecules. The entered light waves are twisted along with the orientation of liquid crystal molecules. The light waves which enter the molecules are in line with the polarisation of the second glass sheet. Therefore, the region in which the light passes through the glass sheet is displayed. On the other hand, a liquid crystal does not pass the light when it is untwisted. Therefore, the light is not passed through the second glass sheet, and hence, it creates a dark region on the display. The position of the liquid crystal is controlled by applying necessary charge.
15.4.3
Classification of Liquid Crystals
Liquid crystals consist of three different types of states namely, nematic, cholesteric and smectic states. In most of the electrooptic devices, the first two types of states are used for practical display devices. (1) Nematic Liquid Crystals In nematic ordering, the molecules known as directors are arranged parallel to each other. Rod or disclike molecules oriented with respect to each other as well as the liquid crystal surface are known as directors. In other words, a director is a unit vector pointing along the orientation of molecules in a small volume. In nematic ordering, molecules are free to move along each other due to their liquid properties. Generally, two benzene rings are linked with a central group to form the nematic phase. In nematic ordering, the parallel alignment of molecules (or directors) is shown in Fig.15.6. Thus, it acquires liquid properties. In nematic crystals, two benzene rings are linked with a central group. The chemical formula for the nematic crystal molecule 4–methoxy benzylidene–4–butyl analine (MBBA), is given below.
CH3
O
CH
N
C6H9
Fig. 15.6 Liquid crystalline phases – Nematic ordering The schematic arrangements of nematic liquid crystal molecules are shown in Fig.15.6. The MBBA shows liquid crystal behaviour in the temperature range of 293 to 320 K.
Display Devices
397
(2) Cholesteric Liquid Crystals A small modification in the nematic crystal results in a cholesteric liquid crystal. The structure of a cholesteric liquid crystal is derived from cholesterol molecules. The molecules in the crystal are optically active, and hence, have the ability to rotate the plane polarisation of light passing through it. The structure of the cholesteric liquid crystal is shown in Fig. 15.7. Rod or disclike molecules are used in liquid crystal phase.
Pitch
Fig. 15.7 Liquid crystalline phases – Cholesteric ordering A cholesteric liquid crystal consists of a large number of vertical sheets stacked one above the other as shown in Fig 15.7. The molecules in the respective sheets are aligned in the nematic state, keeping the orientation of the molecules in each sheet twisted when compared with the molecules in other sheets. Thus, the director directions of the sheets represent a helical twist in the molecules. The distance between any two successive planes is known as pitch. When a light beam is propagated parallel to the helical axis, it undergoes phenomena like reflection, rotation and change of polarisation based on the wavelength of the incident light to pitch ratio. Similar to the direction, the elliptically polarised light is rotated above the helix axis when wavelength to pitch ratio is very small. The cholesteric liquid crystals show colour effects. When a white light is incident on it, it shows as a strongly coloured light. The pitch of the crystal and colour of reflected light depends on temperature. Under this condition, it obeys the Bragg’s reflections, i.e., p = nl (where n is equal to 1, 2, 3, etc.). The cholesteric liquid crystals consisting of mixed materials are used for visual display devices like a surface temperature measurement thermometer. For example, a mixture of material with 20% cholesterol carbonate and 80% cholesterol nonanoate scatters bright yellow and deep violet lights respectively, at wavelengths of 0.55 mm at 298 K and 0.39 mm at 318 K. (3) Smectic Liquid Crystals A smectic liquid crystal is also called lyotropic liquid crystal (lyo means liquid). An example of smectic liquid crystals is soap water. When soap is melted, it forms liquid crystals. The molecules in liquid crystals are arranged parallel to each other with irregular spacing as shown in Fig. 15.8. A layered structure is known to exist only in smectic structure. Thus, it gives rise to a strong lateral force between molecules within a layer and weak interactions between layers. Therefore, a smectic liquid crystal is slippery.
Fig. 15.8 Smectic liquid crystal—molecular arrangements
398
Materials Science
water
water
Fig. 15.9 Lyotropic smectic liquid crystal–molecular arrangements Similarly, molecules which are arranged in a lyotropic liquid crystal also exhibit a similar property. The arrangement of molecules in a lyotrpic liquid crystal is shown in Fig 15.9. The molecular layers are separated by a thin film of water. The layers can stack one above the other and hence, give properties of soap. Examples of lyotropic liquid crystals are body fluids like mucus and saliva.
15.5
DIFFERENT MODES OF LCD
We know that LCD depends on electrooptic effects. Based on the effects, LCD operations are categorised as: (1) Dynamic scattering (2) Twisted nematic (3) Phase change, and (4) Memory effects A brief explanation about the different modes of LCD is given in the following headings:
15.5.1
Dynamic Scattering
In dynamic scattering, positive nematic materials with homogeneous alignment of molecules having low impendence are used. The material is purely transparent when there is no external field. The molecular ordering depends on the external field. The orientation of positive homogeneous molecules in LCD on application of electric field is shown in Fig. 15.10. For example, when the field is lower than Ec, the molecular ordering is not affected. However, when the field reaches Ec, the molecules tend to align parallel to the field. When the field is extremely high, most of the molecules align along the field direction. At very high field, the existing current carries the movement of the liquid. As a result, the incident light gets a strong scattering. Thus, it gives a frosted appearance to the material. Dynamic scattering is possible only at low frequency, while at higher frequency, it is not possible due to the electrolysis of the liquid. E
(a) E< Ec
(b) E>_ Ec
(c) E>>Ec
Fig. 15.10 Orientation of positive nematic material with homogeneous ordered– applications of electric field
Display Devices
399
LCD is used as an effective scatterer of white light under a suitable external field. However, in the absence of a field, it is purely a transparent liquid crystal. The major disadvantages of LCD are poor contrast due to reflection, short lifetime and huge power consumption when compared to twisted nematic or field effect display.
15.5.2 Twisted Nematic Mode In this method, dielectric properties of the molecules play a major role in the transport property of light. Consider that the molecules are arranged in a manner as shown in Fig. 15.11(a), during the absence of the field. When an external field is applied (E>>Ec), the molecules align themselves in the field direction as shown in Fig. 15.11(b). The twisting of the molecules is eliminated under the influence of the field. When a light is incident on the LCD, it does not have effect on the incident polarised light. The portion in which the twisted nematic LCDs action takes place appears as a block in the ON condition. On the other hand, a shiny surface is obtained on the other faces. These kinds of LCDs help to produce frosty white characters on a dark background. E
d (a) E=O
d (b) E>>Ec
Fig. 15.11 Arrangement of molecules in liquid crystal operating in twisted nematic mode
15.5.3 Phase Change Effect In this mode, cholesteric materials with positive dielectric anisotropy and high resistivity are used. In this method, with proper biasing, the cholesteric planes are maintained perpendicular to the cell walls. When a small field is applied, the widely scattered liquids cause the helix to unwind, leading to the arrangement of molecules in the direction of the field. Thus, the LCD is more nematic and highly transparent.
15.5.4
Memory Effect
Cholesteric materials with negative anisotropy and low resistance are required to achieve this effect. The functions are very similar to dynamic scattering. The transition from the scattering to the transparent state is very slow.
15.6
LIQUID CRYSTAL DISPLAY SYSTEM
It consists of two glass plates, each attached with a crossed polaroid as shown in Fig. 15.12. On both sides of the glass plate, silicon monoxide is coated. The distance of separation between the coating surfaces is typically 10 mm. The liquid crystal is sealed in between the two glass surfaces. Thus, the liquid molecule has a transition
400
Materials Science
in between the two glass plates. LCD devices are usually constructed in the form of sandwich cells. The sandwich cells consist of two conducting glass plates made up of SnO2 by coating on both sides of the plate by In2O3, etc. A thin layer of liquid crystal of the order of 3–50 mm is placed between the two conducting plates. The cell is perfectly sealed in order to avoid chemical reactions by interacting with the environment. Glass Seal
Transparent conductive coating (electrodes)
Fig. 15.12 Liquid crystal display The lifetime of LCD is very high when the device is operated under AC conditions. Liquid crystal is operated under two modes namely, reflective and tranmissive mode. In the reflective mode of operation, the incident light gets reflected back from the surface of the reflective aluminum film which is placed near the glass plate. In the transmission mode, the light is transmitted through the cell. There are two types of LCD displays namely, dynamic scattering and the field effect type. Letters on a dark background are produced in dynamic scattering while in field effect, black letters on a silver background are produced.
15.6.1
Twisted Nematic Liquid Crystal Display
A positive nematic material with parallel alignment of molecules to the field directions is used in Twisted Nematic Liquid Crystal Display (TNLCD) or field effect display. The liquid crystal cell shown in Fig. 15.12 is placed in between the two polarising filters known as polaroid (I and II). The polarizing directions of the filters are made very near to the molecular ordering direction. The arrangements of the filters and the LCD are shown in Fig. 15.13. In the absence of an electric field, the molecules in LCD undergo a gradual twist. When an unpolarised light is incident on the first polaroid, it gives a polarised light. When the polarised light is incident on the cell, the twisted molecules rotate the plane polarised light through 90°. Thus, it gives horizontal polarised light and it passes through the second polaroid. In the absence of a field, it gives a clear bright cell. The action of an LCD is shown in Fig. 15.13(a). On the other hand, when a field is applied, the molecules are aligned in the field direction. Under this condition, when a light is incident on the first polariser, it is passed into the liquid medium. Therefore, the polarised light is simply absorbed by the liquid molecules. Therefore, no light is reflected back from its original path and hence, the liquid medium appears dark. The corresponding display action of an LCD is shown in Fig. 15.13(b). A reflector is placed behind the second polaroid in case of reflective mode of operation. It rotates the incident polarised light through 90° similar to the light when it passes through the cell. The polarised light passes through the second polariser and then, it is reflected back along its path. Therefore, it appears bright. It is clear from the above study that during the absence of a field, LCD reflects the incident light and appears bright. During the presence of a field, light is not passed through the second polariser due to the absence of 90° twist. Hence, there is no reflected light and the device appears dark. The amount of light reflected from LCD depends on the applied voltage. In LCD, the amount of light reflected as a function of applied voltage is shown in Fig. 15.14. The reflected light remains constant up to the critical voltage Vc. The critical voltage Vc is equal to Ecd, where d is the cell thickness. When the applied voltage is increased, an exponential decay is obtained up to the saturation voltage Vsat.
Display Devices
401
Bright light
unpolarised light
Polaroid 1 LC cell (a) Absence of electric field
Polaroid 11
Dark
unpolarised light
Polaroid 1
LC cell E>>Ec
Polaroid 11
(b) Presence of electric field
Fig. 15.13 Twisted nematic liquid crystal display function
Reflected light
The turnon time Ton and turnoff time Toff are important factors which are considered for the operation of an LCD device. In twisted nematic LCD, Ton is directly proportional to average viscosity h and inversely proportional to DŒE2, where Œ is dielectric anisotropy and E, the electric field. The electric field has more influence on Ton than DŒ and h. Similarly, Toff is directly proportional to ld2, where l is the twist viscosity coefficient. The nature of mode of display and transformation temperature of a few a LCDs given in Table 15.3.
Vc Vsat Applied voltage
Fig. 15.14 Reflected light versus applied voltage
Table 15.3 Liquid Crystals Operating Mode and Transition Temperature Liquid crystals
Mode
Transition temperature (K)
npMethoxy Benzylidene pn ButylAniline Nematic (MBBA)
293.4
4 Methoxy 4nButylAzoxBenzene (MBAB)
Nematic
315.8
npEthoxy Benzyliden pn ButylAnidene (EBBA)
Nematic
308.4
CholesterylErucate (CE)
Cholesteric
283.6
Cholesteryl Nonanoate (CN)
Cholesteric
351.9
402
Materials Science
15.6.2
Numeric Display
The commonly used simple format for numeric display is the sevensegment display. It is based on the dynamic scattering method. It consists of two glass plates coated with a transparent conductive material like SnO2. These two glass plates are separated through a small distance of nearly 10 mm. The liquid crystal material is filled in between the glass plates. The conducting coating available at the lower electrode is used as common electrodes. The upper electrodes are energised through latch and driver unit separately. The schematic representation of a seven–segment display is shown in Fig. 15.15. Edge connectors
a) Lower electrode
b) Upper electrode
Fig. 15.15 Seven segment display—dynamic scattering display When the electric field is absent, the liquid appears transparent. On the other hand, when an electric field is applied, the interaction of the doped ions with molecules takes place. Thus, the molecules are oriented in the field direction. Therefore, the incident light on the liquid gets scattered and hence, the liquid appears white in colour. The required electrical field is applied to each segment employing external devices. The power required to generate the electric field is very low. Thus, the required display either in dots or segments is made with the application of electric field by designing the glass plate with a conductive layer on one side. LCD is not suitable for use in matrix displays mainly due to the dependence of the threshold voltage, the flow response on the operating temperature and the flow response time.
15.6.3
Advantages and Disadvantages of LCDs
Following are the advantages of LCDs: a. LCD displays are used in conventional televisions and computer screens. b. LCDs are much lighter in size and consume less power. c. It provides an opportunity for the development of many portable devices. d. LCDs improve the quality of the image and meet the increasing demand for quality display. e. LCDs are replacing CRT screens in many household appliances owing to their lower price. f. It can be viewed over a wide range of lighting conditions. g. The device is very small in thickness.
Display Devices
403
Following are the disadvantages of LCDs: a. The decay time of LCD is very small. Therefore, the segments slowly fade when the power is switched off. b. It requires external illumination and is invisible in darkness. c. The angle of view is limited. d. The intensity of the light produced is very small. e. Its functions are limited in the temperature range of 293 to 333 K. f. It is highly sensitive to environmental conditions like temperature, interference due to electromagnetic field, etc.
15.7 COMPARISON BETWEEN LEDS AND LCDS A comparison between the LEDs and LCDs is given in Table 15.4 for easy understanding.
Table 15.4 Comparison of LED and LCD Sr. No
Light emitting diode
Liquid crystal display
1.
An electronic device that lights up when an electricity is passed through it.
Digital display that uses liquid crystal cells that change reflectivity in a applied electric field.
2.
LED or OLED displays does not have any light loss.
Backlit by a light source, hence, there is a little light loss passing the light through the LCD panel.
3.
Requires 10–250 mW power per digit.
Requires 10–200 mW power per digit.
4.
Generates visible light.
Reflects a part of the surrounding light.
5.
Gives high intensity light.
Gives high intensity light.
6.
Operate over wide range of temperatures (303 – 358 K).
Limited range of temperatures (293– 333 K).
7.
Higher lifetime.
8.
Emits different colours.
Limited lifetime due to chemical degradation. Extra illumination required.
9.
Operating voltage ranges from 1.6 to 5 V dc. Operating voltage ranges from 3 to 20 V dc.
10.
Response time is 50–500 ns.
Response time is 50–500 ns.
15.8 APPLICATIONS The following are the applications of display devices, namely, CRT, LED and LCD in various fields.
CRT a. CRT is an important versatile display device used for the analysis of electrical signals and optical display. b. CRTs are used in radar systems, televisions and computer monitors.
404
Materials Science
LED a. b. c. d. e. f. g. h. i.
Traffic lights and signals Exit signs Bicycle lights Railroad crossing signals Flashlights Light bars on emergency vehicles. Thin and lightweight message displays at airports, railway stations, buses, trains, ferries, etc. Remote controls, of TVs, VCRs, DVDs In optical fibre and Free Space Optical (FSO) communications.
LCD In recent years, the applications of LCDs have been endless. Most of the watches and pocket calculators use LCD. A simple example of a liquid crystal display in a digital watch is shown in Fig. 15.16. The display is created in a sandwich liquid crystal which is placed in between two glass sheets, G2 and G3. G2 and G3 glass sheets are not polarised. However the one in front of G2 has grooves etched into it, and electrodes inside those grooves are used to determine charge required for the liquid crystal. The glass sheet G4 is coated with a conducting layer and acts as an electrode. Glassfilm sheets G1 and G5 are with perpendicular polarisation and are placed on either side of these two glass sheets. As a result, the direction of the grooves line up with the direction of their nearest polarising films. The reflective surface glass plate G6 is placed behind the system. This helps to view the light excited by liquid crystal pixel of LCD.
Fig. 15.16 Digital water — LCD display a. Liquid crystal display devices are now preferred to cathode ray tube (CRT) devices as they can offer superior performance in terms of maximum luminance and intensity. b. It can also offer some features like automatic calibration and remote quality assurance.
Key Points to Remember Solids are classified based on energy band structure, arrangements of electrons and forbidden bands like conductors, insulators and semiconductors. In conductors, the valence band is completely filled while the conduction band is half filled. Solid materials which do not conduct electric current under normal conditions are known as insulators. In insulators, the valence band is completely filled and these are no electrons in conduction band. Three different types of semiconductors namely, elemental, compound and oxide semiconductors.
Display Devices
405
Semiconductors are classified into two types namely, pure or intrinsic and doped or extrinsic semiconductors. In intrinsic semiconductors, the carrier concentration of electrons and holes are equal. These semiconductors are highly pure semiconductors. Doping is the process of adding impurity to an intrinsic semiconductor. Doped semiconductors are called extrinsic semiconductors. Extrinsic semiconductors are of two types namely, ntype and ptype. In ntype semiconductors, electrons are majority carriers while in ptype semiconductors, the holes are majority carriers. When a dopant with valency higher than the parent atom is doped, then the resultant semiconductor is known as ntype semiconductors. When a dopant with valency lower than the parent atom is doped, then the resultant semiconductor is known as ptype semiconductors. A solar cell is nothing but a pn junction diode based on the principle of photoelectric effect and it converts light into electrical energy. Characteristics of solar cells are analysed from the VI curve. Efficiency of a solar cell is defined as the ratio of the total power converted by the solar cell to the total power available for energy conversion. The requirements of a solar cell are that band gap energy of semiconducting materials is comparable with the energy of the photon present in the solar spectrum. Different classification of solar cells is pn homojuction, pn heterojunction, Schottky barrier, homojuction heterostrcuture, metalinsulator semiconductor cell and semiconductorinsulatorsemiconductor cell. Active display device is the one which emits radiation on its own. Passive display device is the device which modulates incident radiation to provide necessary display information. The energy of the emitted photon is E = hv. LED is a forwardbiased pn junction. In LED, the emitted light colour depends on the materials used. Alphanumeric characters are displayed employing array LEDs and seven segment LEDs. In LEDs, the energy loss during radiation is reduced employing plastic encapsulation. The colour of light emitted from LED depends on the semiconductor materials used. Large band gap (ª 2 eV) materials are used for LED applications. Lifespan of an LED is more than 1,00,000 hours. Two different types of principles, namely, polarisation and twisted nematic property of liquid crystal are employed for LCD. The process of filtering certain unwanted wavelengths employing glass with parallel thin impenetrable black lines is known as polarisation. In twisted nematic display, the molecules in the liquid crystal are twisted and hence, the incident light entering the liquid crystal comes out as polarised light. Liquid crystals are classified as nematic, cholesteric and smectic liquid crystals. LCD has four different types of modes of display, namely, dynamic scattering, twisted nematic scattering, phase change and memory effects. Dynamic scattering and twisted nematic scattering methods are mostly used for LCD devices. Letter on a dark background are produced in dynamic scattering methods. Black letters on a silver background are produced in field effect type. In twisted nematic LCD, the Ton is directly propositional to viscosity of the liquid medium. LED generates visible light while LCD reflects a part of the surrounding light.
406
Materials Science
Solved Problems Example 15.1 Calculate the wavelength of light emitted by an LED with band gap of energy 1.8 eV. Given Data: Bandgap of given LED is Eg = 1.8 eV = 1.8 ¥ 1.609 ¥ 1019 = 2.8962 ¥ 1019 J Solution:
We know that wavelength emitted from given LED l=
hc Eg
Substituting the values, we get =
6.626 ¥ 1034 ¥ 3 ¥ 108 2.8962 ¥ 1019
= 6.863 ¥ 107 m The wavelength of light emitted from given LED is 0.6863 mm. Example 15.2 ∞
Calculate the bandgap energy of GaAsP semiconductor whose output wavelength is 6715 A . Given Data: The wavelength of green light from mercury lamp = 6715 ¥ 1010 m Solution:
We know that band gap is Eg =
hc l
Substituting the values, we get =
6.626 ¥ 1034 ¥ 3 ¥ 108 = 2.944 ¥ 1019 J 6751 ¥ 1010
= 2.944 ¥ 1019 J or,
=
2.944 ¥ 1019 = 1.8 eV 1.6 ¥ 1019
The band gap of the given GaAsP is 1.8 eV.
ObjectiveType Questions 15.1. _______ device display the information on the screen. 15.2. The device which emits radiation is known as _______. (a) Passive device (b) Active and passive device (c) Active device (d) None of the above
Display Devices
15.3. 15.4. 15.5. 15.6. 15.7. 15.8. 15.9. 15.10. 15.11. 15.12. 15.13. 15.14. 15.15. 15.16. 15.17. 15.18. 15.19. 15.20. 15.21. 15.22. 15.23.
The device which modulates the incident light is known as _______. _______ is the principle behind LED. LED is a _______ biased pn junction. Energy of the emitted photon is _______. The colour of the emitted LED light depends on _______. _______ and _______ LEDs are used to display alphanumeric character. The loss of emitted light energy in LED is due to _______. _______ band gap materials are used to emit visible light. Lower band gap materials are used to emit _______ and _______ light. The wavelength of light emitted by GaAs LED lies between _______ and _______ nm. GaP is a _______ bandgap semiconductor with energy _______. The bandgap energy for GaAs1xPx at x = 0.45 is _______ eV. The nonemissive display device is known as _______ display device. _______ device reflects lights. MBBA shows liquid crystal behaviour in the temperature range from _______ to _______ K. A mixture of 20% cholesterol carbonate and 80% cholesterol nonanoate scatter _______ and _______ colours. Dynamic light scattering is possible at _______ frequency. The twisted molecules in a liquid crystal rotate the plane polarised light through an angle _______ . In dynamic scattering, letters on _______ background is produced. In field effect scattering type, black letters on _______ background are produced. Response time for an LED is from _______ to _______ ns.
Answers 15.1. 15.3. 15.5. 15.7. 15.9. 15.11. 15.13. 15.15. 15.17. 15.19. 15.21. 15.23.
407
Display Passive devices Forward Materials Reflection loss Infrared and far infra red Indirect and 2.26 eV Passive 293 and 320 Low Dark 50 and 500
15.2. 15.4. 15.6. 15.8. 15.10. 15.12. 15.14. 15.16. 15.18. 15.20. 15.22.
c) Electroluminescence hn Array and seven segments Larger 910 and 1020 2.1 LCD Bright yellow and deep violet 90° Silver
Short Questions 15.1. What is meant by display devices? 15.2. Explain the classification of display devices. 15.3. Why do we need a suitable material for LED?
408
Materials Science
15.4. 15.5. 15.6. 15.7. 15.8. 15.9. 15.10. 15.11. 15.12. 15.13. 15.14. 15.15. 15.16. 15.17. 15.18. 15.19. 15.20. 15.21. 15.22. 15.23.
Explain how LED emits light radiations. What is meant by electromagnetic radiation? Why is the shape of the LED made hemispherical? Explain plastic encapsulation. Explain the different types of LED materials along with their radiant colour. What is meant by passive display devices? Mention a some of the properties of passive display devices. What is meant by Liquid Crystal Display? Mention a few applications of LCD. What is meant by liquid crystal state? Explain how LCD illuminates light. What is the range of wavelength emitted by LCD? What is meant by a director? Explain why extra light is required to illuminate LCD. Mention the different types of LCD display. Mention a few applications of LCDs What are the drawbacks of LCD? List some of the applications of display devices in solid state electronics. What is the difference between active and passive display devices? Explain the active display devices.
Descriptive Questions 15.1. 15.2. 15.3. 15.4.
Explain with a neat sketch the basic principle, working and the applications of LED. Explain with a neat sketch the working of LCD along with their salient features. Compare the relative merits of LCD and LED. Write notes on the following: a. LED b. LCD
Chapter
16
PHOTOCONDUCTIVITY
OBJECTIVES To understand the principle, process and the application of photoconductivity. To study the principle and characteristics of photoconductivity. To study the characteristics of photoconductive materials, photoconductors and their application. To study the application of photoconductivity.
16.1 INTRODUCTION Most of the optical detectors used in various solid state devices to detect the visible and infrared radiations are based on the principle of photoconductivity. The optical detectors that are used to produce both voltage and current in an external circuit are known as photodetectors. The materials used for the detectors are semiconductors such as cadmium sulphide (CdS), cadmium selenide (CdSe), indium antimony (InSb), etc. In the following sections, the principle, performance, materials and applications of photoconductivity have been discussed:
16.2 PHOTOCONDUCTIVITY Photoconductivity is the process of increase in the electrical conductivity of a semiconducting material, when a radiation falls on the material. This phenomena is due to the excitation of electrons across the energy gap resulting in the increase of the charge carriers, i.e., electron–hole pairs. Thus, the conductivity of the radiated material increases considerably. Photoconductivity will take place only if the energy of the incident photon (hv) is greater than the energy gap (Eg). If the incident photon energy is less than Eg, the process will not take place (no energy will be absorbed). The permissible energy levels in a semiconductor material are given in Fig. 16.1 using the energy band diagram.
410
Materials Science
Let Eg be the minimum band gap energy in a semiconducting material, then the longest wavelength which may cause this effect is, lg =
hc Eg
(16.1)
where h is the Planck’s constant and c the velocity of light. The electrical conductivity of an insulator or a semiconductor is given by
(
σ = e n µn + pµp
)
(16.2)
where n and p are the electron and hole concentrations and µn and µp are the electron and hole mobilities. Energy Conduction band
Electron Hole
Forbidden region
Band gap energy
Photon
Valance band
Fig. 16.1
Semiconductor material—electron–hole pair
In a homogeneous material, the concentration of hole and electrons are uniform. The absorption of light increases the value of n and p, and hence, photoconductivity increases:
(
Ds = e Dn mn + Dp m p
)
(16.3)
In insulators, the increase of Dn and Dp is very large corresponding to the free carrier density in the dark, whereas in semiconductors, the increase of Dn and Dp is very small compared to the dark carrier density. In a nonhomogeneous material, in which n and p are not uniform, the increase in photoconductivity may be due to the increase in µn and µp . In these materials, there is a barrier which restricts the flow of electric current. The light absorbed by the material reduces the barrier height and hence the current flow will increase. This effect of barrier is described as effective mobility. Therefore, the barrier type photoconductivity can be expressed as,
(
Ds = e n Dm bn + p Dm bp
)
(16.4)
Consider that the light falling on the material produces f electron–hole pair per unit time per unit volume of the photoconductor, then
Dn = f t n and
Dp = f t p
(16.5)
Photoconductivity
411
where, t n and t p are the lifetime of the electrons and holes, respectively. ∆n and ∆p are the additional carriers produced. The expression for conductivity can then be written as,
(
Ds = e f t n mn + f t p m p
)
(16.6)
The photosensitivity of a photoconductor is given by, S=
σph
(16.7)
σd σph = σtotal  σd where σph is the photoconductivity and σd the dark conductivity. For a nonconductive material, the photosensitivity is zero. A parameter known as photoconductive gain G is defined as the ratio of the rate of flow of electrons per second from the device to the rate of generation of electron–hole pairs within the device is given as G=
t c ( me + mh )V L2
(16.8)
where, t c is the lifetime of the carrier, µe and µh are respectively, the mobility of the electrons and holes, V, the applied voltage, and L, the length of the material. It is clear from Eq. (16.8) that the photoconductive gain G is directly proportional to the voltage V and inversely proportional to the square of the length L of the material. In some materials like CdS, the recombination could not take place because of the existence of barriers within the energy gap due to the presence of impurities. These levels are known as traps or sensitisation centers. The existence of traps depends on the illumination level and temperature. For example, at high illumination level and temperature, the traps will increase and hence, the photosignals will be produced. Therefore, low temperature and low illumination levels are good for observing significant effects.
16.2.1 Spectral Response The variation of photoconductivity with photon energy is known as spectral response. The maximum value of photocurrent corresponds to the band gap energy and the spectral response is shown in Fig. 16.2. This energy ranges from 3.7 eV for ZnS to 0.2 eV for cooled PbSe. GaAs Relative response (%)
Ge
0
Fig. 16.2
0.5
1.0 hv
1.5
CdSe
2.0
Spectral response for photoconducting materials
412
Materials Science
16.2.2
Speed of Response
It is the rate of the change in photoconductivity with the change in photo excitation intensity. It is studied by switching off a steady photonexcitation, which is followed by the decay of photocurrents. For the materials which possess exponential decay, the photocurrent reaches the dark current very quickly. In case of other materials which possess nonexponential decay, the decay of photocurrent takes a longer time to reach the dark current. From this study, the lifetime of charge carriers and the presence of traps can be studied. In certain materials, the energy absorbed by the material is not only sufficient to create the electron– hole pairs, but also enough energy is given out to the free electrons for emission. This effect is known as photoemissive effect. The devices that are based on this effect are known as photoemissive tubes, photomultipliers and image intensifiers.
16.3
CHARACTERISTICS OF PHOTOCONDUCTIVE MATERIALS
The choice of photoconductive materials is based on the characteristic features such as wavelength response, operating temperature and detection range. The photoconductive materials such as cadmium sulphide (CdS), cadmium selenide (CdSe), lead sulphide (PbS), indium antimony (InSb), mercury cadmium telluride (HgxCd1–xTe) and doped semiconductors are given in details along with the necessary information. (1) Cadmium Sulphide (CdS) and Cadmium Selenide (CdSe) They are low cost materials and are used as visible radiation sensors because they are highly sensitive (103 to 104). Due to their high sensitivity, the response time is poor, which is about 50 ms. The response time strongly depends on the illumination level, which is much less at higher illumination, indicating the existence of traps. A typical construction of a photodetector is shown in Fig. 16.3. The material in its polycrystalline form is deposited on an insulating surface. The electrodes are formed by evaporating a suitable metal, such as gold, employing a mask to obtain the comblike pattern as shown Fig. 16.3. Thus, having a larger area for sensitive surface and a small interelectrode spacing results in a high sensitivity device.
Evaporated metal electrodes
CdS
Fig. 16.3
Cadmium sulphide photoconductive cell: top view of the electrogeometry
Photoconductivity
413
(2) Lead Sulphide (PdS) These detectors are used to detect near infrared in the wavelength range from 1 to 3.4 mm. The most sensitive region of this material is 2 mm with a typical response time of about 200 ms. (3) Indium Antimony (InSb) These detectors are formed from single crystals with low impedance (~50 W). It can be used up to 7 mm with a response time of 50 ns. It can be operated at room temperature; however, one can have an improved noise performance at low temperatures, such as liquid nitrogen temperature. (4) Mercury Cadmium Telluride (HgxCd1xTe) It is a combination of semi metal HgTe and semiconductor CdTe alloy with a varying band gap of 0–1.4 eV, the band gap of pure CdTe. The sensitivity of these detectors lies in range from 5 to 14 mm. The gain of these detectors is about 500, which can be further increased at low temperature and low illuminations due to the effect of traps. (5) Doped Semiconductors Instead of using a bandtoband transition, one can achieve the transition from the impurity levels within the band gap to the appropriate band edge. Zinc and boron doped germanium detectors are the examples of doped semiconductor detectors. The wavelength response is extended from 20 to 100 mm by cooling to liquid helium (4 K) temperature. The useful range of some commonly used photodetectors are given in Table 16.1.
Table 16.1 Photoconductors Along with their Detection Ranges Material Lead sulphide
Symbol
Detection range (mm)
PbS
0.6–3.0
Indium antimony
InSb
1.0–7.0
Mercurydoped germanium
Ge:Hg
2.0–13
Cadmium mercury telluride
CdHgTe
3.0–15
Copperdoped germanium
Ge:Cu
2.0–2.5
Cadmium sulphide
CdS
0.4–0.8
Cadmium selenide
CdSe
0.5–0.9
16.4 PHOTODETECTORS When an electron–hole pair is generated due to the incident radiation, the pair is separated at the junctions as a result of the existence of electric field. As a result, it generates open circuit voltage or short circuit current. This is the principle applied in the photodiodes to produce both voltage and current in an external circuit. The geometry of the slab of a photoconducting material is shown in Fig. 16.4. Let L, W and D be respectively, the length, width and thickness of the semiconducting material. It consists of two electrodes on opposite faces. The incident radiation falls on the opposite surfaces of the material. The detectors are the terminal devices and are used as lightdependent resistors. The commonly used symbol for a photoconductive detector consists of a resistance symbol with incident arrows representing the radiation, as shown in Fig. 16.5. The detectors are available in the form of photodiodes and phototransistors.
414
Materials Science
Incident radiation
W Electrodes D L
Fig. 16.4
16.5
Photoconducting material: geometry of slab
Fig. 16.5 Photoconductor detector: circuit symbol
PHOTODETECTOR BIAS CIRCUIT
The photodetector (P) is connected in series with a voltage source and a load resistor RL, as shown in Fig. 16.6. When a light radiation is incident on the photodetector, whose energy is greater than Eg, increase in conductivity of the detector takes place. As a result, the flow of current in the circuit leads to an increase in potential across the load resistor RL. The same can be measured using a high impedance voltmeter. A blocking capacitor C is introduced in the output line to remove any dc components while measuring the current in the circuit, due to time variations of the incident light.
P C
Bias voltage RL
Fig. 16.6
Output voltage
Photodetector: bias circuit
The sensitivity and linearity of the detector depends on RL. One can obtain the optimum value of RL by a fractional change in the resistance of the photodetector when it is under illumination. When the change in the fractional resistance is less than 5%, the sensitivity shows a large value at RL = RD, where Rd is the resistance of the photodetector. On the other hand, if the change in the resistance is large, i.e., RL < < RD, which is required for output voltage measurements. Let Io and I be the intensities of the incident and transmitted radiations, respectively, on the semiconductor detector materials. Therefore, the average generation of charge carriers, i.e., electron–hole pairs per unit volume is rg =
η v
(16.9)
where, h is the quantum efficiency of the absorption process, and v, the frequency of radiation (= c/l).
Photoconductivity
415
16.6 PERFORMANCE OF PHOTODETECTOR The performance of different types of detectors are compared by means of certain parameters which are called the figure of merits of the detectors. The most common parameters used are responsivity, noise equivalent power and specific detectivity. (1) Responsivity Responsivity is defined as the ratio of the electrical output to the radiation input. Responsivity =
Electric output Radiation input
(16.10)
(2) Noise equivalent power It is defined as the amount of energy that will give a signal equal to the noise, in a bandwidth of 1 MHz. It can also be written as the ratio of noise per band width to the responsivity, i.e., NEP =
W (∆f
)1 2 (VS
/ VN )
(16.11)
where, W is the radiation power incident on the detector, ∆f , the bandwidth of the amplifier, and Vs and VN are respectively, the signal and noise voltage across the detector terminals. In general, both responsivity and NEP vary with the size and shape of the active element of the detector. (3) Specific detectivity NEP is directly proportional to the square root of the area of the active element. Thus, NEP is related with a quantity known as normalised detectivity D* as, D* =
A1 2 NEP
(16.12)
where, A is the area of the active element of the detector. The dependences of responsivity, noise and detectivity with bias current are shown in Fig. 16.7. It is inferred from the Fig. 16.7 that the noise increases more rapidly than signal at high bias current and leads to a peak value in the signaltonoise ratio. Based on these curves, an optimum value for the detector bias current can be chosen. However, for sensitivity applications, a fine tuning in the bias current is essentially required.
Responsivity Noise Detectivity
Bias current
Fig. 16.7
Dependence of responsivity, noise and detectivity with change in bias current
416
Materials Science
16.7
APPLICATIONS
Following are some of the applications of photoconductivity: a. Photoconductivity detectors in the form of single crystal or polycrystal materials are prepared in the form of Schottky barriers, n–p homojunctions, n–p heterojunctions, n–p–n or p–n–p transistors with gain greater than 1. b. The television camera vidicon and electrophotography are the two applications in the device form. c. It is used to detect a variety of light and particle as a light controlled switch. d. The silver halide coated on the photographic film is also based on photoconductivity.
Key Points to Remember Photodetector is an optical detector used to produce both voltage and current in an external circuit. Photoconductivity is the process of increase in electrical conductivity of a semiconducting material when a radiation falls on the material. σ ph The photosensitivity of a photoconductor is equal to S = , where σ ph is the photoconductivity σd and σd , the dark conductivity. Photoconductive gain is defined as the ratio of the rate of flow of electrons per second from the device to the rate of generation of electronhole pairs within the device. Spectral response is the variation of photoconductivity with photon energy. Speed response is the rate of change in photoconductivity with the change in the photo excitation intensity. Photodetectors absorb the incident light radiation and hence, they generate current or voltage in the open circuit. Resistivity is defined as the ratio of electrical output to the radiation input.
Solved Problems Example 16.1 A cadmium sulphide photodetector crystal is irradiated over a receiving area of 4 × 10–6 m2 by a light of wavelength 0.4 × 10–6 m and intensity 200 W m–2. Assuming that each quantum generates an electron–hole pair, calculate the number of pairs generated per second. Given Data: The wavelength of the light l = 0.4 ×10−6 m The area of the crystal
= 0.4 ×10−6 m2
The intensity of the light
= 200 W m−2
Photoconductivity
Solution:
417
Intensity ¥ area hv 200 ¥ 4 ¥ 106 = hv
The number of photons =
=
200 ¥ 4 ¥ 106 l hc
=
200 ¥ 4 ¥ 106 ¥ 0.4 ¥ 106 6.626 ¥ 1034 ¥ 3 ¥ 108
= 16.098 ¥ 1014 We know that each quantum will generate one electron–hole pair. Therefore, the number of pairs generated per second is 16.098 ¥ 1014. Example 16.2 Determine the wavelength of radiation emitted by a LED made up of GaAs. Given that the band gap energy is 1.43 eV. Given Data: Band gap energy Eg = 1.43 eV = 1.43 × 1.6 × 10–19 J Planck’s constant h = 6.626 × 10–34 Js c = 3 × 108 ms–1 Solution:
The wavelength of radiation emitted lg =
=
hc Eg 6.626 ¥ 1034 ¥ 3 ¥ 108 1.43 ¥ 1.6 ¥ 1019
= 0.87 mm The wavelength of the emitted radiation is 0.87 mm.
ObjectiveType Questions 16.1. The device which is used to produce both voltage and current in an external circuit is known as _________. 16.2. The materials used for optical detectors are _________, _________ and _________. 16.3. The process of increasing the electrical conductivity of material is known as ________ . 16.4. The energy of incident photon is equal to _________. 16.5. The longest wavelength of energy emitted by semiconductor is equal to (a) lg =
2hc Eg
(b) lg =
hc 2 Eg
(c) lg =
hc Eg
(d) lg =
3hc Eg
418
Materials Science
16.6. The electrical conductivity of an insulator is equal to _________.
(
(a) s = e n µ n + p µ p
(
)
(c) s = 3e n µ n + p µ p
( s = 4e ( n µ
) +pµ )
(b) s = 2e n µ n + p µ p
)
(d)
n
p
16.7. The photoconductivity of a photoconductor is equal to σ ph σ ph (a) S = 2 (b) S = 3 σd σd (c) S =
σ ph
(d) S = 4
σd
σ ph σd
16.8. The photoconductive gain of a device is equal to 2Tc (µe  µn )V 2T (µ + µn )V (a) G = (b) G = c e L2 L2 Tc (µe  µn )V T (µ + µn )V (d) G = c e 2 L L2 The variation of photoconductivity with photon energy is known as _________. The rate of change in photoconductivity with the change in photo excitation intensity is known as _________. Examples of photoconductive materials are _________, _________, _________ and _________. Lead sulphide detectors are used to detect the _________ radiations. The average generation of electronhole pair per unit volume is equal to η η (a) rg = 2 (b) rg = V V η η (c) rg = 3 (d) rg = 4 V V (c) G =
16.9. 16.10. 16.11. 16.12. 16.13.
16.14. The resistivity of a detector is equal to Electrical output (a) Radiation input Conductive output (c) Radiation input
Insulating output Radiation input Electrical output (d) Conductive input (b)
16.15. The noise equivalent power of a photo detector is equal to W 2W (a) NEP = (b) NEP = 1 2 1 (∆f ) (VsVn ) (∆f ) 2 (Vs / Vn ) (c) NEP =
W (∆f )1 2 (Vs / Vn )
(d) NEP =
2W (∆f )1 2 (VsVn )
16.16. The specific detection of photo detectors is equal to A1/ 4 A1/ 2 (a) D∗ = (b) D∗ = NEP NEP 3 / 2 A A3/ 4 (c) D∗ = (d) D∗ = NEP NEP
Photoconductivity
419
Answers 16.1. 16.3. 16.5. 16.7. 16.9. 16.11. 16.13. 16.15.
Photo detectors Photoconductivity (c) (c) Spectral response Cds, CdSe, PbS, Insb (b) (c)
16.2. 16.4. 16.6. 16.8. 16.10. 16.12. 16.14. 16.16.
cadmium sulphide cadmium selnide, indium antimony hn (a) (d) Spectral response near infrared (a) (b)
Short Questions 16.1. 16.2. 16.3. 16.4. 16.5. 16.6. 16.7. 16.8. 16.9. 16.10.
What is photoconductivity? Explain why photoconductivity cannot take place when the incident energy is less than Eg. What is the principle applied in a photo diode? Explain photoconductive gain. What are the minimum characteristic features for good photoconductive materials? What is meant by doped semiconductors? Define responsivity. Explain noise equivalent power. Define specific detectivity. Mention some of the applications of optical detectors.
Descriptive Questions 16.1. Explain with a neat sketch the principle of photoconductivity. 16.2. Explain with a neat sketch the working of photodetectors and derive the necessary equation for photoconductive gain. 16.3. Write an essay about the characteristic features of different photoconductive materials. 16.4. Write notes on the following: (a) Performance of a photoconductor, and (b) Applications of optical detectors.
Exercise 16.1. Determine the wavelength of radiation emitted by a LED made up of cadmium selenide with an energy gap Eg = 1.74 eV.
Chapter
17
THERMOGRAPHY
OBJECTIVES To study the principle of thermography. To understand the experimental techniques and instrumentation to obtain the thermal images of an object. To study the different applications of thermography.
17.1
INTRODUCTION
Thermography is one of the most important branches of medical sciences. Generally, materials emit electromagnetic radiations when their temperature is greater than 0 K. According to block body radiation, the emitted radiations are infrared radiations (IR), whose frequency lies in between visible light and radio waves in the electromagnetic spectrum. The emitted radiations are used to obtain infrared images of the material. The obtained images are highly sensitive and informative. The frequency of the emitted IR radiation depends on temperature of the object. The frequency of the commercial thermograms available for the field applications are in the range of 0.75 – 15 µm. One can obtain the image of the object without any damage to the material and hence, it is known as nondestructive method. Further, it will not produce any harmful effect to humans and thus, it is also known as noninvasive method. In addition, thermography is a simple method, cost effective, easy in operating and fast to interpret the observed results. In view of the above salient features, it finds wide applications in industry, medicine and defence. In this chapter, a brief discussion on basic principle, instrumentations used to obtain thermal images and their applications with reference to biomedical and industries are given.
17.2
PRINCIPLE
The principle behind thermography is the emission of energy from the surface of the materials. The material at 0 K does not emit any energy, however, when the temperature of the material exceeds 0 K, it emits infrared
Thermography
421
radiations. The observed infrared radiations are used to obtain the thermal image of the object surface known as thermograms. The infrared images are the visual displays of the amount of infrared energy emitted from the materials. The obtained thermal images are also known as thermograms. Generally, the thermal radiations from the materials depend on the emissivity of the materials, surroundings and atmosphere. The radiation emitted from the object is welldefined by the popularly known four formulae namely, Kirchoff’s, Stephan Boltzmann, Wiens displacement and Planck’s equation. When the material is under equilibrium, according to Kirchoff’s law the coefficient of absorption and emission are equal. Stephan Boltzmann’s law states that any high temperature material emits more infrared radiation (s = T4). At maximum energy, the wavelength of emitted radiation is inversely proportional to temperature (Wien’s displacement law). According to Planck’s equation, it is inferred that the radiation depends on spectral emissivity and temperature. Therefore, the emissivity of materials, its surroundings and atmosphere are more important for a material to obtain its thermal images. The emissivity of the materials depends on the nature of the material and its environment. The environment of the materials is a key factor for the measurements of temperature. Thus, the whole material should be free from any external radiation sources which prevents the influence on increasing radiation temperature. Similarly, the atmosphere surrounding the material is an another important factor to be considered. Any sudden change in the atmosphere may lead to a loss in radiation from the object. One can overcome the radiation losses by introducing high temperature filters to obtain the images. The high temperature filters require correction factor which helps to obtain radiation at ambient temperature and to overcome radiation losses due to attenuation of the filters. Emissivity is the density of the material to emit thermal radiation. Emissivity of the material depends on the nature of the material. The theoretical emissivity of the materials ranges between 0 and 1. Generally, the thermal image or thermogram of the material is displayed in the CRT screen as light, dark and hot spots. The warm areas of the material appear as light in the screen, while the cool areas appear as dark. However, the intermediate temperature of the material appears as grey on the thermogram. On the other hand, in case of the medical field local disorders like burns, infection and tumors lead to a hot spot on the thermogram. The image is obtained due to the increased object surface area temperature of the material due to the increase in blood supply.
17.3 CLASSIFICATION OF THERMOGRAPHY Thermography is classified into two categories namely, active and passive thermography. In active thermography, the thermal image of the material is obtained using an energy source. The energy source is used to obtain the thermal contrast between the feature of interest and the background of the material. Active thermography is used to obtain the image of the object under thermal equilibrium. In passive thermography, the images of the object are obtained without any energy source by keeping the material either at lower or higher temperature than the background temperature. Passive thermography is generally used to obtain the surveillance of people.
17.4 EXPERIMENTAL TECHNIQUES One can obtain the thermograms of an object by means of two ways namely, contact and noncontact methods. In contact system, the surface systems are simple to operate and cost effective and give better
422
Materials Science
resolution. However, the noncontact systems like telecamera systems are integrated and require skill to operate. The noncontact system finds wide applications in industry and medicine. The block diagram of a simple noncontact thermographic system used in medicine is shown in Fig. 17.1. Infrared scanner
Control console
B &W/Colour monitor
Personal computer
Video thermal recorder
Colour printer
Fig. 17.1 Block diagram of the noncontact thermographic system The important components of noncontact systems are infrared detectors, optical systems, computer and scanning mechanism. It also includes additional accessories for recording, storing and processing of the observed images. As we discussed earlier, one can obtain the thermograms of an object either through active or passive technique. The surface profile of the object can be obtained by measuring the movements and redistribution of the temperature profile during the active technique. However, the passive technique gives only the natural distribution of radiation on the surface of the object. The applications of contact systems are very limited. The most important component of thermography system is detector and camera.
17.4.1
Detector
Generally, photoconductor is used to detect the infrared radiations. The photo detector is made up of indium antimony alloy (InSb). When a light radiation is incident on the crystal, the resistance of the crystal changes depending on the intensity of incident light. Using the conventional electrical circuits, the variations in resistance is converted into voltage variations. The observed voltage variations are further amplified and displayed properly. The intensity of the infrared radiations observed from the surface is very low. Therefore, a disturbance in the amplified voltage is observed during the amplification. One can reduce the thermal noises by cooling the detectors employing liquid nitrogen. Therefore, liquid nitrogen cooled detectors are used to obtain the thermal noise reduced infrared radiations. The amplified voltage is used to explore the surface nature of the object. Thus, detectors with good sensitivity and stability are required to obtain thermal images of object. The sensitivity of InSb, PbxSn1x and SnHg1xCdx detectors at liquid nitrogen temperature (77K) ranges respectively from 3 – 6 µm, 8 – 13 µm and 7 – 13 µm. Pyroelectric (BaTiO3) detectors are used to obtain high sensitivity and stability at room temperature without liquid nitrogen.
Thermography
423
17.4.2 Camera In medicine, thermograms are obtained using the noncontact systems employing thermographic camera. A simple experimental setup used to obtain the thermal image is shown in Fig.17.2. It consists of camera, beam chopper, optical systems and accessories for processing, storing and displaying the thermal images on the screen. The thermographic camera is fixed just above the object table. The infrared radiations from the surface of the object skin are received by the plane image scanning mirror. The received radiations are focused into the small infrared detector through the beam chopper. The light energy (infrared signal) received by the detector is converted into electrical signal by the detector. The incident radiation is chopped through the polishing rotating table to provide a reference temperature similar to that of the skin and also to compensate the electronic drift during the conversion. Thus, one can use the detectors to view the image of the skin and detector in an alternative display. Vacuum flask
Liquid nitrogen Infrared detector Amplifer Object
Beam chopper Synchroniser
Display
Plane image scanning mirror
Concave focusing mirror
Fig. 17.2 Thermographic camera The converted electrical signal is amplified by the amplifier. The amplified signal is passed into CRT to display the image. The image displayed on the screen consists of different intensities of light like bright, dark and light spots. Thus, the obtained intensity distribution of light gives the profile of the temperature of infrared radiation emitted from the surface of the skin. The different steps to be carried out to obtain the image of the object are as follows: As a first step a small strip is scanned by oscillating the image scanning mirror. Then, the angle of the scanning mirror is changed and hence, the scanned strip of the object is scanned. During the end of the scanning, the image of each strip is transformed into CRT in synchronisation with the movement of the mirror. Thus, the display of spot on CRT is exactly the same as that of the spot scanned on the surface of the skin. The above procedure is repeated both in horizontal and vertical mode in order to scan the whole surface. The corresponding
424
Materials Science
images are displayed on the CRT. The CRT gives the thermal image of the skin, i.e., the temperature distribution of the surface of the skin. The modern instruments can scan about 500–600 strips within two seconds. The resolution of temperature profile obtained on the skin is more than ±273.07K. Germanium and silicon focusing len elements are used to avoid the short wave length radiations emitted from the human body. One can increase the speed, accuracy and reliability of the above equipment by keeping under controlled condition.
17.5
NONCAMERA DETECTORS
One can detect the defects in the surface of the material without using camera, known as noncamera detector. In noncamera detector method, the change in the colour of the chloestric liquid is used to explore the surface profile of the object. The chloestric liquid, which is a chemical compound coated on the surface of the object. Firstly, a thin layer of black point is coated on the material surface. Secondly, the chloestric liquid is coated on the surface of the material using a spray technique. Any change in temperature on the surface of the object leads to a corresponding change in the colour of the chloestric liquid. The chloestric liquid covers the whole range of colours from red to violet in the temperature range of 277 to 310 K. The observed colour changes can be received by taking photographs. Thus, the photographs are used to identify the defects in the material.
17.6
ADVANTAGES AND LIMITATIONS OF THERMOGRAPHY
Even though, thermography is a very simple, nondestructive and noninvasive method, it has its own advantages and limitations when compared with other studies. The following are the advantages and limitations of the thermography:
Advantages a. It gives a visual image of the material and hence, one can compare with other related techniques. b. It is possible to obtain the online images of moving targets and hence, online assessment of the problem is very easy. c. It is possible to explore the premature failure of the components. d. It is possible to obtain the image areas of inaccessible or hazardous region which are not possible by other techniques. e. It is a noninvasive test method. f. It is more comfortable and easy operation technique. g. It is used to find defects in shafts, pipes and other metal or plastic components and hence, used to extend the components life. h. It gives high resolution and reproducible images.
Limitations a. The cost of camera used for recording the thermal images is expensive. b. Accurate interpretation of the images is very difficult due to erratic temperature of the materials. In active thermal imaging, this problem is resolved.
Thermography
425
c. The accuracy of the thermal images depends on the emissivity and the reflectivity of the surface of the material. d. The maximum accuracy of the camera is ±2%. e. It affects the temperature of the surface directly.
17.7 APPLICATIONS Thermography finds wide applications both in industry and medicine. The applications of thermography in the field of industry and medicine are highlighted in the following headings: a. Petroleum industry Thermography is used to explore the corrosion in oil tank shell as well as its oil level. It is used to maintain plant equipment like reaction towers, refining furnaces and ducts. b. Condition monitoring Thermography is an ideal technique for condition monitoring components like furnace tubes, gas and fluid transfer lines. Thus, the structural resistance help to improve the life of the components. c. Electrical power systems The thermographic study on electrical systems like core insulation, slip ring temperature, etc. of the turbo generator helps to explore the defects. d. Transmission lines The important application of thermography is the inspection of transmission lines, substations and distribution systems. e. Mechanical systems It is used as a nondestructive testing tool to extend the life of the component during the working conditions. The components used for testing are pipeline, heat ventilation, air conditioning equipment evaluation, mechanical bearing inspection, power plant, etc. f. Detection of tumors One can explore breast and thyroid tumors by comparing the thermal images of breast and thyroid. Generally, more bloods are drawn into the tissues due to the growth of tumors than the surrounding tissues. The extra blood flowing through the tissues results in a hot spot in the thermograph while the normal blood flowing tissues show a light area. The obtained light spots in comparison with hot spot helps to identify the tumor affected area in the tissues. g. Mapping of blood vessels One can easily monitor the blood vessels using thermogram. We know that blood vessels are the key tool in locating the constrictions or abnormal dilations. Further, it is also used to monitor the conditions of blood vessel during the influence of drugs or diet. In order to explore the constrictions or abnormal dilation, one has to first cool the skin of the body below the normal low temperature. The thermogram of the skin is taken and then the cooling is removed. Thermogram shows light spot which indicates a rise in the temperature of blood vessels. The observed increase in the temperature of blood vessels is due to fast heating of blood vessels than the surrounding tissues. One can explore the effects of drugs or diet on the blood vessels using the above procedure. h. Investigation of bone fracture Thermogram is one of the best methods to obtain information about the hairline fracture on bone which are not detectable using the conventional Xray technique. The existence of hairline fracture on the bone may cause the surrounding tissues and muscles, and hence leads to irritations. The irritated part of the surrounding tissues and muscles leads to a hot spot on thermogram. The obtained hot spot helps to identify the hairline fracture on the bone. i. Placental localisation Thermography is one of the best tools to locate the placenta during the pregnancy. During the mapping of placenta, the mother and child are completely safe guarded. Whenever the increase in placenta, there is an increase in blood flow which results an increase temperature. This in turn, increases the temperature of the mapped thermogram. Thus, by monitoring the variations in the temperature of thermal images, one can map the movement of placenta.
Materials Science
426
j. Burns and frostbite Thermography is used to explore the depth of tissue destructions by mapping the temperature variation in the images. For example, in case of burns, there are two stages in the temperature of the blood flow. A high temperature blood flow is observed due to the reactive hyperaemia during the first degree burns. On the other hand, a low temperature blood flow is observed due to the second degree burns. Therefore, one can detect the depth of burns by measuring the changes in temperature.
Key Points to Remember Materials emit infrared radiations when the temperature is greater than 0 K. Thermograms or thermography is the thermal image of the object obtained from the emitted infrared radiations from the object surface. Thermal radiations depend on emissivity, surroundings and atmosphere of the material. Kirchoff’s law, Boltzmann law, Wien’s displacement law and Planck’s equation are used to explain the radiation emitted from the surface of the material. Thermography is classified into two types namely, active and passive. In active thermography, the images are obtained using an energy source. In passive thermography, the images are obtained without any energy source. Thermograms are obtained both by contact and noncontact mode of operations. Photo detectors are used to convert the incident infrared radiation into electrical signals. In photo detector, the resistance of the crystal changes depending on the intensity of incident light. Liquid nitrogen cooled detectors are used to obtain thermal noise reduced infrared radiations. In noncontact systems, thermographic camera is used to obtain images. Tissue destructions are mapped by measuring the variation in the temperature of thermal images. Hair line fractures in bones are obtained using thermograms. Thermography is a nondestructive technique. Thermography is a noninvasive technique. Thermography is used to detect the defects in industrial components. The limitation of thermography is the cost and accuracy of the camera.
Fill in the Blanks 17.1. 17.2. 17.3. 17.4. 17.5. 17.6.
When the temperature is greater than 0 K, the material emits infrared radiation (Yes/No). Thermal images are obtained from the emitted _________ from the object surface. The two different types of thermography are _______ and ________. An energy source is used in _________ thermography. In passive thermography, __________ sources are not used. __________ is used to convert infrared radiation into electric signal.
Thermography
427
17.7. The principle behind the photo detector is _________. (a) Change in resistivity with intensity of the incident light (b) Change in resistivity with frequency of the incident light (c) Both (a) and (b) (d) None of the above. 17.8. In medical application, thermography is used as a _________ method. 17.9. In industry, thermography is used as ____________. 17.10. The frequency of the commercial thermograms available for the field applications are in the range of ______ to ________. 17.11. According to Kirchhoff’s law, the coefficient of absorption and emission are equal. (Yes/No) 17.12. The sensitivity of InSb detectors at liquid nitrogen temperature (77 K) ranges from _______ to ________. 17.13. The sensitivity of PbxSn1x detector at liquid nitrogen temperature (77 K) ranges from _______ to ________. 17.14. The sensitivity of SnHg1xCdx detector at liquid nitrogen temperature (77 K) ranges from _______ to ________. 17.15. ____________ detector is used to obtain high sensitivity and stability at room temperature without liquid nitrogen. 17.16. The photo detector is made up of ___________ alloy. 17.17. __________ detector is used to detect the defects in the crystal. 17.18. The maximum accuracy of the thermography camera is _______. Answers 17.1. 17.4. 17.7. 17.10. 17.13. 17.16.
Yes Active (a) 0.75 to 15 µm 8 – 13 µm Indium antimony alloy (InSb)
17.2. 17.5. 17.8. 17.11. 17.14. 17.17.
Infrared Energy Noninvasive method Yes 7 – 13 µm. Noncamera
Short Questions 17.1. 17.2. 17.3. 17.4. 17.5. 17.6. 17.7. 17.8. 17.9.
What is thermography? What is the principle behind thermography? What are the classifications of thermography? Mention the materials used in infrared detectors. Explain constant telesystem. Define active thermography. Explain passive thermography. What is the difference between active and passive thermography? How is the light radiation converted into electrical signal?
17.3. 17.6. 17.9. 17.12. 17.15. 17.18.
Active and passive Photo detector Nondestructive method 3 – 6 µm Pyroelectric (BaTiO3) 2%
428
Materials Science
17.10. What is meant by chopping? 17.11. What are the applications of thermography in industry? 17.12. Mention any four applications of thermography in medical field.
Descriptive Questions 17.1. Explain with block diagram the noncontact telesystem thermography along with industrial applications. 17.2. Explain with neat sketch the working of thermography camera and explain how is the mapping of the defects in the surface of the object made. 17.3. Write an essay on the thermography principle, working and applications both in industry and medicine.
Chapter
18
DIELECTRIC MATERIALS
OBJECTIVES To explain the dielectric nature of the material with necessary definitions. To discuss the different types of polarisation according to its dipoles. To derive the local field of dielectric materials. To discuss the various types of dielectric materials and their applications. To derive the Claussius–Mosotti equation for dielectric materials and discuss its importance. To discuss the dielectric loss and explain the various factors to destroy dielectric properties. To discuss the change in the polarisation of selected dielectric materials as a function of applied temperature and applied frequency. To discuss the active and passive dielectric materials. To find some applications of dielectric materials.
18.1 INTRODUCTION All dielectric materials are insulators. The distinction between a dielectric material and an insulator lies in the application to which one is employed. Insulating materials are used to resist the flow of current through it when a difference of potential is applied across its ends. On the other hand, dielectric materials are used to store electrical energy. A dielectric material is one which stores electrical energy with a minimum dissipation of power, since the electrons are bound to their parent molecules and hence, there is no free charge. Let us consider some important terms related to this section.
430
Materials Science
18.2
DEFINITIONS
(1) Electric Field Intensity or Electric Field Strength Consider a point charge dq in the region of an electric field. Let F be the force acting on the point charge dq. The force per unit test charge dq is known as electric field strength (E), given by E=
F Q = dq 4p e r 2
(18.1)
From Coulomb’s law, when two point charges Q1 and Q2 are separated by a distance r, the force of attraction or repulsion between the two charges is F=
Q1Q2 nˆ 4p e r 2
(18.2)
where e is the permitivity or dielectric constant of the medium in which the charge is placed. For vacuum, e = e0 = 8.854 ¥ 10–12 F m–1. (2) Electric Flux Density or Electric Displacement Vector The electric flux density or electric displacement vector D is the number of flux lines crossing a surface normal to the lines, divided by the surface area. The electric flux density at a distance r from the point charge Q can be written as, D=
Q 4p r 2
(18.3)
where, 4pr2 is the surface area of a sphere of radius r. From Eqs. (18.1) and (18.2), we get D = eE = e0E + P
(18.4)
where P is the polarisation and it has the same unit as D, i.e., coulomb per square metre (Cm–2). (3) Dielectric Parameters The dielectric parameters are as follows. a. Dielectric constant (er) b. Electric dipole moment (m) c. Polarisation (P), and d. Polarisability (a). a. Dielectric Constant: The dielectric constant (er) of a material is defined as the ratio of the permitivity of the medium (e) to the permitivity of free space (e0), er =
e e0
(18.5)
where er is the dielectric constant, which is a dimensionless quantity. The measure of dielectric constant or relative permitivity gives the properties of a dielectric material. The dielectric constant of air is one. b. Electric Dipole Moment: Consider two charges of equal magnitudes but of opposite polarities separated by a distance r, as shown in Fig. 18.1.
Dielectric Materials
431
Electric dipole
Fig. 18.1
The arrangement of two equal and opposite charges + Q and – Q, separated by a distance r is known as electric dipole. The product of magnitude of the charge and the distance of separation is known as electric dipole moment (m). m = charge ¥ distance = Qr
(18.6)
where m is the dipole moment and its unit is coulomb metre (Cm). Since the dipole moment is a vector, it points from the negative to the positive charges as shown in Fig. 18.1. The total dipole moment of a system constituting of point charges Q1, Q2, Q3, ..,Qn and the distances of separation r1, r2,.., rn is n
mtotal =
ÂQ
i
ri
(18.7)
i =1
c. Polarisation: When an electric field is applied to a solid material consisting of positive and negative charges, the positive charges are displaced opposite to the direction of the field, while the negative charges are displaced in the direction of the field. The displacement of these two charges create a local dipole in the solid. This type of displacement of positive and negative charges by the application of electric field leads to polarisation. P=
m volume
(18.8)
where, P is the polarisation in Cm–2. The term, ‘polarisation’ is defined as the induced dipole moment per unit volume. d. Polarisability: When a dielectric material is placed in an electric field, the displacement of electric charges gives rise to the creation of dipole in the material. The polarisation P of an elementary particle is directly proportional to the electric field strength E i.e.,
PµE P=aE
(18.9)
where a is a proportionality constant known as polarisability. The unit of a is F m2. If the solid material contains N number of particles per unit volume, then the polarisation can be written as, P=NaE
(18.10)
where a = ae + ai + a0. Here ae, ai and a0 are the electronic, ionic and orientation polarisability, respectively. In the following sections, the above three polarisations are discussed in detail.
432
Materials Science
18.3
DIFFERENT TYPES OF POLARISATIONS
The application of an electric field to a dielectric material creates or realigns the dipoles resulting in polarisation. There are four different types of polarisations. They are listed below. (1) Electronic or induced polarisation (Pe) (2) Atomic or ionic polarisation (Pi) (3) Orientation polarisation (P0), and (4) Interfacial or space charge polarisation
18.3.1
Electronic or Induced Polarisation
A dielectric material consists of a large number of atoms. Let us consider a dielectric material consisting of only one atom, as shown in Fig. 18.2(a). The nucleus is at its centre while the electrons are revolving around the nucleus. When an electric field is applied to this atom, the nucleus moves away from the field while the electrons move towards the field. Therefore, there is a displacement between the nucleus and the electrons. This displacement produces an induced dipole moment, and hence, polarisation. The polarisation produced due to the displacement of electrons is known as electronic polarisation.
e
Ze
Ze
R
x
(a)
Fig. 18.2
(b)
Electronic polarisation
Let Z and R be the atomic number and radius of an atom, respectively. Similarly, let e be the charge of an electron. If E is the electric field intensity applied to the atom, then the force acquired by the nucleus is ZeE. Due to the application of the electric field, there is a displacement x of the nucleus from its position. If a sphere is drawn by taking x as the radius, then the entire portion of the atom is splitted into two. From Gauss’s theorem it can be proved that the electron cloud present outside the small sphere of radius x has no impact on the nucleus. Therefore, the nucleus exerts force only due to the electron cloud present in the inner portion of the sphere of radius x. Let the nucleus be present at the centre of the sphere of radius x and the electron clouds are present throughout this sphere. 4 3 px The charge inside the sphere = 3 Ze 4 p R3 3 ﬁ
=
x3 Ze R3
(18.11)
Dielectric Materials
433
The Coulomb force acting between the nucleus and the electron clouds inside the sphere of radius x is given by, Ê  x3 ˆ Z e Á 3 Z e˜ Ë R ¯ F= 4p e 0 x 2
(18.12)
At equilibrium, the nucleus is balanced and hence, the total force on the nucleus is zero. Therefore, Ê x3 ˆ Z e Á 3 Z e˜ ËR ¯ ZeE = 2 4p e 0 x Simplifying the above equation, we get x=
4p e 0 R 3 E Ze
(18.13)
The induced dipole moment is given by mind = Ze x Substituting the value of x from Eq. (18.13) in the above equation, we get mind = 4p e0 R3E mind = ae E
or,
where, ae is the electronic polarisability and is equal to ae = 4p e0 R3 It is clear from Eq. (18.14) that the electronic polarisability is directly proportional to Eq. (18.14), the electronic polarisation can be written as Pe = N ae E
(18.14) R 3.
From
(18.15)
Substituting the value of ae from Eq. (18.14) in the above equation, we get Pe = N 4p e0 R3 E i.e., e0(er – 1) E = 4 N p e0 R3 E er – 1 = 4 N p R3
(18.16)
where er is the dielectric constant of the material. The dielectric constant of Al at 1 atmospheric pressure is found to be 1.0000192129 and the number of dipoles per unit volume present is 2.7 ¥ 1025 atoms m–3. The value of R obtained from Eq. (18.16) is 0.384 Å, which is of the order of the radius of an atom. The displacement of electrons and nucleus due to the application of electric field is a crude assumption which is not accepted by the atomic model. Anyhow, the results obtained by using this assumption give the correct values of the atomic parameters. Therefore, even though it is a crude model, it cannot be neglected.
434
Materials Science
18.3.2
Atomic or Ionic Polarisation
When an electric field is applied to an ionic crystal, the polarisation that arises due to the displacement of the positive ions away from the field and the displacement of the negative ions towards the field is known as atomic or ionic polarisation. This type of polarisation is produced in ionic molecules such as NaCl, KBr, KCl and LiBr. Consider the arrangement of ionic molecules as shown in Fig. 18.3. In the absence of electric field, there is no displacement of ions. When an electric field is applied, there is a displacement of the positive and negative ions which produces an induced dipole moment mi. This induced dipole moment in turn produces an induced polarisation. The induced average ionic polarisation produced per ionic dipole is given by Pi = ai Ei No field
With field x2
x1
Fig. 18.3
Ionic polarisation
The polarisation produced for a crystal having N number of dipoles per unit volume is given by, Pi = N ai Ei
(18.17)
Let x1 and x2 be the displacements of the positive and negative ions, produced due to the application of an electric field. The dipole moment induced is given by, mi = e (x1 + x2) Let F be the force experienced by the ions due to the application of the electric field. The restoring force acting on the ions is directly proportional to their displacements. i.e.,
F µ x1 µ x2 = b1 x1 = b2 x2
(18.18)
where, b1 and b2 are the proportionality constants and they are directly proportional to the mass and angular frequency of the respective ions. i.e.,
b1 µ m and
b2 µ M
µ w02 From Eq. (18.18), the force experienced by the positive and negative ions is given by, F = eE = mw02 x1 = Mw02 x2
Dielectric Materials
x1 =
Therefore,
eE mw 02
and
x2 =
435
eE Mw 02
Substituting the values of x1 and x2, the induced dipole moment can be written as, mi =
e2 w 02
ai =
The ionic polarisability
1˘ È1 Ím + M ˙ E Î ˚
e2 Ê 1 1ˆ + ˜ 2 Á Ë w0 M m ¯
(18.19) (18.20)
Using Clausius–Mosotti equation, the dielectric constant for an ionic crystal can be written as er  1 Na i = 3e 0 er + 2
(18.21)
In addition to ionic polarisation, an ionic molecule also possesses electronic polarisation due to the displacement of electron clouds. The electronic polarisation of an ionic molecule will be in the order of 1/10th of ionic polarisation. Hence, its magnitude is much smaller than the ionic polarisation.
18.3.3 Dipolar or Orientation Polarisation The dipolar or orientation polarisation is produced only in case of polar molecules such as H2O, HCl and nitrobenzene. When an electric field is applied to a polar molecule, the dipoles experience a torque and try to align parallel to the applied field, which results in a rotation of the dipoles. The mechanism of dipolar polarisation is shown in Fig. 18.4.
Cl
–
+
H
(a) the dipole in a HCl molecule
+Q
(b) the random orientation of dipoles in the absence of electric field
F = QE E
F
–Q
(c) the rotation of a dipole due to the applied electric field
Fig. 18.4
(d) the dipoles try to align parallel to the applied field
Dipolar polarisation
Consider a polar molecule is subjected to an electric field of strength E. Let q be the angle of rotation of the dipoles. Then the torque produced by the field on the dipole is t = mp E sin q where mp is the permanent dipole moment.
(18.22)
436
Materials Science
The maximum work is done when the dipole is rotated through an angle of q = 180°. When the dipole is already parallel to the applied field, i.e., when q = 0°, the work done is minimum. Therefore, the maximum energy is given by Emax =
Ú
p 0
m p E sin q dq
= 2mp E
(18.23)
The average dipole energy Edip Edip = mp E
(18.24)
The ratio of the average dipole energy to average thermal energy is, given by mpE Average dipole energy = 5 Average thermal energy kT 2
(18.25)
If this ratio is greater than unity, then the orientation polarisation is said to be effective. The average orientation polarisation is Po µ or,
Permanent dipole moment ¥ Average dipole energy Average thermal energy
Po µ mp
mpE 5 kT 2
(18.26)
If the calculation for average dipole energy is properly done using Boltzmann's statistics, then the average orientation polarisation is Po =
2 1 mp E 3 kT
(18.27)
Therefore, the orientation polarisability can be written as, ae =
m 2p 3kT
(18.28)
It is clear from Eq. (18.28) that the orientation polarisation is temperature dependent.
18.3.4 Interfacial or Space Charge Polarisation Consider a dielectric medium is placed between any two electrodes, as shown in Fig. 18.5. When no field is applied to the electrode, the positive and negative charges are not separated and there are fixed number of charges. On the other hand, when an electric field is applied, the charges are separated. The positive charges are accumulated near the negative electrode. Therefore, a dipole moment is induced due to displacement of the ions. Then, the induced dipole moment per unit volume gives the induced polarisation. This polarisation is known as interfacial polarisation.
Dielectric Materials
Electrodes
Electrodes
+
+
+
– –
+
– –
– –
+
–
+ +
+
437
+ + + + + +
E (a) absence of an electric field
Fig. 18.5
(b) presence of an electric field
Spacecharge polarisation
18.3.5 Total Polarisation In the calculation of total polarisation, the space charge polarisation is not taken into account, since it occurs at interfaces and it is very small and hence negligible. In addition to this, the fields are not well defined at interfaces. Therefore, the total polarisation is the sum of the electronic, ionic and orientation polarisation. Therefore, total polarisation is given by P = Pe + Pi + Po
(18.29)
Substituting the values of Pe, Pi and Po, respectively from Eqs. (18.15), (18.18) and (18.27) in Eq. (18.29), we get P = N aeEi + N ai Ei + N ao Ei
(18.30)
Substituting the values of ae, ai and ao, respectively from Eqs. (18.14), (18.20) and (18.28) in Eq. (18.30), we get Ê m p2 ˆ e2 Ê 1 1ˆ 3 + ˜+ P = N Ei Á 4p e 0 R + 2 ÁË ˜ w 0 M m ¯ 3kT ¯ Ë
(18.31)
1 , a straight line is obtained, as shown in Fig. 18.6. The T 1 straight line makes an intercept at the yaxis, when = 0. The value of the temperatureindependent T 1 portion in the plot is NEi(ae + ai). Therefore, by drawing a plot between P and , one can determine T the orientation polarisation and the sum of electronic and ionic polarisation. When a plot is drawn between P and
Slope
P
N mp2
3k
N( ae + ai) 1/T
Fig. 18.6
Plot of P versus 1/T
438
Materials Science
18.4
LOCAL OR INTERNAL FIELD
In a dielectric material, the field acting at the location of an atom is known as local or internal field Ei. The internal field seen by an atom is not equal to the externally applied electric field E. The internal field Ei must be equal to the sum of applied field plus the field produced at the location of the atom by the dipoles of all other atoms. Ei = E + the field due to all other dipoles
(18.32)
Calculations of Internal Field for Solid Dielectrics To calculate the internal field seen by an atom in a solid dielectric, let us consider a simple example which consists of an array of atoms represented as A, B1, B2, C1, C2, etc. They are atoms equidistant from A, arranged in the form of a string, as shown in Fig. 18.7. Let a be the polarisability of these atoms. C1
B1
A
B2
C2 .. ...
mind a E
Local field
Fig. 18.7
From the symmetry of the system, it is clear that the internal field Ei acting on the site of atom A will be parallel to the applied field E, and will be same in all other atoms B1, B2, C1, C2, etc. The induced dipole moment on each atom of the string mind = a Ei
(18.33)
where, Ei is the local field acting at the atom A due to the external field E and the field by the dipoles on atoms B1, B2, C1, C2, etc. Ei = E + the field due to all other dipoles at the atom A.
(18.34)
Consider the point dipole on atom B1, whose dipole moment is m. According to the field theory, the potential around a point dipole in vacuum is V(r, q) =
1 m cos q 4pe 0 r2
(18.35)
where, r is the distance from the dipole to the point charge and q, the angle between r and m, as shown in Fig. 18.8. The field around the dipole has two components, one due to r and the other due to q. The r component field Er =
∂V ∂r
Er =
1 m cos q 2pe 0 r3
(18.36)
Dielectric Materials
439
The q component field Eq. = –
1 ∂V ¥ r ∂q
sin q m ¥ r3 4pe0
=
(18.37)
Eq
Er P
q m
Fig. 18.8
Potential at a point P due to a dipole
[The negative gradient of potential is due to the electric field at A]. The field produced by B1 atom at the location of the atom A can be obtained by taking r = a and q = 0 in Eqs. (18.36) and (18.37), since the point dipoles lie on the axis of the dipole. The field acting on the atom A by the atom B1 = Er + Eq
(18.38)
Substituting the values of Er and Eq. in the above equations, we get =
mind +0 2p e 0 a 3
=
mind 2p e 0 a 3
where m = mind, since the dipole is an induced one. The field produced at A by dipole on B1 is equal to that produced by B2. The atoms are separated by a distance a. Therefore, the internal field at A Ei = E + 2 ¥ =E+2¥ =E+ where
mind mind +2¥ + ... 3 2p e 0 a 2p e 0 (2a )3 mind 2p e 0 a 3
1 1 È ˘ Í1 + 23 + 33 + ...˙ Î ˚
mind 1 ¥Â 3 3 p e0 a n
n = 1, 2, 3, etc.
(18.39)
440
Materials Science
We know from Riceman's zeta function be written as
Â
1 = 1.2. Alternately, these values in Eq. (18.39) can n3
Ei = E +
1.2 mind p e 0 a3
(18.40)
From Eq. (18.40), it is clear that the internal field is greater than the external field for the model chosen, suggesting that the dipoles cooperate with each other. The cooperation becomes stronger as the polarisability of the atom increases and the distance between them decreases. The internal field Ei in a threedimensional case is very complicated and depends upon the crystal structures as defined by Ei = E +
gP e0
(18.41)
where, P is the dipole moment per unit volume (polarisation) and g proportionality constant known as internal field constant. When the atoms in a solid are surrounded cubically by other atoms, the value of 1.2 g= ª 1/3. p Equation (18.41) can be written as, Ei = E +
P 3e 0
(18.42)
This field is known as Lorentz internal field. It is clear from the expression of Lorentz field that the internal field of the atoms is larger than the applied field by an amount directly proportional to the induced dipole moment.
18.5
TYPES OF DIELECTRIC MATERIALS
The dielectric materials are classified into three types as given below. (1) Solid dielectric (2) Liquid dielectric, and (3) Geseous dielectric
18.5.1 There (1) (2) (3)
Solid Dielectric
are three types of solid dielectric materials. They are Elemental solid dielectrics Ionic nonpolar solid dielectrics Polar solid dielectrics
(1) Elemental Solid Dielectrics Solid materials consisting of single type of atoms, such as diamond, sulphur, germanium, etc., are said to be elemental solid dielectric materials. These materials exhibit electronic polarisability only.
Dielectric Materials
441
(2) Ionic Nonpolar Solid Dielectrics In ionic crystals such as alkali halides, the total polarisation is ionic and electronic in nature. These solids contain more than one type of atoms, but no permanent dipoles. These types of dielectric materials are said to be ionic nonpolar dielectric materials. (3) Polar Solid Dielectrics In solids, whose molecules possess permanent dipole moments, the total polarisation has all the three components, i.e., it is the sum of electronic, ionic and orientation polarisations. These types of materials are known as polar solid dielectric, e.g., solid C6H5NO2.
18.5.2 Liquid Dielectric Materials Liquid dielectric materials are also classified into three types as given below. (1) Mineral insulating oils (2) Synthetic insulating oils, and (3) Miscellaneous insulating oils (1) Mineral Insulating Oils Transformer oil, capacitor oil and cable oil are said to be mineral insulating oils. They are directly obtained from crude petroleum by distillation. They are used as coolant in transformers and capacitors. (2) Synthetic Insulating Oils Synthetic insulating oils are also used for the purpose of cooling in hightension transformers. Compared to mineral insulating oils, synthetic oils are inferior. Also, they are very cheap, e.g., karels, sovol, etc. (3) Miscellaneous Insulating Oils Silicone liquid and vegetable oil are said to be miscellaneous insulating oils. The silicone liquid is costly compared to synthetic insulating oils. It is used in high tension transformers.
Applications Petroleum oils are used for electrical insulation. Nowadays, mineral insulating oils are being replaced by synthetic hydrocarbon oils. Polychlorinated biphenyls (askarels) are widely used, where noninflammable insulation is required for transformers and capacitors. But, due to environmental pollution, askarels are being withdrawn and silicone liquids are being used for noninflammable insulation in transformers and capacitors. Castor oil is used as an insulating liquid in the developing countries. Some of the uses of liquid dielectrics are given as follows. a. As a filling and cooling medium in transformers and other electronic equipment. b. As a filling medium in capacitors and bushing, etc. c. As an insulating and arcquenching medium in switch gears. d. As an impregnate of absorbent insulation, e.g., paper, press board and porous polymers. They are used in transformers, switchgears, capacitors and cables.
18.5.3 Gaseous Dielectrics Air, nitrogen, hydrogen, sulphur hexafluoride are some of the gaseous dielectric materials used. (1) Air Air is one of the most important and naturally available gas used for electrical insulation. Its resistivity is infinity under normal conditions, when there is no ionisation. The relative permittivity of air is 1. It is used as a dielectric in longdistance electrical transmissions, and in aircapacitors. Compressed air is used as an arcextinguishing medium which provides dielectric insulation in airblast circuit breakers.
442
Materials Science
(2) Nitrogen Nitrogen is chemically inert and is used as a dielectric medium to prevent oxidation. It is used in gasfilled highvoltage cables as an inert medium to replace air in the space above the oil. It is also used in transformers and in lowloss capacitors for highvoltage testing, and so on. (3) Sulphur Hexafluoride It is an electronegative gas and is used as a dielectric in Xray equipment, waveguides, coaxial cables, transformers and as an arcquenching medium in circuit breakers. Its dielectric strength is nearly 2.3 times higher than that of air or nitrogen. It sublimes at about 209 k and may be used up to a temperature of 423 k. It is nontoxic, noninflammable and chemically inert. (4) Hydrogen The dielectric strength of hydrogen is about 65% higher than that of air. It is used as a cooling medium in large turbogenerators and synchronous motors. The injurious effects of hydrogen gas are considered to be negligibly small, since during the discharge it does not produce ozone or oxides of nitrogen. Further, the high voltage discharge of hydrogen is not so severe.
18.6
CLASSIFICATION OF ELECTRICAL INSULATING MATERIALS
Electrical insulating materials are generally in the form of solids, liquids or gases. These materials may be either organic or inorganic and can be either natural or synthetic. The electrical insulating materials used in generators, motors, transformers and switchgears, etc., are classified into seven temperature classes, according to their temperature limits based on their thermal stability (Table 18.1).
Table 18.1 Classification of Insulating Materials Temperature K
Class
363
Y
378
A
393
E
403
B
428
F
453
H
>453
C
(1) Class Y Materials such as unimpregnated paper, cotton or silk, vulcanised natural rubber, aniline, urea and various thermoplastics fall under this class. They can be used up to a temperature of 363 K due to the softening points. (2) Class A The following are some of the materials that fall under this class: (i) cotton, silk, paper or similar organic materials impregnated with oil or varnish, (ii) laminated materials with cellulose filler phenolic resins and (iii) a variety of organic varnishes which can be used for wire coating and bonding. (3) Class E Polyurethane, epoxy resins and varnishes, cellulose triacetate, phenol formaldehyde, polyethylene teraphthalate, etc., are the materials which come under the class E. (4) Class B Mica, glass and asbestos fibres and fabrics bonded and impregnated with suitable organic materials such as shellac bitumen, epoxy, phenol or melamine formaldehide are the materials that come under class B.
Dielectric Materials
443
(5) Class F Same as class B, but with resins which are approved for class F operations. For example, alkyd, epoxy and silicone alkyl. (6) Class H Same as class B, but with silicone resins or other resins suitable for class H operations. For example, silicone rubber. (7) Class C Mica, asbestos, ceramics, glass, quartz and similar inorganic materials such as polytetrafluoro ethylene are the materials under class C. Let us discuss some of these solid insulating materials. a. Mica: Mica is an inorganic compound of silicates of aluminium, soda potash and magnesia. It is crystalline in nature and can be splitted into thin sheets. Muscovite and phlogopite are the two important types of mica. Muscovite mica is one of the best insulating materials. Its dielectric constant varies from 5 to 7.5 and its loss tangent varies from 0.0003 to 0.015. The dielectric strength of mica lies between 700 and 1000 kV mm–1. It is used as an insulating material in electrical machines, switch gears, armature windings, and electrical heating devices like electric iron and hot plates. b. Glass: Glass is a brittle and amorphous material. The essential structural constituent of most of the commercial glasses is SiO2. The dielectric constant of glass varies from 3.7 to 10 and its dielectric strength lies between 3000 and 5000 V m–1. The dielectric loss of glass is more complicated. It is used as an internal support in articles like electric light bulbs, electronic valves, mercury switches, Xray tubes, etc. It is also used as a dielectric material in capacitors. c. Ceramics: Ceramics are brittle and can be either amorphous or crystalline. The dielectric and mechanical properties of ceramics are excellent. Their dielectric constant varies from 4 to 10. Ceramics are used as insulators in switches, plugholders and cathode heaters. They can also be used as dielectric materials in capacitors. Porcelein, alumina and titanates are some of the examples of ceramics. d. Asbestos: It is an inorganic material made of magnesium silicate. It has good dielectric and mechanical properties. It is used as an insulator in the form of paper tape, cloth and board. e. Rubber: Rubber is an organic polymer and is available both in natural and synthetic forms. The dielectric constant of rubber varies from 2.5 to 5 and its loss tangent lies between 0.01 and 0.03. It is widely used in electric wires, cables, tapes, coatings, transformers, motor windings, etc.
18.7 CLAUSSIUSMOSOTTI EQUATION Elemental solid dielectrics like germanium, silicon, diamond, sulphur, etc., have no permanent dipoles or ions and will have only cubic structure, thereby exhibiting only electronic polarisation. The total polarisiation is written as, P = N a Ei where
a = ae + ai + a0
Elemental solid dielectrics have only electronic polarisation and the remaining polarisation namely, ionic and orientation, are equal to zero, since there is no ionic character or permanent dipoles. Therefore, the total polarisation P = N ae Ei where ai = a0 = 0, and N is the number of atoms per unit volume.
(18.43)
444
Materials Science
Substituting the value of internal field from Eq. (18.42) in above equation, we get È P ˘ P = N ae Í E + ˙ 3e 0 ˚ Î
(18.44)
We know that, D = e0 E + P P D = – e0 E E From the definition of electric displacement vector,
(18.45)
D=eE Therefore, P = e – e0 = er e0 – e0 E where
er = ere0 P = e0(er – 1) E
or,
P = E e0 (er – 1)
(18.46)
Substituting P value in Eq. (18.44), we get È E e 0 (e r  1) ˘ E e0 (er – 1) = N ae Í E + ˙ 3e 0 Î ˚ È e 0 (e r  1) ˘ e0 (er – 1) = N ae Í1 + ˙ 3e 0 Î ˚ N ae =
e 0 (e r  1) È e 0 (e r  1) ˘ Í1 + ˙ 3e 0 Î ˚
N ae e 0 (e r  1) = 3e 0 3e 0 + e 0 e r  e 0 Simplifying the above equation, we get N ae e 1 = r 3e 0 er + 2
(18.47)
where, N is the number of dipoles per unit volume. Equation (18.47) is known as Claussius–Mosotti equation. In this equation, by substituting the values of er , e0 and N, one can determine the electronic polarisability ae. For a dielectric material consisting of N number of dipoles er  1 1 = 3e0 er + 2
Â Niaei i
where Ni and aei are the appropriate quantities for the types of atoms or molecules.
(18.48)
Dielectric Materials
445
18.8 EXPERIMENTAL DETERMINATION OF DIELECTRIC CONSTANT The Schering bridge is used to determine the dielectric constant of any solid material experimentally. It is one of the modified forms of Wheatstone’s bridge. The experimental arrangement of Schering bridge is shown in Fig. 18.9. Consider that P, Q, R and S are the four arms of the Schering bridge. The arm P consists of a fixed resistance R1 and a variable capacitor C1, while the arm S is made by connecting a resistor R4 and variable capacitor C4 in parallel. The arms Q and R consist of respectively the variable resistor R3 and the fixed capacitor C2. The high frequency oscillator AC is used to give necessary potential to the bridge circuit. The balanced condition of the bridge is obtained by adjusting the values of R3 and C4 in order to get a null deflection in the galvanometer G. The dielectric material whose dielectric constant is to be determined is placed in between the parallel plate capacitor C1. The dielectric constant of the material is determined by measuring the change in capacitive value of capacitor C1 before and after introducing the material in between the parallel plate of C1¢. Therefore, the capacitance of a capacitor C1¢. =
Fig. 18.9
eA d
(18.49)
Scherring bridge—Dielectric constant
where, e is the permitivity of medium present between the parallel plates, d, the thickness of the sample and A, the area of crosssection. After measuring the capacitance of the capacitor, the dielectric material is removed. Therefore, the capacitance of the capacitor C1 is again determined, and is equal to C1 =
e0 A d
(18.50)
where eo is the permitivity of free space. The dielectric constant of a material is equal to the ratio of the capacitance of the capacitor with material and free space.
446
Materials Science
Dielectric constant =
C1¢ C1
(18.51)
Substituting the values of C1 and C1¢, we get Dielectric constant = =
Therefore, the dielectric constant er =
eA d ¥ d eo A e eo
e . e0
(18.52)
The value of C1 and C1¢ of the capacitor are determined by considering the balanced condition of Wheatstone bridge network, i.e., P R = Q S
(18.53)
We know that from Fig. 18.9, 1 j w C1
P = r1 + Q = r3 R=
(18.54) (18.55)
1 j w C2
S = C4  r4 =
(18.56) C 4 r4 C4 + r4
(18.57)
Substituting the value C4 (= 1/jwC4) in the above equation, we get r4 jw C 4 S= r4 +r jw C 4 4 =
r4 1+ r4 jw C 4
Substituting the values of P, Q, R and S in Eq. (18.53), we get r1 +
1 jw C1 = r3
1 jw C2 r4 1 + jw C4 r4
(18.58)
Dielectric Materials
447
Rearranging the above equation, we get r3 r1r4 r 1 = + 4 [ ] jw C2 1 + jw C4 r4 jw C1 1 + jw C4 r4 r3 (1 + jw C4 r4 ) r = r1r4 + 4 jw C2 jw C1
or,
r3 + jw C4 r4 r3 = r1 r4 jw C2 +
or,
r4 C2 C1
(18.59)
Equating the real parts in the above equation, we get
Therefore,
r3 =
r4 C2 C1
(18.60)
C1=
r4 C2 r3
(18.61)
The resistance r4 and capacitor C2 are fixed. Therefore, the value of C1 is determined by varying the variable resistance r3. Therefore, dielectric constant of material er =
C¢ 1 C1
(18.62)
where, C1¢ is the capacitance of the capacitor with dielectric material and C1, the capacitance of capacitor with air as the dielectric. Equation (18.62) is used to determine the dielectric constant of any material experimentally using Schering bridge method.
18.9 DIELECTRIC LOSS When an AC field is applied to a dielectric material, some amount of electrical energy is absorbed by the dielectric material and is wasted in the form of heat. This loss of energy is known as dielectric loss. The dielectric loss is a major engineering problem. In an ideal dielectric, the current leads the voltage by an angle of 90° is shown in Fig. 18.10. But in case of a commercial dielectric, the current does not exactly lead the voltage by 90°. It leads by some other angle q that is less than 90°. The angle f = 90 – q is known as the dielectric loss angle. For a dielectric having capacitance C and voltage V applied to it at a frequency f Hz, the dielectric power loss is given by P = VI cos q Since I = V/Xc where, Xc is the capacitive reactance and is equal to 1/jwC. Therefore,
P=
V2 cos (90 – F) = V2 jwC sin F Xc
(18.63)
448
Materials Science we0 er¢E 0 I
I
J f
f f q
90° V
Fig. 18.10
we0 er ¢¢E0 V
E0
Relation between current and voltage in dielectrics
Since q is very small, sin F = tan F and P = j V2 wC tan F, where tan F is said to be the power factor of the dielectric. The power loss depends only on the power factor of the dielectric as long as the applied voltage, frequency and capacitance are kept constant. The dielectric loss is increased by the following factors: (1) High frequency of the applied voltage (2) High value of the applied voltage (3) High temperature, and (4) Humidity The frequency dependence of the dielectric loss is shown in Fig. 18.11. The dielectric losses in the radio frequency region are usually due to dipole rotation. The dielectric losses at lower frequencies are mainly due to dc resistivity. The dielectric losses in the optical region are associated with electrons and they are known as optical obsorption.
18.10 DIELECTRIC BREAKDOWN
Power loss
When a voltage is appplied to a dielectric material and thereby the electric field is increased, it can withstand up to a certain maximum voltage before it permits large currents to pass through it. This phenomenon in which the dielectric material fails to offer insulation resistance for large applied voltage is known as dielectric breakdown and the corresponding voltage is known as breakdown voltage.
Electrical frequencies Power Audio Radio Frequency
Fig. 18.11
Optical Infrared Visible
Frequency versus dielectric loss
The different types of dielectric breakdown are given below. (1) Intrinsic breakdown (2) Thermal breakdown (3) Electrochemical breakdown
Dielectric Materials
449
(4) Defect breakdown, and (5) Discharge breakdown
18.10.1
Intrinsic Breakdown
If a dielectric material is subjected to a large amount of electric field, then the electrons in the valence band acquire sufficient amount of energy so that they easily cross the energy gap. These electrons while flowing through the conduction band produce a large current. This large current causes the dielectric material to undergo a breakdown.The large number of conduction electrons in the conduction band may collide with the covalent band and consequently, they dislodge more number of electrons. These dislodged electrons, in turn, dislodge some other electrons. Thus, this process goes on as a chain reaction. The breakdown produced in this way is said to be intrinsic breakdown or avalanche breakdown.
Characteristics (1) (2) (3) (4)
It can occur even at low temperature. It requires relatively large electric field. This kind of breakdown occurs mostly in thin samples. It does not depend on the electrode configuration and shape of the material.
18.10.2
Thermal Breakdown
In a dielectric material when an electric field is applied, some amount of heat is produced. The heat produced in the material should be dissipated from it. In some cases, the amount of heat generated is very high compared to the heat dissipated and this excess of heat may produce breakdown of the dielectric material. This type of breakdown is known as thermal breakdown.
Characteristics (1) It can occur only at high temperatures. (2) The strength of the electric field to create dielectric breakdown depends upon the material’s size and shape. (3) The breakdown time is in the order of few milliseconds.
18.10.3
Electrochemical Breakdown
The chemical and electrochemical breakdowns have close relationship with thermal breakdown. If the temperature of a dielectric material increases, it will increase the mobility of the ions and hence, electrochemical reaction will take place. When ionic mobility increases, leakage current will increase, thereby decreasing the insulation resistance, and this will result in dielectric breakdown. In case of rubber, oxides are produced in air and hence, it gradually loses its dielectric property. If one can bring rubber into ozone atmosphere, some cracks are produced.
Characteristics (1) Electrochemical breakdown is determined by the leakage current, density of ions, temperature and permanent dipoles in the material.
450
Materials Science
(2) To avoid electrochemical breakdown, impurities should not be mixed with the pure dielectric materials. (3) Electrochemical breakdowns are accelerated by temperature. To avoid electrochemical breakdown, the dielectric material should not be operated at high temperatures.
18.10.4 Discharge Breakdown Some dielectric materials may have occluded gas bubbles. If these dielectric materials are subjected to high voltages, the gaseous substances are easily ionised and they produce a large ionisation current. This large ionisation current may produce dielectric breakdown. This type of breakdown is known as discharge breakdown.
Characteristics This type of breakdown can occur at low voltages where there are large number of occluded gas bubbles.
18.10.5 Defect Breakdown Some dielectric materials may have surface defects like cracks, pores, etc. Moisture and other impurities can get filled up at these places leading to breakdown. This is known as defect breakdown.
18.11 FERROELECTRIC MATERIAL In certain dielectric materials, polarisation is not a linear function of applied electric field. Such materials exhibit hysteresis curve similar to that of ferromagnetic materials and are known as ferroelectric materials. The hysteresis curve exhibited by a ferroelectric material is shown in Fig. 18.12. P
Psat
Pr A
– Ec
E
0
Fig. 18.12
Hysteresis curve for ferroelectric material
Hysteresis Properties When an increasing electric field is applied to a ferroelectric material, it results in an increase in polarisation and it reaches a maximum value for a particular field strength. On the other hand, if we decrease the electric field, the polarisation decreases. When the field strength is zero, i.e., E = 0, a small amount of polarisation exists in the material. This polarisation is known as remanent polarisation. Now the ferroelectric material is said to be spontaneously polarised. In order to reduce the value of polarisation to zero, an electric field strength (–Ec) should be applied. This field is known as coercive field.
Dielectric Materials
451
The hysteresis loop of a ferroelectric material is explained on the basis of the domain concept. Domain is experimentally observed by applying polarised light, which makes the domain visible. Figure 18.13 explains the domain structure of barium titanate crystal. Domains which are opposite in direction to the applied field decrease in size and domains which are parallel to the field direction increase in size in the form of needles of approximately 10–6 m width. Substances like Rochelle salt (sodiumpotassium salt of tartaric acid; NaKC4H4O21.4H2O), potassium dihydrogen phosphate (KH2PO4), barium titanate (BaTiO3), etc., are typical examples. Ferroelectric crystals lack centre of symmetry.
E
Fig. 18.13
Domain structure of barium titanate
Classification of Ferroelectric Crystals Ferroelectric crystals are classified into three groups namely, (1) Rochelle salt (2) Potassium dihydrogen phosphate, and (3) Barium titanate (1) Rochelle Salt It behaves as a ferroelectric material in the temperature range from 255 to 296 K, i.e., it possesses two transition temperatures (Curie temperature). The crystal structure is orthorhombic above upper curie temperature. Below this transition temperature, the crystal structure is monoclinic in nature. A plot of polarisation versus temperature is shown in Fig. 18.14.
Fig. 18.14
Temperature versus polarisation of Rochelle salt
452
Materials Science
(2) Potassium Dihydrogen Phosphate It has only one Curie temperature and its value is 123 K. It possesses ferroelectric property below this temperature. Above Curie temperature, its crystal structure is tetragonal. Below Curie temperature, the crystal structure is orthorhombic. Other ferroelectric crystals belonging to this family include KD2PO4, RbH2,PO4, CsH2AsO4, CsD2AsO4. The variation of polarisation with respect to temperature is shown in Fig. 18.15.
Fig. 18.15
Polarisation versus temperature in potassium dihydrogen phosphate
(3) Barium Titanate This crystal exhibits three different ferroelectric phases. The transition temperatures of barium titanate are 278 K, 193 K and 393 K. The structure of barium titanate is cubic above 393 K. It has orthorhombic structure when the temperature lies between 278 K and 193 K. Below 193 K, it has rhombohedron structure. The structure of BaTiO3 above 393 K and the variation of polarisation with temperature are given, respectively, in Figs 18.16 and 18.17. Ba 2+ 2–
O 4+ Ti
Fig. 18.16
Crystal structure of barium titanate (above 393 K)
18.12 DIELECTRIC PROPERTIES The following are some of the key properties of dielectric materials that determine their suitability for specific applications: (1) Relative Permittivity Relative permitivity of a material may be expressed by er relative to that of vacuum by er = e/e0. Since the dielectric constant is frequency dependent, it should be taken into account while selecting a dielectric material for a particular use. (2) Dielectric Strength The dielectric strength is the maximum electric field that can be maintained in the dielectric. The dielectric strength depends on the material, its thickness, the shape and size of the conductors between which the dielectric is placed, moisture content of the material, temperature and pressure.
Dielectric Materials
453
16 12 Ps –2 (X10 2 cm ) 8 4 73
Fig. 18.17
113
153 193
233 273 313 T(k)
353
393 433
Polarisation versus temperature in barium titanate
(3) Dielectric Losses The extent to which a dielectric, in an alternating electric field, loses energy is indicated by the loss factor, tan f. A very good dielectric would have a loss factor of the order of 10–5 with a poor one of about 0.1. (4) Mechanical Properties In selecting a dielectric there may be a need to consider the mechanical properties of the material. Many of the dielectrics are very brittle. Properties which may need to be considered are the effects of bending, impact strength, tearing strength, tensile strength, compressive strength, shear strength, and machinability. (5) Insulation Resistance Dielectrics need to have a high insulation resistance in order to prevent leakage of charge. The resistance of these materials should be very high. (6) Temperature Effects One of the main effects of an increase in temperature is a decrease in resistivity and higher leakage currents through the dielectrics. The leakage current increases with increase in temperature and it will produce breakdown in the dielectric material. Other thermal properties that need to be considered in selecting a dielectric are melting points, freezing points for liquid dielectrics, thermal expansivity, specific heat capacity and ageing effect.
18.13
ACTIVE AND PASSIVE DIELECTRICS
A dielectric material which exhibits gain (current or voltage or both) and has directional electronic properties is said to be active dielectric. Piezoelectric, ferroelectric and several other voltage induced or voltage inducing materials are said to be active dielectrics. For example, quartz is an active dielectric material even though it is a piezoelectric material. Similarly, a dielectric material which does not exhibit any gain or directional property is said to passive dielectric. Most of the insulating materials like ceramics, mica, etc., belong to this category.
18.14
FREQUENCY AND TEMPERATURE DEPENDENCE OF DIELECTRIC PROPERTIES
The dielectric properties such as polarisation, dielectric constants and dielectric loss depend on the frequency of the applied field and temperature. Let us discuss the frequency and temperature dependence of polarisation and dielectric constant.
454
Materials Science
18.14.1 Frequency Dependence of Dielectric Properties (1) Polarisation When an AC field is applied to a dielectric material, the polarisation of the dielectric material is a function of time. It follows the equation È Ê t ˆ˘ P(t) = P Í1  exp Á  ˜ ˙ Ë t r ¯ ˙˚ ÍÎ
(18.64)
where P is the maximum polarisation attained by a dielectric due to the prolonged application of the electric field, and tr, the relaxation time for the particular polarisation process is the average time between molecular collisions (in case of liquid), during the application of the electric field. The relaxation time is a measure of the polarisation process and is the time taken for a polarisation process to reach 67% of the maximum value. From Fig. 18.18, it can be inferred that the space charge polarisation occurs at very low frequencies (less than 102 Hz). Space charge polarisation refers to the diffusion of metal ions over several interatomic spacing. It also occurs at machine frequencies in the order of 50–60 Hz. Space charge polarisation is one of the slowest process compared to other types of polarisation.
Space charge
Polarisation
Orientation Ionic
Electronic
10
–2
Fig. 18.18
1
10
6
10
12
10
16
Frequency dependence of the polarisation processes
Orientation polarisation mechanism arises in the polar molecules when an AC field is applied. This polarisation mechanism is faster than space charge polarisation but is slower than the ionic and electronic polarisations. In many liquid dielectrics, orientation polarisation occurs between the radio wave and microwave frequency range at room temperature. In some polymeric liquids, it involves a limited rotation of molecules and occurs even at low frequencies. Ionic polarisation mechanism occurs in the ionic molecules, whenever the frequency of the applied field is less than 1013 Hz. Ionic polarisation does not occur at optical frequencies (ª1015 Hz), since the ionic molecules require time nearly 100 times greater than the frequency of the applied field. Ionic polarisation is faster than orientation and space charge polarisations, but it is slower than electronic polarisation. Electronic polarisation is the fastest polarisation and it occurs immediately after the supply is switched on. This polarisation occurs even at optical frequencies.
Dielectric Materials
455
(2) Dielectric Constant The frequency dependence of the real and imaginary part of dielectric constant is shown in Fig. 18.19. The curve is similar to that of the frequency dependence of polarisation as shown in Fig. 18.18. Figure 18.19 shows distinct peaks in er and some distinct features in er¢, but in reality these peaks and features are broader. The variations in er¢ and er≤ are produced by the presence of different polarisation mechanisms. Interfacial and space charge Orientational, dipolar Ionic
Electronic
er
e r¢ = 1
e¢¢r
10–2
Fig. 18.19
18.14.2
6
1
10 Frequency
10
12
10
16
Frequency dependence of dielectric constant
Temperature Dependence of Dielectric Properties
Orientation polarisation is produced due to the alignment of dipoles in polar molecules in the presence of electric field. The increase in temperature disrupt the alignment of dipole due to the electric field. This effect decreases the value of dielectric constant with increase in temperature. For example, the dielectric constant of solid HCl decreases from 19 to 14, when the temperature is increased from 100 to 160 K. At the melting point of 160 K, it drops to 12. This shows that the number of molecules per unit volume decreases due to the expansion on melting. Solid nitrobenzene is a polar molecule, but it does not exhibit orientation polarisation in its solid state because the rotation of the molecules is prevented under an applied field. But in liquid state, the molecules have sufficient energy to reorient themselves in the applied field. The relative dielectric constant increases from 3 to 37 on melting. This is in contrast with the results obtained for solid HCl. The dielectric properties of four insulators are given in Table 18.2.
Table 18.2 Dielectric Properties of Different Insulators at Two Different Frequencies f = 60 Hz
Material er¢
f = 1 MHz
tan d
er¢
tan d
Polycarbonate
3.17
9 ¥ 10–4
2.96
1 ¥ 10–2
Silicone rubber
3.7
2.25 ¥ 10–2
3.4
4 ¥ 10–3
Epoxy with mineral filler
5.0
4.7 ¥ 10–2
3.4
3 ¥ 10–2
Alumina
8.5
8.5
1 ¥ 10–3
1¥
10–3
456
Materials Science
In case of the polymer film Polyethyleneterephthalate (PET), the dielectric constant er¢ measured at f = 10 kHz is found to increase with increase in temperature as shown in Fig. 18.20. 2.60 e¢r 2.58 PET, f = 10 kHz 2.56 293
Fig. 18.20
313
333 T(K)
353
Variation of er¢ with temperature in PET material
18.15 USES OF DIELECTRIC MATERIALS Some of the most important properties of insulating materials are that they possess excellent mechanical and electrical strength, high thermal and electrical stability, etc. In view of the above properties, dielectrical materials are used as insulating materials in applications like power distribution transformers, capacitors, cables, transmission equipment, etc.
18.15.1 Capacitors Dielectric materials are used to manufacture capacitors of different ranges. The selection of right dielectric materials for capacitor applications is based on various parameters like value of capacitance, frequency, tolerance lens, size and operating voltage. Dielectric materials, paper and plastic film, mica film, single layer ceramic, multilayer ceramic, solid electrolytic (Al, Ta) and electrolytic (AI, Ta) are used in capacitors to obtain a range of capacitance 1 pf to 104 m f. (1) Single and Multilayer Dielectric Capacitors The schematic representation of a single layer capacitor is shown in Fig. 18.21. It consists of a thin ceramic disk or plate and metal electrodes. The ceramic plate is placed inbetween the metal electrodes. The leads for the electrical connections are taken from the metal electrode. In order to prevent the degradation of dielectric properties of ceramic plate due to moisture the whole setup is encapsulated in an epoxy coating. The capacitance of single layer capacitor for an area of 1 cm2 is 885 pf. One can increase the capacitance of the capacitor by connecting N number of ceramic plate in parallel by providing a sufficient space as shown in Fig. 18.21(b). The capacitor with stacking of ceramic plates in different layers is known as multilayer capacitor. The capacitance of multilayer capacitor is in the range of a few hundred microfarads. (2) Polymeric Film Capacitors Polymer thin film capacitors are constructed to work as midfrequency capacitors. Two separate thin polymer sheet metals coated by having a small margin on one side employing vacuum deposition. The two metal coated films are placed in parallel by keeping the margin in the opposite side. Thus, the two margins are opposite in directions. In order to get the capacitor, the two metal sheets are rolled together like Swiss roll. The electrical connections are taken from the opposite sides of the metals by proper soldering. One can also produce multilayer polymeric thin film capacitors like multilayer ceramic capacitors.
Dielectric Materials
457
Metal termination
Ceramic
Epoxy
Leads Metal electrode (a) Singlelayer ceramic capacitor (e.g., disk capacitors)
Fig. 18.21
(b) Multilayer ceramic capacitor (stacked ceramic layers)
Dielectric capacitors
(3) Electrolytic Capacitors Large values capacitors are achieved using electrolytic capacitors. Electrolytic capacitors are of different types namely, aluminum electrolytic and solid electrolyte tantalum capacitors. A crosssectional view of aluminum electrolytic capacitors is shown in Fig. 18.22. The Al electrolytic capacitor consists of two Al foils. Electrolyte Al2O3 Cathode Anode
Al foils
Al +
Al _
Al case _ +
Fig. 18.22
Cross sectional view
Aluminum electrolytic capacitors
A thin layer of Al2O3 as a dielectric medium is grown on the rough surface of one of the foils. The two foils are wound together in the form of disk and kept inside the cylindrical case as shown in Fig. 18.3. The thickness of Al2O3, grown on the foil is 0.1 m and hence, it gives large capacitance value (i.e, small thickness and large area. The Al2O3 is grown on the Al foil eleeterolytically and hence, this capacitor is known as electrolytic capacitor. A thin film of Al2O3 dielectric coated on the surface of Al foil acts as anode, on the other hand, Al foil act as a Cathode. Polymer film Al metallization
(a) Aluminium Coating on film
Fig. 18.23
(b) Capacitor
Aluminum electrolytic capacitors
458
Materials Science
The structure of a solid electrolyte tantalum capacitor is shown in Fig. 18.24(a). The anode is made up of tantalum (Ta) pellet. The surface of Ta pellet is anodized to get the tantalum pentoxide (Ta2O2). A thick solid electrolyte like MnO2 is coated above Ta2O2. The process is completed by coating graphite and silver paste as shown in Fig. 18.24(b). The above system is then coated by an epoxy. Tantalum capacitors are widely used in electronic applications. Ta2O2 Graphite Silver Ta MnO2 paste
Epoxy Silver paint Ta +
–
–
+ Leads (a) Solid electroyte tantalum capacitors
Fig. 18.24
(b) Crosssectional view
Aluminum electrolytic capacitors
(4) Power and Distribution Transformers Following are the applications of insulating materials in power and distribution of transformers: a. Transformer oil is used as a liquid dielectric and coctat b. Electrical grade paper is used as layer binding insulation such as a cover to cover the cable and as a backing paper is used for applications such as top and bottom coil clamping ring, washer, etc. c. The insulation tape is used for applications such as taping and banding, core insulation, banding of transformer cores, etc. d. Materials such as synthetic rubbers are used as a gasket in different places to percent oil leakages from joints In order to meet the above requirements the insulating dielectric material requires the following properties: Excellent electrical properties to withstand high voltages. High dielectric strength and adequate chemical stability. Very high moisture resistance.
18.16 APPLICATIONS Some of the applications of dielectric materials are given below. a. Quartz crystal is used for the preparation of ultrasonic transducers, crystal oscillators, delay lines, filters, etc. b. Barium titanate is used for the preparation of accelerometers. c. Lead zirconate titanate (PbZrxTi1–xO3) is used for the preparation of earphones, microphones, spark generators (gas lighter, car ignition, etc.), displacement transducer, accelerometers, etc. d. The insulating dielectric liquids are used in transformers, switchgears and generators. e. Dielectric materials are used as insulating material in power cables, signal cables, electric motors, electric iron, etc.
Dielectric Materials
459
f. Dielectric materials are used in radiation detectors, thermoionic valves, strain gauges, capacitors, resistors and many other electric devices, and g. The electrooptic devices are prepared using dielectric material.
Key Points to Remember The force per unit charge is known as electric field strength E. The permitivity of free space, i.e., vacuum eo = 8.854 ¥ 1012 F m1. The electrical flux density is defined as the number of flux lines crossing a surface normal to the lines divided by the surface area. The dielectric constant of a material is defined as the ratio of permitivity of the medium to e permitivity of free space e r = . eo The product of magnitude of charge and distance of separation is known as electric dipole moment. Polarisation is defined as induced dipole moment per unit volume. There are four different types of polarisations namely, electronic, atomic, orientation and interfacial polarisation. The electronic polarisation of a solid material which contains large number of atoms is equal to Pe = 4N p eo R3 E. An electronic polarisation is polarisation produced due to the displacement of electron when an electric field is applied to the atom. An atomic or ionic polarisation is polarisation due to the displacement of positive ions away from the field and the negative ions towards the field due to the application of an electric field. The internal field or local field in a solid dielectric material is equal to the sum of the applied field plus the field produced at the location of an atom by dipoles of all other atoms. Dielectric materials are classified into solid dielectric, liquid dielectric and gaseous dielectric materials. The Claussius–Mosotti equation for a solid material is N ae er  1 = 3e0 er + 2 Dielectric loss is the loss of energy in the form of heat wasted due to absorption of electrical energy by a dielectric material when an AC field is applied to the material. Dielectric breakdown is the phenomenon in which the dielectric material fails to offer insulation resistance for a large applied voltage. There are five different types of dielectric breakdown namely, intrinsic, thermal, electrochemical, defect and discharge. The dielectric materials which exhibit hysteresis curve similar to that of ferromagnetic materials are known as ferroelectric materials. Ferroelectric materials are classified into three major classes as Rochelle salt, potassium dihydrogen phosphate and barium titanate. Active dielectric materials are the materials which exhibit gain in current or voltage or both and have directional electronic properties. Passive dielectric materials do not exhibit any gain or directional properties.
460
Materials Science
Solved Problems Example 18.1 The lattice parameter of KCl is 0.629 nm. It crystallises like the NaCl crystal structure. The electronic polarisability of K+ is 1.264 ¥ 10–40 F m2 and that of Cl– is 3.408 ¥ 10–40 F m2. Calculate the relative permitivity of KCl crystal at optical frequencies. Given Data: Lattice parameter of KCl = 0.629 ¥ 109 m The electronic polarisability ae, for K+ = 1.26 ¥ 10–40 F m2 The electronic polarisability ae, for Cl– = 3.408 ¥ 10–40 F m2 Solution:
The electronic polarisability ae for KCl = (ae for K+ + ae for Cl–1) = 1.264 ¥ 10–40 + 3.408 ¥ 10–40 = 4.672 ¥ 10–40 F m2 The number of dipoles per m3 (N) = =
Number of atoms Volume of the unit cell 4 (0.629 ¥ 109 )3
= 1.607 ¥ 1028 atoms m–3. The dielectric constant is given by e0 (er – 1) = Nae er =
=
Na e +1 e0 1.607 ¥ 1028 ¥ 4.672 ¥ 10 40 +1 8.854 ¥ 1012
= 1.8479 The dielectric constant of KCl is 1.848. Example 18.2 Calculate the electronic polarisability of an isolated Se atom. The atomic radius of an Se atom is 0.12 nm. Given Data: The atomic radius of Se = 0.12 ¥ 109 m
Dielectric Materials
Solution:
461
The electronic polarisability is given by ae = 4pe0R3 = 4p ¥ 8.854 ¥ 10–12 (0.12 ¥ 10–9)3 = 1.9226 ¥ 10–40 F m2 The electronic polarisability of an isolated Se is 1.9226 ¥ 10–40 F m–2.
Example 18.3 The following data refers to a dielectric material er = 4.94 and n2 = 2.69, where n is the index of refraction. Calculate the ratio between electronic and ionic polarability for this material. Given Data: The dielectric constant er = 4.94 The refraction index Solution:
n2 = 2.69
We know that, the Clasius  Mosotti relation e  1 Na = r 3e 0 er + 2 (i) At optical frequencies er = n2, the electronic polarisation alone occurs at optical frequencies e  1 Na = r 3e 0 er + 2
Therefore,
We know that the electrical polariability a = ae + ai + ao Since the orientation polariability (a0) is very less it can be neglected. a = ae + ai
Therefore,
Substituting Clausius–Mosotti relation, we get N (a e + a1 ) e r  1 = er + 2 3e 0 Simplifying the above equation, we get ae + ai (e  1) (n 2 + 2) = r ae (e r  2) (n 2 + 1) Substituting the values of er and n2, we get \ or,
1+
a i (4.94  1) (2.69 + 2) = ¥ a e (4.94 + 2) (2.69  1) ai = 0.5755 ae
462
Materials Science
ae = 1.7376 ai The ratio of the electronic to ionic polariability is 1.7376. Example 18.4 The polarisability of Ne gas is 0.35 ¥ 10–40 F m2. If the gas contains 2.7 ¥ 1025 atoms m–3 at 0 °C and 1 atmospheric pressure, calculate its relative dielectric constant. Given Data: The electronic polarisability ae = 0.35 ¥ 10–40 F m2 The number of atoms N = 2.7 ¥ 1025 atoms m–3 Solution:
The dielectric constant is given by e r  1 Na i e r + 2 3e 0 Substituting N, ae and e0 values in the above equation, we get 2 Na e 3e 0 er = Na e 13e 0 Substituting the values of N, ae and e0 in the above equation, we get 1+
Na e 2.7 ¥ 1025 ¥ 0.35 ¥ 1040 = 3e 0 3 ¥ 8.854 ¥ 1012 = 3.5577 ¥ 10–5 Therefore, 1 + 2 (3.5577 ¥ 105 ) 1  3.5577 ¥ 105 = 1.00010673
The dielectric constant er =
The dielectric constant of Ne gas is 1.00010673. Example 18.5 A parallel plate capacitor consists of 2 plates each of area 5 ¥ 104 m2. They are separated by a distance of 1.5 ¥ 103 m and filled with a dielectric of relative permittivity 6. Calculate the charge on the capacitor if it is connected to a 100 volts DC supply. Given Data: Area of the capacitor plate
A = 5 ¥ 104 m2
Distance between the plates
d = 1.5 ¥ 103 m
Relative permittivity of the dielectric
er = 6
Applied voltage
V = 100 V
Permittivity in free space
e0 = 8.85 ¥ 1012 F m1
Dielectric Materials
Solution:
463
We know that, the capacitance of the capacitor is Q = C V C= Q=
e0 er A d e 0 e r AV d
Substituting the values, we get =
8.85 ¥ 1012 ¥ 6 ¥ 5 ¥ 1014 ¥ 100 1.5 ¥ 103
= 1.77 ¥ 109 The charge on the capacitor is 1.77 ¥ 109 C. Example 18.6 Ar gas contains 2.7 ¥ 1025 atoms m–3 at 0 °C and at 1 atmospheric pressure. Calculate the dielectric constant of the Ar gas at this temperature, if the diameter of the Ar atom is 0.384 nm. Given Data: The number of Ar atoms m–3 = 2.7 ¥ 1025 m–3 The diameter of Ar atom = 0.384 ¥ 109 m Solution:
The electronic polarisability of Ar atom ae = 4pe0R3 = 4p ¥ 8.854 ¥ 10–12 ¥ (0.384 ¥ 10–9)3 = 0.63 ¥ 10–40 F m–2 The dielectric constant of Ar, using Clausius–Mosotti equation is 2 Na e 3e 0 er = Na e 13e 0 1+
Substituting the values of N, ae and e0 in the above equation, we get 2 ¥ 2.7 ¥ 1025 ¥ 0.63 ¥ 1040 3 ¥ 8.854 ¥ 1012 2.7 ¥ 1025 ¥ 0.63 ¥ 1040 13 ¥ 8.854 ¥ 1012
1+ er =
1.000128078 0.9999359611 = 1.000192129
=
The dielectric constant of Ar is 1.000192129.
464
Materials Science
Example 18.7 A parallel plate capacitor has a capacitance of 2mF. The dielectric has permitivity, er = 80. For an applied voltage of 1 kV, find the energy stored in the capacitor as well as the energy stored in polarizing the dielectric. Given Data: The capacitance C = 2 mF = 2 ¥ 10–6 F The permittivity of the dielectric er = 80 Applied voltage V = 1 kV = 1000 V Solution:
The energy stored in the capacitor E1 =
1 C V2 2
1 ¥ 2 ¥ 106 ¥ (1000) 2 = 1 J 2 The capacitance of the capacitor when the dielectric is removed =
C0 =
C er
2 ¥ 106 = 2.5 ¥ 10–8 F 80 The energy stored in the capacitor with vacuum as dielectric, 1 E2 = C0 V2 2 =
=
1 ¥ 2.5 ¥ 108 ¥ (1000) 2 = 0.0125 J 2
Energy stored in the capacitor in polarising the dielectric, C = E1 – E2 =
1 (C – C0) V2 2
E = 1 – 0.0125 = 0.9875 J The energy stored in the capacitor = 1 J The energy stored in polarising the capacitor = 0.9875 J Example 18.8 A solid contains 5 ¥ 1028 identical atoms per m3, each with a polarisability of 2 ¥ 10–40 F m2. Assuming that the internal field is given by the Lorentz relation, calculate the ratio of the internal field to the applied field. Given Data: Number of atoms present per m3 N = 5 ¥ 1028 m3 Polarisability
ae = 2 ¥ 10–40 F m2
Dielectric Materials
Solution:
465
P 3e 0
The Lorentz relation
Ei = E +
The polarisation
P = Nae Ei = 5 ¥ 1028 ¥ 2 ¥ 10–40 ¥ Ei = 1 ¥ 10–11 ¥ Ei Ei = E +
The Lorentz field
i.e.,
1 ¥ 1011 ¥ Ei 3e 0
È 1 ¥ 1011 ˘ Í1 ˙ E =E 3e 0 ˚ i Î
or,
Ei 1 = E È 1 ¥ 1011 ˘ Í1 ˙ 3e 0 ˚ Î Ei È ˘ 1011 = Í1 12 ˙ E Î 3 ¥ 8.854 ¥ 10 ˚
1
= 1.60379
The ratio of the internal field to the applied field = 1.6038. Example 18.9 If a NaCl is subjected to an electrical field of 1000 V m1 and the resulting polarisation is 4.3 x 108 C/m2, calculate the relative permittivity of NaCl. Given Data: E = 1000 V m1
Applied electrical field
P = 4.3 ¥ 108 C m2
Polarisation Permittivity in free space Solution:
e0 = 8.85 ¥ 1012 F m1
We know that the relative permittivity of NaCl is er = 1 +
P e0 E
Substituting the values, we get =1+
4.3 ¥ 1018 (8.85 ¥ 1012 ) (1000)
= 5.86 The relative permittivity of NaCl is 5.86.
466
Materials Science
Example 18.10 Calculate the electronic polarisability of argon atom given er = 1.0024 at NTP and N = 2.7 ¥ 1025 atoms/m3. Given Data: Relative permitivity
er = 1.0024
Number of atoms
N = 2.7 ¥ 1025 atoms m3 e0 = 8.85 ¥ 1012 F m1
Permitivity in free space Solution:
We know that the polarisability of argon atom is, P = e0 (er – 1)E P = NaeE ae =
e 0 (e r  1) N
Substituting the values, we get ae =
(8.85 ¥ 1012 ) (1.0024  1) 2.7 ¥ 1025 ae = 7.9 ¥ 1040 F m2
Therefore, the polarisability of argon atom is 7.9 ¥ 1040 F m2. Example 18.11 The dielectric constant of He gas at NTP is 1.0000684. Calculate the electronic polarisability of He atoms if the gas contains 2.7 ¥ 1025 atoms per m3. Given Data:
Solution:
The dielectric constant of the gas at NTP
er = 1.0000684
The number of He atoms
N = 2.7 ¥ 1025 m3
Permitivity in free space
e0 = 8.85 ¥ 1012 F m1
We know that the electronic polarisability ae is ae =
e 0 (e r  1) N
Substituting the values, we get =
8.85 ¥ 1012 ¥ (1.0000684  1) 2.7 ¥ 1025
= 2.242 ¥ 1041 Fm2. Therefore, the electronic polarisability of He atoms at NTP is equal to 2.242 ¥ 1041 Fm2.
Dielectric Materials
467
Example 18.12 An elemental dielectric material has a relative dielectric constant of 12. It also contains 5 ¥ 1028 atoms m3. Calculate the electric polarisability assuming the Lorentz field. Given Data:
Solution:
The relative dielectric constant of the material
er = 12
The number of atoms in the element
N = 5 ¥ 1028 m3
Permittivity in free space
e0 = 8.85 ¥ 1012 F m1
We know that the electronic polarisability is ae =
e 0 (e r  1) N
Substituting the values, we get ae =
8.85 ¥ 1012 ¥ (12  1) 5 ¥ 1028
= 1.947 ¥ 1039 Therefore, the electronic polarisability of given element is 1.947 ¥ 1039 F m2. Example 18.13 A parallel plate condenser has a capacitance of 2 mF. The dielectric has permitivity er = 100. For an apllied voltage of 1000 V, find the energy stored in the condenser as well as the energy stored in polarizing the dielectric. Given Data:
Solution:
Capacitance of plate condenser
C = 2 ¥ 106 F
The applied voltage
V = 1000V
The dielectric permitivity
er = 100
1 2 Total energy stored in the capacitor E = CV 2 Substituting the values of C and V in the above equations, we get 1 ¥ 2 ¥106 ¥ (103 ) 2 2 =1J
E=
We know that the energy stored in the dielectric material which is introduced in between the parallel plates of the condenser, capacitance has to be calculated removing the dielectric material. C0 =
C er
468
Materials Science
Substituting the values, we get =
2 ¥ 108 = 0.02 mF 100
Energy stored without the dielectric =
1 C0 V 2 2
Substituting the values, we get 1 ¥ 0.02 ¥ 106 ¥ (103 ) 2 2 = 0.01 J
=
Therefore, the energy stored in the dielectric = 1 – 0.01 = 0.99 joules The energy stored in the dielectric is 0.99 J. Example 18.14 The dielectric constant of sulphur is 3.4. Assuming a cubic lattice for its structure, calculate the electronic polarisability of sulphur. Given, density of sulphur = 2.07 g/cc and atomic weight = 32.07 Given Data: The dielectric constant of sulphur er = 4.94
Solution:
The density of sulphur
= 2.07 ¥ 103 kg m3
Atomic weight of sulphur
= 32.07
We know that number of atoms per unit volume is N=
N A ¥ 103 ¥ density Atomic density
Substituting the values, we get 6.023 ¥ 1023 ¥ 103 ¥ 2.07 ¥ 103 32.07 28 = 3.89 ¥ l0 m−3.
=
We know that the Claussius–Mosotti relation for cubic structure of sulphur Nae er  1 = 3e 0 er + 2
Dielectric Materials
469
Therefore, the electronic polarisability is given by ae =
3e 0 Ê e r  1 ˆ N ÁË e r + 2 ˜¯
Substituting the values of N, e0, and er, we get =
3 ¥ 8.854 ¥ 10 12 Ê 3.4  1 ˆ Á ˜ 3.89 ¥ 1028 Ë 3.4 + 2 ¯ = 3.035 ¥ l0−40
Therefore, the electronic polarisability of sulphur is 3.035 ¥ 10−40 F m2. Example 18.15 A parallel plate capacitor has an area of 6.45 ¥ 10−4 m2 and the plates are separated by a distance of 2 mm across which a potential of 10 V is applied. If a material with a dielectric constant of 6 is introduced between the plates, determine the capacitance, charge stored on each plate, and polarisation. Given Data: Area of the capacitor plate
A = 6.45 ¥ 10−4 m2
Distance between the plates
d = 2 ¥ 10−3 m
Relative permittivity of the dielectric er = 6
Solution:
Applied voltage
V = 10 V
Permitivity in free space
e0 = 8.85 × 10−12 F m−1
We know that the capacitance of the capacitor is e0e r A d Substituting the values of e0, er, A and d in the above equation, we get C=
5
8.85 ¥ 10 12 ¥ 6 ¥ 6.45 ¥ 10 4 2 ¥ 10 3
= 17.13 ¥ l0−12 The capacitance of the capacitor is 17.13 pF. We know that the charge stored on the capacitor is Q = CV Substituting the value of C and V, we get = 17.13 ¥ l0−12 ¥ 10 = 17.13 ¥ 10−11 The charge stored on the capacitor is 16.147 ¥ 10−11 C.
470
Materials Science
Similarly, we know that the electric field strength is V d Substituting the values of V and d in the above equation, we get 10 = 2 ¥ 103 E=
= 5 ¥ l03 Vm−1 We know that the polarisation is P = e0 (er21)E Substitute the values of e0, er and E in the above equation, we get = 8.854 ¥ l0−12 ¥ (6  l) ¥ = ¥ l03 = 2.214 ¥ 10−7 The polarisation produced in plate is 2.214 ¥ 10−7 Cm−2. Therefore, the capacitance of the capacitor is 17.13 pF. The charge stored on the capacitor is 16.147 ¥ 10−11 C. The polarisation produced in plate is 2.214 ¥ 10−7 Cm−2. Example 18.16 What is the polarisation produced in sodium chloride by an electric field of 600 V/mm if it has a dielectric constant of 6? Given Data: E = 600 V mm−1 or 600 ¥ 103 V m−1
Electric field strength
Dielectric constant of sodium chloride er = 6 Solution:
We know that the polarisation is P = e0 (er  1)E Substitute the values e0, er and E, we get = 8.854 ¥ 10−12 ¥ (6 − 1) ¥ 600 ¥ 103 = 2.656 ¥ 10−5 Therefore, the polarisation produced in sodium chloride is 2.656 ¥ 10−5 Cm−2.
Example 18.17 If NaCl is subjected to an electrical field of 1000 V m−1 and the resulting polarisation is 4.3 ¥ 10−8 C/m2, calculate the relative permitivity of NaCl. Given Data: Applied electrical field
E = 1000 V m−1
Polarisation
P = 4.3 ¥ 10−8 Cm−2
Permitivity in free space
e0 = 8.85 ¥ 10−12 F m−1
Dielectric Materials
Solution:
471
We know that the relative permitivity of NaCl is P e0 E Substituting the values P, e0 and E in the above equation, we get er = 1 +
= 1+
4.3 ¥ 1018 (8.85 ¥ 1012 )(1000)
5 5.86 Therefore, the relative permitivity of NaCl is 5.86. Example 18.18 What is the resulting voltage across the plates of a parallel plate capacitor with plates of area 1000 m2, carrying a charge of 3 ¥ 10−10 C, and separated by 5 mm, when a material of dielectric constant 4 is introduced between them and to determine the electric field? Given Data: Area of the capacitor plate
A = l000 ¥ 10−6 m2
Distance between the plates
d = 5 ¥ 10−3 m
Relative permitivity of the dielectric er = 4
Solution:
The charge on the capacitor
Q = 3 ¥ 10−10 C
Permitivity in free space
e0 = 8.85 ¥ 10−12 F m−1
We know that the capacitance of the capacitor is C=
e0e r A d
Substituting the values, we get 5
8.85 ¥ 10 12 ¥ 6 ¥ 7.45 ¥ 10 4 5 ¥ 10 3
= 7.0832 ¥ l0−12 The capacitance of the capacitor is 7.0832 pF. We know that voltage across the capacitor is V=
Q C
Substituting the values of Q and C in the above equation, we get 3 ¥ 1010 =
7.0832 ¥ 1012
= 42.35
472
Materials Science
The voltage across the capacitor is 42.35 V. We know that the electric field strength is E=
V d
Substituting the values of V and d in the above equation, we get 42.35 =
5 ¥ 103
= 8470 Therefore, the electric field strength is 8470 V m−1. Example 18.19 The dielectric constant of He gas at NTP is 1.0000684. Calculate the electronic polarisability of He atoms if the gas contains 2.7 ¥ 1025 atoms per m3. Given Data: The dielectric constant of the gas at NTP er = 1.0000684
Solution:
The number of He atoms
N = 2.7 ¥ 1025 m−3
Permitivity in free space
e0 = 8.85 ¥ 10−12 F m−1
We know that the electronic polarisability is ae =
e 0 (e r  1) N
Substituting the values e0, er and N in the above equation, we get =
8.85 ¥ 1012 ¥ (1.0000684  1) 2.7 ¥ 1025
= 2.242 ¥ l0−41 F m2. Therefore, the electronic polarisability of He atoms at NTP is equal to 2.242 ¥ 10−41 F m2. Example 18.20 A parallel plate capacitor has an area of 3 ¥ 10−3 m2 and the plates are separated by a distance of 1 mm. If a material with a dielectric constant of 3.5 is introduced between the plates, determine the capacitance of the capacitor and the electric field that is required to be applied for a charge of 20 nC to get stored on each plate. Given Data: Area of the capacitor plate
A = 3 ¥ 10−3 m2
Distance between the plates
d = 1 ¥ 10−3 m
Relative permitivity of the dielectric
er = 3.5
Dielectric Materials
Solution:
The charge on the capacitor
Q = 20 ¥ 10−9 C,
Permitivity in free space
e0 = 8.85 × 10−12 F m−1
473
We know that the capacitance of the capacitor is C=
e0e r A d
Substituting the values of e0, er , A and d in the above equation, we get 8.85 ¥ 1012 ¥ 3.5 ¥ 3 ¥ 103 =
1 ¥ 103
= 92.925 ¥ 10−12 The capacitance of the capacitor is 92.93 pF. We know that, the electric field strength is E=
Q Cd
Substituting the values of Q, C and d in the above equation, we get 20 ¥ 109 =
92.93 ¥ 1012 ¥ 1 ¥ 103
= 215.22 ¥ l03 Therefore, the electric field strength is 215.22 ¥ 103 V m−1. Example 18.21 A parallel plate capacitor has an area of 7.45 ¥ l0−4 m2 and its plates are separated by a distance of 2.45 ¥ 10−3 m across with a potential of 10 V applied. If a material with dielectric constant 6 is introduced between the plates, determine the capacitance, the charge stored in each plate, the dielectric displacement D and the polarisation. Given Data: Area of the capacitor plate
A = 7.45 ¥ 10−4 m2
Distance between the plates
d = 2.45 ¥ 10−3 m2
Relative permitivity of the dielectric er = 6
Solution:
Applied voltage
V = 10 V
Permitivity in free space
e0 = 8.85 × 10−12 F m−1
We know that the capacitance of the capacitor is C=
e0e r A d
474
Materials Science
Substituting the values of e0, er , A, and d in the above equation, we get 5
8.85 ¥ 10 12 ¥ 6 ¥ 7.45 ¥ 10 4 5 ¥ 10 3
= 16.147 ¥ l0−12 The capacitance of the capacitor is 16.147 pF. The charge stored on the capacitor is Q = CV Substituting the value of C and V, we get = 16.147 ¥ l0−12 ¥ 10 = 16.147 ¥ l0−11 The charge stored in the capacitor is 16.147 ¥ 10−11 C. Similarly, we know that the electric field strength is E=
V d
Substituting the values of V and d in the above equation, we get 10 =
2.45 ¥ 103
= 4.08 ¥ 103 V m−1 We know that the polarisation is given by P = e0(er  1)E Substituting the values of e0, er and E in the above equation, we get = 8.854 ¥ 10−12 ¥ (6  1) ¥ 4.08 ¥ 103 = 1.806 ¥ l0−7 The polarisation produced in sodium chloride is 1.806 ¥ 10−7 Cm−2 We know that the dielectric displacement is D = e0er E Substituting the values of e0, er and E in the above equation, we get = 8.854 ¥ l0−12 ¥ 5 ¥ 4.08 ¥ l03 = 2.167 ¥ 10−7 Therefore, the dielectric displacement is 2.167 ¥ 10−7 Cm−2.
Dielectric Materials
475
Example 18.22 What is the polarisation produced in sodium chloride by an electric field of 500 V m−1 if it has a relative permitivity of 6? Given Data:
Solution:
Electric field strength
E = 500 Vm−1
Dielectric constant of sodium chloride
er = 6
We know that the polarisation is P = e0(er  1)E Substituting the values of e0, e r and E in the above equation, we get = 8.854 ¥ l0−12 ¥ (6  l) ¥ 500 = 2.214 ¥ 10−8 Therefore, the polarisation produced in sodium chloride is 2.214 ¥ 10−8 Cm−2.
Example 18.23 Find the polarisation produced in a dielectric medium of relative permitivity 15 in the presence of an electric field of 500 V/m. Given Data:
Solution:
Electric field strength
E = 500 V m−1
Dielectric constant of sodium chloride
er = 15
We know that the polarisation P = e0 (er  1)E Substitute the values of e0, er and E in the above equation, we get = 8.854 ¥ l0−I2 ¥ (15  l) ¥ 500 = 6.198 ¥ 10−8 Therefore, the polarisation produced in sodium chloride is 6.198 ¥ 10−8 C m−2.
Example 18.24 A parallel plate capacitor of 650 mm2 area and a plate separation of 4 mm have charge of 2 ¥ 10−10 C on it. What is the resultant voltage across the capacitor when a material of dielectric constant 3.5 is introduced between the plates? Given Data:
Solution:
Area of the capacitor plate
A = 650 mm2
Distance between the plates
d = 4 mm
Relative permittivity of the dielectric
er = 3.5
Charge on the capacitor
Q = 2 ¥ 10−10 C
We know that, the capacitance of the capacitor is Q = CV C=
e0e r A d
476
Materials Science
C=
and
Q V
Comparing the above two equations, we get Q e0e r A = V d V=
or,
Qd e0e r A
2 ¥ 1010 ¥ 4 ¥ 103 =
8.85 ¥ 1012 ¥ 650 ¥ 106 ¥ 3.5
= 39.73 V Therefore, the voltage across the capacitor is 39.73 V. Example 18.25 A parallel plate capacitor consists of 2 plates, each of area 5 ¥ 10−4 m2. They are separated by a distance 1.5 ¥ 10−3 m and filled with a dielectric of relative permitivity 6. Calculate the charge on the capacitor if it is connected to a 100 volts DC supply. Given Data: Area of the capacitor plate
A = 5 ¥ 10−4 m2
Distance between the plates
d = 1.5 ¥ l0−3 m
Relative permitivity of the dielectric er = 6
Solution:
Applied voltage
V = 100 V
Permitivity in free space
e0 = 8.85 ¥ 10−12 F m−1
We know that the capacitance of the capacitor is Q = C V C=
e0e r A d
e 0 e r AV d Substituting the values e0, er , A, V and d in the above equation, we get Q=
and
8.85 ¥ 1012 ¥ 6 ¥ 5 ¥ 1014 ¥ 100 =
1.5 ¥ 103 = 1.77 ¥ 10−9
Therefore, the charge on the capacitor is 1.77 ¥ 10−9 C Example 18.26 The atomic weight and density of sulphur are 32 and 2.08 ¥ 103 kg m−3, respectively. The electronic polarisability of the atom is 3.28 ¥ 10−40 F m2. If sulphur solid has cubic structure, calculate its dielectric constant.
Dielectric Materials
Given Data: The density of sulphur
= 2.08 ¥ 103 kg m3
Atomic weight of sulphur = 32 Electronic polarisability Solution:
= 3.28 ¥ 10−40
We know that the Claussius–Mosotti relation for cubic structure of sulphur Nae er  1 = 3e 0 er + 2 Substituting the values of N, ae, and e0 in the above equation, we get e r  1 3 ¥ 1028 ¥ 7 ¥ 10 40 = er + 2 3 ¥ 8.854 ¥ 10 12 = 0.7906 Rearranging the above equation, we get er−1 = (er + 2) ¥ 0.7906 or, Therefore,
er−1 = 0.7906 er + 1.5812 er (1  0.7906) = 2.5812 er =
2.5812 0.2094
= 12.327 Therefore, the dielectric constant of the given material is 12.327.
ObjectiveType Questions 18.1. The force acting per unit charge E is equal to Q Q Q2 Q2 (a) E = (b) E = (c) E = (d) E = 2 2 p r2 4pe r 4pe r 2pe r2 18.2. The value of permitivity of free space is equal to ______. 18.3. The dielectric constant of a solid material is equal to ______. e e (a) eo = (b) er = e eo (c) eo = e er (d) er = er eo 18.4. The polarisation of a solid material is equal to P = ______. 18.5. The unit for polarisation is______. 18.6. The polarisation of a solid which contain N number of particles per unit volume is equal to (a) Pe = N a E (b) Pe = 2 N a E (c) Pe = N a2 E (d) Pe = N a2 E2 18.7. The electronic polarisation of a solid material which contains N number of atoms are (a) Pe = N2pe0 R3 E (b) Pe = Npe0 R3 E (c) Pe = N4pe0 R3 E (d) Pe = N4pe0 R3 18.8. The atomic polarisation exihibit in ionic molecules like______and______.
477
478
Materials Science
18.9. The value of ionic polarisability is equal to ai ______. 18.10. Dipolar or orientation polarisation is produced in______molecules. 18.11. The value of orientation polarisation is equal to______. 1 Ê m2 E ˆ (a) Pe = Á F ˜ 3 Ë RT ¯
18.12. 18.13. 18.14. 18.15.
1Ê m Eˆ (b) Pe = Á F ˜ 3 Ë RT ¯
Ê m2 E ˆ
(c) Pe = Á F ˜ Ë RT ¯
value of orientation polarisation is equal to______. total polarisation in a solid material is equal to P 5 ______. internal field, i.e., equal to Ei 5 E 1 ______. internal or Lorentz field is equal to P2 P (a) Ei 5 E 1 Ec (b) Ei = (c) Ei = E + 3e0 3 e0
3 Ê m2 E ˆ (d) Pe = Á F ˜ 4 Ë RT ¯
The The The The
(d) Ei = E +
P 3 e0
18.16. Give an example for dielectric solid materials______. 18.17. Give an example for polar solid dielectric materials______. 18.18. The ClaussiusMosotti equation for a solid dielectric material is equal to N ai e r  1 3N ai e r  1 N ai e r + 1 N ai e r  1 = = (a) (b) (c) (d) = = 3 e0 e r + 2 e0 er + 2 3 e0 e r  2 e0 er + 2 18.19. Dielectric materials which exhibit hysteresis curve are known as ______materials. 18.20. Curie temperature for Rochelle salt is______and______K. 18.21. The transition temperature for Barium titanate ferroelectric phases are (a) 278 and 193 K (b) 278 and 393 K (c) 278, 193 and 393 K (d) 278, 193 and 300 K 18.22. Examples for active dielectric materials are______, ______and______. 18.23. Give two examples for passive dielectric materials______and______. 18.24. Polarisation is a function of time È È ˘ Ê ˆ˘ (a) P (t ) = P Í1  exp Ê t ˆ ˙ (c) P (t ) = P Í1  exp t ˙ ÁË T ˜¯ ÁË T ˜¯ ÍÎ ÍÎ r ˙ r ˙ ˚ ˚
18.25. 18.26.
18.27. 18.28.
18.29.
È È Ê ˆ˘ Ê ˆ˘ (b) P (t ) = P Í1 + exp t ˙ (d) P (t ) = P Í1 + exp t ˙ ÁË T ˜¯ ÁË T ˜¯ ÍÎ ÍÎ r ˙ r ˙ ˚ ˚ A pair of equal and opposite charges q are separated by a distance L. The dipole moment of the system is (a) q/L (b) qL (c) L/q (d) q/L2 Electronic polarisation (a) Increases with temperature (b) Decreases with tempertaure (c) Independent of temperature (d) None of these The polarisation that occurs in the frequency range 1012 Hz is (a) Ionic (b) Electronic (c) Orientational (d) None of these In the inverse piezoelectric effect (a) Ultrasonic waves are produced (b) Electromagnetic waves are produced (c) Microwaves are produced (d) None of these The unit of dipole moment/unit volume is (a) coulomb /metre (b) coulomb /metre2 (c) coulomb /metre3 (d) coulomb
Dielectric Materials
18.30. Flux density is related to the electric field as (a) D = e + E (b) D = e – E
(c) D = e
479
(d) D = eE
E
18.31. In a solid or liquid dielectric with external applied electrical field, as the electronic polarisability ae increases, the internal field Ei, (a) Increases (b) Reduces (c) Remains constant (d) None of these 18.32. In a dielectric, the polarisation is (a) Linear function of applied field (b) Square function of applied field (c) Exponential function of applied field (d) Logarithmic function of applied field Answers 18.1. 18.3. 18.5. 18.7.
(b) (d) Cm2 (c)
18.9. ai =
18.2. 18.4. 18.6. 18.8.
e2 Ê 1 1 ˆ Á + ˜ w02 Ë M m ¯
18.10. Polar
18.11. (a)
18.12.
18.13. 18.15. 18.17. 18.19. 18.21. 18.23. 18.25. 18.27. 18.29. 18.31.
18.14. 18.16. 18.18. 18.20. 18.22. 18.24. 18.26. 18.28. 18.30. 18.32.
Pe + Pi + Po (d) C6H5NO2 Ferroelectric Pe + Pi + Po Ceramic, mica (b) (a) (b) (a)
8.854 ¥ 1012 F m1 M/Volume (a) NaCl, KBr
mF2 3 RT The field due to all other dipoles Diamond (b) 255, 296 Piezoelectric, ferroelectric and quartz (d) (c) (a) (a) (a)
Short Questions 18.l. Distinguish between a dielectric material and an insulator. 18.2. What is meant by polarisation in a dielectric material? 18.3. What is meant by dielectric loss? 18.4. What is meant by local field in a solid dielectric? 18.5. Explain the term dielectric breakdown. 18.6. Write the ClaussiusMosotti equation for a solid dielectric and explain the terms. 18.7. Mention the different types of dielectric materials? 18.8. What are the properties of dielectric materials? 18.9. What are the uses of dielectric materials?
480
Materials Science
18.10. 18.11. 18.12. 18.13. 18.14. 18.15. 18.16. 18.17. 18.18. 18.19. 18.20. 18.21. 18.22. 18.23. 18.24. 18.25. 18.26. 18.27. 18.28. 18.29. 18.30. 18.31. 18.32. 18.33.
What are ferroelectric materials? Give an example. What is ferroelectricity? List the different types of ferroelectric materials. Explain the crystal structure of Rochelle salt. What are the changes observed in the crystal structure of BaTiO3 with change in temperatures? What is a domain in a ferroelectric material? What is remanent polarisation? What is coercive field in a ferroelectric material? What are active and passive dielectrics? What is electronic polarisation? What is ionic polarisation? What is dipolar polarisation? What is space charge polarisation? What are dielectric materials? Explain their properties. Give examples. What are dielectrics? Write about important applications of dielectric materials. Define dielectric constant of a material. Explain the phenomenon of electric polarisation in dielectric materials. What is polarisation in dielectrics? What is electric polarisation of an atom? Define dielectric polarisation. Derive the relation between dielectric polarisation and dielectric constant. Explain electronic polarisation mechanisms. Explain the changes observed in a dielectric material with increase in temperature in terms of polarisations with the help of diagrams. 18.34. Explain dielectric polarisability.
Descriptive Questions 18.1. What is meant by polarisation? Write an essay about the different types of polarisation mechanisms involved in a dielectric material? 18.2. What is meant by local field in a solid dielectric? Deduce an expression for the local field in a solid dielectric and hence obtain ClausiusMosotti relation. 18.3. What is meant by dielectric loss? Explain the phenomenon of dielectric loss in detail. 18.4. Write an essay about the different types of dielectric breakdown. 18.5. What are the different types of dielectric materials? Explain them in detail. 18.6. What is ferroelectricity? Explain the hysteresis curve exhibited by a ferroelectric material with a suitable sketch. Give examples for ferroelectric materials. 18.7. Explain with the help of a neat sketch the frequency and temperature dependence of dielectric properties. 18.8. Explain the classification of insulating materials based on their temperature stability.
Dielectric Materials
481
Exercises 18.1. A condenser of 1mF contains titanium oxide as a dielectric with er = 100. For an applied DC voltage of 1000 V, find the energy stored in polarising the titanium oxide. Answer the same question for a 1 mF mica condenser, assuming the dielectric constant er = 5.4 for mica. 18.2. An atom of polarisability a is placed in a homogeneous field E. Show that the energy stored in a polarised atom is equal to 1/2 a E2. 18.3. The electronic polarisability of the Ar atom is 1.7 ¥ 1040 F m2. What is the static dielectric constant of solid Ar (below 84 K) if its concentration is 2 ¥ 1025 atoms m3? 18.4. The dielectric constant of Si is 11.9. What is the electronic polarisability due to the valence electrons per Si atom? 18.5. An elemental dielectric material has er = 12 and it contains 5 ¥ 1028 atoms m3. Calculate the electronic polarisability assuming Lorentz field. 18.6. The relative permitivity of Ar at 0ºC and 1 atmospheric pressure is 1.000435. Calculate the polarisability of the atom. 18.7. The dielectric constant of He at 0ºC and 1 atmospheric pressure is 1.000074. Calculate the dipole moment induced in each He atom at an electric field intensity of 3 ¥ 104 Vm1. 18.8. What is the resulting voltage across the plates of a parallel plate capacitor with plates of area 1000 mm2, carrying a charge of 3 ¥ 1010 C, and seperated by a distance of 5mm, when a material of dielectric constant 4 is introduced between them? 18.9. Same as above problem and added to it is to determine the electric field. 18.10. A parallel plate capacitor has an area of 3 ¥ 103 m2 and the plates are separated by a distance of 1mm. If a material with dielectric constant of 3.5 is introduced between the plates, determine the capacitance of the capacitor and the electric field that is required to be applied for a charge of 20 nC to get stored on each plate.
Chapter
19
MAGNETIC MATERIALS
OBJECTIVES To understand the principle, theory, properties and applications of magnetic materials. To study the different types of magnetic materials along with suitable examples. To derive the necessary theory for diamagnetism, paramagnetism, ferromagnetism and antiferromagnetism. To discuss the experimental methods used to study the paramagnetic properties of materials. To discuss the structure, property and applications of ferromagnetic materials. To study the hard and soft magnetic materials and the energy product of magnetic materials. To study the magnetic materials used in storage devices and their applications.
19.1
INTRODUCTION
The materials which strongly attract a piece of iron are known as magnetic materials or magnets. The magnetic property of a material arises due to the magnetic moment or magnetic dipole of materials. Materials which are magnetised by the application of an external magnetic field are known as magnetic materials. Similarly, materials which are not magnetised due to the application of an external magnetic field are known as nonmagnetic materials. The magnetism of materials is responsible for magnetic moment of materials. When a current flows through a conductor, it produces a magnetic moment along the axis of the coil. Similarly, the electrons revolving around the nucleus leads to an orbital magnetic moment. The spin magnetic moment arises due to the spin ( ±1 / 2 ) of electrons. Magnetic materials are more important in terms of potential practical applications like magnetic storage and biomedical uses. General classes of magnetic materials are diamagnetic, paramagnetic, ferromagnetic, antiferromagneitc and ferrimagnetic materials.
Magnetic Materials
483
In this chapter, the basic parameters and classification of magnetic materials are discussed in the first few sections. The different types, theories, properties and applications of magnetic materials are discussed in following sections.
19.2 MAGNETIC PARAMETERS The magnetic property of materials depends on the degree of magnetisation. The parameters such as magnetisation, magnetic susceptibility and magnetic permeability are used to characterise magnetic materials. Let us discuss the important magnetic parameters which are used to characterise magnetic materials. (1) Magnetic Dipole The magnetic dipoles, generally known as north and south poles, commonly exist in magnetic materials. The magnetic dipoles are not separate poles unlike an electric dipole. (2) Magnetic Field Strength The magnetic field strength H at any point in a magnetic field is the force experienced by a unit north pole placed at that point. Its unit is A m1. (3) Magnetic induction or Flux density The magnetic induction or flux density B in any material is defined as the number of lines of force through a unit area of crosssection perpendicularly. Therefore, Magnetic induction B =
f A
(19.1)
where A is the area of crosssection and f, the magnetic lines of force. The unit for B is Wb m2. (4) Magnetic Dipole Moment Consider that m is the magnetic pole strength and 2l, the length of magnet. The magnetic dipole moment is equal to the product m × 2l. Magnetic dipole moment mm = m × 2l
(19.2)
The magnetic dipole moment is a vector quantity. (5) Magnetisation or Intensity of Magnetisation Magnetisation, or intensity of magnetisation is the measure of magnetism of magnetic materials and is defined as the magnetic moment per unit volume. M=
mm V
(19.3)
where V is the volume. The unit for M is A m1. (6) Magnetic Susceptibility Magnetic susceptibility (c) is used to explain the magnetisation of materials. It is defined as the ratio of magnetisation to the magnetic field strength. Magnetic susceptibility c =
M H
(19.4)
(7) Magnetic Permeability The magnetic permeability m is defined as the ratio of amount of magnetic density B to the applied magnetic field intensity H. It is used to measure the magnetic lines of forces penetrating through a material. m=
B H
(19.5)
484
Materials Science
Rearranging the above equation, we get Magnetisation B = m0 (M + H)
(19.6)
where m0 is the permeability of free space and is equal to 4p ¥ 107 H m 1.
Relation Between Magnetic Parameters Relative permeability of a material is defined as the ratio of permeability of the medium to free space, i.e.,
Relative permeability mr =
m m0
(19.7)
Substituting the values of m = B/H, we get mr =
B m0 H
(19.8)
Substituting the value B from Eq. (19.6) in the above equation, we get mr =
m0 ( M + H ) m0 H
mr = Therefore, relative permeability
M H + H H
(19.9)
mr = 1 + c
(19.10)
It is clear that the magnetic parameters are analogous to dielectric parameters. The comparisons of magnetic and dielectric parameters are given in Table 19.1.
19.3
BOHR MAGNETON
The magnetic moment of an atomic particle is represented by unit ampere metre2. The magnetic moment of an atomic particle is very low, and it is usually represented by a unit known as Bohr magneton. The value of one Bohr magneton is, 1 Bohr magneton =
eh 4p m
(19.11)
Substituting the values of e, m and h, we get 1 Bohr magneton (b) =
1.6 ¥1019 ¥ 6.626 ¥1034 4p ¥ 9.1¥1031
1b = 9.27 ¥ 1024 A m2 The magnetic moment of an electron is 1 Bohr magneton.
(19.12)
Magnetic Materials
Table 19.1
485
Comparison of Magnetic and Dielectric Parameters
Sr. No. Dielectric parameters
Magnetic parameters
1.
Electric field
Magnetic field
2.
Electric displacement
Magnetic induction
3.
Electric dipole moment
Magnetic dipole moment
4.
Permitivity
Permeability
5.
Polarisation
Magnetisation
6.
Nonpolar dielectric
Diamagnetic
7.
Polar dielectric
Paramagnetic
8.
Ferroelectric hysteresis
Ferromagnetic hysteresis
9.
Remanent polarization
Remanent magnetisation
10.
Coercive electric field
Coercive magnetic field
11.
Ferroelectric domain
Magnetic domain
12.
Ferroelectric Curie temperature
Ferromagnetic Curie temperature
13.
Converse piezoelectric effect
Magnetostriction effect
19.4 CLASSIFICATION OF MAGNETIC MATERIALS Magnetic materials are classified into two categories based on existence of dipole moment and the response of the magnetic material to external magnetic fields. (1) Diamagnetic materials—no permanent magnetic moment. (2) Paramagnetic, ferromagnetic, antiferromagnetic and ferrimagnetic materials—possess permanent magnetic moment. Generally, diamagnetic and paramagnetic materials are known as nonmagnetic materials, due to poor response to an external magnetic field. Ferromagnetic, antiferomagnetic and ferrimagnetic materials are known as magnetic materials. These materials are strongly responsive to an external magnetic field. The different types of nonmagnetic and magnetic materials are discussed briefly in the following sections:
19.4.1 Diamagnetic Materials All materials exhibit diamagnetic properties. In diamagnetic materials, magnetic dipoles are oriented in such a way that the resultant dipole moment is zero. When an external magnetic field is applied, the individual dipoles are rotated and hence, produce an induced dipole moment. The induced dipole moment opposes the external magnetic field. As a result, the magnetic fields are repelled from the materials. This effect is known as diamagnetism. The existence of diamagnetism is represented by means of simple representation as shown in Fig. 19.1. During the absence of an external magnetic field, the magnetic moment of atoms is zero. On the other hand, when an external field is applied, atoms acquire induced dipole moment and hence, move opposite to field directions. This results in repulsion of magnetic lines of force.
486
Materials Science
H = 0 and M = 0 (a) Absence of field
Fig. 19.1
H = H0 and M = M0 (b) Presence of field
Diamagnetic properties
Properties Following are the properties of diamagnetic materials: (1) They do not have a permanent dipole moment. (2) Magnetic effects are very weak and hence, often masked by other kind of magnetism. (3) They repel the magnetic lines of force. The existence of this behaviour in a diamagnetic material is shown in Fig. 19.2.
Bπ0
B =0
Normal conductor
Fig. 19.2
Diamagnetic material
Diamagnetic material—Magnetic field
(4) The magnetisation becomes zero on removal of the external field. (5) The susceptibility of a diamagnetic material is negative. (6) The susceptibility is independent of temperature and external field. Examples of diamagnetic materials are copper, gold, mercury, silver and zinc.
19.4.2
Paramagnetic Materials
Paramagnetic materials possess a permanent magnetic moment. During the absence of an external magnetic field, the dipoles are randomly oriented. This is due to thermal agitation present in materials. Therefore, the net dipole moment and hence, magnetisation of the material is zero. When an external magnetic field is applied, the magnetic moments of individual atoms align themselves in the direction of the field and hence, give nonzero magnetisation. The behaviour of a paramagnetic material under the influence of an external field is shown in Fig. 19.3.
Magnetic Materials
487
H = H0 and M = +M0
H = 0 and M = 0 (a) Absence of field
Fig. 19.3
(b)
Presence of field
Paramagnetic properties
Properties Following are the properties of paramagnetic materials: (1) Paramagnetic materials possess a permanent dipole moment. (2) The magnetic dipoles are aligned randomly. The magnetic spin alignment is shown in Fig. 19.4.
Fig. 19.4
Paramagnetic material—spin arrangement
(3) They attract the magnetic lines of force. (4) The susceptibility is positive and depends on temperature: c=
C T
(19.13)
where C is the Curie constant and T, the temperature. Equation (19.13) is known as the Curie law of paramagnetism. (5) Paramagnetic susceptibility is inversely proportional to temperature. Examples of paramagnetic materials are aluminum, chromium, sodium, titanium, zirconium, etc.
19.4.3 Ferromagnetic Materials Ferromagnetic materials possess permanent magnetic moment which is mainly due to the spin magnetic moment. The magnetic dipoles are aligned parallel to each other due to interaction between any two dipoles. The ferromagnetic materials exhibit spontaneous magnetisation, even in the absence of an external field. Due to the strong internal field which exists in materials, the alignment of magnetic moments results. On the other hand, when a small magnetic field is applied, it produces a large value of magnetisation due to the parallel alignment of dipoles. In a ferromagnetic material, the influences of internal and external fields make them different from other magnetic materials. The molecular field theory, or Weiss theory, is used to explain the ferromagnetic properties of materials.
488
Materials Science
Properties The properties of ferromagnetic materials are as follows: (1) The magnetic dipoles are arranged parallel to each other. The dipoles arrangement is shown in Fig. 19.5.
Fig. 19.5
Ferromagnetic materials—dipoles arrangements
(2) They possess permanent dipole moment. (3) They attract the magnetic lines of force strongly. (4) They have characteristic temperature, namely, ferromagnetic Curie temperature (qf ). Materials below qf behave as ferromagnetic materials and obey hysteretic curve. A material behaves as a paramagnetic when it is above qf . (5) During the absence of a magnetic field, it exhibits magnetisation which is due to the property of spontaneous magnetisation. (6) The susceptibility of a ferromagnetic material is C T q where, C is Curie constant and q, the paramagnetic Curie temperature. c=
(19.14)
Equation (19.14) is shown as Curie–Weiss law. This law holds good when the temperature is greater than (T > q). Examples of ferromagnetic materials are iron, cobalt and nickel.
19.4.4
Antiferromagnetic Materials
In ferromagnetic materials, we know that the magnetic dipoles are parallel to each other. This is due to the existence of a strong interaction known as exchange interaction between the spin magnetic moments. Similarly, in a few materials, the exchange interaction leads to antiparallel alignment of dipoles. The magnitudes of all dipoles are equal and hence, resultant magnetic moment and magnetisation is zero. The antiparallel alignment exists in materials below a critical temperature known as Neel temperature.
Properties The important properties of antiferromagnetic materials are as follows: (1) The dipoles are aligned antiparallel as shown is Fig. 19.6.
Fig. 19.6
Antiferromagnetic materials—dipole arrangements
Magnetic Materials
489
(2) When the temperature increases, susceptibility increases and reaches a maximum at a temperature known as Neel temperature, beyond which it decreases. (3) The value of susceptibility is positive and is very small when T is greater than the Neel temperature, TN. C c= (19.15) T +q (4) Antiparallel alignment of dipole is due to exchange interactions. Examples of antiferromagnetic materials are ferrous oxide, manganese oxide, manganese sulphite, chromium oxide, etc.
19.4.5 Ferrimagnetic Materials Ferrimagnetic materials are a special case of antiferromagnetic materials. The magnetic dipoles are antiparallel, similar to an antiferromagnetic material. However, their magnitudes are not equal. This is due to the magnetic interactions existing between dipoles. Therefore, ferrimagnetic materials possess net magnetic moments due to the antiparallel dipoles with different magnitudes. Hence, they produce a large magnatisation even for a small applied external field.
Properties The properties of ferrimagnetic materials are as follows: (1) The dipoles are antiparallel as shown in Fig. 19.7. However, the dipoles are not equal in magnitude. (2) Net magnetisation is larger even for a small external field. (3) The susceptibility is positive and very large when the temperature is higher than TN, c=
C T ±q
(19.16)
(4) They behave as paramagnetic and ferromagnetic materials, respectively, above and below Curie temperature. (5) Ferrimagnetic domains are used as magnetic bubbles in memory elements.
Fig. 19.7
Ferrimagnetic materials—dipole arrangements
19.5 ORIGIN OF PERMANENT MAGNETIC MOMENT The term permanent magnetic moment represents the presence of magnetic moment in an atom of a magnetic material even in the absence of a magnetic field. The magnetic moment arises in an element due to the presence of angular momentum. There are three different types of angular momentum namely, (1) Orbital Angular Momentum of an electron, (2) Spin Angular Momentum of an electron, and (3) Nuclear Spin Angular momentum. Let us discuss the contribution of magnetic moment due to the above different types of angular moments.
490
Materials Science
19.5.1
Orbital Angular Momentum of an Electron
The orbital angular momentum of an electron arises due to its orbital motion. The relation between the magnetic moment and orbital angular momentum is mm =
e ma 2m
(19.17)
where ma is the orbital angular momentum and is equal to ma =
lh 2p
(19.18)
According to quantum theory, quantum numbers such as n, l, m1 and ms are used to represent the state of an electron. The quantum number n is called the principal quantum number. It represents the energy possessed by an electron. It takes integer values such as 1, 2, 3… n. The quantum number l is known as orbital quantum number. It takes values such as 0, 1, 2 …. (n1). It represents the orbital motion of an electron. The quantum number m1 is known as magnetic orbital quantum number. It represents the orientation of electronic orbits based on the externally applied magnetic field. It takes discrete values ranging from –l to +l including zero. The angular momentum of an electron due to its orbital motion is given by l ( h / 2p ) . The quantum numbers for an electron in K shell are n = l, l = 0, m1 = 0 and ms = ± ½. Substituting l = 0 in Eq. (19.18), we get the orbital angular momentum is zero. For an electron in the L shell, the quantum numbers are n = 2, l = 0, 1, m1 = 0, ±1, ms = 0, ±1/2. Substituting l = 1 in Eq. (19.18), we get the angular momentum of an electron as (h/2p). There are three possible directions (m1 = 0, +1, 1) for the orbital motion of an electron with l = 1. These three values for m1 contribute three different values of h h the angular momentum of an electron. They are , 0, . The magnetic moment contributed by 2p 2p electrons with l = 1 is written from Eq. (19.18) as, mm =
e h eh , 0, 2m 2p 4p m
(19.19)
For an element having completely filled shells, the total orbital magnetic moment is zero because the sum of the magnetic moment is zero. Therefore, if there is an unfilled electronic state in an atom for an element, then the total orbital magnetic moment is not equal to zero. Therefore, materials with unfilled electronic states are important for physicists and electrical engineers. The elements with atomic numbers 21 through 28 (the iron group), 39 through 45, 58 through 71 (the rare earths) and 89 through 92 have unfilled electronic states. For an electrical engineer, the iron group elements with atomic numbers 21 through 28 are the most important. The above information shows that elements with unfilled electronic states have permanent dipole moments.
19.5.2
Spin Angular Momentum of an Electron
The electrons possess angular momentum due to their spinning motion. The magnetic spin quantum number ms gives the direction of spin vectors of an electron. There are two possible directions for spin vectors, namely, upward and downward spins. Therefore, the quantum number ms takes only two values namely, ±1/2.
Magnetic Materials
491
The relation between magnetic moment and spin angular momentum is, mm = 
e ms m
(19.20)
where ms is the angular momentum contributed by the spinning motion of an electron. The possible values 1 h 1 h of ms = . ,2 2p 2 2p Therefore, from Eq. (19.20), the magnetic moment contributed by the spinning motion is, mm = 
eh eh or + 4p m 4p m
=  1 b or 1 b
(19.21)
For elements having completely filled electronic states, the magnetic moment contributed by the spin motion is zero. It confirms that a material with unfilled electronic states possesses permanent dipole moment due to spin motion.
19.5.3 Nuclear Magnetic Moment The magnetic moment of a nucleus is known as nuclear magneton and it is given as, mm =
eh 4p M N
(19.22)
where MN is the mass of the nucleon. The mass of the nucleon is MN = 1.66 ¥ 1027 kg. This mass is nearly 1824 times greater than that of an electron and hence, the nuclear magneton is nearly 103 times smaller than the electron magnetic moment. Therefore, this value is negligible compared to the magnetic moment of an electron.
19.6 DIAMAGNETISM Diamagnetic materials possess a weak induced magnetic field when an external magnetic field is applied. The induced magnetic field is produced due to electromagnetic induction. Lenz’s law states that the magnetisation (M) will oppose the applied magnetic field (H). The susceptibility of a diamagnetic material is very small and negative. It is usually less than 105. Diamagnetism is very weak and it is present in most materials. Examples of diamagnetics are copper, gold and germanium. Let us discuss the theory about diamagnetic materials in this section.
19.6.1 Langevin’ s Theory of Diamagnetism The permanent magnetic moment arises if there is any unfilled electronic state in the atoms of an element. When all states are completely filled, then there is no permanent dipole moment. Inert gases such as He, Ne and Ar have c